3 Wiley Series on Polymer Engineering and Technology Richard F. Grossman and Domasius Nwabunma, Series Editors Polyolefi n Blends Edited by Domasius Nwabunma and Thein Kyu Polyolefi n Composites Edited by Domasius Nwabunma and Thein Kyu Handbook of Vinyl Formulating, Second Edition Edited by Richard F. Grossman Total Quality Process Control for Injection Molding, Second Edition M. Joseph Gordon, Jr. Microcellular Injection Molding Jingyi Xu Poly(lactic acid): Synthesis, Structures, Properties, Processing, and Applications Edited by Rafael Auras, Loong - Tak Lim, Susan E.M. Selke, and Hideto Tsuji Hyperbranched Polymers: Synthesis, Properties, and Applications Edited by Deyue Yan, Chao Gao, and Holger Frey Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation Sven Engelmann
4 Advanced Thermoforming Methods, Machines and Materials, Applications and Automation Sven Engelmann Director of Polymer Technology Gerhard Schubert GmbH Crailsheim, Germany A John Wiley & Sons, Inc., Publication
5 Copyright 2012 by John Wiley & Sons, Inc. All rights reserved Published by John Wiley & Sons, Inc., Hoboken, New Jersey Published simultaneously in Canada No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, recording, scanning, or otherwise, except as permitted under Section 107 or 108 of the 1976 United States Copyright Act, without either the prior written permission of the Publisher, or authorization through payment of the appropriate per-copy fee to the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, (978) , fax (978) , or on the web at Requests to the Publisher for permission should be addressed to the Permissions Department, John Wiley & Sons, Inc., 111 River Street, Hoboken, NJ 07030, (201) , fax (201) , or online at permissions. Limit of Liability/Disclaimer of Warranty: While the publisher and author have used their best efforts in preparing this book, they make no representations or warranties with respect to the accuracy or completeness of the contents of this book and specifically disclaim any implied warranties of merchantability or fitness for a particular purpose. No warranty may be created or extended by sales representatives or written sales materials. The advice and strategies contained herein may not be suitable for your situation. You should consult with a professional where appropriate. Neither the publisher nor author shall be liable for any loss of profit or any other commercial damages, including but not limited to special, incidental, consequential, or other damages. For general information on our other products and services or for technical support, please contact our Customer Care Department within the United States at (800) , outside the United States at (317) or fax (317) Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic formats. For more information about Wiley products, visit our web site at Library of Congress Cataloging-in-Publication Data Engelmann, Sven. Advanced thermoforming : methods, machines and materials, applications and automation by / Sven Engelmann. p. cm. Includes index. ISBN (cloth) 1. Thermoforming. I. Title. TP1151.T48E '23 dc Printed in the United States of America
6 For my lovely wife Ulrike and my wonderful children Leo, Peter, and Luzy.
7 Contents Preface xi 1. Introduction 1 2. Basics of Thermoforming and Thermoplastics 5 3. Production of Semifinished Products, Extrusion, and Coextrusion Introduction to Technical Parts Antenna Radome Manufacturing Fuel Tank Production on Sheet Machines Automotive Body and Commercial Vehicle Applications Production of Refrigerator Liners Paint Replacement in Automotive Applications Motor Air Intake Made from PA 6 GF Sanitary Equipment (Sheet Machine) Thermoforming and Milling of Large-Scale Formed Parts (Sheet Machine) Changeover of Sheet Machines Chromed Parts Applications in Aircraft and Mass Transportation High-Quality and Fully Transparent Products (Sheet Machines) Deco Molding and Multi-deco Molding 106 vii
8 viii Contents 18. Automotive Body Parts Made of PA + ABS Softfeel Made from ABS/TPU Material Introduction to Packaging Optimizing a Thermoforming Process for Packaging Analysis of Thermoforming Films Advanced Analysis of Thermoforming Films Analysis of Thermoformed Products Analysis of Completely Formed, Filled, and Sealed Containers Automated Packaging Production of Flowerpots Steel Rule Die Punching Production of Meat Trays Multilayer Films for Thermoforming Applications PET in Thermoforming Applications Thermoformed Packaging Made of PLA Peel and Reseal Foam Packaging with PP and PS Blister Packaging of Syringes The Production of Drinking Cups Ultrasonic Sealing and Cutting in Thermoforming Understanding the Brittle Behavior of Polystyrene Cups Preprinted Film for Lid Thermoforming 308
9 Contents ix 40. Flexible Films Simulation Recycling 324 Glossary 328 Index 329
10 Preface This book focuses on practical applications. It deals with technical parts, but also with packaging (the topics range from bathtubs to syringe blisters). Beside the applications, the respective machine and tooling technologies, automation, and, of course, semifinished products and materials are described. Also a large part of the book is dedicated describing innovations in materials, so that the book can serve as a useful reference work on raw materials and semifinished products. Also discussed are multilayer structures, which are finding increasing use for fuel tanks as well as cheese packaging. Reliable applications of machine, tooling, and materials are demonstrated. The basic principles of extrusion, which are important for thermoforming are named for clarity s sake without going into depth. The basic principles of thermoforming and thermoplastics are covered briefly, as there are already several standard works dealing with these subjects. The present book is intended to complement, not replace the existing literature on thermoforming, and to open up new perspectives on the applications considered within. The author is grateful to all those writers who have advanced, described, and explained thermoforming and made it popular. The aim of the book is to communicate points worth knowing about thermoforming and to arouse interest. The author hopes this book will show the reader the diversity and sophistication of the thermoforming industry and ways of implementing cost - effective production. S ven Engelmann xi
11 Chapter 1 Introduction Reference books can be difficult to read and understand. Often technical connections and contexts are described by using a lot of mathematics and often right from the beginning so that a large part of the target group is overcharged or quickly loses interest. However, reading books on technology and engineering can be fun. Books dealing with technology should impart knowledge at an adequate pace. We live in a world that is dependent on a multitude of technologies. Yet it can be observed that fewer and fewer young people are interested in technical professions. What are the reasons for this development? It is true that the rush of today s technology can initially have a discouraging effect. A lot of technology has become so complex and abstract that it is no longer possible to understand the connections through mere reflection or observation. As the modifications to technologies and processes come even faster, is it possible to keep up with these developments? The answer is yes! There will always be technological development because economic issues and ecology are driving forces. Technological advancements, however, depend on the degree to which enthusiasm for technology can be aroused in persons with a certain talent and a disposition toward engineering. To some extent this book is based on a series of lectures called the Basics of Thermoforming. Among these lectures the discussions range over many topics, even to the mere production of a yogurt cup. There are many people who are not directly involved in the development of technologies but who exert nonetheless an influence on technological developments. These decision makers, however, do depend on basic knowledge of the technological linkages and contexts. This book is intended as a reference book for the relatively small industrial sector of thermoforming applications. This book focuses on thermoformed products and applications. All of us once had the experience of asking ourselves, when contemplating a formed part, how was this part produced? This book is subdivided into the description of technical formed parts and of packaging. Some parts may not even look like thermoformed parts to the casual observer. This book will discuss the enormous possibilities of thermoforming at a level that Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 1
12 2 Chapter 1 Introduction presents an overview of the diversity of this plastics - processing method for nonprofessionals. At the same time the book includes useful detailed knowledge for the professional practitioner. This book takes the thermoformed part and traces it back to the process chain. Machine and tooling technologies and the possible automation steps are explained in full detail, as are the materials used. For the description of the materials, the effects of the extrusion process are also considered and the characteristics of the raw materials are explained. Where the process chains are similar for some of the described applications, only the distinctive features are identified. The book also describes methods for the optimization of the thermoforming process. If you look closely at your surroundings, you will find countless objects in your daily use that were produced using the thermoforming process. Bath and shower tubs are thermoformed parts and among the first thermoforming products you will see on entering your bathroom in the morning. If you decide to use a new toothbrush, you have to tear open its packaging made of thermoformed material. Opening your fridge, you will see thermoformed yogurt cups, and even your fridge itself has a thermoformed interior housing (liner). Even though thermoforming is being more and more used for automobile interiors and exteriors, the automotive industry has not yet played a big role in plastics engineering. But the pressure for more efficiency, cost cutting, and longer durability of some products has managers changing their outlook on thermoforming. Thermoforming has a vast area of applications. From bathtub to toothbrush blister, from a cookie tray to a car roof, it does not matter which product you look at; most often it is a high tech application. This book should help give an overview and insight in this advanced technology. There are different processes you can use depending on the application you need. The machine technology is getting more refined, enabling users to get with higher productivity, better quality, less material cost, and so forth. With the use of new machine drive concepts and digital machine control systems, modern machines need less energy. The mold technology has dramatically developed in the past few years. Flexible molds require less change over times. This book shows the possibilities available with the new standard technology. The literature so far has covered little regarding the handling of the semifinished products and formed parts, as well as further handling in inline processes. Automation is well on its way and will not stop for technical parts or in the packaging industry. This book will show the possibilities of automated processes. The forming, filling, and sealing processes will be reviewed in particular, as these processes are not exhaustively treated in other works of literature. Many innovations, such as thermoformed automobile body parts or fully automated packaging assembly lines, include end packaging. These innovations need to be discussed in a written work and so are addressed in this book. A discussion of thermoforming should also include the various developments from the resin producers and semifinished product producers. A large part of the book will cover such materials, so that the book will serve as a useful reference.
13 Chapter 1 Introduction 3 The discussions of multilayer laminates have applications ranging from fuel tanks to the packaging of cheese. The simulation of formed parts will be covered in another chapter in this book. The thermoforming simulation is even less discussed than, for example, simulation for injection molding. This and many other procedures of the entire field of thermoforming are described in this book. The book therefore takes a comprehensive view of thermoforming and shares the expert knowledge of experienced thermoformers. With regard to the available literature, the application of thermoforming differs significantly from that of injection molding, and it is all the more important to assemble the available knowledge on thermoforming, as it is in this book. While much information contained in this book can be researched, the thermoforming applications assembled here will help the user to better understand the end results. Of course, companies that specialize in thermoforming processes are dependent on their workers know - how. In many circumstances knowledge of the tricks of thermoforming can lead to significant competitive disadvantages. Indeed I have benefited from people who supported the ideal of this book by divulging their knowledge. Experienced thermoformers, for example, Dr. Manfred Reichert, Horst R. D ä nzer, and above all Rudi Salmang, have greatly contributed to the writing of this book. For several decades they have collected experiences in the field of thermoforming and the related processing steps. They were all willing to share their knowledge. For these persons it is certainly true that tradition does not mean the keeping of the ashes, but the passing on of the fire. The compilation of the book was also supported by a number of companies that, despite the hard times during the economic crisis in 2009 to 2010, made a point of describing interesting applications and providing information. First of all Kiefel GmbH, Freilassing, Germany, must be mentioned. Here the support was chiefly provided by Erwin Wabnig and Reinhold Plot, who in the European Thermoforming Division are deeply involved with the Society of Plastic Engineers. Both men significantly contributed to the development of this book by drawing attention to interesting research at their company and providing relevant information. Likewise Geiss AG, Se ß lach, Germany, contributed to the making of this book by providing information. Manfred Geiss, in particular, must be mentioned, who, as is well known, always presents up - to - date technologies in his speeches. Thanks must additionally be extended to the tooling manufacturer Bosch Sprang BV, Netherlands, especially to Berry Smeulders, who gave information about interesting examples arising from engineering practices. A large part of the book deals with the description of raw materials. It is very gratifying that so many companies and persons who were interviewed were so willing to share their knowledge; they significantly raised my understanding of thermoforming materials. My particular interest in writing this book is to sensitize the user to the connection between knowledge of the materials and successful thermoforming production. So far this is an area where not all phenomena have been recognized. The more knowledge we have about materials and their processing characteristics, the more economic efficiency we can impart to production.
14 4 Chapter 1 Introduction Special thanks goes to Paul de Mink of Borealis, Austria, who shared his knowledge about extrusion and thermoforming of PP. Rudi Salmang also contributed his profound knowledge on extrusion and thermoforming of PS. Furthermore, he shared his vast experience in helping to proofread the final typescript of this book. Additional thanks go to Willy Onclin, PhD, of Eastman Chemical BV, the Netherlands, and Frank Kleinert of Kl ö chner Pentaplast GmbH & Co. KG, Germany, for their counsel regarding the development of the articles dealing with PET material. I want to thank Senoplast Klepsch & Co. GmbH, Piesendorf, Austria, especially Claudia Pichler, Erich Bernsteiner, Lukas Schwaigh öfer, Thomas Höfels, and Walter Kö rmer, for their help on the chapters dealing with the processing of semifinished sheet products. For their help regarding the topic of semifinished film products in the packaging sector, I want to express my thanks to Claudia M ü ller and Peter Brass of S ü dpack Verpackungen GmbH & Co. KG, Ochsenhausen, Germany. Thanks also go to Daniel Ganz of Sukano Products Ltd., Switzerland, and Holger M üller of Omya International AG, Switzerland, for their contribution regarding filling material and additives. For his help with the chapter dealing with simulation, I would like to thank Karel Kouba, whose work has led to advancements in simulation processes. The stimulus for the development of this book also came from Hannes Jacob, Klaus Wlasak, and Marcus Schuck of Jacob Plastics GmbH. Special thanks go to Thorsten Eymael and Nina Schick of SE Kunststoffverarbeitung GmbH & Co. KG for their help as well. To Gerlind zum Hingst, Sabine Jettke, B ä rbel Beyhl, and Karin Scherer, I want to express my gratitude for their support with the organization of this book and help with the translation. Also many thanks to Hartmut Thimig and Tobias Vogt. All other persons who contributed to the development of this book are referred to in the relevant chapters. Last, but not least, I would particularly like to thank Gerhard Schubert, one of the most innovative machine designers, for his support. In this book a semifinished product that can be wound is referred to as film. Any semifinished product that, due to its material thickness, cannot be wound, is referred to as sheet. While this book is an attempt to explain the world of thermoforming, it lays no claim to completeness or universal validity and assumes no liability. Several persons and companies which deal with thermoforming are deliberately cited. The experiences of the author show that this provides support for someone who is seeking advice. Naturally, the number of applications described in the book is not all - encompassing, because this book can only provide an overview about the various possibilities. Also, in this regards, only one reference per topic is mentioned in order not to create a competing impression.
15 Chapter 2 Basics of Thermoforming and Thermoplastics Several very good books on the basics of thermoforming and thermoplastics have already been published. Some institutes and machine manufacturers are offering training courses for the acquisition of basic knowledge about thermoforming as well as of basic knowledge about thermoplastics. For this reason the present book does not describe in detail the basics of thermoforming. The plastics discussed in this book are illustrated by means of an example of use. Thermoforming normally consists of heating a thermoplastic semifinished product until the forming temperature is reached, and subsequently the desired form is obtained by means of pressure difference and mechanic stretching. Mostly, this is carried out with only one mold half. Thus it can already be discerned that, compared with other plastic processing methods, thermoforming presents economic advantages relating to the forming tool. Thermoforming is a forming method that, by means of several process steps, facilitates the production of an inherently stable plastic part. Basically the raw material is transformed by heating into a viscous - flexible phase and a relatively low load. The formed part cools in the tooling and is subsequently demolded. Due to the cooling down the orientations of the molecule chains keep their stretched positions. Re - heating results in a recovery to the original sheet state. The process steps generally take the following order: Heating of the semifi nished product. The semifinished plastic product is heated until the forming temperature is attained. This can be effected with heating elements, contact heating units, or convective heat. These heat sources can also be combined. Forming. This is mostly effected by means of a thermoforming tool. Cooling. Cooling is effected under a mold constraint until a temperature is attained for which the formed part is inherently stable. Demolding. Demolding of the inherently stable formed part. Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 5
16 6 Chapter 2 Basics of Thermoforming and Thermoplastics Over many decades different thermoforming methods have been developed based on the above - mentioned principle. Semifinished plastic products and thermoforming machines are, of course, subject to certain standards. The semifinished products can be processed either as film or as sheet, and they can be manufactured in an upstream process step in a machine placed directly in front of the thermoforming machine. Generally, films are commercialized as wound reels. If the semifinished product cannot be wound on reels due to its thickness, it is cut and handled as sheets. Most plastics that have a thickness of more than 2.5 mm are processed as sheets. PC, PMMA, PA, POM, and ABS as well as fiber-reinforced composites and self - reinforced materials are semifinished products for technical applications. For the automobile industry, often thermoplastic elastomers and thermoplastic polyolefins are used. PET, PS, PP, PVC, and PE are semifinished products for packaging applications. They are provided with corresponding additives for the modification of their characteristics. Modifying agents are necessary to obtain food compatibility and resistance, such as to improve their permeation characteristics. For the manufacturing of technical parts as well as in the packaging sector, foamed semifinished products are increasingly utilized as they reduce weight and offer insulation advantages. Many semifinished products consist of several different layers in order to provide the final product with the best possible characteristics. In the food - packaging sector the following characteristics are especially demanded: High oxygen, gas, water vapor, and aroma barrier High product neutrality Light protection and UV barrier Excellent thermoforming and sealing characteristics Good mechanic properties Good printability Peelability However, multilayered semifinished products are also available for technical products, for example, in lacquer coats for car bodies. Recycled material may even be incorporated into the intermediate layer of semifinished product. 2.1 THERMOFORMING METHODS Because thermoforming is normally effected in one mold half, only a one - sided definition is possible. The advantage is that only one mold half must be designed, dimensioned, and manufactured. The forming technologies are differentiated into the following subgroups: Positive Negative Compressed air
17 2.4 Advantages and Disadvantages of Thermoforming 7 Vacuum Plug assisted Lamination To some extent these methods can also be combined. 2.2 POSITIVE FORMING In the positive forming method the heated semifinished product is drawn over the forming mold. The definition is on the inside of the finished part. During the forming process the inside has contact with the forming mold and takes over its shape. In a first step, the thermoplastic semifinished product is brought to its forming temperature. In order to receive a uniform wall thickness distribution, the material is pre - streched by means of pre - blowing. After this, the mold closes, and vacuum is applied to bring the material to its final shape. Demolding takes place after the plastic has cooled. The positive forming method is often used in sheet machine applications. 2.3 NEGATIVE FORMING A common application of negative forming is in the production of cups. After the heated film has been positioned in the forming station, the mold closes. As the plug assist pulls down, the trapped air in the cavity is released by means of venting holes. Then the forming air is applied and the part receives its final shape. Demolding takes place after the plastic has cooled down. 2.4 ADVANTAGES AND DISADVANTAGES OF THERMOFORMING Thermoforming is mostly in concurrence with injection molding. The advantages and disadvantages listed below principally refer to a comparison with injection molding. The manufacturing of technical articles by forming has the following advantages: Heavy parts can be produced (up to 125 kg) Large parts can be manufactured (up to 4 m 2 ) Flexible wall thickness ( mm) Cost-effectiveness for small batches (tooling costs) Low costs for modifications and for color change Homogeneous multilayer applications are possible The manufacturing of packaging parts by forming has the following advantages:
18 8 Chapter 2 Basics of Thermoforming and Thermoplastics Shorter cycle times High output Processing of printed semifinished product is possible Processing of multilayered semifinished product is possible The disadvantages of thermoforming are the following: Less scope for design (undercuts) No uniform distribution of wall thickness Temperature control is difficult For a given semifinished product, the manufacturer has no influence over the formulation of the film, if dealing with purchased film 2.5 THERMOFORMING MACHINES In order to fulfill the requirements of the different thermoforming methods, different types of thermoforming machines are available Sheet-Processing Machines Sheet - processing machines are used in the following circumstances: For small- and medium-sized batches For rapid color changes For large-scale products Typical formed parts are the interiors of refrigerators and automobile interiors and body parts Roll-Fed Machines Roll-fed machines process semifinished thermoplastic products that are delivered on rolls. For the production of high quantities, it is possible to place an extruder upstream of the thermoforming line. Depending on application and machine, it is possible to produce medium to high quantities. Typical formed parts are yogurt cups, drinking cups, and cookie trays Skin and Blister Machines In the skin method a heated film is formed over the product to be packaged. Unlike the blister method, no forming tool is necessary. Some examples of the
19 2.6 Semifinished Thermoplastic Products 9 use of the skin method are the packaging of pocket lighters, padlocks, and batteries Forming, Filling, and Sealing Machines Forming, filling, and sealing machines have the following components: A forming station A filling station A sealing station A punching station These machines consist of complete packaging lines into which the thermoforming process is integrated. The formed part is immediately filled and subsequently sealed with a lid film and then punched out. Some examples of multipack use are for yogurt, cheese, cold - cuts, single - portion packs, toothbrushes, and batteries. 2.6 SEMIFINISHED THERMOPLASTIC PRODUCTS Attention must be paid to two factors that influence the shape of the formed part and the process sequence for thermoforming: Free shrinkage Mold shrinkage Free Shrinkage If thermoplastics are heated beyond glass transition temperature, there is shrinkage caused by a relaxation of the molecules orientation. The amount of shrinkage depends on the extent of relaxation of orientation forced during the heating processing. Extruded semifinished products are subject to free shrinkage after heating. This fact must be taken into consideration for, to cite only one example, thermoforming machines with downstream production steps. The free shrinkage of the film creates tolerances that can lead to quality problems. For example, an offset may occur between a formed part and the punching position Mold Shrinkage Thermoplastics are subject to a volume contraction during freezing in the cavity and so can cause the dimensions of the formed parts to be smaller than the respective tool dimensions by the shrinkage value.
20 10 Chapter 2 Basics of Thermoforming and Thermoplastics Semicrystalline plastics have higher mold shrinkage values than amorphous plastics: total shrinkage = processing shrinkage + post shrinkage where PS = % PP = % Mold shrinkage and free shrinkage are primarily influenced by the following: Shape of the formed part Evenness of the wall thickness of the formed part Temperature of the tooling Deep drawing ratio Forming temperature Filling additives in the semifinished product In this book mainly the characteristics of PET, PP, PS, and PLA are described by way of examples of their use. Materials such as A - PET/PE and ABS/PMMA and other multilayer structures as well as flexible films are also discussed. Blends and certain engineering polymers are covered to a lesser extent. Additives are utilized in order to give plastic parts certain defined characteristics. The semifinished products that are used for thermoforming are blended with additives during manufacturing, for example, during the extrusion process. The typical additives are as follows Antiblocking agent. The antiblocking agent facilitates the unwinding of film from the reel and is useful for the reliable stacking and destacking of the formed parts. An antiblocking agent can be added during extrusion of the semifinished product. However, it is also possible to apply an anti - blocking agent to the surface of the semifinished product. Antifogging agent. The antifogging agent prevents the accumulation of condensate on the inside of packaging (e.g., salad cups), which impairs the transparency. Static inhibitors. The packaging of electronic components necessitates the use of an electroconductive material in order to avoid overvoltages und damage to these electronic parts. Talcum powder and chalk. Talcum powder and chalk are reinforcing and filling materials. The principle task of these additives is to make the application as cost - effective as possible. Nucleating agent. Nucleating agents affect the crystallization behavior of semicrystalline materials. Nucleating agents are used to improve the transparency and the processability of PP.
21 2.6 Semifinished Thermoplastic Products 11 Foaming agents. Foaming agents are used for the production of foam materials. There is a distinction between physical and chemical foaming agents. (1) Foaming gas is conducted into the extruder when using the physical process. (2) The chemical process requires substances that are mixed into the polymer melt. These substances cause the foaming phenomena. Crystallization accelerator (C- PET). Crystallization accelerators are used in the production of C - PET to effect temperature resistance. Crystallization inhibitor (PET-G). Crystallization inhibitors prevent crystallization and thus the opacity of PET - G, improving sealing behavior and enabling broader processing temperature range to be obtained. Glass fiber, carbon fiber, or aramid fiber. Glass fibers, carbon fibers, or aramid fibers are used to increase the mechanic properties of thermoform parts. These reinforcements can significantly improve the stability and load limits compared with unreinforced plastics. Plasticizer. Plasticizers are used to adjust the transition temperature of plastics. In particular, they are used if a plastic is too brittle in the range of the service temperature. Aging inhibitors and light stabilizers. These are additives that delay or prevent brittleness, a type of damage caused by exposure to light and deterioration of the material over time. Colorants. Colorants facilitate the use of color in the design of the material.
22 Chapter 3 Production of Semifinished Products, Extrusion, and Coextrusion Written in cooperation with Rudi Salmang, Terneuzen, The Netherlands, and Horst R. Dänzer, Büchlberg, Germany 3.1 EXTRUSION No Thermoforming without Extrusion Experienced thermoformers have a proverb: It is possible to produce bad formed parts from good semifinished products, but it is impossible to produce good formed parts from bad semifinished products. Experience is also defined as the summation of the mistakes one has made in the past! Over time, thermoforming in packaging evolved from processing PVC to PS to PP and PET. Whereas PVC showed hugh and PS comfortable operating windows, PP and PET are known for their narrow operation windows. Knowledge about the extrusion process is essential to mastering the thermoforming process. The success of a thermoforming application depends on correct extrusion of the semifinished product. If the extrusion is not carried out according to the rules, this can have serious effects on the thermoforming. Film thickness variations can diminish the quality of a thermoformed part. For a multi - cavity tool, different wall thicknesses of products will not meet the quality standards. Longitudinal and diagonal shrinkages of semifinished products are caused by different orientations during the extrusion process, and these too are recurring issues that lead to variations in the batch quality. Variations in the batch quality are therefore due to variations in the thermoforming results. Clearly, it is advantageous for the thermoformer to be familiar with extrusion. Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 12
23 3.1 Extrusion 13 Huge thermoforming companies depend on their inhouse extrusion departments to be flexible and able to react quickly to customer demands. Inhouse extrusion facilities can help deal economically and intelligently with the regrind of the thermoforming skeleton. For a thermoforming operation in need of doing an extrusion, certain questions need to be addressed: Offline or inline extrusion? Which extruder from what supplier? Which materials are going to be processed? Extruders tend to have a long service life. This requires a long-term strategy. Which output, film widths, and thicknesses? Is an extrusion process control system and documentation required? Factory data capture enables easy postcalculation. Gravimetric dosing delivers set actual comparisons basically for free. This is very important if one considers that 60 to 70% of the costs for producing packaging are related to the material. If more extrusion lines are necessary, which line and with which output and properties is going to be the first purchased? New or used extrusion line? Experienced personnel might be able to deal with used equipment. What is the correct evaluation of offers for extruders? Who is giving training to the shift personnel? Which material type from what supplier is going to be used? Material incoming inspection? Measurement of MFI, foreign particles, moisture, weighing of incoming material. Development of recipes for film properties? Regrind handling? Business profit is dependent on how the regrind is handled. Inspection of film quality? Shrinkage, thickness, winding, and migration. Maintenance in operation? Scheduled maintenance. Each new product creates some further questions regarding the film: Color? Thickness? Width? Number of layers? Raw materials? Recipes? Extrusion process? Use of regrind from extrusion and thermoforming?
24 14 Chapter 3 Production of Semifinished Products, Extrusion, and Coextrusion Just what is extrusion? Extrusion is a process by which a plasticized material flows through a die to take up the form of the die in a continuous form. An extrusion line consists of some basic components. Important components are, for instance, the dosing unit, the extruder unit with infeeding zone barrel, screw(s), and the heating and cooling system, as well as the vent, drive, breaker plate, screen pack, and gear pump. Last but not least is the die. The dosing system can function according to either the volumetric or the gravimetric principle. Masterbatch granulates and additives are fed to the extruder according to a determined formulation via the dosing system. It is important to understand the calculation for the unit that is dosing the masterbatch into the material system. It has to be kept in mind the regrind of the skeleton of the colored film already contains masterbatch; this amount has to be considered carefully when adding new masterbatch to the process. Too much masterbatch will have a negative impact on the thermoformability of the film Description: Volumetric/Gravimetric Gravimetric dosing is preferable to volumetric dosing. With volumetric dosing there is the risk that the ratios in the funnel will vary and thus lead to variations in quality. Powder density variations have to be compensated for. Nevertheless, compared with gravimetric dosing, the costs are lower, even though more effort must be made to control the process and the output is limited. Gravimetric dosing facilitates a precise, continuous, and high - capacity material infeed. The result is constant quality and cost reduction for the subsequent processes. The cylinder barrel houses the screw and provides the bearing surface to impart shear to plastic granules. The cylinder barrel also provides the means for heating and cooling. Air cooling is smoother than water cooling and therefore mainly used. To keep the heat within the system and for operator protection, the cylinder barrel has a cover. For each material and also each melt flow index there is an optimized screw geometry. Some vented extruder for PS processing might also be used for PP, but with less output, not with less quality. The principal item of an extrusion line is the screw. For applications used for the manufacturing of semi - finished products for thermoforming a single - screw extruder is utilized. The screw acts as a positive displacement pump. It conveys, melts, and feeds melt to the die. The screw provides homogeneous mixing of the melt and ensures pressure stability to the melt via the breaker plate and filter. The output is controlled by head pressure. The screw is defined by its diameter ( D ), its length ( L ), and a length to diameter ratio: L /D. The use of a single screw extruder or a twin screw is dependent on the application. Twin - screw extrusion is often used for compounding and sometimes also for the production of foam. For better ventilation of the melt, a two - or even
25 3.1 Extrusion 15 three - stage screw is recommended: for instance, for the processing of polystyrene since it is a relatively strong material (granules). Granules from silos especially in the winter time tend to have moisture, which can be eliminated by a vacuum zone. Masterbatch and the PS for the gloss layer require pre - drying above the hopper loader, so it drags more air into the system. Polypropylene granules are softer. The air exits the system much faster. When the screw is cooled, it is usually done with water. The wall of the barrel is cooled in most cases by air. The drive (torque) of the screw is important because it is 50% of the extruder costs. For instance, to protect the screw pressure relief devices, rupture disks are recommended. A typical extruder screw is divided into sections. There is a feed section, a transition section or compression section in the case of PS production a vacuum section and a metering section. For better temperature distribution a pin mixing screw is recommended, often with a torpedo placed at the end of the screw Feed Section Solids Conveying Mechanism The granules enter the channel and are propelled forward by friction forces at the barrel s surface as the screw rotates. Heat is generated, and the granules begin to melt on the barrel s surface, forming a thin film when the melting point is reached. The bulk density is around 0.6 g/cm 3 for polystyrene. The density of the shredded packaging film skeleton is between 0.3 and 0.55 g/cm 3. The bulk density should never be below 0.2 to 0.3 g/cm 3 ; otherwise, regranulation is recommended. To prevent output loss of the extruder when running recycled material, regranulation is also recommended Transition or Compression Section Drag induces melt removal of the film into the melt pool. Contiguous solids melt until all the material is melted. The film thickness depends on the screw flight clearance and so determines melting efficiency. Viscous heat generation is the main contributor to the melting rate Metering Section The melt is conveyed by viscous drag, establishing a rotational flow within the channel. The viscous force on the barrel conveys the material forward while screw is retarding. Therefore the generated viscous heat is the result of shearing flow. The melt density is around 0.96 g/cm 3 for polystyrene. The ratio between the feeding and metering sections of polystyrene and polypropylene is between 3:1 and 4:1. When using a two stage screw the next section is the venting section and the venting stack.
26 16 Chapter 3 Production of Semifinished Products, Extrusion, and Coextrusion Venting Section Melt is decompressed in order to remove volatiles Second Transition Section Melt is compressed and forwarded to the second metering section Second Metering Section Melt is conveyed by viscous drag as in the first metering section. Viscous heat is generated as a result of the shearing flow. The melt density is around 0.96 g/cm 3 for polystyrene. To prevent vent flooding, this section is around 1.6 times deeper than the first metering section Mixing Section The mixing section should not have any dead spots. There are distributive mixers (shear strain, split flow, and reorientation) as well as dispersive mixers (elongational stress). There are also static mixers on the market Screw Materials and Tolerances Extrusion screws are made from steel and soft (or stainless) steel and treated with nickel alloys. The outer diameter of the screw has a tolerance of ±0.06 mm. The flight depth of the screw is between 6 and 19 mm for most extruder sizes. Any size smaller than 6 mm may result in excessive shearing and hence melt overheating and output loss. To reduce friction and protect it, the screw is treated with chrome, nickel, or PTFE - based materials. The screw flight lands are flame hardened to increase their wear resistance. A worn screw leads to output loss. Wear on a screw can be measured as shown in Figure 3.1 : Measure the metering zone internal diameter = ØB. Measure the metering zone screw flight diameter = ØA. Measure the metering zone screw root diameter = ØC. Determine screw flight height H (H = [ ØA ØC ]/2). Calculate the radial clearance d (d = [ ØB ØA ]/2). Calculate the radial clearance-to-flight-height ratio d /H. Screw wear is characterized by the following formulas: If d /H < 0.05, screw wear is normal. If d /H = 0.07, there is onset of wear.
27 3.1 Extrusion 17 Figure 3.1 Extrusion screw wear If d /H = 0.10, there is a 5% output loss. If d /H = 0.15, there is a 15% output loss, and need to repair screw. If d /H > 0.15, there is a 15% output loss, and need to repair the screw and cylinder The Barrel The infeed zone determines the output and the quality of the film. If infeeding is too fast, inhomogeneous melt results. This leads to tensions in the film and to problems in the thermoforming process. If infeeding is too slow, the output will be unsatisfactory. Barrel temperatures also influence output and quality. The barrel is essentially a cylinder that houses the screw and provides a means for heating and cooling. It is normally provided with a protective cover to keep the heat in the system for energy saving as well as for process stability. This way the cover also provides a measure of safety for the operators The Vent The vent is a low pressure point and is also called starved section. It allows trapped air and moisture to escape (volatiles) as well as reduces residuals. To achieve this, the vent is normally operated with a vacuum, and the operator needs to be trained to maintain a starved section. Excessive back pressure has to be avoided; otherwise, polymer melt will flow out of the venting hole. This can be controlled by a clean
28 18 Chapter 3 Production of Semifinished Products, Extrusion, and Coextrusion screen or larger mesh size or temperature. The use of a restrictor valve or gear pump is recommended if available. A gear pump guarantees uniform film thicknesses. The extrusion of polyolefins requires the use of gear pumps. Efficient venting will raise an extruder s efficiency The Drive The drive sets the screw into motion. The drive speed determines the output of the screw. Speed variation is achieved by the variable speed drive. Drives with a high torque operate at a more constant speed and provide longer service life Breaker Plate and Screen Pack These items are often optional. The breaker plate and screen pack filter out impurities in the polymer and, in addition, control and provide more uniform head pressure. Impurities can amass and lead to screen clogging and machine downtime. A screen changer keeps these problems from arising. The breaker plate and screen pack promote mixing of additives in the polymer. There are manual or hydraulic screen pack changers. Available are almost continuously and fully continuously screen pack changers, which always maintain equal pressure The Die The die is important to achieving good quality. Commonly used is a manifold geometry to equalize the pressure across the whole width whereby the die is equipped with an adjustable restrictor bar and flexible die lips for thickness control Static and Dynamic Mixers Static mixers are used to optimize the melt s homogeneity, thus improving dispersion of additives, colorants, and pigments as well as avoiding temperature gradients. The static mixer is essential for high - output extruders. Dynamic mixers are less prone to damage, but more costly and more difficult to incorporate Gear Pumps Gear pumps are used to stabilize extruder output pressure. These pumps operate on volumetric principles that keep a constant pressure at the entrance of the die and control the speed of the screw. The gear pump provides uniform pressure to the die. The gear pump pressure can be regulated to maintain extruder output. The gear pump
29 3.1 Extrusion 19 regulates the rpm of the extruder to keep the gear pump inlet pressure constant. Keeping a constant minimum pressure results in maximized output Granulation and Material Feed Issues Blenders automatically control, feed, and mix all the materials required by the process: Virgin resin Regrind Color concentrate Other additives Blenders work either volumetrically or gravimetrically, and they are linked to the conveying systems. Pre - drying is preferred. This prevents moisture pickup, particularly when using non - vented screws. In addition, pre - drying maintains a constant feed temperature. In processing hydrophilic materials, a drying system is required. Crammers or augers can be installed in the hopper to support the feeding of the material to the extruder, especially when using regrind coming naturally from the thermoforming skeleton web Bridging and Regrind Considerations The use of regrind with consistent size is recommended. The minimum thickness should around 2 mm to be consistent with the raw material granule size. It is important that virgin material and the regrind show similar melting behavior. Otherwise, the quality of output will be inconsistent and the process will be disrupted The Output (Flow) of an Extruder The output (flow) of an extruder is proportional to the following parameters: Width, w Die gap effects exponentially to the third power, G Pressure drop, dp The output is inversely proportional to the following parameters: Die land length, L Viscosity, η Ȯ wg 3 dp = 12L η
30 20 Chapter 3 Production of Semifinished Products, Extrusion, and Coextrusion When processing a recipe of, for example, 70% PS HI and 30% PS GP, the regrind should be also 70% PS HI and 30% PS GP Sheet Roll Stack and Take -Away Equipment The sheet roll stack extracts heat from the sheet and provides the required surface finish. If the sheet is thin, it can be wound up into rolls. A rigid sheet is sheared to the desired length The Polishing Roll Stack Melt flow is controlled by the restrictor bar in the die. The film thickness is set in the die gap. The purpose of the roll stack is to finish the film by providing cooling and gloss. The purpose of the roll stack is not to set film thickness or control melt flow! For example, the evenness of a sealing rim of a yogurt cup is controlled by the die gap. It is important to calibrate 110% of the film thickness in the die gap, decrease the thickness to about 95% in the first gap of the roll stack, and set 100% of film thickness in the second gap. The evenness of the sealing rim of a yogurt cup is also influenced by a nucleating agent and the speed of relaxation. Fast relaxation is preferred (see Figure 3.2 ). If the extrusion temperature is low, orientation will be high and free shrinkage low as a result of slow relaxation. If the extrusion temperature is high, orientation will be low and free shrinkage high. To control free shrinkage in the semifinished product, samples should be cut out. Typically, the specimen s dimensions should be mm. According to the width of the sheet three or more specimens should be taken from the sheet. The samples are heated in an oven (e.g., PS: 135 C/5 minutes). For packaging purposes (thin gauge), 1% of transversal shrinkage and 14% of longitudinal shrinkage is allowed, but for the thick gauge (e.g., refrigerator sheets), less than 4% in the longitudinal direction. Samples that become wider after the shrinkage test reveal the existence of rolling bank in the polishing roll stack during the extrusion. 1 There are several causes of high levels of orientation in extruded sheet to consider: Die gap too open for the desired sheet thickness. Nip gap too tight for the desired sheet thickness. Too high temperature gradient between polishing roll stack. Pull speed too high versus roll stack speed (tension on sheet). Existence of a rolling bank. 1 Rudi Salmang, Interview, Extrusion f ür Thermoformfolien, 2010.
31 3.1 Extrusion 21 Figure 3.2 Polishing roll stack A wrongly adjusted extruder die will lead to an uneven film thickness in a cross direction of the film. Residue and contamination under the restrictor bar or in the die can also lead to uneven film thickness. Material accumulation may occur during the winding of the film to create so - called hoops, especially when using the chill roll system. Material accumulation of only a few microns leads eventually to a noticeable change of shape of the film reel. This may result in difficulties in unwinding the film from the reel. The phenomenon of a telescoped film may occur whereby the film loses its track and the production line malfunctions. Some film winders allow for the possibility of having to alter the reel across the machine direction by a few centimeters. While this can diminish the material accumulation and the creation of hoops, the altered film reels call for a higher production cutoff, which has a negative impact on material costs. It is better to solve this problem by optimizing the settings of the extruder die or even by cleaning and maintenance or by replacement of the die. 2 An important consideration in the cooling of film in the polishing stack is the symmetric static and thermal support of the stable roll shell regarding the cooling channels. For the production of thin gauge thermoforming film, the use of bending resistant rolls is required or chillroll or steelband. The production of the thermoforming film must be uniform so that downcooling occurs across the film as well as in 2 Horst Dänzer, Interview, Extrusion für Thermoformfolien, 2010.
32 22 Chapter 3 Production of Semifinished Products, Extrusion, and Coextrusion the machine direction on both sides of the film. Otherwise, the film runs the risk of bowing or warpage. There are several existing types of polishing stack cooling systems. Each roll has its own system. And each roll requires its own drive. One system uses a mill in a spiral channel that is positioned directly on the inside of the roll shell surface. The roll shell surface is supported by a spiral channel. Support from the outside is also possible from the face walls of the polishing roll. Another system uses bars and a second smaller inside cylinder to create channels through which water is able to flow. Uneven cooling conditions of the film inevitably lead to poor film quality (warpage and sideways curling) and to many other problems in the thermoforming process. The contamination of cooling channels, such as with lime, will cause uneven cooling of the film. Material accumulates in the machine direction as a result. This becomes evident when quality issues arise in cavities that are inline. If the film is fed in the machine turned and the phenomenon travels to the other side, then the film is the cause for poor part quality. This root cause analysis may also be applied for problems in the die Sideways Curling Sideways curling can be the cause for great difficulties in terms of machinability, especially when form -, fill -, and seal applications are operated without a chain rail system or walking beam. Uneven heating of the film may occur, and the film may moves off track throughout the machine. The machine will then malfunction and stop. Sideways curling can occur if the temperature distribution is uneven within the polishing roll or if the rolls are beveled. Single - sided pressure is another situation that can lead to sideways curling. The quality of cooling water should be always monitored, and when indicated, the rolls should be cleaned. 3 The rolling bank can be on the top or the bottom of the film. As the rolls are forced slightly apart by pressure from the bank, the film thickness increases. Another cause of film thickness variation is pressure fluctuation in the extruder Effects of a Rolling Bank Up and/or down movement, even if no rolling bank is visible at the first calender gap, will lead to variations in film thickness along the length of the film. This is a type of cyclical variation that correlates with the shot - to - shot variation in the weight of a thermoformed part (e.g., a yogurt cup). Residual tensions on the surface will show as undesirable warping of the sealing rim in a yogurt cup, or stress concentra- 3 Horst Dänzer, Interview, Extrusion für Thermoformfolien, 2010.
33 3.1 Extrusion 23 Figure 3.3 Effects of rolling bank tion leading to cracks for refrigerator liners. Residual tension may be present even where the surface quality appears greatly improved. 4,5 (See Figures 3.3 and 3.4.) The Slitting Unit and Draw Rolls The slitting unit and draw rolls determine a product s width. Any number of implements may be used for slitting: Stationary cutoff saws Razor blades Rotary cutters Cutting shears The draw rolls have three important functions: Provide required tension in the extruded sheet Maintain flatness in sheet during its contact cooling 4 Rudi Salmang, Interview, Extrusion für Thermoformfolien, Rudi Salmang, EX/TF training for rigid packaging, Extrusion, Dow, 2005.
34 24 Chapter 3 Production of Semifinished Products, Extrusion, and Coextrusion Figure 3.4 Looking for effects of rolling bank Control speed by way of the roll stack speed (in combination with the draw rolls, to maintain orientation) The Finishing Section The Winder for Film Films with thicknesses smaller than 1.8 mm (in some cases 2.5 mm with increased core diameter) can normally be wound, depending on the web stiffness. A core diameter that is too small will cause microcracking on the surface. The core diameters often used are 3, 6, and 9 inches. The 3 - inch variety is only recommended for processing very thin films. Winding polystyrene is a far less critical process than winding polypropylene. If PP film is wound too loosely, different conditions of cooling are created. So the temperature differences will lead to crystallization differences. This different processing behavior is particularly noticeable in multiple film lanes when a mother reel is slit into two or three lanes. 6 6 Horst Dänzer, Interview, Extrusion für Thermoformfolien, 2010.
35 3.2 Coextrusion Cutoff Shear The cutoff shear is used to cut flat sheets. Sheets can be cut up to a thickness of about 13 mm. The cutting device is either stationary or traveling. Upon admitting a pack of sheets, the system travels 30 mm in 0.5 s. Enough allowance is made for the sheets to bend a little under the cutting action The Stacker for Thick Sheets A stacker is used to store sheets on a pallet. Storage of three days is recommended to allow for temperature equalization to the center of the pallet. It is important that the semifinished product have an even temperature distribution; otherwise, the parameter settings will keep changing and cause variations in the parts quality. The same situation happens in the processing of film reels: the warm core of the reel has to cool down after processing. Similar problems occur if the film reel is stored in an environment with different ambient temperatures, such as cold or frozen company yard floors on a sunny winter day. Then the different temperatures per spin of film cannot be handled by any heating system. It will lead to a bad production batch. All semifinished products must be stored under constant temperature conditions Typical Barrel Temperature Profile for Polystyrene Barrel temperatures Feed section 180 C Transition section 205 C Metering section 210 C Downstream components 230 C Run the cool feed zone (zone 1) for maximum output and melt pressure control. Note that the regrind melts earlier than granules. Full vacuum venting is used to remove volatiles, moisture, and so forth. Reduce temperature after venting to control melt viscosity and to prevent backflow to vent Effect of Regrind on Extruder Output The impact of a high temperature in zone 1 of the extruder on regrind in shown in Figure 3.5. The output will decrease with increasing temperature. Figure 3.6 shows a typical barrel temperature profile for polystyrene. 3.2 COEXTRUSION Coextrusion is used where one layer cannot satisfy performance requirements economically. Early layered products were made via lamination. This was a two - step
36 26 Chapter 3 Production of Semifinished Products, Extrusion, and Coextrusion Regrind Addition Rate versus Zone 1 Measured Temperature, (data from 120 mm extruder) kg/hr zone # 1 C Figure 3.5 Effects of regrind on extruder output kg/hr 1.3 mm kg/hr 0.8 mm kg/hr 0.5 mm granulation 7 Figure 3.6 Typical barrel temperature profile for polystyrene process. Step one is to make the film. Step two is the lamination of the film to the substrate. Coextrusion combines polymer layers, then thins and spreads them in a manifold die or in a coextrusion feedblock and die. When different resins are used they should have the following properties: Similar viscosities to flow evenly together Similar chemical compatibility for bonding and recycling Thermal compatibility for overall stability
37 3.2 Coextrusion 27 Structures involving dissimilar resins should be thoroughly tested, as this is particularly relevant for recyclability. The economical advantages of coextrusion are as follows: Usage of high performance, more expensive resin possible Scrap layers can be incorporated Barrier layers can be added for reduced oxygen permeation or reduced water permeation.
38 Chapter 4 Introduction to Technical Parts Thermoforming offers many possibilities in the production of formed parts for technical applications. Depending on the requirements, it can be used for the manufacture of prototypes or for series manufacturing. In fact, nearly all plastics that can be processed by means of thermoplastic methods can be run on thermoforming machines. Thermoforming of parts for technical applications makes specialization in many industrial sectors possible. The comparably low cost for forming tools makes this technology especially well suited for the manufacturing of prototypes of small parts. As soon as the design of the part is fixed, and a large number of items must be produced, the injection molding method is applied. In such a way thermoforming can contribute to reducing development costs. However, if large - size formed parts are required, the costs for thermoforming are in most cases comparable to those of other plastics processing methods. Large parts, for example, garden ponds or tractor roofs, can be produced in a very cost - effective way with thermoforming. Often the decision makers are not aware of the savings potential that thermoforming provides. Due to the quickly changing life cycles and innovations in the automobile industry, manufacturers nowadays experience frequent tool and format tool exchanges. So the importance of thermoforming is on a continual rise. Often thermoforming is combined with other manufacturing methods (e.g., injection molding). Back - injection molding is a good example of this connection. Recently, fiber - reinforced plastics have experienced an upward trend. Particularly noteworthy is the simultaneous forming of a pre - heated organo sheet (composite sheet) combined with the injection of a reinforcement structure using an injection molding tool. In the part of the book dealing with thermoforming applications the extensive possibilities of this technology will be illustrated on the basis of examples. Although not all applications will be discussed, those mentioned will provide a window on the wide range of possibilities offered by the thermoforming process. Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 28
39 Chapter 5 Antenna Radome Manufacturing Written in cooperation with Marieke Rijkse, Ineos Styrenics, The Netherlands 5.1 WEATHER-RESISTANT HIGH -IMPACT POLYSTYRENE The high demands made of the materials of telecommunication antennas may not at first be discernible. Signals are sent and received throughout all continents, day and night, in winter as well as in summer, and also under extreme climatic conditions. Microwave (radome) antennas were developed to get more capacity in data transport (see Figure 5.1 ). For these applications higher frequencies are required. The range decreases with higher frequencies. Radomes also provide environmental protection. The four main factors of the polymer choice for antenna manufacturing are: Mechanical impact retention UV resistance Wetting resistance (low hygroscopicity) Dielectrics Mechanical impact retention has to do with weather resistance outdoors. Failure in impact resistance means the end of the antenna s application life. For antenna applications the polystyrene grade Styrosun (from Ineos Styrenics) is superior to ABS, PC, and ASA due to the suspension polymerization process and a specific way of grafting the rubber particles. 1 1 Styrosun information, Marieke Rijkse and Stephan Gschwind, Ineos Styrenics, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 29
40 30 Chapter 5 Antenna Radome Manufacturing Figure 5.1 Microwave antenna radome cover (Courtesy of Ineos Styrenics) UV radiation is the major factor in polymer degradation: PS - HI and ABS perform worst in terms of UV resistance. ASA and Styrosun perform best. ASA maintains, on average, better color. UV radiation increases the hydrophilicity of the surface. By its natural hydrophobic properties Styrosun performs best compared with ABS, ASA, and PC. 5.2 THE EFFECT OF UV LIGHT Just 5% of UV light is present in sunlight. Because UV light has the shortest possible wavelength of light, it has the highest energy and destructiveness. Virtually all polymers undergo discoloration and deterioration of their mechanical properties as they degrade due to UV light. Some polymers crosslink due to UV light (e.g., polybutadiene, which is present in PS - HI and ABS).
41 5.5 Water and Antenna Gain 31 Other polymers undergo polymer chain breakup (e.g., styrenics, acrylics, polycarbonates). 5.3 WETTING RESISTANCE Wetness is the main inhibitor of antenna gain. Wetting resistance is therefore an important requirement for antenna gain (within a pre - selected range of weather resistance). Styrosun outperforms competing polymers like PC, ASA, and ABS. Antenna radomes thermoformed from sheets made of Styrosun will build up water films that evaporate fast. Retained humidity (droplets) on the antenna surface that have the best angle for antenna gain will dry up quickly. The water level (saturation) within the polymer will also quickly drop. 1 Combined, the factors that most raise concern about UV and wetting resistance are: Dielectrics Antenna gain 5.4 ANTENNA GAIN Antenna gain is a parameter that relates the intensity of an antenna in a given direction to the intensity that would be produced by a hypothetical ideal antenna that radiates equally in all directions (isotropically and without losses). Antenna gain thus shows how much data are successfully transferred by an antenna. Antenna gain is reduced by two forms of energy: Absorbing energy, which is a dielectric loss factor that depends on radome material Reflecting energy (transmission loss), which is a dielectric constant that depends on materials and design The antenna gain can be maximized by choosing the best polymer for the radome thermoforming application. Large radomes are thermoformed. Polystyrene shows low dielectric loss factor compared with polycarbonate (PC), styrene - acrylonitril - copolymerizate (SAN), acrylonitril - butadiene - styrene - copolymerizate (ABS), acrylnitril-styrene-acrylester (ASA), polymethylenemethacrylate (PMMA), and polyamide (PA). 5.5 WATER AND ANTENNA GAIN Water is the main enemy of antenna gain at microwave and higher frequencies. Water in any form and location lowers antenna gain. If water is retained within the polymer (saturation), it reduces the antenna gain; if water remains on the surface of the polymer, it reduces the antenna gain. The worst case is if the water collects as an
42 32 Chapter 5 Antenna Radome Manufacturing uninterrupted body (film) on the surface of the polymer, which entirely reduces the antenna gain. To avoid this situation, the polymer used has to be hydrophobic. Water molecules are dipoles and react on electric fields at microwave and higher frequencies in their natural state. Dipoles have a chaotic structure. If the field passes through water, the dipoles align with it. If the field changes (wave), the dipoles rotate. At certain frequencies this rotation cannot keep up, and the water absorbs the field energy (heats up) just as water does in a microwave oven. This reduces the antenna gain. Water is a strong dielectric material, which causes the antenna losses. The water may be droplets of rain on the surface or moisture in the material. A water film on the surface of the radome can decrease by 3 db ( = 2 power loss). Droplets and rivulets are much weaker attenuators. 2 A very low loss material compared with ABS, ASA, and PC is the polystyrene grade Styrosun. The values of water - saturated Styrosun are lower (better) than those of unsaturated PC and ABS or ASA. Styrosun also shows less discoloration over time. 1 2 M. Kurri and A. Huuskonen, Measurements of the Transmission Loss of a Radome at Different Rain Intensities, Proceedings of ERAD, 2006.
43 Chapter 6 Fuel Tank Production on Sheet Machines Written in cooperation with Manfred Geiss, Geiss AG, Sesslach, Germany By law, fuel tanks are required to have certain internal components. The twin sheet procedure is suitable for the production of a closed tank with all the parts integrated in one production step. Producing high - quality twin sheet parts such as fuel tanks calls for adequate heater control, sheet support during heating, and independent prestretching of the sheets. The machine described in this application has four independent heater fields. Each single element is infinitely adjustable. Individual override of each field is possible. The temperature of each field is controlled by a pyrometer. There is a function control to each element. The closed chamber machine types such as those from Geiss AG allow pressurization. Sheet temperature adjustment is independent of sagging effect. Any material can be chosen. Special extrusion methods are not necessary to make the semifinished product thermoformable. To obtain better material distribution, the lower sheet can be prestreched upward or downward. The same is possible for the upper sheet and independent of the lower sheet. Both sheets are loaded automatically and simultaneously, and all four sides are clamped on top of a closed chamber. Then both sheets are simultaneously heated and automatically supported. After the heating process both sheets are prestretched simultaneously. The lower mold and the upper mold move into the sheets simultaneously. Both sheets are held under one heater during loading of the insert on the lower part. The section II frame is released and removed from sheet station II. The section II mold and sheet lowers and is transported to upper section. The mold is taken over by section I and moved upward and welded against the upper mold. To reach demolding temperature, a cooling time is required. The lift flaps on the clamping frame grip under the edge of upper part. The sheet loader moves in with two new sheets. The lift flaps open and loads the formed part on top of the loader wagon (see Figures ). Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 33
44 Mold Section II Picture I: Both sheets heated Both sheets fully controlled Both sheets both side heated Heater 1: Top heater station I Heater 3: Top heater station II Clamping frame section I Sensor sheet temp Sensor sheet temp window plate section I Sheet section I Sheet section II windowplate station II auto sagging control section II auto sagging control Heater 2: Bottom heater station I Heater 4: Bottom heater station II auto sagging control twinsheet frame section II Mold Section II Center system for movable table Figure 6.1 Sheet heating 34
45 Picture II: both parts formed simultaneously both parts fully clamped both parts kept warm under heater insert applied automatically Mold Section II Clamping frame section I Heater 3: Top heater station II Sheet section I window plate section I insert set windowplate station II Sheet section II auto sagging control section I auto sagging control twinsheet frame section II Heater 2: Bottom heater station I Mold Section II Center system for movable table Figure 6.2 Forming both parts 35
46 Picture III: twinsheet frame released and moved out section II mold lowered section II mold moving over Mold Section II Clamping frame section I Heater 3: Top heater station II Sheet section I window plate section I window plate section II Heater 2: Bottom heater station I twinsheet frame section II insert set Sheet section II Mold Section II Center system for movable table Figure 6.3 Lower mold to upper mold 36
47 Picture IV: welding insert welded in pressure applied cooling time on lift flaps gripping Mold Section II Clamping frame section I insert set Sheet section I lift flap window plate section I windowplate station II Sheet section II twinsheet frame section II Mold Section II Center system for movable table Figure 6.4 Welding 37
48 Picture V: Clamping frame section I Mold Section II lifting part by means of lift flaps sheet wagon comes in lift flaps open part laid down on wagon bottom mold released and lowered section I frames released Sheet section I lift flap insert set Sheet section II window plate section I windowplate station II twinsheet frame section II Mold Section II Center system for movable table Figure 6.5 Lifting parts by means of lift flaps 38
49 Clamping frame section I Mold Section II Picture VI: sheet wagon comes in with new sheets lift flops open part laid down on wagon Sheet section I lift flap insert set Sheet section II window plate section I windowplate station II twinsheet frame section II Mold Section I Center system for movable table Figure 6.6 Loading of new sheets 39
50 Mold Section II clamping frame section I Picture VII: lift flaps open part laid down on wagon upper mold moves to top pos Sheet section I Sheet section II window plate section I window plate section II twinsheet frame section II Mold Section II Center system for movable table Figure 6.7 Discharging of part 40
51 Chapter 7 Automotive Body and Commercial Vehicle Applications Written in cooperation with Lukas Schwaighofer, Senoplast Klepsch & Co. GmbH, Piesendorf, Austria, Thorsten Eymael, and Nina Schick, SE Kunststoffverarbeitung GmbH & Co. KG, Germany 7.1 APPLICATIONS FOR CAR BODIES ABS/PMMA For car body applications, for example, for caravans or recreation vehicles, special ABS/PMMA multilayer sheets have been developed. Unlike glass fiber reinforced plastics, these semifinished products can be formed in a more economical and environmentally friendly way. Also for the recreation vehicle and caravan industry the developers must work out cost - effective manufacturing processes and methods. Certain manufacturing processes that are not up to date may, in many cases, be too costly. In particular, the material technologies used until recently have been too expensive. The elimination of complex and costly paint work, weight reduction by means of a lightweight mode of construction, and the reduction of the CO 2 emission values are already the well - defined aims of manufacturers of caravans or recreation vehicles. A cost - saving consideration is to use ABS/PMMA multilayer sheets. ABS/ PMMA multilayer sheets, which are the current trend and for which there are rising demand in the automobile industry this market, have been developed by Senoplast Klepsch & Co. GmbH, a company based in Austria. Until the 1990s in the caravan sector mainly GRP (glass fiber reinforced plastics) composites were used for the front and rear panels. The production of Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 41
52 42 Chapter 7 Automotive Body and Commercial Vehicle Applications these GRP parts involved huge costs because their production could not be fully automated. To process GRP composites, their specified MAC values (maximum allowable concentration at the workplace) had to be maintained by employing elaborate air ventilation systems with efficient filters. Then, added to that, time - consuming and cost - intensive postprocessing treatments were necessary. As these vehicles gained popularity in the 1990s, competing demands as to their design increased to attract customers with modern and unusual forms. The original angular form was replaced and the caravan became redesigned. Demand rose for a material that could produce panels with curves and smaller radii. Because GRP composites could not meet these needs, manufacturers turned to thermoplastic multilayer sheets in order to manufacture the front and rear panels; these panels were thus thermoformed. During their manufacture, the thermoformed parts were clamped to a frame, directly at the manufacturer s site, and combined with other materials by means of sealing materials and adhesives. The thermoplastic ABS/PMMA semifinished parts offered certain advantages compared with thermoset processing: Low costs of the formed parts due to the high degree of automation for the thermoforming process No painting because the sheets are already pigmented and present an excellent surface quality with outstanding UV properties Color variety, including standard and metallic colors Design freedom due to thermoforming Weight reduction Good environmental sustainability because parts can be recycled and paint applications are no longer necessary High elasticity and thus less sensitivity to outer influences, such as hail Over the years pigmented and coextruded multilayer sheets with ABS as the carrier sheet and PMMA as the coating layer became widely accepted. ABS proved to be a good carrier material due to its impact resistance (also in cold weather), breaking strain, and a corresponding stiffness. PMMA (acryl) could meet the high standards regarding the coating layer (gloss, scratch resistance, and ultraviolet resistance). The company Senoplast Klepsch & Co. GmbH (based in Piesendorf, Austria) provides co - extruded multilayer sheets with the brand name Senosan AM50 SOLAR EG for the caravan and recreation vehicle industry. Additionally, these ABS/ PMMA sheets are equipped with a so - called Easyglide reverse side that has the advantage for the thermoforming process of reducing the coefficient of friction. In the course of a caravan symposium, which was organized in 2006 by Senoplast Klepsch & Co. GmbH, a survey concerning customer satisfaction and room for improvement of ABS/PMMA composites was conducted. For this survey more than 100 participants from international caravan manufacturers and the thermoforming industry were asked: Which criteria and product characteristics have the highest priority at the moment and what expectations do you have in the future relating to
53 7.1 Applications for Car Bodies ABS/PMMA 43 these composite materials, in particular, what characteristics do such materials need to possess? For the majority of the interviewed customers, the improvement of the mechanical properties and the related decrease in scrap rate for the subsequent processing as well as an increase in the life expectancy had the highest priority. In second place came the desire to improve chemical resistance and the compatibility of the thermoplastics regarding adhesives, primers, and sealing materials. This would present the advantage of being able to choose from a broader range of commercially available adhesion and sealing systems. Thus, on the one hand, more cost - effective systems can be applied, and, on the other hand, better sealing materials can be used which were regarded up to then as being chemically aggressive and damaging to the existing composite materials. Third was a request for better surface resistance to the chemicals of detergents, since formed parts have to be extensively cleaned in the manufacturer shops. The development of a multilayer sheet process was started in order to fulfill all these requirements, with a special focus on the caravan industry. For the coating layer, a compound based on acryl is used in order to maintain the good surface properties of Senosan ABS/PMMA sheets with regard to gloss, scratch resistance, and UV resistance. Compared with the standard acryl types of material available, this acryl blend has more resistance against chemicals and is highly impact resistant. For the reverse side of the sheet, a special blend was developed. Priority was given to chemical resistance against adhesives, primers, and sealing materials. The blend is called Easyglide. This ABS/PMMA multilayer sheet was already being manufactured for trial productions in serial scales on industrial lines and it was being thoroughly analyzed in a laboratory. The chemical resistance of the surface and reverse side of the semifinished product were compared with conventional adhesion and sealing systems. The test was carried out as per DIN EN ISO For this test method the sheet is clamped to a bended template having an outer fiber strain of 0.66% in order to simulate inner strain, as can be created within a formed part through wrong processing or assembly. The test medium is applied to the clamped sample. After a residence time of 24 hours, the air is exhausted from around the sample and a tensile test is carried out. The decisive criteria for this is the breaking strain, which drops for a chemical attack. Altogether, 37 media from different manufacturers were tested. Also comparisons were made with conventional ABS/PMMA sheets available on the market. The tests showed that for semifinished parts made from conventional ABS/ PMMA, only approximately 27% of the media could be used on the reverse
54 44 Chapter 7 Automotive Body and Commercial Vehicle Applications side and on the surface. For these 27% media, no mechanical decomposition as a consequence of a chemical attack could be observed. For Senosan AB50 SOLAR PREMIUM, however, 67% of all tested media can be used on both sides without causing damage to the material. If only the reverse side is examined as to a chemical attack, the test result is even more striking: for the new material type, 36 of 37 test media were positive. Interestingly, these analyses suggested that the adhesion and sealing systems should be tested not only with regard to their adhesion characteristics but also regarding the chemical influence on the mechanical properties of the component part. Modifications to the system of semifinished part and adhesive should always be based on compatibility tests. When the caravan panels are cleaned subsequent to processing and assembly stress cracks often appear. This can be due to the use of detergents that are not suitable for plastic materials, but more often the cracks are due to a high inner stress created in the component part in combination with aggressive media. To resolve this problem, a special acryl blend was developed that has significantly lessened the appearance of stress cracks. The coating layer s resistance to stress cracks was further verified by subjecting it to norm EN For this test the sheet is clamped to a bended template and a test medium is applied. The test medium chosen was isopropanol, a well - established medium in the caravan industry used for cleaning the final assembly. The time until the first cracks appeared was measured. This test was carried out with a defined outer fiber strain of 0.082% to simulate the internal stress that would be created subsequent to an improper further processing of the formed part. In this test the surface of Senosan SOLAR PREMIUM was compared with other commercially available PMMA surfaces, and significant improvement was noticeable. While for standard PMMA the first cracks appear after a residence time of 0.5 minutes, the special acryl blend can be treated for over 3 minutes without eliciting surface damage. In practice, the cleaning time is under 3 minutes, but when standard PMMA is intensely cleaned, the cracks may appear after 0.5 minutes. Mechanical tests were another focal point of the evaluation phase. Through product modification the number of rejects during subsequent processing could be diminished. When large component parts are handled, damage can occur at both the thermoformer s and the manufacturer s side and finally at the very end, which constitutes the customer s side. The tests carried out were tensile tests according to EN ISO 527-2, impact strength tests according to Charpy EN ISO 179, and impact penetration tests according to Once again, Senosan SOLAR PREMIUM was compared with a conventional ABS/PMMA composite. The result was that the mechanical properties of Senosan considerably improved, in comparision to conventional ABS/PMMA sheets. Senoplast Klepsch & Co. GmbH succeeded in launching an innovative product with Senosan AM50 SOLAR PREMIUM, namely a semifinished product for the caravan sector especially adapted to the requirements of the thermoformer, the manufacturer, and the end customer. All product modifications could be imple-
55 7.2 Car Bodies for Utility Vehicles 45 mented in a cost - effective way so that altogether, a product with a good cost performance ratio was created. The risk to the manufacturer confronted with cost - intensive customer complaints could be significantly reduced as a result. 7.2 CAR BODIES FOR UTILITY VEHICLES The utility vehicle industry is continually under pressure to produce exterior and interior component parts that meet the latest design standards. Sheared panel sheets are no longer considered up to date. At the same time these component parts need to offer an increased functionality. The utility vehicle industry prefers prefabricated modules that can easily be integrated. Often systems with clip - in mechanisms are used. Because the market demands a large number of models with the overall quantity remaining the same, methods that lower tooling costs are in great demand. Additionally, ever - increasing environmental specifications have made painting an expensive proposition. For all the above - mentioned sectors, ABS and ABS/PMMA sheets such as Senosan semifinished products offer performance and price advantages. Additionally, ABS/PMMA sheets can be strengthened with different materials and technologies to facilitate the production of structural components. Suitable thermoforming machines, forming tools, and materials must be used by utility vehicle parts manufacturers to maintain their competitive advantages regarding design and component parts. Today well - known European and globally active manufacturers of trucks, tractors, construction vehicles, buses, and special - purpose vehicles count on the competitive advantages of thermoforming for the production of outer panels and interior cover parts. Manufacturers of utility vehicles make the following demands on parts made of co-extruded ABS/PMMA sheets: Very good, nearly perfect surface quality even up to class - A surface quality Elimination of the painting process Color matching with the painted component parts Excellent UV property Corresponding impact resistance and breaking strain Simple adhesion with regard to availability of flexible adhesion techniques Reinforcement techniques, particularly for structural components The semifinished products for the thermoforming process must be subject to a color shade management so that the thermoformed parts can meet the demands for high quality of the utility vehicle industry. So it is important that the producer of semi - finished products have a good color laboratory and be able to create colors according to customer demand. In this laboratory colors are developed in cooperation with all concerned parties. Some producers of semifinished products have a color spectrum of up to 5000 colors, as is the case with Senoplast Klepsch & Co. GmbH.
56 46 Chapter 7 Automotive Body and Commercial Vehicle Applications Figure 7.1 Tractor with thermoformed top (Courtesy of New Holland) Figure 7.2 Head lamp cover for van (Courtesy of SE Kunststoffverarbeitung GmbH & Co. KG)
57 7.3 Cover for Head Lamp 47 Most manufacturers do not want to paint thermoformed parts for cost - related reasons, so the semifinished sheets are often pigmented and manufactured in desired matching colors based on customer demands. Competent handling of color shade is what ensures color success. Compliance with customer - specific color shade tolerances between color type and the recurring production of sheets is necessary. Additionally, the pigmented sheets must withstand exposure to changing environmental conditions and keep their color for years, avoiding the stress caused by constant exposure to ultraviolet rays COVER FOR HEAD LAMP Another example for an application in the sector of commercial vehicles is the cover of head lamps of a delivery truck. Covers for head lamps are developed in limited editions. These are thermoformed parts that are formed from PC and subsequently lacquered on the rear side. A high depth of sharpness must be attained with the transparent material despite the different radii of the tool contour/outline at the front side of the part. Thus a high degree of design freedom is achieved and the thermoformed part captivates with its optical refinement. 1 Product brochure senosan utility vehicles, Senoplast Klepsch Co. GmbH, Piesendorf, Austria 2007.
58 Chapter 8 Production of Refrigerator Liners Written in cooperation with Rudi Salmang, Terneuzen, The Netherlands, and Kurt Brunner, Kiefel GmbH, Freilassing, Germany Thermoforming offers significant advantages for the manufacture of large formed parts. Just based on the costs of forming tools, thermoforming is superior to injection molding. While most large - size formed parts are vacuum formed, there is also the possibility to use compressed air or a combination of vacuum and compressed air. In this chapter the manufacturing of plastic refrigerator inner liners is discussed. The refrigerator body consists of an inner liner (Figure 8.1 ), polyurethane foam, and a metal outer case. Approximately 15 years ago inner liners consisting of steel sheets were still being used; worldwide these products are nowadays almost exclusively manufactured in plastic. For the manufacturing of refrigerator inner liners mainly PS - HI and ABS are used. 8.1 HIGH-IMPACT POLYSTYRENE ( PS-HI) 1 Polystyrene and styrene copolymers are noted for their high tensile strength and optical clarity, but these polymers are brittle under many normal use conditions. Some general - purpose polystyrene grades (PS - GP) cannot be unwound from the reel after being extruded to film. The material is also so brittle that it cracks after being 1 Mark E. Soderquist and Robert P. Dion, The Dow Chemical Company, Styrene Polymers. Reprinted from Encyclopedia of Polymer Science and Engineering, Volume 16, second edition, pages 88 97, John Wiley & Sons, Inc., Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 48
59 8.2 Synthesis 49 Figure 8.1 Refrigerator liner (Courtesy of Senoplast Klepsch & Co. GmbH) penetrated with the chain pins of the thermoformer s transport system. A high - speed blow at temperatures below glass - transition temperature causes catastrophic failure without significant deformation, crazing, or yielding of the polymer. Toughness for unmodified polystyrene is generally not measured in terms of Izod or Gardner impact values. Specimens exhibit significant stress whitening during these tests because of craze formation and cavitation. Rubber modification opens up many markets unavailable to unmodified polystyrene. 8.2 SYNTHESIS Commercial high - impact polystyrene (PS - HI) products are made by polymerization of an unsaturated rubber dissolved in styrene in a solution or mass - suspension process. The rubber, generally polybutadiene, is dispersed throughout the polystyrene matrix in the form of discrete particles. In commercial PS - HI, particle size and particle size distribution are largely controlled by the applied shear rate during and after phase conversion (i.e., when polystyrene becomes the continuous phase and polybutadiene rubber is dispersed as droplets), by the relative viscosities of the
60 50 Chapter 8 Production of Refrigerator Liners continuous phase and the rubber phase, and by the interfacial tension between the phases. If shear agitation is stopped or insufficient, phase inversion does not occur, and the product becomes a quasi - interpenetrating network of cross - linked rubber with polystyrene. Rubber - in - styrene polymerization usually results in a superior product when compared with blended products; that is, a higher modulus and equivalent impact strength are achieved with less rubber. The property improvement is due to a chemical interaction (grafting) between the growing polystyrene chains and the rubber, chemical cross - linking of the rubber, and occlusion of the continuous - phase polymer inside the rubber particles, which increases the effective volume of the rubber phase. Rubber reinforcement produces other physical property improvements such as increased elongation, ductility, and environmental stress - crack resistance (ESCR). These improvements in the composite polymer are accompanied by loss of clarity and large decrease in tensile strength and modulus from the unmodified polymer. The impact strength of PS - HI generally increases with the rubber - phase volume. The rubber content of commercial resins is limited to about 14 wt% for a PS - HI solution polymerization process due to the high viscosities of the feed solutions. This apparent limitation of the rubber - phase volume is overcome by filling the rubber particles with polystyrene occlusions, which can increase the volume fraction of the reinforcing rubber phase by 10 to 40%. At a constant rubber level, increasing rubber particle size and polystyrene occlusion content can also produce tougher materials. However, if the particles have diameters much larger than 5 to 10 μm, toughness decreases, and the finished part has a low gloss surface. Particle size distribution also affects impact strength. Toughness can be improved with use of a dual rubber particle size population where the majority of particles have diameters below 1 μ m. Such PS - HI resins show good retention of their initial high gloss property. 8.3 MORPHOLOGY Many electron microscopy techniques have been developed for evaluating the morphology of PS - HI resins. The structural differences among the PS - HI resins are primarily a result of differences in production processes, types of rubber, and rubber concentrations. Most commercial PS - HI resins have particle sizes ranging from about 1 to 10 μ m. Figure 8.2 shows the typical rubber morphologies for solution - polymerized PS - HI and mechanical blend of butadiene - styrene block rubber in polystyrene. The solution process generally produces spherical, cellular particles; blending tends to yield irregular particle shapes. The mass - suspension process produces a rubber morphology similar to that of the solution process. Other rubber morphologies can be obtained when styrene - butadiene block copolymers are used in place of polybutadiene rubber. Cylindrical core - shell, lamellar, and cellular structures have been produced. These morphologies are the result of polymer polymer interactions between the rubbers and the polystyrene matrix, the intramolecular phase separation
61 8.4 Mechanism of Rubber Reinforcement 51 Figure 8.2 Typical rubber morphologies for solution - polymerized PS - HI and mechanical blend of butadiene - styrene block rubber in polystyrene (Mark E. Soderquist and Robert P. Dion, The Dow Chemical Company, Styrene Polymers. Reprinted from Encyclopedia of Polymer Science and Engineering, Volume 16, second edition, page 91, John Wiley & Sons, Inc., 1989) within the polybutadiene and the polystyrene sequence of the rubber, and the shear applied during the polymerization process. 8.4 MECHANISM OF RUBBER REINFORCEMENT The role of rubber in reinforcing glassy polystyrene and the mechanism of rubber particle formation have been described in detail. For PS - HI the multiple craze theory seems to best explain the elongation, impact, and tensile properties of the resin, including stress whitening and the decrease in density that occurs without lateral contraction. This theory is based on the premise that rubber particles both initiate and control craze growth. Under tensile stress, crazes are initiated near the equators of the particles (which act as stress concentrators) and propagate outward. The typical craze consists of highly orientated polystyrene fibrils and a network of voids. Craze formation involves a large local increase in volume of the stressed polymer. The craze propagates at a 90 angle to the tensile axis in an unoriented, isotropic
62 52 Chapter 8 Production of Refrigerator Liners polymer. Craze growth is terminated when the stress concentration at the tip of the craze falls below the critical level for propagation. In the presence of rubber particles a large number of small crazes are formed prior to failure (crack formation). This contrasts with glassy polymers, where only a small number of crazes form prior to failure. Energy is absorbed upon formation of the craze. As long as the stress concentration does not become catastrophic, leading to the formation of a crack, the material retains its structural integrity. In addition, at temperatures approaching the glass - transition temperature, the crazed material can recover (crazes disappear) after the stress is removed. Factors that increase craze formation include good rubber matrix adhesion, the correct particle diameter (1 6 μ m), high rubber concentration, low glass - transition temperature rubber, spherical rubber particles, high testing temperatures, and high coefficient of thermal expansion (of the rubber). The molecular weight of the matrix has a negligible effect on the formation of crazes, but a high molecular weight stabilizes these crazes once they are formed. Rubber - toughened styrenics other than PS - HI exhibit similar, but not identical, behavior. Most rubber - reinforced styrene - acrylonitrile copolymer (ABS) resins, for example, deform by a more complicated mechanism. Both stress whitening (crazing) and necking (shear yielding) are observed. The growth of crazes is controlled by both rubber particles and the developing shear band, with the rubber particles playing the primary role. Because of shear yielding, the high stress and strain levels are localized within the neck region, and the specimen usually displays a lower apparent ultimate elongation than PS - HI. These mechanisms explain the failure of fabricated subjects to instantaneous large deformations. Molded parts also fail because of repeated cyclic loads. This type of failure has been described as fatigue. Much recent research has focused on developing an understanding of fatigue failure of polymers. 8.5 PROPERTIES OF PS-HI 1 Standard PS - HI materials are used in both injection molding and extrusion processes. Generally, resins with low melt viscosity (melt flow rate, MFR, greater than 3) are used for injection - molding applications; resins with high melt viscosities (MFRs less than 3) are more suitable for extrusion applications. Typical end uses are toys, appliance parts, packaging, and furniture. These applications require property improvements over polystyrene, such as increased impact strength and ductility. A balance of flow and heat resistance is needed, but optical clarity is not required. Specialty grades of PS - HI offer improvements in toughness, processibility, surface aesthetics, heat resistance, environmental stress - cracking resistance, and ignition resistance. In addition to varying the basic parameters of the polymers, such as molecular weight, rubber content, rubber particle size, cross - link density of the rubber, and rubber chemical composition, the property balance of PS - HI resins can be altered by additives such as plasticizers, mold release agents, and stabilizers. Since the variables that affect properties are not independent, the optimization of
63 8.6 Rubber-Modified SAN Copolymers (ABS) 53 one property can be detrimental to other properties. The addition of plasticizers can increase impact strength and processibility. The heat - distortion temperature of the resin can be raised by decreased volatiles, decreased plasticizer levels, increased matrix molecular weight, or decreased rubber concentration. Environmental stress - cracking resistance can be improved by increased rubber particle size, increased rubber cross - link density, increased molecular weight of the matrix, or reduced plasticizer concentration. Gloss is usually improved by the use of small rubber particles ( <1 μ m). Higher tensile properties are achieved by reduced rubber concentration, decreased rubber particle size, increased rubber cross - link density, and increased matrix molecular weight. Elongation is increased by increased rubber particle size, increased percentage of rubber, decreased rubber cross - link density, or addition of plasticizer. When PS - HI is exposed to direct sunlight, it tends to discolor, become brittle, and crack. Damage is primarily due to the photooxidation of the rubber phase. This usually excludes unprotected PS - HI from long - term outdoor applications. Ultraviolet stabilization of PS - HI can be accomplished in a number of ways, including the use of monomeric ultraviolet absorbers, carbon black, zinc oxide, and weather - resistant surface coatings, alone or in combination. Other unsaturated rubbers with more ultraviolet resistance can be substituted for polybutadiene. The ignition resistance of PS - HI can be increased by copolymerizing or blending with chemicals that prevent efficient combustion of polymer substrate. These additives interfere with the free - radical burning process and/or remove the fuel from the source of the flame. Generally, the additives are compounded into the base resin at 10 to 20%. The additives drastically reduce the strength and elongation of the resin. The ignition - resistant additives most frequently used in PS - HI are decabromodiphenyl oxide at 11 to 13% combined with 3 to 4% antimony oxide. The opacity of PS - HI precludes its use in applications requiring transparency. Transparent PS - HI can be prepared by eliminating light scattering within the resin. Two solutions to this problem involve matching the refractive indexes of the rubber and the glassy matrix or reducing the rubber particle size to less than approximately 0.1 μ m, which is smaller than the wavelength of visible light. 8.6 RUBBER-MODIFIED SAN COPOLYMERS ( ABS) 2 General - purpose SAN copolymers have improved properties when compared with polystyrene, but still fail in brittle fashion when subjected to a sudden, high - speed impact. Rubber reinforcement of SAN increases its ability to withstand a high - speed impact. These materials are called acrylonitrile butadiene styrene (ABS). ABS has the processibility of styrene - based resins and excellent toughness. There is increased toughness due to the addition of rubber as a 10 - fold improvement in Izod impact 2 Thomas D. Traugott, The Dow Chemical Company, Styrene Polymers. Reprinted from Encyclopedia of Polymer Science and Engineering, Volume 16, second edition, page 72, John Wiley & Sons, Inc., 1989.
64 54 Chapter 8 Production of Refrigerator Liners strength. The importance of impact resistance is reflected in the comparison of sales of SAN (45 million kg) versus ABS (463 million kg) in GENERAL GRADES OF ABS The most common method of producing ABS starts by emulsion grafting of polybutadiene latex. The desired rubber particle size is attained before grafting by direct growth or by agglomeration of smaller particles. The particles are then grafted. The resulting ABS resin is generally 30 to 60% rubber and may be mixed with SAN latex before coagulation and drying, or with SAN pellets after coagulation and drying, to produce the desired 15 to 25% rubber level. ABS is also produced by solution polymerization. In solution polymerization a polybutadiene or styrene - butadiene copolymer rubber is dissolved in the monomer. Rubber particles are formed during polymerization with agitation. The rubber particle size can be controlled by agition speed and type. Resins produced by solution polymerization tend to have better color and toughness (at equal rubber concentrations) than the emulsion products, but lower gloss Weather-Resistant Impact Grades Unpainted ABS resins tend to yellow and lose impact strength when exposed to sunlight. This is primarily caused by photooxidation of unsaturated polybutadiene rubber particles and has prompted development of resins with saturated elastomers to replace polybutadiene partially or totally. Further protection from oxidation is usually obtained by adding a UV stabilizer and perhaps an antioxidant. When acrylic ester - based elastomers are used to impact - modify SAN matrices, the resins are known generically as acrylonitrile - styrene - acrylate resins (ASA). When ethylene propylene elastomers are used, the products are known as AES resins Extrusion and Coextrusion of Polystyrene 3 Fifty-five percent of all styrene polymers and copolymers are processed by extrusion and mainly by single - screw extruders. Because the resins are easy to plasticate and have good melt strength, they are readily fabricated into sheet, film, rod, pipe profiles, tubing, and monofilament. More complicated shapes and geometries can be made by postextrusion treatments such as thermoforming or embossing. The process is very economical because single - screw extrusion is a relatively low - cost technique and trim and scrap can be efficiently ground and re - extruded, with little change in 3 Richard E. Skochdopole, Theodore C. Wallace, and Gery C. Welsh, The Dow Chemical Company, Styrene Polymers. Reprinted from Encyclopedia of Polymer Science and Engineering, Volume 16, second edition, pages , John Wiley & Sons, Inc., 1989.
65 8.8 The Thermoforming Production Process 55 appearance or properties. (See also Chapter 3 on the production of semifinished products extrusion and coextrusion.) Coextruding of styrenic polymers is a rapidly advancing science. Worldwide there are many lines of barrier sheet coextrusion for commercial production of food packaging. Although commercial coextruded products may have as many as nine layers, the largest volume of extruded styrenic polymers is used in simple two - and three - layer structures. The application for these relatively simple composites include dairy containers, two - color drink cups and dinnerware, and sheets for outdoor use. An example of a more complex coextrusion structure for barrier packaging consists of polystyrene/evoh/polyethylene and appropriate adhesive layers. Each layer carries out a specific function in the composite (see also Chapter 30 on multilayer films for thermoforming applications). Screw plasticating is also used for injection molding, and is frequently accomplished by a reciprocating screw. Moreover, extrusion is used to develop the parison for blow molding. Projected bosses, recesses, and undercuts, which are easily made by injection molding and blow molding (finished parts), are not possible with extrusion (semifinished products). In recent years there has been much progress in extrusion technology. Compared with same screw (diameter dimension) technology, the output has doubled. With the advent of low - cost computers, sophisticated gauging systems, and automatic die adjustment, closed loop control of the sheet gauge has become commonplace. Extrusion processors are using computer - integrated manufacturing to improve productivity and quality. Considerable work has been done to develop mathematical models of the extrusions process, with particular emphasis on screw design. Polymer extrusion is usually divided into the functions of conveying, melting, and metering. The melting or plasticating function is the most difficult to model accurately because of the extremely low thermal conductivity of polymers and poor understanding of frictional coefficients in the softening range. With this exception, the other functions have been treated with relative success. A large fraction of extruded styrenic polymers are made into films or sheets, which range in thickness from 25.4 μ m to 7.6 mm. The standard cooling method is by cooling or polishing rolls. Cooling is achieved by direct contact with the polishing rolls on one side and air cooling on the other. Calculating a complete heat balance to size the rolls is difficult and is not usually done. A more standard procedure for obtaining correctly sized rolls is to extrapolate from the experience of the equipment supplier in an application as similar as possible to the desired one (see also Chapter 3 on the production of semifinished products, extrusion, and coextrusion). 8.8 THE THERMOFORMING PRODUCTION PROCESS Positive forming is the most widespread procedure for the manufacture of refrigerator inner liners. Besides obtaining the dimensional accuracy necessary for perfect positioning of shelves and plug - in parts, a perfect surface quality is obtained by this
66 56 Chapter 8 Production of Refrigerator Liners Figure 8.3 Thermoforming machine (Courtesy of Kiefel GmbH) method. For an automatic further treatment of the thermoformed receptacles, a high repeat accuracy of the material distribution at the body as well as at the plane - parallel flange is necessary. Automatic sheet thermoforming lines (e.g., Kiefel KIV or KID) are used for the production of refrigerator interior liners (see Figure 8.3 ). The sheet forming machines consist of a sheet insertion station, a transport system for sheets, a heating station with upper and lower heating elements, and a forming station with motor - driven table drives. A pre - blowing box, that is, a pressure chamber, facilitates the pre - stretching of the sheet and thus a good wall thickness distribution. The trimming of the formed parts is carried out with help of a cutting station containing a guillotine and a cross-cutting station. To produce high - grade refrigerator inner liners, a quick and precise forming procedure is necessary. To guarantee this, servo - motor drives and proportional valves are integrated into the machine. The heating elements must provide homogeneous heating of the semifinished sheets. Infrared pyrometers facilitate the adjustment of a constant processing temperature. Quick and repeatable pre - stretching is also necessary. The pre - stretching height is controlled via a laser control. Motor - driven linear movements facilitate a dimensionally accurate trim. The forming tool can have one, two, or even three cavities. A centering frame for the trimming of the parts is necessary. The undercuts are made by movable pushers that are controlled by the machine. The temperature control of the tooling is effected with the help of a base plate (contact transmission to the forming tool), pipes, and deep boring holes (direct cooling). The rigidity of the forming tool and the load capacity of the pusher is defined according to the thermoforming type (vacuum/compressed air). For a standard refrigerator inner liner only semifinished products with a material thickness of approximately 3.5 mm are used. When ABS
67 8.9 Environmental Stress Cracking 57 is utilized, it is possible to reduce this thickness. The cycle times range from 35 to 40 seconds. Complex products make material thicknesses of up to 4.5 mm necessary. The cycle times are approximately 40 to 50 seconds. The thermoformed liner is only a part of a complete assembly group. Pipings, mountings, and the cooling device are also integral parts. The clearance between the inner liner and the outer body is normally filled with polyurethane foam. If a fault occurs in the thermoformed part, the whole assembly group must be taken into consideration. Causes of cracks in the thermoformed part may not immediately be found from the thermoformed part. The application should always be considered in the context of a root cause analysis. For example, cracks may appear at the rear sides of the formed parts of a manufactured refrigerator. If the cracks developed within the first four days after commissioning, a characterization of the defects of the various types of refrigerators would be necessary. Within the root cause analysis it could be demonstrated that these defects may have several causes and also that the time that passed until the cracks appeared was dependent on: The level of tension within the material (depending on design and working environment of the refrigerator) Material properties (size of the rubber particles, quantity, plastifiers) Thermoforming conditions (temperature, stretching speed) It is known that in a chemically aggressive environment the time necessary for the development of cracks is inverse to the level of tension. The material is plastified and thus the critical tension is reduced (critical tension = status when the first cracks appear). The higher the pre - tension, the higher is the critical tension. Plastifiers reduce this difference and weaken the fibers. 8.9 ENVIRONMENTAL STRESS CRACKING 4 The premature fracture of polymers at stresses considerably below the nominal yield stress, while in contact with aggressive environments, is a well - documented observation and an engineering problem encountered in practice. Enhanced craze growth and breakdown under load is the cause, and this is under the influence of an agent that is often only moderately interactive with the polymer. Crazes are cracklike fissures with microfibrils that bridge the top and bottom surface of the interface between the fibrillar matter and the bulk polymer. The degree to which the aggressive agent promotes the formation, drawing, and breakdown of craze fibrils largely determines the extent to which the critical stress for environmental crazing is decreased below the nominal yield stress of the polymer. This fracture process is called environmental stress cracking. 4 Robert A. Bubeck, The Dow Chemical Company, Styrene Polymers. Reprinted from Encyclopedia of Polymer Science and Engineering, Volume 16, second edition, pages , John Wiley & Sons, Inc., 1989.
68 58 Chapter 8 Production of Refrigerator Liners There are two types of environmental stress cracking, characterized by either a liquid or a gas as an aggressive agent. Liquid - induced environmental stress cracking is given much greater emphasis in the literature Liquid Agents An aggressive liquid agent acts upon the polymer at a flaw located at or near the polymer surface and causes localized plasticization and suppression of the glass - transition temperature T g under an applied stress. The critical stress σ c at which this process can lead to the onset of craze and crack formation is considerably less than the yield stress and is a function, to a first approximation, of the difference between the solubility parameter of the polymer δ p and of the solvent δ s. Decreasing the internal surface tension can also decrease critical stress. The surface tension of polystyrene against air is 33 to 36 mn/m ( = dyn/cm). The effects of surface tension, as well as molecular size and shape of the solvent and δ s, must be considered in the assessment of the crazing and cracking tendency of a given liquid. Once the deformation zone at the forming environmental craze tip is plasticized, the craze begins to advance, forming new fibrils by the Taylor meniscus instability process. At this point, craze - growth kinetics are governed liquid transport through the craze - fibril structure, where capillary pressure is the driving force Rubber Modification A principal means of improving the environmental stress - cracking resistance of a styrenic polymer is by rubber modification to make high - impact polystyrene (PS - HI). The polymer parameters used to optimize environmental stress - cracking resistance are molecular weight, rubber particle size and morphology, rubber level, and mineral oil (plasticizer) level. Environmental stress - cracking resistance is enhanced in PS - HI, varying the polymer parameters that govern incubation time for crazing and craze microstructure and stability. The incubation time for crazing is influenced by the compressive pre - stress in the polystyrene matrix imposed by the rubber particles. Rubber particles in PS - HI are usually gel particles composed of the rubber and occluded polystyrene polymer. The thermal pre - stress results from the larger thermal expansion coefficient of the occlusion - filled rubber particles compared with the relatively unmodified matrix. The net compressive thermal stress on the matrix is increased by increasing the volume fraction of the rubber in the polymer and, for a given fraction of rubber, decreasing the gel fraction, which is volume fraction of the rubber plus occlusions. Minimizing the amount of occluded polystyrene in the gel particle maximizes the difference between the thermal expansion coefficients of the matrix and the gel particles as a composite microstructural entity. Increasing the fraction of rubber and decreasing the gel fraction can raise the critical stress for environmental stress cracking by several MPa, depending on the aggressive environment.
69 8.9 Environmental Stress Cracking 59 The craze microstructure and stability are controlled primarily by molecular weight, rubber particle size, and mineral oil content. In practice, it is assumed that the rubber or gel particles have sufficient cross - linking in the rubber to endow the particle with the required mechanical tenacity and sufficient chemical graft to couple the particles to the matrix effectively. Increasing the molecular weight and increasing the gel particle size can improve environmental stress - cracking resistance. A larger particle size nucleates more crazes within its correspondingly larger deformation zone, so there are more crazes to accommodate a given strain. A large particle is also a better craze stabilizer under load for low strain rate conditions (e.g., environmental stress cracking), so a large particle helps postpone craze breakdown. It should be noted, however, that proposals of rubber particles being craze stoppers during craze - crack propagation have been shown to be incorrect. Increasing mineral oil content in PS - HI decreases environmental stress - cracking resistance because the mineral oil adds to the plasticization of the craze fibrils, thereby weakening them. There is evidence suggesting that the fibril volume fraction of the crazes is decreased, thus facilitating hydrodynamic flow of the aggressive liquid through the crazes. The relative effectiveness of the polymer variables in increasing environmental stress - cracking resistance depends on the aggressive environment. The environmental stress cracking for PS - HI has been studied for hexadecane, various alcohols, and for cottonseed - oleic acid. Similar measurements have also been made for ABS copolymers (rubber modified SAN). Silicone oil as an environmental stress - cracking agent for polystyrene has also been reported Gaseous Agents Near their boiling points, nitrogen, oxygen, helium, argon, and carbon dioxide have been found to be strong crazing agents for a fairly wide range of amorphous and semicrystalline polymers. Trichlorofluoromethane (boiling point 26 C), a urethane foam blowing agent, is a very aggressive cracking agent in commercial applications of styrenic polymers. Helium, nitrogen, and hydrogen have been shown to be very mild craze growth enhancers in polystyrene at 25 C. It has been proposed that diffusion of the gas at the craze tip controls the craze - growth velocity, whereas the craze fibril structure poses very little resistance to gas flow. Environmental crazing has been studied for polystyrene in CO 2 at 34 and 45 C over a pressure range from 6 to 105 MPa. The critical stress intensity factor is proportional to critical stress when composition and specimen dimensions are constant. The critical stress intensity factor for crazing decreases by over 2.5 orders of a magnitude at a CO 2 pressure of 15 MPa, then increases with increasing pressure beyond about 20 MPa. The minimum in critical stress intensity factor is a result of the compensating effects of the plasticization of the CO 2 and the hydrostatic pressure from the gas. The fact that T g of polystyrene can be lowered to about 35 C at 10 MPa of pressure shows the strong plasticization effect of CO 2 on polystyrene.
70 60 Chapter 8 Production of Refrigerator Liners Oxidation-Induced Embrittlement The ultraviolet degradation of polystyrene and rubber - modified styrenics involves the photooxidation of the rubber phase and chain scission of the polystyrene. This general condition leads to weaker crazes that are poorly stabilized, resulting in enhanced stress - cracking and embrittlement. Thermoforming conditions (forming temperatures) change the status of the preliminary tension and the surface. The temperature is inversely proportional to the shrinkage modules and directly proportional to the surface tension. Generally, the highest tensions can be found at places where the thinner material experiences more directional changes, and at areas of bonding or with adhesives REFRIGERATOR OUTSIDE COVERS The outside covers of refrigerators are also examples of thermoformed products (Figure 8.4 ). Figure 8.4 Thermoformed refrigerator cover (Courtesy of Senoplast Klepsch & Co. GmbH)
71 Chapter 9 Paint Replacement in Automotive Applications Written in cooperation with Thomas Höfels and Walter Körmer, Senoplast Klepsch & Co. GmbH, Austria, and Thorsten Eymael and Nina Schick, SE Kunststoffverarbeitung GmbH & Co. KG, Germany 9.1 PAINT REPLACEMENT Paint is always a cost driver in car manufacturing. In a modern car plant, paint lines consume approximately 50% of the available surface and approximately 50% of the investment. In addition there are environmental regulations that make the construction of paint lines more and more difficult in western Europe. With film technology, colored plastic films are reinforced with other plastic materials. The result is an entire car component made of plastic. Thus the car component requires no painting, weight is reduced, and before or during reinforcement various elements like antennas, connection screws, and hinges can be integrated. For all these reasons the automotive industry is increasingly using thermoformed high - quality polymer films and sheets. One of the first applications using colored sheets that were thermoformed was exterior body parts of driving - license - free vehicles. The manufacturers of these vehicles have high standards regarding metallic color effects and color consistency. These standards are very similar to those of the automotive industry. Also when it comes to surface quality, the standards are as high. Although driving - license - free vehicles cannot be compared to regular cars, the learning experience was great in the early stages of paint replacement in thermoforming applications. 1 1 Wilhelm Klepsch, Kompetenz in Kunststoff, Page 47, Esperanza Holding, Piesendorf, Austria, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 61
72 62 Chapter 9 Paint Replacement in Automotive Applications 9.2 REASONS FOR REPLACEMENT OF PAINT IN AUTOMOTIVE APPLICATIONS 2 There are many reasons why original equipment manufacturers (OEMs) would like to eliminate the painting processes: High investment cost for paint lines High operating costs of paint lines Expensive pre-painting part preparation High scrap rates Environmental regulations Capacity dictates price Danger of stranded investments License - free cars are paint - free cars. License - free cars are a specific market segment in some European countries. These cars have body parts that are completely made from thermoformed, coextruded inline colored plastic sheets. Most parts are made from single - shell, thermoformed plastic sheets that easily can be fastened to an aluminium frame by adhesive systems or mechanical systems, such as bolts, screws, or rivets. For some parts a two - shell construction, consisting of an outer shell with a high - gloss colored surface glued to an inner shell of an embossed material, is used. The result is a very stiff reinforced body part. Robots are used to mount the thermoformed body panels onto the aluminium frames. Such vehicles are very lightweight, with a total maximum weight of 350 kg. Because of the lightweight construction these vehicles are ideally suited to be equipped alternatively to the traditional diesel engine with an electric zero emission engine. As may be expected, such vehicles have great potential for inner city transport. 9.3 LAYER CONSTRUCTION OF COEXTRUDED INLINE COLORED PLASTIC SHEETS For license - free cars typically a coextruded ABS/PMMA sheet, which is colored to customer specification inline, such as Senosan AM50C SOLAR EG (Senoplast), is used. Senosan combines selected PMMA and ABS polymers in a five-layer sheet. Each polymer plays its particular role, supported by a sophisticated formulation with functional additives, such as colors and UV stabilizers, and elaborated layer distribution in coextrusion. The result is a unique combination of properties, tailor - made to meet demand specifications. 2 Thomas Höfels, Presentation, Under the Skin, 6th European Thermoforming Conference, Berlin. Reviewed and extended edition, April 2008.
73 9.4 Color Management during Product Development and Production 63 Customers request a perfect surface finish, free from any defects, with high gloss and a deep 3D color effect. Mechanical properties, such as impact strength, must be high and must not change over time. And finally, the processing by thermoforming must be easy, reliable, and with short cycle times. Perfect flow of material allows high draw ratios and ensures the best gauge distribution in the finished part. This is important to support the physical properties in the finished parts of a difficult design. Senoplast introduced Easyglide for thermoforming to improve flow and reduce cycle time. Easyglide is an additional layer of ABS designed for the backside of the sheets. 9.4 COLOR MANAGEMENT DURING PRODUCT DEVELOPMENT AND PRODUCTION Color Formulation Process Colors, including metallic colors and colors with special effects that exactly match the customers specification, need to be consistent from delivery to delivery. The colors must not stain or fade over time. Appearance simply should not change during the whole lifetime of a vehicle. The process Senoplast has introduced to meet these color requirements follows several steps and confirms color match, reproducibility during the extrusion process, and durability (e.g., UV stability, general weatherability). These steps include first careful selection and formulation of colors. Durability is confirmed by 310 hours MEGASUN quick test, 1500 hours XENON weathering (EN ISO 4892), and one - year Florida weathering (ASTM D , ASTM G ) of sheet and thermoformed parts. Finally, samples are assessed according to DIN EN ISO Depending on the results, Senoplast will either provide full guarantee or reject the color formulation for outdoor use Color Approval by Customer Once a color is formulated, the limits of color deviation need to be established in consultation with the customer. During the first production run an internal specification is set as the maximum tolerance. This tolerance could be, for example, a Delta E CMC value < 1.5 (DIN 5033). Within this tolerance variations may be seen along three axes: light dark, red green, and blue yellow. In effect, color variations can occur in a three - dimensional color space, as a color bubble. The input from the customer is crucial for the first production runs, as only the customer can decide what is an acceptable color. This input could be that the color should be lighter or darker than a certain reference, more or less green, more or less red, and so forth. This narrows the color bubble and reduces it to a color cone. It also allows an internal specification to be set for the first production run.
74 64 Chapter 9 Paint Replacement in Automotive Applications After the first production run an internal analysis on statistics of color deviations is made. The customer is asked to inspect the parts for color deviations and provide feedback. Finally, an agreement on a color specification will be signed by both parties, which sets the quality standards for all subsequent production runs. Many difficulties can arise in color matching Two common ones are known as metamerism and the flip effect. For each color formulated to match a given sample, the spectrum of light by which the samples are compared needs to be defined. A number of standardized light sources (DIN 6173) are available, known as, for example, D 65 ( Daylight, 6500 K), TL 84 (4100 K), or CWF ( Cool White Fluorescence, 4150 K). Colors that match under one light source with a given spectral distribution may look quite different when viewed under another light source. This effect is known as illuminant metameric failure. The reason for this disparity is that different pigments absorb wavelengths at different rates. This is a typical problem when trying to match painted metal and colored plastic. Another typical situation is when trying to match colors used in exterior and interior applications. Metamerism is the effect when colors match under all light conditions (e.g., under light of different spectral distribution). Metameric color matches can be achieved in near - neutral grays, white colors, and dark colors. Metameric color matches are problematic, however, when intense colors or colors with special effects are used. Flip effects, also called geometric metameric effects, present when samples match when viewed from one angle but fail to match when viewed from another angle. This may be caused by alignment of color pigments during the extrusion process. The effect can be quite pronounced in metallic colors and special effect colors. It is important to consider this effect when mounting several plates of plastic sheet next to each other. Plates always should be placed in the same direction of extrusion Quality Assurance of Colors during Production During regular production, inline camera systems and offline color readings are used to continuously measure, compare, and record color values. This is complemented by visual comparison to a master sample. Pigmentation is adjusted inline if deviation from the limits is noticed. The key to consistent coloring is careful pre - production preparation and communication between the color laboratory and production team. Color masterbatches could be compounded to ensure consistent results during production. 9.5 REQUIREMENTS FROM THE AUTOMOTIVE INDUSTRY ON SURFACE QUALITY The glossiness of coextruded PMMA surfaces is determined by the raw material. Extrusion or thermoforming equipment has a small influence. Once in use, the
75 9.5 Requirements from the Automotive Industry on Surface Quality 65 glossiness of coextruded inline colored surfaces is relevant to the surfaces scratch resistance. PMMA is the material of choice for surface layers of coextruded film and sheet. A coextruded PMMA surface layer exhibits the same scratch resistance as a standard PMMA, as it is used in injection molding for a variety of exterior automotive parts. Although PMMA is known to be somewhat brittle, coextruded sheets and films have excellent mechanical properties. It is important to select PMMA grades that are particularly suitable for coextrusion and maintaining the optimum layer thickness of the PMMA. Today, for a number of reasons, there is no alternative to PMMA when it comes to coextrusion with ABS or PC/ABS: PMMA has very good adhesion to ABS and PC/ABS. PMMA easily can be polished. PMMA can be colored in many different ways. PMMA is UV-stable. PMMA has very good chemical resistance. PMMA also has demonstrated good scratch resistance. In the automotive industry scratch resistance is always tested against a wash brush test, known as Amtec Kistler wash brush test (DIN 55665), which pushes PMMA to its limits. The test setup consists of a sample plate treated several times by a wash brush and water in which a certain percentage of quartz sand is dispersed. Gloss before and after treatment is measured and residual gloss or loss of gloss (percentage) is the main criterion. Under these test conditions coextruded PMMA surfaces show a brittle scratch behavior. The only polymer, however, that shows better test results is a special PC copolymer. The PC copolymer develops scratches of the same length and depth, but of a more ductile behavior compared with PMMA. Therefore residual gloss is a little better, too. However, the PC copolymer has a number of disadvantages, such as limited coloring possibilities and inferior chemical resistance. The Amtec Kistler test results of paint or the new paint - film technology are clearly superior to coextruded surfaces with PMMA or the PC - copolymer top layers. While residual gloss of paint - film is around 78 gloss units after the Amtec Kistler test, the PC copolymer is at 30 gloss units and PMMA at 15 gloss units. Automotive requirements are typically at around 75 to 85 gloss units. To compensate for this gap, extrusion companies are developing various options to improve scratch resistance. Adding a layer of hard-coat is one option to improve scratch resistance. The surface is lacquered and hardened, for example, UV - cured. Hard - coated PC or PMMA surfaces show excellent scratch resistance but cannot be thermoformed any longer. Unfortunately, all coatings known so far that can be thermoformed after cure do not show any better scratch resistance than a coextruded, uncoated PMMA layer. As an alternative to coating, inline polishing may improve scratch resistance. Another alternative may be found by turning to nanotechnology, but
76 66 Chapter 9 Paint Replacement in Automotive Applications there is no commercial product available at the moment, and much more research is still needed. 9.6 REQUIREMENTS FROM THE AUTOMOTIVE INDUSTRY ON COLOR MATCH There are several technical limits when it comes to matching automotive paint with coextruded inline colored sheets or films: Orientation of the pigments in extrusion direction, as already discussed above. Limits to the concentration of pigments in the polymer matrix. Concentrations that are too high can cause delamination. Limited choice of color pigments for extrusion due to lack of temperature resistance of pigments. Effect pigments may lose their brilliance during the extrusion process. Difficulties due to variation in thickness of layers of paint and coextrusion: thicker PMMA layers with lower pigment concentration have to match with thin paint layers with high pigment concentration. In addition, there are commercial limits when it comes to matching automotive paints with coextruded inline colored sheets or films. For example, the color portfolio of a typical OEM has been analyzed. Typically, 12 standard colors are in use. From these 12 colors, 7 colors require less than 7 tons of plastic sheet each per year, based on an annual production of 200,000 vehicles. To match colors and to produce colored sheet for quantities of less than 7 tons per year usually cannot be done economically. Sometimes cars show clearly visible color deviations on spray - painted plastic and metal parts (see Section 9.4 on the discussion of metamerism and illuminant or geometric metameric failure). It may be helpful to show such examples to OEMs to illustrate the limits of color matching. 9.7 AUTOMOTIVE INDUSTRY AND ORANGE PEEL Solvent - based automotive paints are sprayed onto steel. Variations in the spray process can cause variations in the paint layer or variations in the paint/solvent mixture. After drying, these small variations result in a surface waviness, referred to as orange peel. Coextruded surfaces, however, show no or very little surface waviness. When extrusion processes are well controlled, surfaces become mirror-like. An orange - peel surface can be achieved using a thermoforming mold with a slightly structured surface. This technique is used to hide defects from the extrusion or the forming process or to better match surface structures of thermoformed and painted surfaces.
77 9.8 Examples of Paint Replacement in Automotive Applications EXAMPLES OF PAINT REPLACEMENT IN AUTOMOTIVE APPLICATIONS Use of Color Contrasts Because color matching of automotive paint is challenging, early applications of coextruded inline colored sheets and films were in contrasting colors. Some examples are: The roof module of a car the contrast color being high gloss black, which forms a perfect unit with the dark tinted glass of the sunroof. The front grill of the MAN trucks the chrome logo of MAN contrasting the high - gloss black surface, also in contrast to the color of the truck (Figure 9.1 ). Tuning parts many are made from coextruded inline colored sheets in a contrasting color Approved Color Match: Thermoformed Pickup Covers Some car manufacturers produce pickup covers, typically consisting of an inner and an outer thermoformed coextruded sheet, a honeycomb core, and polyester adhesive layers. The outer coextruded sheet has to match several standard colors used for the body paint. In one particular case, four metallic colors and three uni - colors were matched. The typical angle of view between the thermoformed part and the surface of body paint on metal is tilted by 90. Therefore, metameric effects appear to be Figure 9.1 Radiator cover for a truck (Courtesy of MAN Truck & Bus AG)
78 68 Chapter 9 Paint Replacement in Automotive Applications less critical, and the large surface areas of different materials next to each other can be matched very well. 9.9 PAINT-FILM TECHNOLOGY: PAINTING PRIOR TO THERMOFORMING In the case of the new paint - film technology a coextruded film is painted prior to thermoforming and parts manufacturing. The current series applications of paint - film technology are for the roof modules of different car types. Today s paint-film technology can meet all automotive requirements regarding color match, scratch resistance, chemical resistance, and so forth. Senotop was developed for the automotive industry and for this application by Senco (Europe), a subsidiary of Senoplast, coextruding an ABS - PC compound with PC on the top. The selection of polymers provides excellent mechanical and chemical properties, excellent thermoformability, and perfect adhesion to the supporting foamed structure as well as to the paint. The conversion process of Senotop at the customer s premises includes painting and drying under cleanroom conditions, thermoforming of the part, and UV curing of the paint. The last steps are inserting the glass fiber and the PU back - foaming of the thermoformed part, and, finally, trimming and inspection. The first commercial high - volume thermoforming application for large - area exterior automobile parts was established for a customer of Senoplast in Germany. The highlights of the results of this application are: Use in 250,000 car roofs per year. Very short cycle time for thermoforming, UV curing, foaming, and trimming. Fully automated production, with two operators manning the entire line. The latest technology of thermoforming includes the following features: Thermoforming under cleanroom conditions. Thermoforming tools mounted on a rotating table, change of tools done between thermoforming cycles. Automated loading, unloading, and UV curing with robots. The latest technology of PU foaming includes the following features: Use of rotating foaming tools. Random production of partial roof modules: antenna covers, partial roof covers Outlook Thermoforming of coextruded colored sheets and films has the potential to replace paint in automotive applications: 1
79 9.9 Paint-Film Technology: Painting Prior to Thermoforming 69 Weight reduction drives the use of plastic parts in automotive applications. Class A surfaces can be achieved with thermoforming; solutions for high scratch resistance are available. While injection - molding is now standard in the automotive industry, the full potential of thermoforming has yet to be attained when it comes to high - volume exterior applications. Paint-film technology is the first to apply thermoforming in a high - volume exterior application; other technologies and applications are sure to follow. New areas of interest are body panels for trucks, utility vehicles, and niche vehicles such as battery powered zero - emission city cars (E- mobility), in particular to reduce the vehicle s weight. The automotive industry is looking for partners that can provide thermoformed parts in high quantity and quality Chrome Optics Parts with the optical appearance of chrome can be produced by thermoforming. For semi - finished products with metallic d é cor surfaces, the carrier layers are typically ABS cast with a special lacquer film. Many different surfaces can be simulated: Chrome Stainless steel Aluminium Metallic Brushed metal Silver These surfaces are also UV - and scratch - resistant. Postsurface treatment is not necessary. Low mold costs promote faster face lift cycles, especially in the automotive branch. Large parts are put into practice. Applications extend to metallic decoration found on the interiors as well as exteriors of automobiles.
80 Chapter 10 Motor Air Intake Made from PA 6 GF 15 In the past, when technical parts consisting of polyamide were thermoformed by means of sheet thermoforming machines, it was recommended to use polyamide 12. Extruded sheets made of ordinary linear polyamide 6 have a very small range of forming temperatures, so that in praxis it is nearly impossible to produce acceptable formed parts. Semifinished products of polyamide 6 are relatively ductile when they are warmed up to their crystallite melting point. However, for temperatures above the melting point, polyamide 6 s stretching viscosity for thermoforming is too low. The material lacks the adequate melt strength. For some years Lanxess Deutschland GmbH has offered a specially developed, branched polyamide 6 having the necessary structural viscosity. By adding an additional 15% glass fiber reinforcement, the manufacturing of temperature - resistant (permanent service temperature: 140 C, temporary 170 C) and mechanically highly resilient formed parts is possible. Durethan BKV 315 Z H2.0 offered by Lanxess is extruded to sheets that are used as the semifinished product for thermoforming. For processing of this fiber - glass - reinforced polyamide 6 type, attention must be paid to the fact that the heating elements in the thermoforming line can attain high temperatures. High temperatures are of utmost importance for processing because the forming temperature of polyamide 6 is approximately 250 C (measured at the sheet surface). Moreover the high temperatures of the heating elements facilitate a reduction of the cycle time. No noteworthy sagging can be observed when the semifinished sheets are heated, and thus a uniform heating of the material is guaranteed. Because polyamide is hygroscopic, semifinished products of polyamide 6 must by dried at 110 C before thermoforming. Otherwise, voids will occur in the thermoformed part. A temperature - controlled male mold was used for tests. The temperature of the tool was approximately 90 C. The sheets formed were 2 and 6 mm thick. Very good forming accuracy was achieved for each sheet thickness. Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 70
81 Chapter 10 Motor Air Intake Made from PA 6 GF Formed parts made of the impact - resistant modified polyamide 6 can easily be trimmed with a band saw. The parts can be cut directly after production, and no reconditioning is necessary. For thermoforming it is essential to pay attention to the extrusion direction because the fiber - glass - reinforced polyamide 6 has a different behavior for lateral and diagonal shrinkage, relating to the extrusion direction. Polyamide 6 can be used in all sectors for which temperature resistance and mechanic resistance are necessary. For example, the material can be used in the engine compartments of automobiles or ships. Here there are applications for protective covers and air intake systems. It is also a possible material for oil pans. One argument in favor of using polyamide 6 for ship engines is, among other things, the higher heat resistance in comparison to other established thermoforming materials. Thermoforming is the most cost - effective solution for this application. Other reasons for the use of PA 6 semifinished products are their high tensile strength and rigidity. In comparison to other thermoforming materials, the wall of the finished product can be reduced in thickness because of the high rigidity of PA 6. Although engine covers have large dimensions, they have low distortion and are dimensionally stable. Furthermore, they possess a high breaking strength, due to the fact that polyamide 6 is impact - resistant modified. This, in combination with their low weight, is particularly important with regard to the high dynamic load of motor vibrations. Thanks to the high heat resistance of Durethan BKV 315 Z H2.0, the cover parts can endure permanent service temperatures of 140 C and also temporary temperature peaks of 170 C. For use in the engine room they also have the necessary resistance against oil, grease, diesel, and other chemicals that are typically used on board ships. To some extent these motor covers can replace former sheet metal structures.
82 Chapter 11 Sanitary Equipment (Sheet Machine) Written in cooperation with Manfred Geiss, Geiss AG, Sesslach, Germany From a historical point of view, the plastic (ABS - based) mass - marketed bathtub derives from England, as there were no foundries. In England the bathtub was formed on a rig. Before the forming process, the sheet was heated hanging in an oven. Afterward the sheet was taken out by two operators, placed on a support plate, and fixed in a clamping frame. Hydraulically movable tooling entered into the plate and a vacuum was applied. During the cooling phase the work continued on another rig. At the best of times 700,000 bathtubs were produced each year by this method! The first thermoforming machines for serial production were introduced in FROM THE RIG TO THE THERMOFORMING MACHINE The thermoforming process for the production of bathtubs can easily be automated since the pre - cut part does not shrink during heating in the thermoforming line and the individual heating control enables a targeted influence of the wall thickness that results in a reduction of the original sheet thickness for bathtubs from 5 to 4 mm. The production of tubs in a closed thermoforming process results in an improvement in quality as, for example, contamination by dust particles is reduced. Furthermore, in comparison to the rig, it is possible to reduce the size of the clamping rim in an automated machine, which results in advantages concerning material costs. The material can be pre - stretched before the commissioning of the form. This way a better distribution of the material wall thickness is possible and chill marks can be avoided. The early thermoforming machines did not yet have tempered clamping frames, and for this reason the manufactured tubs deformed somewhat as the formed part shrank during its cooling. Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 72
83 11.3 Reinforcement Methods for Bathtubs 73 Thermoforming machines with so - called sanitary equipment, as offered by the company Geiss, AG, prevent the deformation of the formed part. The sanitary equipment also provides other functions that facilitate the production of high - quality bathtubs. Included in the scope of supply is a temperature control system for the adjustable window plates. The machine provides higher retention forces for the holding of partly cross - linked plastics. A higher vacuum performance is attained through the use of a second vacuum pump. Pressure water equipment is used in the temperature control circuits to allow temperatures to rise up to 120 C and achieve higher mold and clamping frame temperatures without being limited by the water evaporation. The most important point in order to guarantee even clamping edges is the control system of this sanitary equipment for the clamping procedure. The market for thermoformed sanitary products has grown to include many thermoforming machines with different format ranges. Shower tubs, standard tubs, angular tubs, covers, pools, and even double and triple tubs are thermoformed with format areas of up to mm FINISHING The demolded form parts need to be cut. Systems were designed in order to overcome the chaotic sequence of the finishing process. A recently patented KS system of the company Geiss AG should be cited, whereby the flat rim of the tub is held by programmable actuated suction devices. The cutting is effected by a five-axis CNC - machine equipped with sawing blade and cutters for whirlpool drillings. A barcode reading system considerably simplifies the program selection. The interlinking of the thermoforming machine with a machine for the postprocessing steps is a significant development for the increase in efficiency REINFORCEMENT METHODS FOR BATHTUBS There are different reinforcement methods for bathtubs, as shown in Figure Additionally, shower tubs are thermoformed, and there are also instances of applications for furniture used in hairdressing salons (Figure 11.2 ).
84 74 Chapter 11 Sanitary Equipment (Sheet Machine) 1. Senosan BM 2. GRP reinforcement 3. base reinforcement 4. adjustable supports 5. Senosan X 1. Senosan BM 2. PUR reinforcement 3. base reinforcement 4. adjustable supports 5. Senosan X Senosan Senosan BM BM 2. Counterpart thermoformed 2. base reinforcement base reinforcement 3. Senosan X 3. adhesive 4. steel frame 4. base board 5. hot-melt-type adhesive 5. adjustable supports 6. adjustable supports 6. Senosan X Figure 11.1 Reinforcement methods for bath tubs (Courtesy of Senoplast Klepsch & Co. GmbH)
85 11.3 Reinforcement Methods for Bathtubs 75 Figure 11.2 Furniture for hairdressing salons (Courtesy of Senoplast Klepsch & Co. GmbH)
86 Chapter 12 Thermoforming and Milling of Large - Scale Formed Parts (Sheet Machine) Written in cooperation with Manfred Geiss, Geiss AG, Sesslach, Germany Several thermoforming methods can be used for the thermoforming of large - scale formed parts, such as those shown in Figure The thermoforming methods are based on two different machine principles: open or closed chamber. In the United States mainly rotary machines are used, and these function by the open chamber principle. In other countries linear machines are often preferred for production. Both systems do not, or only to some extent, support the semifinished parts during heating. For the manufacture of large formed parts, with reduction of the original material thickness, neither of these two methods is suitable. The heating of large parts is not the only problem for production. Primarily it must be guaranteed that the large parts can be handled automatically. The correct material flow with regard to parts having a heavy weight and a large surface area must be obtained, with a quick format changeover for increasingly smaller series. For the handling of the parts the static charge must be counteracted. Subsequently, the automatic further processing of the formed parts also needs to be considered. If for the production of large - scale formed parts, the pre - heating or the finish heating is done in a separate station next to the thermoforming station, then a temperature loss will occur during transportation to the actual forming station. The surface temperature can be reduced by 35 C to 50 C, which may lead to a loss in quality. The development of halogen heater elements enabled closed chamber machines to be developed for the manufacture of large - scale formed parts. In the closed Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 76
87 Chapter 12 Thermoforming and Milling of Large-Scale Formed Parts 77 Figure 12.1 Thermoformed side panels of a harvester (Courtesy of New Holland) chamber machine the semifinished part is clamped in the forming station and heated. The halogen heaters guarantee high efficiencies and relatively short heating times. Because the semifinished part is not transported anywhere when heated, there is no loss of heat before the thermoforming process. The sheet, however, can be supported during heating, which entails significant process and quality advantages. With closed chamber machines and the halogen heater technology the production of goods in any number is possible. Further developments in the machine and tooling technology have led to, for example, quick clamping systems for forming tools and plug assists, infinitely adjustable clamping frames, infinitely adjustable window plate systems, free programmable and storable axes for any setting, and automatic changeover with a tool change machine. The machine should possess heaters, which make the control of each individual halogen heater element possible. Ring zone controls or linear zone controls tend to be inconveniently located. Concerning the setting of the temperature of the heater elements, the rims of the format surface must be hotter than the center. This means that the heater elements heating the edges of the format surface must be set to an even higher temperature in order to guarantee a constant heating. The aim of advanced thermoforming is automation of a batch. Example of the Manufacture of a Luggage Box for Skis In order to understand this application it is necessary to know the difference between positive and negative forming. Regarding positive forming, the plastic is formed with a mold. This mold is a positive core and has no cavity. The forming part protrudes from the clamping section. The use of a positive form is often more economical. Regarding negative forming, the material is sucked into the forming cavity. The mold is a cavity. The formed part goes from the formed part section downward (Figures 12.2 and 12.3 ).
88 78 Chapter 12 Thermoforming and Milling of Large-Scale Formed Parts Figure 12.2 Ski box (Courtesy of Kamei GmbH & Co. KG) Figure 12.3 Negative and positive forming combined in one mold (Courtesy of Geiss AG) The formed parts for the ski box are required to be in batches. In the past, the upper parts were formed and stored. Subsequently the machine was converted and the forming tool for the bottom parts installed. Today, both parts (one positive and one negative forming part) are produced at the same time. The upper part is automatically cut horizontally. Both parts are processed in batches at a CNC working station and delivered without intermediate storage to the assembly station. Example of Handling Problems Concerning the Manufacturing of Table for Plants The manufacturing of a table for plants requires the processing of very large surfaces. For this process the format area of the thermoforming machines is mm. The transfer from the thermoforming machine to the CNC working station is very difficult, as the processed formed parts must be turned and stacked. The manufacturing of such large parts can also be done with a Geiss TT - in - one thermoforming machine. In the Geiss line the CNC milling machine and the turning station are chained, and production is carried out without human intervention up to the shipping palette.
89 12.1 Surface Problems 79 When large - scale parts are thermoformed, some problems may appear that need to be avoided: Surface discoloration Burns Gas release, pits Chill marks Shrinking Expansion 12.1 SURFACE PROBLEMS High - gloss surfaces are required for many applications. However, the production of such high - gloss surfaces can be problematic. The destacking process in the feeding device may cause considerable problems. Static charges result in the adhesion of dust to the semifinished parts. Molded dust is a cause for defective goods. Cleanroom conditions minimize the reject rate significantly. The avoidance of chill marks requires extensive experience of the machine operators as well as accurate settings of the machine parameters. If the baffle plate method is used, these plates must be carefully manufactured. Formed parts with high - gloss surfaces are costly to produce, but for many applications, a good appearance is necessary, and thus the higher operating expenses are justified The Avoidance of Chill Marks In order to guarantee consistent quality of the formed parts, it is necessary to use so - called pre - blow photocells because they facilitate an exact pre - blow height, and thus the pre - blowing of the heated semifinished part is reproducible. In order to avoid chill marks, it is important to always keep the temperature of the forming tools as high as possible. On the other hand, the material temperature should be as low as possible. Another measure to avoid chill marks is pre - blowing against a so - called baffle plate (Figure 12.4 ). Figure 12.4 Baffle plate (Courtesy of Geiss AG)
90 80 Chapter 12 Thermoforming and Milling of Large-Scale Formed Parts 12.2 MOLD SHRINKING AND FREE SHRINKAGE Plastic formed parts are liable to mold shrinkage. During the heating phase the semifinished parts can also create problems for the production of formed parts because of their free shrinking behavior. To some extent this phenomenon is not reproducible. It is possible to counter the mold shrinkage with temperature - controlled forming tools. The temperature set for the tools must be carefully controlled. To ensure a constant mold release temperature, the use of a cooling time pyrometer is advisable. Automatic production is also an decisive factor for the control of the mold shrinkage. Quick further treatment of the formed parts can diminish mold shrinkage. Even separation of the clamping wheel with a horizontal band saw is useful EXPANSION Compared with metal, plastic parts have a thermal expansion that is 10 to 20 times higher. The prevention/avoidance of the expansion significantly reduces the positive characteristics of the used formed parts THE DECISION BETWEEN POSITIVE OR NEGATIVE FORMING The surface texture of the side of the forming tool that is in contact with the form is always matt. This side of the forming tool is also the side that is accurate to dimension. However, there are applications for which the forming mold should present a surface structure. These applications are an exception. Generally, a compromise between dimensional accuracy and quality of the visible side must be found. Example of Choosing between Positive or Negative Forming (see also Chapter 2 on the Basics of Thermoforming and Thermoplastics) For the inner housing of a refrigerator, a compromise is often made between dimensional accuracy and quality of the visible side. On the one hand, the visible side is inside, which means that the negative forming method should be used in order to avoid contact with the mold and the visible side of the part, causing quality issues in terms of surface appearance. On the other hand, parts formed with the injection molding method must be mounted to the internal side, and thus this side must be accurate to dimension. With a certain effort the forming molds can be polished so that good surface qualities can be attained, however, not a high - gloss surface. European manufacturers use the positive forming method. The costs for negative forming molds are considerably higher, the more so as a plug assist is always necessary (Figure 12.5 ).
91 12.5 Twin-Sheet Forming 81 Figure 12.5 Negative forming (Courtesy of Geiss AG) 12.5 TWIN-SHEET FORMING With the twin - sheet method two form parts are created that form a hollow body. This means that the formed parts are in contact with the form at all outer surfaces. Therefore, the outer surfaces are matt or are defined by the surface of the forming tool. A grained semi - finished material is used for certain applications. However, the position of the weld contact areas must be considered, as the grain will very probably be flattened. The characteristic of twin - sheet formed parts is the dimensional accuracy of the complete surface. Generally, undercuts are very difficult to execute. High clamping forces of the thermoforming machine and precise machine movements are necessary for the successful production of twin - sheet parts. For the example of a triple bus seat (Figure 12.6 ), a standard twin - sheet equipment with 70 kn clamping force is used. The optional three - phase current servo motors increase the precision and the clamping force to 200 kn. A special option makes the increase of the clamping forces to 320 kn possible. The Geiss AG CYTEC machine accomplishes this purpose. With this scope of supply the machine tables are moved together and restricted with 1000 kn. An example is the twin sheet application for canopies of pick - up trucks.
92 82 Chapter 12 Thermoforming and Milling of Large-Scale Formed Parts Figure 12.6 Twin sheet application triple seat for bus (Courtesy of Geiss AG) 12.6 AUTOMATION Today, for cost - effective production, the thermoforming machines for most manufacturers of large - surface parts function fully automatically. An important component of the automation is the infeed of sheets. Programmable axes increase the flexibility and facilitate the format changeover. Servo - motor drives also improve the reproducibility and make the production of consistent quality possible. The reject rate can be drastically decreased and productivity can be increased. The thickness and the size of sheets relative to the machine size do not affect the reliability of the automation process Comparison of Semi -Automatic and Fully Automatic Thermoforming Lines For semi - automatic processing, the semifinished sheets have to be manually loaded and the formed parts manually unloaded. The formed parts must be always monitored, as the semi - automatic process is subject to outer influences and time variations. These influences and variations can have negative effects on the quality of the formed parts. The semi - automatic process is monotonous and somewhat slavish work. Fully automatic thermoforming lines function more precisely and are more productive. Direct interlinking with stacking devices and further treatment stations is possible. For large and heavy formed parts it is necessary to use the fully automatic procedure to ensure production of unchanging quality. The percentage of thermoformed parts of the entire plastics processing industry will no doubt increase. While the boundaries are not yet tested, the possibilities for the use of thermoforming methods are manifold. With regard to the machine technology, there are developments under way to produce more flexible machines. In this context the heating technology has a great significance.
93 12.6 Automation Further Treatment of Large -Scale Thermoformed Parts With careful determination of shrinkage, exact fitting can be done of the mill catch. Here it is important to have some experience with shrinkage - free cast resin for the mill catch as well as having a good CAD/CAM coupling. Measuring devices integrated into the CNC milling machine are being used to verify the edges of the formed parts and the shrinkage values. A fixed measuring sensor makes calibration of machine axes possible. Extendible machine tables facilitate the handling, though this leads to an increased space requirement. Modern drive systems (linear induction motors) provide constant infeed speeds at the chip with multiply increased accelerations. The control system of the milling machine should have sufficient storage space. Furthermore the machine should facilitate any cutter radius compensation in any space coordinate and any cutter length compensation. Particularly efficient machines offer an automatic tool change. Five - axes programming by means of efficient CAD/ CAM systems, together with an efficient control system, call facilitate highly flexible processing. The deflashing of drillings is effected with help of special tools that deflash both sides of the drilling in one operation cycle. Deflashing with profile cutters is also possible.
94 Chapter 13 Changeover of Sheet Machines Written in cooperation with Manfred Geiss, Geiss AG, Sesslach, Germany 13.1 THE INCREASING IMPORTANCE OF THE CHANGEOVER PROCEDURE In the thermoforming industry, the same as in many plastics - processing industries, a rapid changeover of a production machine s format is becoming increasingly important (Figure 13.1 ). Manufacturers of thermoforming machines are forced to meet the demand to develop machines that enable the user to effect rapid format changeovers. But what exactly does the term changeover mean? The changeover of a machine is the period during which the machine is converted from one format to another format. The time necessary is measured beginning with the outfeed of the last product of the first format until the outfeed of the first product of the second format. In between there are several process steps concerning the changeover procedure: Machine standstill Cooling Dismounting of mold and frame Mounting of new mold and frame Adjusting of strokes and photocells Programming Heating Start-up Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 84
95 13.1 The Increasing Importance of the Changeover Procedure 85 Figure 13.1 Thermoforming with automatic changeover equipment (Courtesy of Geiss AG) As batch sizes decrease, reductions of the changeover times become more and more central concerns. While the complexity of the format parts keeps on increasing, so do the setting parameters in multiples, and additionally the standards of quality. In particular, the great significance of the changeover can be recognized by the gain per format part. In the past, many companies did not record the changeover times of their machines. A few years ago only approximately 30% of the companies determined the times needed for a changeover procedure. Even though, in the past, the topic changeover was considered a decisive point during the negotiations for the purchase of a machine, an analysis was seldom conducted. Poor practice in archiving and storage of data records led to a prolongation of the changeover times. Older thermoforming machines may have a worse repeatability. The determination of the best parameters also prolongs the changeover. Additionally, there is the phenomenon that every machine operator uses his own program for the production. In order to save costs, and to effect the changeover process with a view to increasing time efficiency, the aim today is an automatic changeover without human intervention. The automatic changeover of a thermoforming machine is facilitated through the availability of a different system with: Quick clamping system for tools Infinitely adjustable clamping frames Infinitely adjustable window plate system Quick and efficient heating (halogen heater elements) Programmable axes Mold change machine
96 86 Chapter 13 Changeover of Sheet Machines Quick Clamping System for Molds The quick clamping system for molds locks the forming tool onto the bottom table with pneumatic force. Pneumatic cylinders enable the lifting of the forming tool so that, for example, a fork - lift truck can seize the forming tool (Figure 13.2 ). Thus a fork - lift truck must be able to pass underneath the machines. The new format mold is adjusted in the machine by using conical head pieces. Quick clamping systems for molds are also available for plug assists The Infinitely Adjustable Clamping Frame In order to avoid the use of a multitude of clamping frames with different sizes, the infinitely adjustable clamping frame was developed. Such clamping frames are adjustable in both axes. The machine retains its thermal balance because neither the warm format tool parts are dismounted from the frame nor cold format tool parts mounted. This is a big advantage regarding unchanging production conditions. Depending on the degree of automation, the clamping frame can be adjusted manually or automatically, since the infinite adjustability of every parameter can be programmed, saved, and started automatically (see Figure 13.3 ) The Infinitely Adjustable Window Plate System Like the infinitely adjustable clamping frame, the infinitely adjustable window plate system is integrated into the machine, enabling a reduction of the parts that need to be changed (Figure 13.4 ). The window plate system serves as the counterplate of the clamping frame for the stretching of the semifinished product in the machine. The frame size of the window plate system can vary laterally up to 1000 mm and, regarding the machine depth, up to 500 mm. No additional parts are necessary. Neither are warm format tool parts dismounted nor are cold format tool parts mounted, so the machine retains its thermal balance. This is a big advantage regarding unchanging production conditions. All positions can be programmed, saved, and automatically started Quick and Efficient Heating (Halogen Heater Elements) The halogen heater element is an important component of the changeover process due to its extremely short reaction time (Figure 13.5 ). The extremely short reaction time of the halogen heater elements allows for the elimination of the disadvantages of a slow single - station machine. The changing of a heater parameter is done in practically zero time. The system reacts immediately to changes in intensity. Very quick adaptation from hot heating to cold heating is possible.
97 Figure 13.2 Quick clamping system for molds (Courtesy of Geiss AG) 87
98 88 Chapter 13 Changeover of Sheet Machines Figure 13.3 Infinitely adjustable clamping frame (Courtesy of Geiss AG) Figure 13.4 Infinitely adjustable window plate system (Courtesy of Geiss AG)
99 13.1 The Increasing Importance of the Changeover Procedure 89 Figure 13.5 Quick and efficient heating (Courtesy of Geiss AG) The Programmable Axes Every changeover process includes several manual adjustments: Stroke of the plug - assist tooling to the lower position limit Upper position limit of the stroke of the plug - assist tooling Upper position limit of the clamping frame Unloading position of clamping frame-feeding Table middle position Table lower position limit Top heater upper position limit of the stroke Feeding side limits Feeding front and rear limits Photocell pre-blow Photocell formed part taken Transport path of cross cutter Roller film width Programmable rails for suction devices Test control unit for material thickness Position of cooling fan Position of radiation pyrometer
100 90 Chapter 13 Changeover of Sheet Machines In order to reduce the changeover time, these settings must be programmable and savable; the program is called up and executed automatically Mold Change Machine The most extensive development in reducing changeover times has involved the mold change machine (see Figure 13.6 ). The mold change machine works automatically and without any human intervention. The forming tools are pre - heated before they are used. The mold change machine is suited for roll as well as for sheet thermoforming lines. A mold change machine can serve any number of thermoforming machines. For a changeover the complete mold package (thermoforming mold and plug assist) is exchanged. The use of a mold change machine necessitates a coordination of the whole production process. Thus the infeed device of the semifinished products needs to be adapted to the space available. The machine tables must allow the automatic change of the forming tools. For this purpose docking systems and on - board data storage mediums are necessary. The tool change machine must be able to transfer/remit two temperature control circuits, electric power, signals, and temperatures. It is also important that the system can transfer pneumatic undercut movements. Each forming tool has its own data storage medium. The reading devices for the data storage mediums are located in the machine table. Figure 13.6 Mold change machine serving two thermoforming machines (Courtesy of Geiss AG)
101 13.2 Shortening of Changeover with High-Quality Equipment 91 A disadvantage of mold change machines is the space required. More elaborate base frames for the forming tools are also necessary. The docking station entails a higher complexity. The draw depth of the machine may need to be increased as the tool package is brought in through the front doors. The mold change system has advantages for machines on which the forming tools must be exchanged frequently due to small batch sizes. The tool change system is also helpful when using multipurpose tools for which the changeover of the forming tool can be done outside the forming station. For example, the system is used for laminating appliances with five different car door laminations. It can be used for several machines (Figure 13.6 ). It also enables the separation of operations for the exchange of forms and blanks from the cleanroom via a passable lock SHORTENING OF CHANGEOVER WITH HIGH-QUALITY EQUIPMENT Complete changeover procedures at old machines with slow reactive heaters require between 1 and 3 hours. The quick clamping system for molds enables a time saving of 10 to 15 minutes per changeover. The use of an infinitely adjustable clamping frame does not shorten the changeover time. However, no additional parts are necessary. The changeover time is shortened by 10 to 15 minutes when an infinitely adjustable window plate system is used. The great improvement is the elimination of the fixed window plates. The halogen heater elements allow for the omission of the pre - heating of the heating and frame systems. This results in a time saving for the changeover of approximately 10 minutes. As it is not necessary to bring the machine laboriously into a thermal equilibrium, it may be possible to bring that time saving even higher. The programmable axes account for a time saving each of approximately 1 minute. So there is a big advantage to reproducibility for the production of repeat parts. The tool change machine reduces the changeover procedure to 10 to 12 minutes. No human machine operator is needed.
102 Chapter 14 Chromed Parts Written in cooperation with Thorsten Eymael and Nina Schick, SE Kunststoffverarbeitung GmbH & Co. KG, Germany The pre - condition for good metallization is adequate adhesion between a metal layer and plastic. This is achieved by using a different pre - treatment for each plastic. It is not possible to make every plastic conductible with justifiable time and effort, and for this reason ABS plastics (acrylonitrile - butadiene - styrene) as well as their polycarbonate blends have become established in the industry. ABS is the plastic that is often used for galvanization. 1 For the galvanization process a composite of metal and plastic is created. By means of a wet chemical process a thin metal layer is applied to the plastic part, whereby ABS is mostly used for the plastic part and chrome for the metallic top layer, whose metal layers may include nickel or copper. Subsequent to the chemical pre - treatment, mostly with acid (so - called acid cleaning), which gives the plastic a rough - textured surface, different metals, stemming from a watery solution, are electrolytically deposited in several process steps at the plastic surface. Whereas for products for the sanitary sector the combination of these metal layers is often not thicker than 25 μ m, for automobile parts the thickness can be up to 40 μm. In order to make adhesion on ABS parts possible in the first place, the butadiene component is extracted by means of an acid cleaning bath at the surface. In the cavernous holes thus created, palladium seed crystals (cores) are intercalated, subsequent to corresponding cleaning and reduction steps in the activation and acceleration baths. However, these palladium seed crystals (cores), nickel, and copper seed crystals (cores) can be absorbed to form a continuous layer. This process is carried out in chemical outer currentless nickel or copper baths, whereby through the immersion of the product with the catalytically effective palladium crystal cores the metal deposition is triggered. 1 Detlef Berndt, Kunststoff-Institut Lüdenscheidt, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 92
103 Chapter 14 Chromed Parts 93 Figure 14.1 Center of dashboard of Actros truck (Courtesy of Mercedes Benz and SE Kunststoffverarbeitung GmbH & Co. KG) The basis for the adhesion is the cavernous holes into which the palladium cores are incorporated. Through the metal layer, which is growing toward the outside, a snap fastener effect is created, which makes the metal layer stick firmly to the plastic surface. Because this layer is still very thin ( μ m), it is increased in a metal bath having slight currents to a thickness of approximately 2 to 3 μm. Next, a normal galvanic copper layer is applied to the layer onto which, in turn, and depending on the requirements to the formed part, the necessary layer systems are added, for example, medium gloss nickel gloss nickel microporous nickel chrome or medium gloss nickel pearlescent nickel chrome. In the case of the application shown in Figure 14.1, a ABS thermoformed part is galvanized and used in the interior of the truck at the center of the dashboard to keep freight papers in place.
104 Chapter 15 Applications in Aircraft and Mass Transportation Written in cooperation with Thorsten Eymael and Nina Schick, SE Kunststoffverarbeitung GmbH & Co. KG, Germany Passenger safety must be a foremost consideration in the use of plastic parts for aircraft and other transportation vehicles. Only material grades that conform to the strict directives of fire prevention can be utilized. In this chapter several such applications will be described. In order to fulfill the requirements of the directives, the materials must have several specific properties, as are detailed in this chapter. The history of flight is about reaching higher upward through innovative design and better materials. 1 As a result, aircraft have become more fuel - efficient, increasingly more comfortable, and safer. With all these developments today s aviation industry is more complex than ever before. To be more competitive and create differentiated designs, manufacturers are tasked with staying abreast of the latest material solutions that ultimately deliver better performance around critical demands such as safety, total cost of ownership, and weight reduction. For the aircraft industry, rising fuel prices and taxes are requiring that aircraft manufacturers design the most lightweight and fuel - efficient aircraft possible. Aircraft manufacturers are also looking to meet safety, aesthetic, and performance requirements in business and first - class seating and other interior components, while at the same time improving passenger comfort. The move to enlarge seating/sleeping areas on some aircraft has caused additional interior components to fall under heat release standards. New and retrofitted planes tend to feature fresh designs and aesthetics, requiring materials that can provide excellent colorability and creative design freedom. 1 Living the Plastic Age, Aerospace Manufacturing, page 18, November Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 94
105 15.1 Current Government and OEM Specifications for Flammability 95 Ultimately key is understanding each individual airline s identity. For this reason material suppliers OEMs, tier suppliers, designers, and the airlines should work together to find the best possible material solutions. When taking such a holistic approach, there arise many thermoset resin composites and metal replacement opportunities. The use of thermoplastics can offer real reductions to the manufacturing cycle, through the elimination of manufacturing steps and part count reduction. Thermoforming of sheet products can also offer a very cost - effective method of achieving low volumes of complex - shaped parts. To be sure, airlines wish to differentiate their product offerings, while at the same time finding innovative solutions for controlling costs and reducing total cost of ownership. Clearly, a one - stop - shop opportunity to the industry for new plastic solutions would facilitate materials and process selection and support design challenges throughout the supply chain. The use of high - performance fire - retardant thermoplastics for the design and fabrication of aircraft interiors has significantly increased over the past few years. 2 The driving factors for this trend have been more demanding and complicated part designs that provide aircraft interior designers with the ability to introduce the desirable level of ambience to an aircraft interior. More designers are choosing parts designed with thermoplastic materials due to their versatility in processing and fabrication and ability to meet demanding aesthetic requirements. Also, as design has advanced particularly for premium seating applications, more plastic and larger plastic parts are being used and the complexity, including the use of decorative laminates, undercuts, and even pressure forming, has increased. Thermoformed thermoplastic sheets are now being used in a large variety of applications, including seatback shells, armrest shells, tray shrouds, decorative trims, and so forth. The advantages of making these parts via thermoforming is the low initial cost (mold cost for complex shapes, setup and manufacturing time, energy costs) as well the ability to maintain a low cost through a program where the quantities for such parts could vary from a few parts to several thousand parts. Although versatility is associated with the use of thermoplastic components in the aircraft industry, these materials have to meet strict mandated FAA/FAR/OEM regulations for flammability and toxicity. The advantage of using thermoplastics (formability, cost, ease of processability, use of decoratives, recyclability, and ease of secondary operations) is being diminished by the required flammability properties of the plastic used. Depending on the chemistry of the material, as the flammability properties of a thermoplastic improve, its ability to be processed with ease may decrease CURRENT GOVERNMENT AND OEM SPECIFICATIONS FOR FLAMMABILITY Some of the current dominant specifications for components to meet commercial aircraft interior requirements include FAA/CAA/JAA smoke density and flammability testing FAR d and FAR a i & ii, respectively and must have OSU
106 96 Chapter 15 Applications in Aircraft and Mass Transportation heat - release rates below 65/65, as per d. In addition the major airframe manufactures have toxicity requirements that must be met. For Boeing, this is D and for Airbus, ABD FAR a, i and ii Components must meet the 60 - and 12 - second vertical burn requirements as per FAA/JAA regulation 14 CFR Part Appendix F. There are two tests used: i. The flame is applied for 60 seconds and then removed: Average burn length <6 inches Average flame time after removal of flame <15 seconds Drippings may not continue to burn longer than 3 seconds ii. The flame is applied for 12 seconds and then removed: Average burn length <8 inches Average flame time <15 seconds Drippings may not continue to burn more than 5 seconds FAR d Components must meet the OSU rate of heat release and the NBS smoke density test: Total heat release within first 2 minutes 65 kw per minute Peak heat release rate 65 kw per square meter 4.0 minute smoke density (Ds) Toxicity Governmental regulations do not have a toxicity component. However, the airframe manufacturers do have toxicity requirements, as shown in Table USE OF ACRYL/PVC In the early 1990s the company Kydex, LLC, responded to impeding regulations to meet the OSU rate of heat release requirements by developing an Acryl/PVC - sheet Table 15.1 Toxicity Requirements Boeing D : Toxic gas emission limits BSS Gas species CO HCN HF HCl SO2 NO X Maximum ppm ABD-0031: AITM Gas species CO HCN HF HCl SO2 NO X Maximum ppm
107 15.2 Use of Acryl/PVC 97 (Kydex 6565). This was the first commercially available thermoplastic sheet product that met all requirements; it was also formed on existing wooden and aluminium tooling at low thermoforming temperatures and at a reasonable price point. (At that time the only available products were exotic polymers that required high thermoforming temperatures on temperature - controlled cooling and were sold at much higher price points.) In addition, complex shapes and contours can be formed with Acryl/PVC, and the texture is retained. For composite structures such as laminated products, another variety of Acryl/PVC (Kydex 5555) was later developed with a lower inherent heat release rate (55/55) to meet final 65/65 heat release rate requirements. This allows designers to incorporate a wide range of laminated decorated film products inline during extrusion. Acryl/PVC materials such as Kydex 6565 and Kydex 5555 offer a balance between the cost/performance and the ability to meet flammability and toxicity requirements. 2 These types of Acryl/PVC products offer also low heat release, low smoke generation, and low toxic gas emissions. However, these two products meet only 95% of the toxicity requirements, with the only exception being HCl generation. While they do not fully comply with all toxicity requirements, they have been the ideal choice for airplane seat manufacturers and their customers because of their overall versatility, value proposition, and ability to meet aesthetic requirements (see Figure 15.1 ). These products have often been selected for use by seat manufacturers Figure 15.1 Business class seat made from Acryl/PVC (Courtesy of SE Kunststoffverarbeitung GmbH & Co. KG) 2 Technical white paper, Aircraft interior applications, Kydex, LLC, 2009.
108 98 Chapter 15 Applications in Aircraft and Mass Transportation in consultation with their airline customers, and their use has generally been through toxicity waivers. The airframe manufacturers recognize that customers want the properties and values that Kydex 5555 and Kydex 6565 deliver, but no longer want to accept waivers POLYCARBONATE Polycarbonate (PC) is one of the materials being used to fully meet toxicity levels in the aircraft industry. 3 The processing window of polycarbonate and the Ohio State University (OSU) 65/65 capability (like polyetherimide [PEI] resins), with extreme low - heat release material grades such as the Lexan XHR6000 sheet, have set a new course for safety compliance, aesthetics, and performance in interior aircraft applications Broad Compliance In addition to full flame/smoke/toxicity (FST) compliance, polycarbonate grades such as the Lexan XHR6000 sheet exceed the current OSU 65/65 heat release standard. It spares manufacturers and suppliers the time - consuming process of obtaining waivers for noncompliant materials and clears the way for emerging interior aircraft designs Outstanding Aesthetics Polycarbonate forms easily into deep draws, crisp angles, and thin walls, and retains its superb performance properties when draped or thermoformed into complex 3D shapes. In addition, its opacity provides excellent opportunities for molded - in colors drawn from a broad palette of high chroma, pastel, and bright whites Low Weight Material grades such as the Lexan XHR6000 sheet enables thinner walls to be formed that do not compromise dimensional stability or strength. The material is inherently lighter than other materials, offering a specific gravity of 1.34 versus 1.47 for OSU - compliant PVC/acrylic sheet systems, and enabling a 10% weight advantage without any gauge reduction Improved Processing and Part Design The polycarbonate Lexan XHR6000 sheet not only meets aircraft compliance requirements, it also has a inherently lower forming temperature than polyphenyl- 3 Higher Safety, Aesthetics and Performance, Extremely Low Heat Release Lexan XHR 6000 Sheet for Interior Aircraft Applications, SABIC Innovative Plastics, 2008.
109 15.3 Polycarbonate 99 sulfone (PPSU). That means there is improved texture retention and the use of lower cost tooling, which could translate into lower parts costs and enhanced productivity. Plus its robust smoke performance can help ease compliance testing for complex decorated parts that incorporate adhesives with films, fabrics, or leathers An Expanding Range of Applications As new aircraft designs introduce larger seating and sleeping areas, an increasing number of interior components will need to comply with the OSU heat release standard, which applies to parts larger than two square feet. Thus the spacious interiors and seating in emerging airframe designs could be added to the list of parts that must meet FST specifications. The superb aesthetics and thermoforming properties of polycarbonate could eliminate the use of paint, thus simplifying the supply chain and reducing production costs and weight. The list of potential applications is long, offering new design options for: Seating Cockpit panels Window shades Window surrounds Door shrouds Fuselage cladding Polycarbonate materials such as Lexan XHR6000 indeed hold much promise for interior applications in aircraft design Case Study 3 High Aesthetics, Simpler Processing 3 The problem : The high temperatures required to thermoform the polyphenylsulfone (PPSU) sheet limits aircraft component suppliers to using metal tooling for prototypes. Besides being very expensive and time - consuming to build, the tools need to be reworked or replaced if a part design is changed. Plus PPSU s high thermoforming temperature wash out texture patterns in the sheet, forcing the producer to instead build texture into the tooling. The solution : Use a polycarbonate (Lexan XHR6000) sheet that, besides complying with all relevant standards for FST and heat release, can be thermoformed at lower temperature than PPSU. The result : The lower temperatures required to thermoform polycarbonate (Lexan XHR6000) sheet enable less expensive tooling and shorter cycle times. This also allows the producer to take advantage of texture in the sheet instead of incurring the cost of texturing the mold. Polycarbonate sheets
110 100 Chapter 15 Applications in Aircraft and Mass Transportation improve aesthetics by enabling colors, including bright white, to be molded in to the part POLYETHERIMIDE (PEI) Tough amorphous polyetherimide (PEI) thermoplastic is already widely used in most of the major aircraft interiors. 4 PEI grades such as SABIC Innovative Plastics Ultem sheet products are based on the company s Ultem resin. A growing number of airline and rail OEMs are selecting PEI sheets for demanding interior applications due to PEI s flame, smoke, and toxicity compliance and tremendous strength, excellent aesthetics, and other high - performance benefits. Two grades, in particular, are making major inroads into this important industry segment: Ultem 1668A sheet (SABIC Innovative Plastics), a material developed for use in interior aircraft components. Ultem R 16SG29 sheet (SABIC Innovative Plastics), a new product designed for interior rail applications. Polyetherimide resin is an amorphous high - performance polymer that is characterized by excellent thermal properties, good chemical resistance, inherent flame retardancy, and exceptional dimensional stability. Flame, smoke, toxicity performance Best in class, with inherent flame retardancy and low smoke emission. Figure 15.2 Train sidewall cover made from PC (Courtesy of SE Kunststoffverarbeitung GmbH & Co. KG) 4 Safe and Sound, Ultem Sheet, High Performance Opaque Sheet for Aircraft and Train Interiors, SABIC Innovative Plastics, 2008.
111 15.4 Polyetherimide (PEI) 101 Chemical resistance Excellent resistance to a broad range of chemicals such as fully halogenated hydrocarbons, alcohols, and aqueous solutions and with easy cleanability. Light weight 15% lighter than PVC/PMMA and 3 to 6% lighter than PPSU. Cycle time Faster cooling allows up to three times faster thermoforming cycles than PVC. Colors Available in a wide array of colors. Heat stability HDT of 350 F (202 C) reduces warpage concerns due to long heat exposure. Toughness Excellent practical impact: Gardner >320 in-lbs (36 J) PEI Sheets for Aircraft and Passenger Train Interiors 4 Aircraft PEI sheets such as the Ultem 1668A sheet offer to the industry an inherent flame resistance with low smoke emission. They meet all current commercial aircraft interior requirements, including an OSU heat - release rate below 65/65, FAA smoke and flammability testing, and an FRA vertical burn criteria, and comply with toxicity standards BSS7239 and ABD0031. The Ultem 1668A sheet also offers aircraft OEMs exceptional impact and heat resistance, modulus and chemical resistance in combination with light weight, exceptional strength, and good surface aesthetics. The product can be thermoformed, pressure formed, twin - sheet formed, or used in flat- or cold-formed applications. The Ultem 1668A sheet is paintable or available from SABIC Innovative Plastics in a range of colors, finding use in various interior aircraft applications, including passenger service units, seating and flight deck components, galleys, stow bins, and sidewalls. Passenger Trains PEI sheet grades such as Ultem R16SG29 are a growing material of choice in train window masks, cladding, walls, seating, and other interior parts due to its design flexibility in three - dimensional shapes, outstanding mechanical properties, and flame, smoke, and toxicity capabilities. Especially important for this sector is this product s excellent cleanability and chemical resistance. It meets US FRA 49 CFR Part 238 flammability and smoke emissions standards for train passenger cars and locomotive cabs and complies with toxicity standard Bombardier SMP 800C. It also meets Germany s DIN5510, Part 2 (S4/SR2/ST2) ratings and is compliant with French standards NF P /5 and NF F (M1, F1). Ultem R16SG29 sheets offer high - performance characteristics for the interiors of passenger trains. This SABIC product can in fact be formed to cover the entire interior of a train car from floor to ceiling. The first train with an Ultem R16SG29 sheet interior,
112 102 Chapter 15 Applications in Aircraft and Mass Transportation formed in 3 - mm thickness, met not only Siemens s demand for exceptional cleanability, durability, and vandal resistance but also the required flame, smoke, and toxicity requirements of the rail industry. The Ultem sheet gives formed parts lighter weight and consistent color, unlike traditional materials such as metal and PVC blends. As a result it is making significant gains, displacing metal, fiber - reinforced plastic (FRP), and sheet - molding compound (SMC) in several application areas POLYPHENYLSULFONE (PPSU) PPSU is a material that is also used for aircraft interiors (see Figure 15.3 ). It is fully compliant, but due to its relatively high density there is a tendency to exchange PPSU gradually with other types of PC, for example, Lexan XHR6000. Table 15.2 presents comparisons of various polymers regarding flame, smoke, toxicity, and heat resistance. Figure 15.3 Seat back cover made from PPSU (Courtesy of SE Kunststoffverarbeitung GmbH & Co. KG) Table 15.2 Material Properties Material Flame Smoke Toxicity Heat Resistance Acryl/PVC x x PC x x x Lexan XHR6000 x x x x PPSU x x x x
113 Chapter 16 High-Quality and Fully Transparent Products (Sheet Machines) Written in Cooperation with Manfred Geiss, Geiss AG, Sesslach, Germany There are areas of application where the surface quality of thermoformed parts must meet very high standards. These challenges are presented when working with pigmented products, for example, in the sanitary area. Even parts for in - mold - decorations need a flawless surface. Class - A surfaces are so called because these surfaces need to hold up to high optical criteria. Class - A formed parts may be self - supporting or reinforced on the back side, called thin Class - A formed parts. Thermoformed parts, which are crystal - clear, need of course a visually flawless surface. For example, skylights, windshields for cars or motor bikes, protective covers, or cockpits must have a high surface quality. The materials used for visually immaculate products are PMMA, PC, PET, and coextruded PMMA/ABS THICK AND SELF -SUPPORTING CLASS -A FORMED PARTS The method of forming thick, self - supporting Class - A parts is being advanced in the United States, in particular, for use in vehicles with great surface areas and when small quantities are being produced. Already vehicles exist that are entirely cased in plastic material. A special polypropylene or coextruded material is used, and the formed components do not need cleanroom equipment because dust particles and small imperfections will not be visible. Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 103
114 104 Chapter 16 High-Quality and Fully Transparent Products (Sheet Machines) Figure 16.1 Sample product untrimmed: keyboard for play console (Courtesy of Geiss AG) 16.2 CLASS-A MOLDED PARTS FOR IN -MOLD DECORATION In - mold decorations are used for interior and exterior parts in the automotive industry. They are formed from film that is 0.17 mm to 0.8 mm thick. Preprinted films require quartz radiator or spedium lamps. It is imperative that the positioning of the film is highly accurate, which requires positioning holes and a special handing over the machines. Polycarbonate is used for thin - walled applications. These applications need extra attention regarding the positioning accuracy for formed parts in the mold, the tools used for postprocessing, contortion of the print, the absolute reproduction of the distorted print, and the postprocessing DEVELOPMENT OF FULLY TRANSPARENT PRODUCTS It is possible to produce entirely transparent formed components by the thermoforming method. A combination of dust - free rooms, a special mold surface, and vacuum pressure control allows fully transparent articles to be producted. In the mold design and construction for fully transparent components, the skeletal mold has to have a different surface. Depending on the product s use, a polished, special smooth, or a blasted surface may be needed Material Using a good - quality, consistent sheet is key to getting thermoformed body parts using paint film. A small difference in sheet quality makes a big difference in the waviness tendency of the finished part. The incoming sheet quality has to be con-
115 16.3 Development of Fully Transparent Products 105 trolled. This is very critical for the process. The only way to reach high - quality targets is to start with a good sheet (see Figure 16.1 ) Creation of the Environment The manufacture of visually perfectly formed parts requires a purified environment. The machine ought to be of stainless steel to avoid contamination by rust particles. The machine should be cleaned before use and the production hall should to be kept clean.
116 Chapter 17 Deco Molding and Multi-deco Molding Written in Cooperation with Klaus Wlasak and Marcus Schuck, Jacob Plastics GmbH, Wilhelmsdorf, Germany Deco molding is a special technology consisting of primary forming processes, for example, thermoforming and injection molding, to create unique formed parts. The objective is to create surfaces that are highly decorated and pleasing to the eye for component parts with extreme 3D shapes and almost limitless geometry. Through the forming of the film even complex geometries with decorations can be implemented to the rear side of the component parts (edge folding). A typical process combines the forming of a film in order to create an insert, as well as the following cut in order to obtain the final contour by means of a separate working process with the injection molding process. So - called inserts, which are three - dimensionally formed, are inserted into the injection molding tool and processed with back - injection molding. The semifinished product is a film that is formed by means of the thermoforming process, printed, and subsequently cut to the desired dimensions. The three - dimensionally formed semifinished part with the final contour is called an insert. The injection molding process must guarantee the adaptation of the film to a basic part, for example, a car dashboard. The back - injection molded material represents the material connection to the insert, which guarantees a rigid structure and a positive fitting or force - fitting connection to the basic part. The main areas of application are the automobile and the entertainment industries. Depending on the utilized pre - forming process (thermoforming or high - pressure forming), even company logos can be applied, accurately fitted, to the injection molded part. The deco - molding process allows much design freedom and flexibility. High color depths, color diversity, symbols, and transmitted light techniques can be imple- Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 106
117 17.2 Injection Molding 107 mented simultaneously through the application of adjusted film systems abrasion resistance. With deco molding it is also possible to change the decoration for each filling, which means that this method is thoroughly flexible. A special type of the deco molding is multi - deco molding. In multi - deco molding a combination of several films is applied. Multi - deco molding basically consists of two process steps: Themoforming Injection molding 17.1 THERMOFORMING First, the film is thermoformed and subsequently trimmed in a cutting process. There are different cutting processes for the trimming. The three - dimensional formed part must be exactly cut in the forming station. In general, it is very important that the punching rim at the edges of the finished insert be as small as possible or that there be even no punching rim at all. This is because the film is to be clamped in the injection molding tooling, so then during the back - injection molding process the rims of the component part would be inexact. If the rim is cut too narrow, there would be flooding due to the spilling of the injection molding material into these areas. Basically, there are three ways to make the cut. The usual, and cost - effective, cutting process with high output is punching. Here the inserts are separated from the superfluous film by means of punching tools made of steel. However, punching cannot be used to create complex geometries. If complex three - dimensional contours (likely with undercut) are desired, a method with a higher flexibility than punching must be utilized. One such method is machining the molded article with a six - axis trimming machine and a suitable trimming tool. The disadvantages of this method are, among others, that chip formation can lead to contamination during the subsequent process steps and that the brittleness of the machined plastics can cause uneven cutting of the contour. Cutting by laser can ensure high flexibility during processing, but the intense heat generated by the laser can cause local melt. In addition, there can be discoloration of the film from the intense heat. Both methods entail high initial costs and possibly long cyclic times. Besides the design freedom of implementing traverse paths, the main advantage is high flexibility. Changes to the cutting contour can be quickly adapted by means of the production program. For the deco - molding process, punching and/or laser cutting is used INJECTION MOLDING The second process step is injection molding. In order to provide the thermoformed and cut film insert with the necessary stability, or in order to enable the adaptation to another component part, in the last step the insert will be assembled to a complex composite part by means of the injection molding procedure. The insert is placed
118 108 Chapter 17 Deco Molding and Multi-deco Molding into an injection molding tool, having nearly the final contours of the finished part, and subsequently back - injection molded with a compatible plastic. There are several ways to place the film into the tooling. The insert could be fixed and centered into the tooling by its own geometry (apertures, position in the tooling), or the insert could be fixed with mechanic feeders, vacuum, or electrostatic charge into the tooling. For the electrostatic charge the proven procedure is to charge the film only after its placement into the tooling. Thus no dirt or dust from the environment is drawn, which can lead to high reject rates for damageable surfaces, for example, piano lacquer optics. Furthermore, it is advisable to clean the inserts immediately before their placement into the tooling. Usually this is done with brushes or through air blowing. Also in this case the kind of film material and component part geometry that was used is important. It is often difficult to clean complex three - dimensional forms with brushes. An automation of the production and the manufacturing in a cleanroom with grade 10,000 makes cost - effective and efficient production possible. Manual labor, which is performed under normal environmental conditions, can lead to surface imperfections and an increased reject rate of the finished component parts due to dust and cut particles; injection molding faults can result from inexactly positioned inserts. Depending on the application, further manufacturing steps, such as sprue removal, control, fixation of clips/buffers, or coating are carried out afterward. Many other factors influence the quality of the surface: Number, positioning, and width of the injection points Volume flow rate through the sprue bush Melt temperature Cavity pressure for the filling of the molded part Polish of the injection mold tooling Fitting accuracy of the insert respective to the tooling Cleanliness of the environment Positioning accuracy The following examples illustrate developments in deco molding and multi - deco - molding methods. Since 1996 in Europe developments in deco molding have been significantly influenced by the Jacob Plastics company Door Handles In the United States, deco molding has been used since In Europe, vehicle interiors of cars such as roadsters were primarily decorated with films. The experiences collected in these applications ultimately led to the development of multi - deco molding (Figure 17.1 ). For automobile component parts an ABS was used as the carrier material in order to guarantee a sufficient compatibility with the material that was back - injection molded, namely, a PC/ABS. This compatibility allows for the substance -
119 17.2 Injection Molding 109 Figure 17.1 Door handle (Courtesy of Jacob Plastics GmbH) Figure 17.2 Various component parts (Courtesy Jacob Plastics GmbH) to-substance bonds of the film to the carrier material. The ductility and small chip disposition, something that is very important for the passenger compartment, was the reason for the carrier to be manufactured out of PC/ABS. The component parts were thermoformed and subsequently separated by means of a punching process, and thus the final geometry was achieved. In detail these component parts comprise the right and left cover plates of the door handle, the light turn - switch including the frame of the ventilation nozzle, and the ventilation nozzle itself. The visual appearance was made to resemble a carbon surface. The production of thin bars ( <5 mm) posed a challenge for shape accuracy of the film, as illustrated in Figure The
120 110 Chapter 17 Deco Molding and Multi-deco Molding Figure 17.3 Cover plates of electric window lifts, one with wood grain finish (Courtesy of Jacob Plastics GmbH) Figure 17.4 Back injection molded cover plate (Courtesy of Jacob Plastics GmbH) final shape was obtained with accuracy by taking into account the mold shrinkage and the distortion of the film during, and subsequent to, the thermoforming process. In a further production step the symbol indicating the light options was imprinted. By the same deco - molding means two further component parts from the automotive sector could be realized to the satisfaction of the automobile industry. As illustrated in Figures 17.3 and 17.4, the cover plates of the electric window lift in the area of the door handle rail could also be developed using deco - molding technology. The printed ABS film was, first of all, thermoformed, punched, and subsequently back - injection molded with PC/ABS. The used d é cors were applied in wood effect and silver to the ABS film. As it can be seen from Figures 17.3 and 17.4, a
121 17.2 Injection Molding 111 Figure 17.5 Tripartite dashboard (Courtesy of Jacob Plastics GmbH) special feature was the partial decoration of the film. This means that the component part is not decorated over its entire surface with the film but only partially. Thus it was possible to have a specific creative highlight in the area of the window opening lever. The positioning accuracy makes great demands for the definition and the cut of the insert as well as for the handling of the film and its positioning into the injection molding tooling. Through the correct cut, the desired seamless transition of the dé cor between insert and door handle can be achieved The Tripartite Dashboard Subsequent to its launching onto the European market, deco - molding technology is being utilized for all model segments. In 2000 an entire car dashboard was manufactured for the Rover 75 in two different d é cors (wood grain effect and silver). This large - area application had to be separated in three parts: instrument cluster, air bag cover plate, and air vent (Figure 17.5 ). The component parts were first thermoformed and then punched and back - injection molded. The combination of ABS (film) and PC/ABS (back - injection molding material) was used for the already mentioned reasons. The component parts were subsequently mounted onto an aluminium carrier by a hot stamping process. The characteristic of this component part was the important potential savings compared with the use of authentic materials. The challenge was to align exactly all the parts in the total width of 901 mm. In order to ensure this alignment, the assembly of the aluminium carriers had to be precise and also the film had to be even with seamless transitions between the three component parts. As may be seen in this example from the year 2000, the deco - molding technology had already allowed a lot of freedom of design. The two other component parts of the dashboard, the instrument board and the airbag cover, were decorated with film, as shown in Figure As mentioned above, the material used for the instrument board was an ABS film that was back - injection molded with PC/ABS. For the airbag cover, a TPO film was thermoformed and back - injection molded with PP. PP was used due to its better performance regarding head impact tests, and its low ductility and brittleness. The raised lettering SRS Airbag and PT Cruiser were created by means of
122 112 Chapter 17 Deco Molding and Multi-deco Molding Figure 17.6 Instrument board and the airbag cover (Courtesy of Jacob Plastics GmbH) Figure 17.7 Instrument board (Courtesy of Jacob Plastics GmbH) back - injection molding for a tactile effect (Figure 17.6 ). Subsequently, the lettering PT Cruiser was embossed with chrome film. The entire d é cor has eight colors Instrument Board In 2001, there were more applications of the film to create attractive design elements. In that year a total of five different component parts for the instrument board were designed and manufactured. Figure 17.7 shows the three component parts of the instrument board: the right and left frame of the fan nozzle, the airbag cover, and central instrument panel steering wheel cover. Their production was by the classical manufacturing process, with the film first being thermoformed and subsequently punched. The material combination used was ABS (film) and PC/ABS (back - injection material). Altogether, eight decorative devices were created in six colors that reflect the outer lacquered finish
123 17.3 Tactile Effects 113 Figure 17.8 Variety of the utilized films (Courtesy of Jacob Plastics GmbH) of the vehicle. The challenge was to match the film colors used in the interior to the outer lacquered colors (see Figure 17.8 ) Radio Bezel and Gear Shift Cover In 2002, two more component parts were manufactured using film technology: the radio bezel and the gear shift cover. Figure 17.9 shows one version of the many different designs used on these parts. The same as for the other mentioned products, a printed ABS film was thermoformed, punched, and subsequently, in a separate production step, back - injection molded with PC/ABS in order to obtain the finished part. All in all three different wood grain effects were accomplished. These effects required very complex punching geometries with more than 12 cutouts that had to be exactly adjusted. So thermoform films of sufficient quality have to be the pre - condition for such precise punching TACTILE EFFECTS By 2005 requirements increased regarding decorative component parts. Automobile manufacturers demanded decorations with more depth, fixation, and covering the adjacent component parts. For the first time separation by laser technology was implemented for the designed and manufactured component parts (right and left door handle, U - shape of the center console, Figures and ). The designer could make undercuts in the ABS film that could not be made by punching. The laser was linked to a robot with 5 degrees of freedom, and this facilitated an exact separation
124 114 Chapter 17 Deco Molding and Multi-deco Molding Figure 17.9 Radio bezel and the gear shift cover (Courtesy of Jacob Plastics GmbH) Figure Door handle with haptic impression due to a black square film (Courtesy of Jacob Plastics GmbH) of the films. Additionally, with the use of the laser there was less contamination of the production cell, as flying chip particles would be generated if the parts were milled. When the parts are back - injection molded with PC/ABS, these chip particles can increase the number of rejects due to inclusions and/or indentations. The parts were decorated with chrome brushed black square films. The black square film was
125 17.5 Multi-deco Molding 115 Figure Right and left door handle, U - shape of the center console (Courtesy of Jacob Plastics GmbH) screen printed with a pattern of black squares. Subsequent to the thermoforming and back - injection molding, these squares impart tactility to the design OTHER SECTOR PARTS An application that was not destined for the automotive sector was a bipartite set for a vacuum cleaner that was produced in The material combination was also ABS (film) and PC/ABS (back - injection molding material). For a custom - made product with a Porsche design, a light tonal brushed film was used for the decoration. The special feature was the thin bars of the ventilation grille, which had to have an approximate distance of 2 mm. Thus a high positioning accuracy of the film parts, as well as for the punching process, was necessary. Additionally, lettering was created by a hot embossing method MULTI-DECO MOLDING Today, with multi - deco molding it is possible to produce entire large component parts with differing surfaces by back - injection molding several films that have different motifs or textures. The pre - condition is, of course, good formability and high - dimensional accuracy of the films. The form of the films is created by thermoforming and a subsequent laser cut. The multi - deco molding method was developed and patented by the company Jacob Plastics for the manufacture of large - scale applications in deco - molding technology in the automotive industry. Covers for the center console are created by combining several high - gloss films by injection molding. The car buyer can choose between several trim lines with different interior decoration. Besides the
126 116 Chapter 17 Deco Molding and Multi-deco Molding significantly improved appearance, compared with the conventionally lacquered parts process, automation technology requires only a small space for the machines. The automated multi - deco method makes it possible to perfectly combine textured and partly multi - colored surfaces. The present challenge is to position three differently patterned films for the cover of the center console and to combine these by means of the back - injection molding method to one component part. The shape of the insert is defined by thermoforming an ABS film with a corresponding pattern. For the positioning of the films in the tool as well as the absolute position in the injection molding tool, the definition and thus the control of the processing parameters is important. Laser cutting is used instead of punching to make the necessary undercuts and create complex three - dimensional geometries. The insert set of the center console cover, the so - called trim cover center, of a car consists of a center part as well as two lateral parts. For some trim lines this center console cover is designed with different textures and partly also with contrasting colors. While dashboard covers are often directly manufactured as injection - molded parts, sometimes they are subsequently lacquered. However, when the parts are lacquered, it is not possible to attain the demanded quality levels because, despite masking, there are always some flaws in form of color defects at the transition in color. For some vehicles the visual effects must be so exacting that they can be accomplished only with back - injection molded films. For production using the back - injection molding method, this means that the films must be exactly positioned so that a single faultless part with defined clearances is created. In the above - mentioned example a number of separate d é cors were integrated into a narrow distance, and the result was a perfect visual and tactile design. In the end a single large component part had to be assembled from separate small parts THE AUTOMATED SEQUENCE PROCESS The cycle time of the whole automated process takes 75 seconds. The sequence process consists of the following steps: 1. Manual cleaning of the inserts and placement into the magazine. 2. Unloading of the inserts by robot Positioning of the inserts into the centering station and centering. 4. Take-over of the inserts by robot Cleaning of the inserts. 6. Introduction of the inserts into an injection molding device and back - injection molding of the inserts. 7. Unloading of the finished component part and removal of injection molding residues. 8. Positioning of the component part in the intermediate station and subsequent application of clips and rubber buffers. 9. Placement of the finished component part onto the transport belt by robot 2.
127 17.6 The Automated Sequence Process 117 The delivered and pre - formed films are, after the manual cleaning, placed into a double magazine that is accessible from the outside of the robot cell, which functions as a cleanroom. A six - axis articulated robot whose gripper is equipped with three pivotable tools for individual films, film pack, and pre - fabricated part is located in this cell. Because of the heavy weight of the gripper head, a robot with a corresponding load - bearing capacity is used. Via underpressure the robot takes at the same time the three films that must be combined from the magazine and places them into the centering device. In the next step the films are centered in the centering device. In the meantime the robot has turned its tooling to the subsequent position in order to take the exactly positioned films the same way that they will be back - injection molded in the injection molding machine. Now an upstream brush chain again cleans the surface because even the smallest contamination of the upper side of the film can lead to faults and an imperfect finish, especially from the high pressure exerted in the injection molding machine. When the injection molding machine opens, the robot takes the already sprayed part out of the form with its third tool. Now the films that were picked up are placed into the form and exactly kept in position via electrostatic charging until the machine closes and the injection molding process begins. Subsequent to the extraction, the robot transfers the pre - fabricated part to a turning/sprue bush/cutting station. This station also serves as an additional robot axis because the part is turned through 180 and passed on to a second articulated robot. In this station the robot takes a metal clip and a rubber buffer at a time from an infeed/separating station, with help of a combi - gripper, and assembles them at the rear side of the center console. In total seven clips and seven rubber buffers are installed that were separated previously in a separating device and transported correctly positioned to the transfer position. The clips are necessary for the later installation in the vehicle, and the rubber buffers impede noises and rattling, as thus the pre - fabricated part is mounted with a certain tension. In the last step the robot places the finished part onto a conveyor belt with its gripper. On this belt the part is transported to final examination and subsequent packaging. Multi - deco molding was developed in order to manufacture, in a flexible production process, d é cor component parts with inserts. For this the injection molded parts are combined to form one entity with the film and/or a real metal film, leather, or real wood. Thus the subsequent assembly at the vehicle manufacturer is simplified and a finish with exact clearance is obtained (Figures and ).
128 118 Chapter 17 Deco Molding and Multi-deco Molding Figure Robot-manufacturing cell (Courtesy of Jacob Plastics GmbH) Figure Trim cover center (Courtesy of Jacob Plastics GmbH)
129 Chapter 18 Automotive Body Parts Made of PA + ABS Written in cooperation with Thorsten Eymael and Nina Schick, SE Kunststoffverarbeitung GmbH & Co. KG, Germany Thermoforming can be used to produce body parts for military airborne vehicles because of certain critical properties of PA + ABS blends. These properties are, among other things: Excellent impact strength (toughness) Matt effect with grained surfaces High heat resistance under low load Good resistance to chemicals and stress cracking Good surface slip and abrasion behavior Noise damping acoustics High fatigue resistance Paintability In blends such as PA + ABS, the preferred properties of the semicrystalline polyamide and the preferred properties of ABS are combined. Properties of Polyamide Good resistance to stress cracking and chemicals High heat resistance High dynamic strength Good abrasion and wear resistance Very good flowability Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 119
130 120 Chapter 18 Automotive Body Parts Made of PA + ABS Figure 18.1 Wheel arch made of PA + ABS (Courtesy of SE-Kunststoffverarbeitung GmbH & Co. KG) Good antistatic behavior Properties of ABS High toughness Low-temperature impact resistant High E-modulus up to 100 C High dimensional stability Figure 18.1 shows an example of an applied PA + ABS part type, Triax 1220S from Ineos ABS.
131 Chapter 19 Softfeel Made from ABS/ TPU Material To distance themselves from the competition, commercial vehicle manufacturers are looking for materials that offer more user comfort. 1 At the same time, the appearance of the driver cabin area must show increased value - effect. Leather - like feel and matt surfaces are therefore in demand. To achieve this, thermoformed parts are mostly painted using a soft - touch paint. Disadvantages of painting are as follows: High costs Low scratch and abrasion resistance High emissions of volatile organic compounds (VOCs) Solutions offered by using acrylonitrile butadiene styrene (ABS)/thermoplastic polyurethane (TPU) are the following: Coextrusion of a matt TPU top layer over a base layer sheet of ABS achieves a matt, leatherlike feel. No painting of the sheet is required. These advantages are also retained after thermoforming. Products have the following advantages: No painting of sheet required High matt surface level Leatherlike feel High scratch and abrasion resistance Wide color range and color consistency 1 Produktprospekt Senosan A50EG Softfeel Matt, Senoplast Klepsch & Co. GmbH, Piesendorf, Österreich Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 121
132 122 Chapter 19 Softfeel Made from ABS/TPU Material Meets fire regulation standards VOC limit values achieved At the end of the 1990s, to meet the high optical and mechanical requirements for innovative plastic surfaces in car interiors, the development of a leather soft surface was begun. 2 Potential markets such as the commercial - vehicle industry and caravan industry were explored, as well as the automotive industry, buses, and contract thermoformers. The goal was to develop a thermoplastic sheet of semifinished product with a surface that had a soft touch or feel. A leather look and deep mattness but also high scratch resistance and good chemical resistance were included in the product requirement profile. A further surface aspect for system parts was a constant deep mattness after thermoforming with differing sheet thicknesses and thermoforming temperatures. Extensive development work was required to create an ABS/TPU coextruded sheet. Some applications in which ABS/TPU, for instance, Senosan A50 EG Softfeel, is used are dashboards of micro cars, consoles in mobile home interiors, and pillar cladding in commercial - vehicle interiors. In the course of ongoing product development by Senoplast Klepsch & Co. GmbH, the mattness of the Softfeel surface could be significantly improved again according to the demands of the market. There is also a super matt grade, which was introduced to customers in Furthermore, there are ongoing development activities to improve the weather resistance of Softfeel surfaces. These super matt ABS/TPU sheets are used for high quality interior parts such as dashboards and door and side panel cladding in buses, tractors, construction vehicles, trucks, and other vehicles. 3 Subsequent to thermoforming, these parts can be CNC trimmed and then mechanically fixed, adhesively bonded, or reinforced on the back by using PUR foam or other technologies. These thermoformed parts offer an increased comfort due to the leatherlike feel and an increased quality appearance due to the high mattness level. These parts also offer cost advantages compared with painted soft - touch parts. All material trimmed off during thermoforming can be completely recycled. One application of Softfeel is as a cover for a microwave oven in a truck cabin, as shown in Figure Softfeel and soft - touch applications can also be used for buses, where the characteristics of ABS/TPU contribute to increased passenger security. Due to their characteristics and manufacturing process, such parts not only have the potential to present a cost - effective and high quality alternative, but they also win awards. For example, the bus part shown in Figure 19.2 won the SPE Automotive Award, Parts & Components 2006, Third Prize for Body Interior rear dome. 2 Wilhelm Klepsch, Kompetenz in Kunststoff, p. 74, Esperanza Holding, Piesendorf, Österreich, Produktprospekt Senosan A50EG Softfeel Matt, Senoplast Klepsch & Co. GmbH, Piesendorf, Österreich, 2009.
133 Chapter 19 Softfeel Made from ABS/TPU Material 123 Figure 19.1 Cover for microwave oven. (Courtesy of Senoplast Klepsch & Co. GmbH) Figure 19.2 Rear dome of a bus (Courtesy of SE Kunststoffverarbeitung GmbH & Co. KG)
134 Chapter 20 Introduction to Packaging Thermoforming is a cost - effective method for the production of packaging. Over the years different thermoforming alternatives for the packaging sector were developed. There is a differentiation between the manufacturing of packaging materials and the manufacturing of the complete packaging subsequent to the production of the item that is to be packaged. In the packaging sector mostly semifinished products in the form of films are used. These films are either delivered as rolls or produced directly upstream of the thermoforming machine through extrusion. There are several machine types. The following items, among others, are produced with the thermoforming method: Drinking cups Yogurt cups Delicatessen cups Lids Flower pots Blisters The performance and the output of thermoform machines has proved to be superior to machines using other methods. Some packaging applications are described in the following chapters. Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 124
135 Chapter 21 Optimizing a Thermoforming Process for Packaging Written in cooperation with Rudi Salmang, Terneuzen, The Netherlands Thermoforming is achieved by heating and stretching a polymeric film/sheet until it duplicates the surface of a mold. Stretching may be achieved by means of a mechanical plug or by means of air pressure or vacuum, or combinations thereof. Evaluating the performance of different resins in thermoforming processes has been very difficult and sometimes subjective due to the nature of the process itself; that is, isolating the results and main effect of each step of the process is very difficult. In a plug - assisted thermoforming process, typically used in producing deep draw articles, the film is stretched initially by a plug, which may provide up to 90% of the total volume deformation, and then air pressure (or vacuum) generates the last 10% or more of the required deformation, until the film touches the mold walls and cools. The stretching of the film begins with the plug contacting the film and pushing it into the mold cavity. The film sticks to the plug in the initial place of contact while the remaining noncontacting film is stretched. It should be noted that plug temperature has a great influence on this process, and although plug temperature is not typically measured, it must reach a level of equilibrium to obtain consistency in the final articles. Cooling of the film occurs as a result of increasing the surface area and reducing the thickness while stretching. As a result of cooling, the melt strength of the resin increases to a point where the friction force between the plug surface and the film is overridden by the melt strength and the film begins to slide over the plug. This marks a transition point from friction dragging to slippage. The friction force is also affected, as expected, by the normal force on the contacting surface, and hence influenced by the air pressure in the mold cavity. Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 125
136 126 Chapter 21 Optimizing a Thermoforming Process for Packaging In a blow - stretch thermoforming process, the film is stretched first by means of air pressure (positive, vacuum, or combinations thereof) up to over 100% if required, and then allowed to retract into a mold that has been driven into the bubble, i.e., blown film. The film is stretched by air differential pressure, and then contacts the mold in a few confined areas (edges) during the end of its travel stroke. Simulations of this process are quite precise but do not allow conclusive evaluations to be drawn as could be used to totally predict the thermoforming performance of different resins. Specifically, a method for measuring mechanical behavior of polymers in a simulated thermoforming process is suggested by Bernhard Hegemann of the University of Stuttgart, in Improving Our Industry through Technical Developments: The Next Step, a European program sponsored by the EEC presented at many thermoforming events. However, this method is a simulated thermoforming process and thus does not consider all the parameters that influence the performance of the material being thermoformed METHOD FOR OPTIMIZING A PROCESS TO PRODUCE A THERMOFORMED ARTICLE FROM POLYMERIC MATERIAL For the polymeric material used to produce the thermoformed article, obtain at least one profile for one or more thermoforming process parameter(s) using plug force and/or cavity pressure. Next, evaluate the wall thickness of the thermoformed article produced from the different process parameters utilized in the profile(s). The optimum profile(s) results in the desired wall thickness for the polymeric material used to produce the thermoformed article. Thermoforming using the optimum profile(s) ensures that the desired wall thickness is obtained CHARACTERIZATION OF RESINS BY PERFORMANCE PARAMETERS Any thermoplastic polymer that can be thermoformed can be used, including monovinylidene aromatic resins such as polystyrene; rubber - modified monovinylidene aromatic resins such as high impact polystyrene; monovinylidene aromatic copolymer resins such as acrylonitrile/butadiene/styrene copolymers; polyethylene terephthalate, polycarbonate, polyurethanes, nylons, polyolefins such as polyethylene, polypropylene; and thermoplastic foams. In the first step of the thermoforming process, the extruded film is heated to a temperature that is the optimum thermoforming temperature of the thermoplastic polymer being utilized in the process of the present study. This is typically achieved by indexing the extruded film, or introducing it into an oven, while moving the film through the oven while gradually heating it to the desired temperature. The temperature of the extruded film can then be measured by any suitable temperature sensing device, such as an infrared temperature sensing device. The film temperature is subsequently monitored, measured, and recorded. The measurements
137 21.2 Characterization of Resins by Performance Parameters 127 taken throughout the thermoforming process are recorded for easy retrieval at a later time. This can be done manually or by a data acquisition system such as a computerized or automated system in combination with a mechanism that controls the parameters of the thermoforming process. The data are then evaluated, and the process parameters or resin is adjusted in order to optimize the thermoformed article produced. The data may be evaluated manually or by a computerized system programmed to evaluate the data and make appropriate changes to optimize the thermoforming process. The finished articles resulting from the interaction, measurement, and control of the variables above exhibit an optimum thickness distribution and optimum resin characteristics, which greatly enhances the performance of the finished article. In this process there are many thermoforming process parameters that influence the quality of the thermoformed article. It has been discovered that the plug force and/or cavity pressure are critical for the optimization. The first step of the present process is to obtain at least one profile for one or more thermoforming process parameter(s) selected from the plug force and/or the cavity pressure for the polymeric material used to produce the thermoformed article. A profile is defined as the relationship between the measured values over time. For example, a plug force profile for a specific material is the measurement of the force transmitted through the plug over the time of one thermoforming cycle to produce one thermoformed article. Additionally, a cavity pressure profile for a specific material is the measurement of the cavity pressure over the time of one thermoforming cycle to produce one thermoformed article. In plug - assisted thermoforming processes, the plug temperature and the force of the heated film on the plug are also monitored, measured, and recorded. Measurement of the plug temperature can be achieved by any suitable temperature sensing device such as a thermocouple embedded inside the plug. The force of the heated film on the plug is the force that the film places on the plug, as the plug pushes the heated film into the mold cavity. The force of the heated film on the plug can be measured by any suitable force/ gauge measuring device, such as a load cell located at the base of the plug, in between the plug and its base. In one embodiment, this can be achieved by utilizing a load cell attached to the plug stem, thus transmitting all the force required by the plug during its stroke, and measuring the said force at the same time. A fast data acquisition system provides all the process parameters and values to be linked directly to the measured force. Melt strength values can be obtained during the whole process cycle for the resin being tested, and hence the friction to slippage transition point can be accurately measured. Furthermore the resulting thickness distribution is physically measured in the formed part to relate it to the process and resin variables. The resins can be characterized via this apparatus by generating processing windows with the above - mentioned output information. During the thermoforming process, cavity pressure is produced by the influx of polymer film into the mold cavity. The cavity pressure can be measured by any suitable pressure sensing device such as a pressure transducer located at the bottom
138 128 Chapter 21 Optimizing a Thermoforming Process for Packaging of the mold cavity. This cavity pressure is also monitored, measured, and recorded into a data acquisition system as described previously. The profile(s) can be obtained from the plug force alone, the cavity pressure alone, or a combination of both, in determining the optimum conditions and parameters for the thermoforming process. Typically, the plug force is used in thermoforming processes that utilize a plug. However, for processes that do not utilize a plug, such as blow - stretch thermoforming, the cavity pressure profile would be used. In some plug - assisted thermoforming processes, it is beneficial to use both types of profiles to determine the optimum conditions and parameters for the thermoforming process. Once the profile(s) has been obtained, the resultant thermoformed articles produced during the profile runs are evaluated. The articles are evaluated for different quality related properties such as the uniformity of wall thickness. From this evaluation the article having the most desirable physical properties and characteristics is selected and thus the corresponding profile produced is determined to be the optimum profile for the specific articles to be produced. Once the optimum profile(s) has been determined, the thermoforming process is modified, if necessary, in order to perform within the optimum profile(s). The modifications can be accomplished in a number of ways. There are many different process parameters to be considered in thermoforming; however, all can be analyzed by the way the film is initially stretched, and by the different transitions during the process, until the formed part is cooled. Again, the critical parameters selected for the optimization of the thermoforming process are plug force and/or cavity pressure. These parameters can be altered by a number of different variables within the thermoforming process, as is known by those skilled in the art VARIABLES THAT CAN BE ALTERED TO INFLUENCE THE PLUG FORCE AND CAVITY PRESSURE Machine Variables Plug speed. A greater plug speed will increase the plug force. Air pressure differential between the two sides of the fi lm during thermoforming. This is the difference between the cavity pressure and the combination of atmospheric pressure and form air (the air exerted on the plug side of the film to aid in forcing the film into the mold). Thus the cavity pressure can be modified by the amount of venting within the system (e.g., vent holes or vacuum bleed) and by the amount of form air utilized in the process. The resulting force on the plug may increase or decrease depending on the air pressure differential and the moment it is applied or exerted. Film temperature. The greater the film temperature, the lower the plug force. Timing, intensity, and duration of cycle elements. Included are heating the film, clamping and force of clamping the film, stretching the film, rate of
139 21.4 Application Examples 129 evacuation of air during stretching, form air introduction, cooling, ejection air introduction, and opening the tool. For example, introducing form air somewhat earlier will increase the amount of cavity pressure. As said before, this increase in cavity pressure may result in an increase in plug force. Yet an earlier vacuum (rate of evacuation of air) combined with an increased plug speed may result in a decrease in plug force. Mold/Plug Variables Geometrical design of the plug. This includes the draft angle, surface roughness, shoulders to provide a de - nesting function, and other rib and reinforcement lobes that can alter the plug force. Plug composition or material of the plug. The coefficient of friction, specific heat, and conductivity of the material will also affect the plug force. Equilibrium temperature of the plug. A variable temperature will alter the plug force and thus alter the uniformity of the wall thickness of the thermoformed article. With practice, it should be easy to recognize how to modify variables in order to increase or decrease plug force and/or cavity pressure. There are also variables within the polymeric material that can affect the thermoforming process parameters, such as extensional viscosity and coefficient of friction (variable with temperature). Although these properties can be used in determining an optimum material to be utilized for the thermoforming process, they can be modified only within a certain range during the thermoforming process in order to optimize the process for a given polymeric material. Once the optimum profile(s) are determined, the appropriate modifications are made to the plug force and/or cavity pressure by the above - mentioned process variables, such that the thermoforming process is optimized APPLICATION EXAMPLES A five - factor, two - level experiment was designed with three center points that studied a roll - fed thermoformer and a single - cavity - plug assisted tooling for a commercially available 16 - ounce drink cup using high impact PS (PS - HI). The thermoformer was equipped with a control system. The thermoformer was specially equipped to acquire, on a continuous basis, (1) film temperature using infrared temperature sensing equipment at both top and bottom and just prior to the forming station, (2) plug force using an electronically designed load cell positioned at the base of the plug, and (3) cavity pressure using a pressure transducer on the bottom of the cavity mold. Plug temperature (4) was further acquired and controlled on a continuous basis. A monolayer film was extruded from PS - HI, measuring 1.45 mm in gauge and consisting of less than 10% shrinkage in the machine direction and less than the absolute value of 4% shrinkage in the cross machine direction. Shrinkage was measured by exposing a mm sheet sample to 150 C for 1 hour.
140 130 Chapter 21 Optimizing a Thermoforming Process for Packaging The experimental design factors included process variables known to be critical to the performance of a cup. These variables were (1) film temperature, (2) film stretch rate, (3) main vacuum timing, (4) vacuum bleed timing, and (5) vacuum bleed rate. The plug composition was held constant. The plug was made from a syntactic foam and coated with PTFE. The design of the plug was a commercial design, and that was also kept constant. The temperature inside the plug was held constant at 150 C by an internal heating system. Also, the effect of plug temperature on the forming of cups was held constant by allowing it to form 25 cups prior to saving 20 experimental cups for testing. Twenty - five cups were sacrificed prior to collecting the cup samples, since it was determined through experimentation that cup dimensions stabilized after 20 cups were formed. Form air pressure was held constant at 4,1 bar and timing at 95% into the forming cycle. Clamp frame pressure was held constant at 3.5 pounds per linear inch. The experimental design results included (1) critical cup properties that are typically measured to determine if a cup is commercially acceptable to the marketplace and (2) novel process parameters to predict final cup performance. The cup results included (1) cup weight, (2) cup dimensions, (3) side wall compression, (4) instrumented impact properties at 0 C, (5) column compression strength, and (6) orientational properties. Novel process parameters included (1) plug force and (2) cavity pressure. See Table 21.1 for the designed experiment factors. The experiment was completed and run in the order listed in Table The desired film temperatures were obtained by adjusting the oven temperatures. Film Table 21.1 Experimental Designed Factors: Five Factors at Two Levels with Three Center Points Pattern Sheet Temperature ( C) Sheet Stretch Rate (mm/s) Main Vacuum Timing (s) Vacuum Bleed Timing (s) Vacuum Bleed Rate ( )
141 21.4 Application Examples 131 stretch rates were obtained by adjusting the rates of closure of the plug. The main vacuum and vacuum bleed timings were obtained by adjusting the time when either of these turn on, as determined using the velocity curves of the top and bottom plates. The cup had a commercially designed pattern consisting of five radial stacking rings. The linear depth to diameter draw ratio of the cup was 1.2:1. Cup dimensions were measured using specially designed measuring fixtures to obtain nondestructive dimensions. Side wall compression of the cups was measured using a specialized two - point contact holding fixture positioned inside a fully electronically controlled compression/tensile testing machine. The force in pounds was measured after 6.35 mm of deflection at a third of the distance down from the top (rim) of the cup. Cross - head speed was at 254 mm per minute. Column crush was measured using the same testing machine and by positioning the cup vertically between two compression plates and measuring the maximum compression force after the cups were compressed from top to bottom at a rate of 10 inches per minute. All factors and results were entered into a statistical software program and analyzed, in order to develop adequate, new control factors of the plug force and cavity pressure for thermoforming and to model cup properties. Using the statistical software program, the sizes of the experiment s main factor interactions were analyzed. Cup results, plug force, and cavity pressure varied with changes in the process factors. Strong correlations proved to exist between factors and results. For example, strong correlations (i.e., greater than 0.90) existed between sheet temperature, plug force, cup weight, and cup dimensions. Little correlation existed between the cavity pressure and many other factors and results except for vacuum bleed timing (correlation factor of 0.80). Cavity pressure was the only result that correlated to vacuum bleed timing. As shown in Table 21.2, the following correlations were determined: 1. The plug initiates its travel (velocity profile is adjustable to the desired strain rate) and stretches the film until a predetermined depth (also adjustable, and typically 84% of the mold height) is reached. Several things happen in this brief period of time: the film gets engaged to the plug bottom, and the nonengaged area begins to stretch (increasing the surface area and reducing the wall thickness) until the melt strength exceeds the friction force engaging the film to the plug s tip. This moment is known as the stretch/slip transition point. At this point also the timing of the forming air coming in may de-mold the film from the plug; air pressure may build up in the volume under the film as the sheet is displaced into the cavity. The exhaust rate depends on the effective cross - sectional area of the vent holes, and hence the pressure can build up in the volume under the film. 2. At any moment during the plug s down travel, the incoming forming air can be programmed (timing), and the pressure inside the upper volume (above the film) of the cavity to reach the pre - set pressure at a known time. The air pressure would add an extra force on the load cell that pushes the plug. 3. If no air is allowed into the cavity, and the plug initiates its return travel, the film would have adhered and/or shrunk into the plug. As this occurs, a tension force
142 Table 21.2 Parameter Correlations Correlations Sheet Temperature Sheet Stretch Rate Main Vacuum Timing Vacuum Bleed Timing Vacuum Bleed Rate Plug Force (lbf) Cavity Press. (psig) Rim thickness (mils) Stacking Ring 1 (mils) Stacking Ring 2 (mils) Stacking Ring 3 (mils) Stacking Ring 4 (mils) Stacking Ring 5 (mils) Bottom Corner (mils) Bottom (mils) Cup Wt. (g) Sheet temperature Sheet stretch rate Main vacuum timing Vacuum bleed timing Vacuum bleed rate Plug force (lbf) Cavity pressure (psig) Rim thickness (mils)
143 Stacking ring 1 (mils) Stacking ring 2 (mils) Stacking ring 3 (mils) Stacking ring 4 (mils) Stacking ring 5 (mils) Bottom Corner (mils) Bottom (mils) Cup weight (g) Correlations Sheet Temperature Sheet Stretch Rate Main Vacuum Timing Vacuum Bleed Timing Vacuum Bleed Rate Plug Force (lbf) Cavity Press. (psig) Rim thickness (mils) Stacking Ring 1 (mils) Stacking Ring 2 (mils) Stacking Ring 3 (mils) Stacking Ring 4 (mils) Stacking Ring 5 (mils) Bottom Corner (mils) Bottom (mils) Cup Wt. (g)
144 134 Chapter 21 Optimizing a Thermoforming Process for Packaging 100 Ω5a: Force (P = 2bar, T = 145C, SR = 35 mm/s, Mold T = 50) 50 Force (N) Air in 30 PS HI org PS HI Pack 60 PS HI Pack 71 PS HI Pack t (msec) Figure 21.1 Plug force Plug Profile (SR = 35 mm/s) Plug Travel Distance (mm) (instead of a compression force) is exerted on the load cell. The part will show incomplete forming as it will copy only part of the plug and none of the mold. Example 1 One example using the roll - fed thermoformer method was to compare four different lots of a PS resin deemed to be almost identical. The same processing parameters were used in comparing the four lots. The resins were differentiated by their maximum melt strength registered by the load cell (see Figure 21.1 ). None of the cycle elements was changed. The diagonal line in the figure shows the position of the plug (right axis) at any moment in time. The force exerted on the film at any particular deformation distance or time can therefore be found. The air came in for the four samples at roughly 850 ms, equivalent to a travel distance of 30 mm of the plug. The plug contacts the film at roughly 150 ms, equivalent to a 10 - mm displacement of the plug (clearance between film and plug tip in the rest position). The air pressure in the cavity is evidenced by the force on the load cell after about 1000 ms and until 1700 m. Example 2 Another experiment involved the use of the thermoforming device to study the drawing of the resin by air pressure only (without plug travel) (Figure 21.2 ). In this case the resins were compared in terms of height of a bubble formed, the thickness distribution, and the time to reach the no further drawing point. As in Example 1, the four lots of the same PS resin were compared with a similar resin and no dif-
145 21.4 Application Examples Ω5a: Air Pressure (P = 2bar, T = 145C, SR = 35 mm/s, Mold T = 50) 50 Pressure (bar) Plug Profile (SR = 35 mm/s) Air in 1.1 PS HI org PS HI Pack 60 PS HI Pack PS HI Pack t (msec) Figure 21.2 Air pressure Plug Travel Distance (mm) Thickness (mm) Ω5a: Thickness Distribution (P = 3bar, T = 145C, SR = 35 mm/s, Mold T = 50) PS HI org PS HI Pack 60 PS HI Pack 71 PS HI Pack Distance from base (mm) Figure 21.3 Thickness distribution ferentiation was seen; the air drew all the samples at the same rate, while in the previous example the plug exerted different force patterns on each material. Example 3 As in Example 1, the thickness distributions were obtained in the part formed, as shown in Figure 21.3.
146 136 Chapter 21 Optimizing a Thermoforming Process for Packaging Example 4 A subsequent experiment was conducted to observe the behavior of the same resin under different processing conditions (machine settings). Machine settings were pressure (P), stretch rate (SR), and temperature (T). Different thickness distributions were obtained, each having a different melt strength (maximum force). Low stretch rates seem to create uneven results in terms of thickness distribution. See Figures 21.4 and Thickness (mm) HI-PS-Thermoforming Thickness Distribution Distance from base (mm) Figure 21.4 Thickness distribution (Exp.1) P = 2, SR = 80, T = 135 (Exp.2) P = 3, SR = 35, T = 145 (Exp.3) P = 3, SR = 190, T = 145 (Exp.4) P = 2, SR = 300, T = 155 (Exp.5) P = 4, SR = 300, T = 155 (Exp.6) P = 1.6, SR = 190, T = 145 (Exp.8) P = 3, SR = 190, T = 130 (Exp.1) P = 2, SR = 80, T = 135 (Exp.2) P = 3, SR = 35, T = 145 (Exp.4) P = 2, SR = 300, T = 155 (Exp.5) P = 4, SR = 300, T = 155 (Exp.6) P = 1.6, SR = 190, T = 145 (Exp.8) P = 3, SR = 190, T = 130 (Exp.9) P = 4.4, SR = 190, T = 145 (Exp.10) P = 3, SR = 190, T = 160 (Exp.12) P = 2, SR = 80, T = 155 (Exp.13) P = 4, SR = 80, T = 135 (Exp.14) P = 2, SR = 300, T = 135 (Exp.16) P = 3, SR = 345, T = 145 (Exp.18) P = 4, SR = 80, T = 155 (Exp.3) P = 3, SR = 190, T = HI PS Maximum load Maximum load Figure 21.5 Maximum load
147 Chapter 22 Analysis of Thermoforming Films Written in cooperation with Manfred Reichert, Remshalden, Germany 22.1 GENERAL ANALYSIS OF THERMOFORMING FILMS 1 When packages (e.g., cups and bowls) are manufactured for the food industry on thermoform fill - and - sealing machines, the consumer expects consistently good quality packaging. So consistent machinability of the films used for the packaging on these machines must be guaranteed. Currently, a multitude of plastic films exist. Depending on the application and the product, the best suited film is selected. For example, for the manufacture of yogurt cups, mostly PS (polystyrene) and PP (polypropylene) films are used. Delicate products that have a longer shelf life need to be packaged in multilayer films with a barrier layer that protects them mainly from ambient oxygen. Some examples are coffee cream, condensed milk, soups, convenience food, and baby food. For consistent quality the film to be used must be specified exactly for each product. Thus the films must be first subjected to certain tests. Many tests exist, typically to obtain some basic facts: Free shrinkage measurements Thickness measurements (thickness of the complete film as well as the thicknesses of the individual layers) 1 Dr. Manfred Reichert, InnoNET Partner in Cooperation with Innoform Coaching GbR, Hasbergen and Innoform GmbH Testservice, Oldenburg, Germany, Inno Letter Thermoformen, Analytik von Thermoformfolien Teil 1, Innoform GmbH, Oldenburg, Innoform Coaching GbR, Hasbergen, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 137
148 138 Chapter 22 Analysis of Thermoforming Films Tensile strength Surface texture appearance (gloss factor) Flame coloration (rapid test in order to determine the material) Yet all test methods have only limited significance. Often thermoformers utilize films from different manufacturers that nominally seem to be the same. Despite the above - mentioned types of tests, detailed analysis of the films is often not possible. However, some differences that are not easily discernible are possible to ascertain: Quality of the used raw material Quantity and quality of additives The possible use of recycled material as one layer of the film (this layer must not be facing toward the product side) The method of film manufacturing: different manufacturers may use different methods All of these factors can have an impact on the processing behavior of the film, and therefore advance knowledge of a film s composition is advised. Besides the classic test methods mentioned above, other tests can be conducted to obtain further necessary information: Torsion pendulum test DSC (differential scanning calorimetry) DMA (dynamic mechanical analysis) 22.2 TESTS MEASURING FREE SHRINKAGE Free shrinkage refers to the contraction that occurs as film is subjected to a viscous (hot) environment for a defined temperature and residence time. The dimensional changes regarding the film in terms of width and length are a way of determining the specific stress to the film. Shrinkage measurement is therefore a determination of the dimensional changes of the film through thermal exposure. Such measuring is necessary for the quality assessment of the films because, when the films are manufactured (extruded), more or less pronounced molecular orientations as well as internal stress are created, depending on the processing conditions. Tensions (stresses) are created and frozen in place as films are extruded. It is not possible to manufacture a thermoforming film that is completely without tension or stresses. However, when the machine settings are optimized, it is possible to create films having very low specific stresses. The exact definition of free shrinkage is the contraction of a bowl or a film under the impact of heat. Free shrinkage is calculated according to the following formula: L = ( L L )/ L 100% b u u
149 22.3 Tests Measuring Thickness 139 where L = dimensional change created by heat treatment, in %, L b = absolute dimension after the heat treatment, in mm, L u = absolute dimension before the heat treatment, in mm, 100% = conversion factor from the absolute dimension in percentage. There are other possibilities for testing free shrinkage behavior, and a multitude of different tests exist for this purpose. The different companies machine manufacturers and film manufacturers often use their own test methods. Some examples of the methods used by different companies (free shrinkage measuring for PS films) are as follows: Ten square sheets with the dimensions mm are cut from the piece of film to be tested; these are kept for 15 minutes at a temperature of 150 C in a heating cabinet. After cooling these sheets are measured again. Normally, a certain shrinkage mainly occurs in the longitudinal direction; there is hardly a shrinkage in the lateral direction. The measured shrinkage values allow conclusions to be made about the behavior of the film when processed on the machine. This is particularly important for the restart of a machine after its standstill. A square sheet of 140 mm is cut from a film. A circle with a diameter of 100 mm is marked in this square and this circle is later measured. The sheet is placed in a hot oil bath, heated to 150 C. After cooling, the circle is measured again in the longitudinal as well as lateral direction. It is not yet possible to agree on a standardized test method for the whole industry sector. Therefore, when in doubt, the samples should be measured using both methods and afterward the measurement results compared. By the execution of comparative free shrinkage measurements using both methods, significant discrepancies may be revealed. Therefore, in practice, it is necessary to agree on a test method for each individual case in order to avoid subsequent disparities TESTS MEASURING THICKNESS Film thickness testing is done by mechanical scanning. The testing is according to DIN for the determination of the thickness of flat and nonembossed plastic films, and this is carried out in such a way that the irregularities in thickness, both in length and width of the film web, can be checked quickly to be in compliance with the agreed thickness tolerances. Furthermore, the thickness test serves as an auxiliary check for other tests, for example, the tensile strength test. The acceptable limit of a measurement error in thickness, on which depends the measuring instrument to be used, has to be within a certain tolerance range. A rule of thumb is that the measuring instrument should be factor of 10 higher than the tolerance range of the film. This means that for a film produced within a
150 140 Chapter 22 Analysis of Thermoforming Films precision of 1/100 mm, a measuring device with an accuracy of 1/1000 mm should be used. For the processing of a thermoforming film on a machine, it is absolutely necessary to verify the thickness with regard to the thickness tolerances (complete thickness, as noted above, where the thicknesses of the individual layers is determined by microtome cuts, as discussed next). For example, suppose that the tolerance of the complete thickness must be ±5%; otherwise, there may be problems with the preheating process, for the contact with the heating plates, for the contact with the forming tool, and so forth. The tolerance of the individual layers should be ± 10%. This is because production of the film creates tolerances for the complete thickness as well as for the thickness of the individual layers. If these tolerances are not adhered to, in the production process serious problems can arise. Now consider the example of thickness variations regarding the embedding of a barrier layer (EVOH, light gray) into a PP film (dark gray) diagonally to the direction of travel of the film. The thickness variations in the PP film can be clearly seen in Figure The thickness variations are again diagonal to the direction of travel of EVOH in a PP multilayer film (see Figure 22.2 ). The different thicknesses of EVOH also signify, among other things, different qualities of the barrier layers in the cups manufactured from the respective film area (in four pieces, diagonal to the Figure 22.1 Thickness variations of PP film (dark gray) in a multilayer film Figure 22.2 Thickness variations of EVOH (light gray) in a multilayer film
151 22.5 Surface Texture Test for the Gloss Factor 141 direction of travel). Cup number 2 has a considerably thicker EVOH barrier layer than cup 1. The fact that the width of the film is much larger when it is manufactured than when it is later processed on the thermoforming machine has to be taken into consideration as well. In the example above the width of the film is twice as thick at the time of manufacturing than at the time of the processing on the machine. This means that the film must be cut in two halves, a film roll east and a film roll west (official U.S. designation). Depending on whether the roll east or the roll west is being processed on the machine, different conditions and qualities apply. For this reason examination of the thickness of each film layer is very important TENSILE STRENGTH TEST With help of a tensile strength test, according to DIN 53455, the mechanical properties of the thermoforming film can be verified. This test serves to assess the behavior of plastics under the condition of uniaxial stress. The result is a stress strain curve from which the relation between stress and strain is easily discernible. Depending on the type of plastic used for examination (e.g., brittle with a high rigidity or rubber - like with low rigidity), characteristic curves are obtained. For this test the samples are normally cut from the thermoforming films longitudinally and diagonally to the film extrusion direction by a standardized cutting die. However, the results of these tests have in terms of thermoforming behavior only limited significance, because they show only the characteristic mechanical parameters at room temperatures SURFACE TEXTURE TEST FOR THE GLOSS FACTOR Gloss is visually perceived when one gazes at a surface. Gloss is perceived to be higher the more directed light it reflects. It is, of course, possible to see reflections even in flat and polished surfaces. At the surface the directed incident light is reflected, but only toward the main reflection direction. The reflection angle is the same as the angle of incidence. From rough surfaces the light is reflected not only in the main reflection direction but also diffusely in other directions. Thus the reproduction quality of the surface is lessened: a reflected object is blurred. The measuring results of the reflectometer are not referenced to the quantity of incident light but to a black polished glass standard with a defined refraction index. For this standard the measuring value = 100 gloss units (calibration). For materials with a higher refraction index the measuring value can be higher than 100 gloss units, for example, for thermoforming films. For transparent materials this measuring value can be additionally increased by the multiple reflection in the material. Due to the high reflection it is even possible to measure up to 2000 gloss
152 142 Chapter 22 Analysis of Thermoforming Films Table 22.1 Gloss Factor Gloss Factor 60 Value Measured with Semi gloss 10 to geometry High gloss >70 20 geometry Low gloss >10 85 geometry units in metals. For metals it is common to relate the measurement to the quantity of incident light and to state it in a percentage. In order to obtain comparable measuring results, the reflectometers and their handling were internationally standardized. The angle of incidence used for the tests heavily influences the reflectometer value. In order to be able to differentiate low gloss surfaces from high gloss surfaces, three geometries (i.e., three measuring ranges) were standardized (see Table 22.1 ). Semi - gloss surfaces are measured with a incident direction of 60 and should be in the range of 10 to 70 gloss units. High gloss surfaces, which have measuring values of more than 70 units with a 60 geometry, should be measured with 20. However, low gloss surfaces having less than 10 gloss units (for 60 ) are measured with the 80 geometry. In order to obtain a better differentiation of the measuring values, it is recommended to use 85 incident angle even when the 60 value lies below 30 gloss units. For example, when different thermoforming films are pre - heated, these films adhere in varying degrees to the heating plates of the machine. Subsequent to the optimization of the machine, various tests are done. During these tests it was determined that the adhesion (behavior) depends not only on the temperature of the heating plates but also very much on the gloss factor of the films: low gloss films do not adhere to the heating plates, contrary to the behavior of more glossy films. The more glossy the film, the stronger is the adhesion. Transparent thermoforming films are not measured with this device, because a part of the incident light is absorbed and thus the result would be misleading. The adhesion of films to heating plates can cause major problems for subsequent processing. The quality of the containers may be insufficient, and film transport within the machine may be disturbed. Machine malfunction can lead to a slopover of the product (for low viscosity products in forming, filling, and sealing applications). So it is important to know the gloss factor ahead of processing. However, there are no exactly defined gloss factor values that make it possible to determine when afilm will manifest an adhesive behavior and when not. Other factors come into play such as temperature and surface texture of the heating plates FLAME COLORATION A relative simple test that is often used is the flame coloration test. It often happens that the material of a thermoforming film is not clearly known. In order to get a clue
153 22.6 Flame Coloration 143 as to the material s content, a flame coloration test is used. This is a rapid test, because after the sample is lit, its odor and coloration allow for a rapid diagnosis. In this example, we will consider the behavior of PS and PP. PS has a yellow - orange flame coloration, and a black sooty fume; the slightly acrid smell is said to resemble the smell of fresh green plants. PP has a white flame, and smells like candle wax. Specialized companies, testing institutes, and universities, however, are equipped with special testing equipment for the execution of complementary test methods, for example, DSC and DMA. These methods are described in Chapter 23. In Chapter 24 the methods for the examination of the manufactured containers will be described.
154 Chapter 23 Advanced Analysis of Thermoforming Films Written cooperation with Manfred Reichert, Remshalden, Germany The methods used for advanced analyses of thermoforming films are differential scanning calorimetry (DSC), dynamic mechanical analysis (DMA), and torsion pendulum resistance test. 1 These methods are described here to show how the behavior of thermoforming films can be recognized and evaluated before they are processed on the thermoforming machine. For example, films made by different manufacturers that nominally seem to be the same often have significantly different behaviors on the thermoforming machine. Having reliable information will improve processing; however, it is often necessary to consult specialized institutes to obtain more exact analyses and interpretations PRODUCT QUALITY DEMANDS The quality of the films to be thermoformed is extremely important. The production of cups, bowls, and so forth from a flat film constitutes a very important process step for the packaging of food. The operating behavior of a thermoforming machine is considerably affected by the quality of the films, and ultimately the operating behavior determines the efficiency and the productivity of the production process. Film that is not machine processible or that is inferior in quality can cause serious machine malfunctions and disrupt the whole thermoforming process. 1 Dr. Manfred Reichert, InnoNET Partner in Cooperation with Innoform Coaching GbR, Hasbergen and Innoform GmbH Testservice, Oldenburg, Germany, Inno Letter Thermoformen, Analytik von Thermoformfolien Teil 2, Innoform GmbH, Oldenburg, Innoform Coaching GbR, Hasbergen, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 144
155 23.1 Product Quality Demands 145 In practice, it often difficult to trace malfunctions to definite causes: Is the malfunction caused by the machine? For example, problems with the heating of the film or problems during the actual thermoforming process may be caused by a bad calibration of the process sequence, a damaged material being used, the wrong material for the plug assists, and so forth. Is the malfunction caused by the quality of the film? The quality may vary or have irregularities. Is the malfunction due to both machine and film problems? The many possible causes of malfunction need to be analyzed in each individual case. Regarding the film, its quality is very important and should be analyzed precisely using suitable analysis methods. Because the materials used in thermoforming films are continually evolving, this places increasing pressure on the operators of thermoforming lines to test the films. Today there is demand for better and, above all, consistent quality of the manufactured containers as well as for the use of thinner films to save on the cost of packaging materials and thus raise economic efficiency. To this end it is absolutely necessary to ensure that the film has good machinability before the thermoforming process begins on the machine. The situation is exacerbated by the fact that films such as polypropylene (PP), which is relatively difficult to process, are increasingly being utilized. PP is a semicrystalline plastic. In simple terms, this means that the material can be heated only in a very narrow temperature range, and this presents relatively high requirements for the construction of the heating station of the machine. The temperature ranges for the processing of other readily available materials such as polystyrene (PS) and polyvinyl chloride (PVC), which have amorphous characteristics, is wider. In a PP film the morphology (i.e., its inner amorphous state structure with its semicrystalline configuration) also influences the thermoforming process. Other influences are the nature of the film extrusion process, the PP type used, and the conditions for the storing of the films. An extensive analysis of films and their quality control must, as far as possible, facilitate the acquisition and evaluation of these quality features. Until now only the so-called monofilms (PP and PS) were discussed; however, in practice, multilayer films are often used for the packaging of damageable products that must have a very long shelf life. So such multilayer films have an additional barrier layer against oxygen and/or water vapor. For all these films a definition is necessary, and should be as exact as possible. Recall the classic test methods described in Chapter 22, as were used for an exact assessment of the film quality: Free shrinkage measurement Thickness measurement (thickness of the complete film and thickness of the individual layers) Tensile strength test
156 146 Chapter 23 Advanced Analysis of Thermoforming Films Surface texture (gloss factor) Flame coloration (rapid test in order to determine the material) However, these classic methods are not sufficient because they have only a limited informative value. By their means neither the basic material nor its quality can be identified. A pronouncement concerning the respective amorphous state structure and thus the film s thermoformability is only conditionally possible. Often the films from different manufacturers nominally seem to be the same. Sometimes, with the above - mentioned methods, a detailed analysis of the films is not possible. Some films may even present differences that are not easily discernible. These differences may originate from the quality of the raw materials or from the number and quality of the additives in the film. It is also possible for recycled material to be utilized as one layer of the film; however, this layer must not come in contact with the product. Finally, the production of a film meaning the technology of the film extrusion process can differ from manufacturer to manufacturer. All these factors may have an impact on the processing behavior of the machine. Besides the classic testing methods, optimized and practice - oriented methods for analyzing thermoforming films can yield valuable additional information. These methods complement the conventional methods and remove some of their disadvantages: DSC (differential scanning calorimetry) DMA (dynamic mechanical analysis) Torsion pendulum test 23.2 DIFFERENTIAL SCANNING CALORIMETRY With help of the differential scanning calorimetry (DSC) method, thermal effects are determined that are connected to physical transformations such as glass transition, melting, and crystallization. Glass transition is the reversible transition in amorphous materials or in amorphous regions within semicrystalline materials from a hard and relatively brittle state into a molten or rubber - like state. Furthermore, the specific thermal capacity of the films can also be determined through DSC. The DSC is defined according to DIN and DIN For DSC the material is subjected to a controlled temperature/time program whereby the heat flow absorbed and released from the sample measured. The temperature difference between the sample and a reference constitutes the measurand. This temperature difference is proportional to the heat flow that is absorbed or released from the sample. Thus all physical and chemical processes that are related to a thermal effect can be characterized. It is possible to obtain information about endothermal and exothermal heat zones, and thus it is easily possible to discern material differences within the various film batches.
157 23.3 DMA (Dynamic Mechanical Analysis) 147 The DSC offers the best means for recognizing differences in materials. The practical reason for using the DSC method of analysis is as follows: thermoforming machines are adjusted to a particular kind of film for the acceptance runs as defined by the reference film. A DSC analysis of this film is carried out and the data are recorded in a reference diagram. If the customer later uses films that are different from the one defined during the acceptance test and which may be characterized by a different, or worse thermoforming, behavior on the machine this can rapidly and easily be determined through DSC, which registers the thermal behavior of the samples. A characteristic fingerprint of the tested film is thus obtained. At this point an example of the application of DSC analysis for the industry should be mentioned. A dairy company carried out tests with PS thermoforming films from different manufacturers. These films had a different thermoforming behavior (although they should nominally all possess the same qualities). With help of the DSC analysis it could be proved that the results (thermal capacity, glass transition temperatures) for the film that featured good thermoforming behavior were different from the results for the film with worse thermoforming behavior. The DSC signal relating to the first heating beyond the softening point provides the thermomechanic history of the material and thus important information concerning its processing (e.g., relating to the production of the film). With the material completely softened, its previous history is erased. The subsequent cooling creates a homogeneous condition and determines the material s solidification behavior, that is, its crystallization behavior. The material s properties at the second heating of the material thus form the basis for the direct comparability of this material with other samples. DSC also detects: Different basic materials Different conditions for the production of films For the inspection of incoming goods it is therefore recommended that the films be examined using DSC to ensure that the thermoforming process will proceed safely. However, it is not always possible to obtain by DSC analysis exact information on the thermoforming behavior of a film. For this purpose two other methods may be appropriate: dynamic mechanical analysis and the torsion pendulum test DMA (DYNAMIC MECHANICAL ANALYSIS) With help of DMA the viscoelastic properties of films are determined. Plastic consists of two components: a viscous component and an elastic component. The proportion of these two components whether more viscous or more elastic allows conclusions to be made about the thermoformability of a film. With DMA and unlike the DSC analysis it is possible to analyze the potential thermoformability of films. The result of a DMA measurement is, on the one hand, the so - called storage
158 148 Chapter 23 Advanced Analysis of Thermoforming Films modulus or E-modulus E of a material that makes it possible to determine the rigidity of a plastic material. On the other hand, the second result of the analysis, the so - called loss modulus, E, describes its viscous behavior as a plastic. The basic material characteristics determined by means of DMA are in accordance with DIN 53440, DIN 53513, as well as ASTM D Precise statements relating to the mechanical behavior of a sample are possible. The mechanical characteristics are determined in relation to the temperature and a possible stress rate/ frequency. The E - modulus is a measurement of the solidity or the rigidity of a sample and gives a precise value as to the formability of the material. The loss modulus, in contrast, gives information about the viscous components, which are also important for formability. DMA is an analysis that is universally applicable and provides a complete characteristic of a film. Besides the information above, DMA also provides information on glass transitions and the strain characteristics of a material The Functional Principle A sample is subjected to harmonic as defined by amplitude and phase excitation from an oscillating dynamic load F (t ), which creates a deformation in the sample. The sample s reaction to this oscillation is analyzed (according to amplitude height and phasing), and information about the rigidity of the material is obtained. Depending on the kind of material (more viscous or more elastic), an input signal is given to the oscillating excitation, which includes more or less phase lag. Expressed in simplified terms, for a completely elastic material (such as a rubber ball) there is no internal damping through the excitation, and the phase lag is 0. For a completely viscous material (such as honey) the energy brought into the material is entirely dissipated (absorbed). No energy can be stored elastically. The phase lag is 90. The tested plastic films always consist of a viscous and an elastic proportion. According to the quality of the material the percentages of these two components vary (the value of the phase lag lies somewhere between 0 and 90 ), which can have various effects on a plastic s thermoformability The Complex E-modulus E* in Conjunction with Temperature The complex E-modulus E * consists of the storage modulus E and the loss modulus E. For a purely elastic material the complex E-modulus E * equals the storage modulus E (phase lag = 0). The other extreme is a purely viscous material: the complex E-modulus E * equals the loss modulus E (phase lag = 90 ). There are two curves that have a phase lag of the angle ω. The two lower curves are the characteristics/gradient of tan δ, where tan δ is the so - called loss factor: the relation of the loss modulus E to the storage modulus E. It is a measurement of the internal dampening of the film. A high value indicates the presence of a raw material having a pronounced viscous forming part. A low value indicates that the
159 23.5 Summary 149 film would be difficult to use for thermoforming purposes because the forming energy is, to a large extent, elastically stored, so subsequent to the removal of the forming force during the thermoforming process the film would be elastically reset. DMA shows the extent to which a material manifests viscous or elastic behavior. The percentage of viscous and elastic parts has an effect on the thermoformability of the film. DMA results can be further illustrated by means of a so - called strain sweep. The complex E-modulus E * response to dynamic strain is depicted, where the temperature remains constant during the whole process. Tested in the example is the behavior of PP films that were manufactured by different procedures TORSION PENDULUM TEST The torsion pendulum test is another form of dynamic mechanical analysis, but it tests the mechanical thermal behavior of thermoforming films. By the corresponding differences in the characteristic curve progression of semicrystalline thermoplastics, conclusions can be drawn about the thermoforming behavior. In this test the characteristic conditions and transitions for the heating of the plastic are described. These characteristic curves of the mechanical thermal behavior depict, on the one hand, the behavior of amorphous plastics (such as PS) and, on the other hand, the behavior of semicrystalline plastics (such as PP). The curves show that semicrystalline PP is somewhat more difficult to thermoform than amorphous PS. For each plastic the behavior of the shear modulus (elastic component) and the loss factor is referenced to the shown temperature. For amorphous plastics, the shear modulus in the range of the glass transition temperatures drops relatively moderately. For semicrystalline plastics, on the contrary, an abrupt drop of the shear modulus at the temperature of the crystallite melting range can be observed, which signifies that the thermoforming of these materials will be more difficult SUMMARY DSC analysis is the most commonly used field-tested method. Measurement by DMA facilitates recording of the viscoelastic characteristics of the film that determine the thermoforming behavior. When combined with DSC analysis, films can be clearly identified. No prediction about the machinability of a film can be made, however, as the terms machinability and thermoforming quality are not yet clearly defined. Hypothetically, DMA can be carried out to measure unknown contents of films. However, in practice, the correlation of the DMA results with the actual thermoforming results on the machine needs further study.
160 150 Chapter 23 Advanced Analysis of Thermoforming Films The torsion pendulum test yields results close to those of DMA and is used by some companies as the quality test method. End users only rarely test films with any of the methods mentioned above; rather, they are dependent on companies or institutes that specialize in these analyses and provide interpretations of the results, enabling compilation of analysis results with those of the thermoforming process by experiments on a machine. The venue for the testing, of course, would be determined by the cost and the time needed for outside tests.
161 Chapter 24 Analysis of Thermoformed Products Written in Cooperation with Manfred Reichert, Remshalden, Germany The preceding chapters described the analyses used by the industry to test thermoforming films as well as appropriate means of measuring thickness, shrinkage, gloss level, DSC, and DMA, among other factors considered. Subsequently, an issue of importance is how all these factors contribute to the thermoformed results. Thus we address in this chapter the possibilities of testing the produced containers, primarily empty containers. The characteristics of concern are as follows 1 : Wall thickness distribution Top load Visual appearance Water vapor permeability Oxygen permeability Transparency Additionally described will be the main features of a testing device prepared for the practical assessment of the thermoformability by Fraunhofer Anwendungszentrum für Verarbeitungsmaschinen und Verpackungstechnik AVV, Dresden. The above - mentioned qualities of a container created by thermoforming are also important as to how far container qualities deviate from the tolerance ranges within 1 Dr. Manfred Reichert, InnoNET - Partner in Cooperation with Innoform Coaching GbR, Hasbergen and Innoform GmbH Testservice, Oldenburg, Germany, Inno Letter Thermoformen, Analytik der Thermoformergebnisse, Volume 3, Innoform GmbH, Oldenburg, Innoform Coaching GbR, Hasbergen, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 151
162 152 Chapter 24 Analysis of Thermoformed Products Figure 24.1 Points for measuring the wall thickness distribution of cups a multicavity matrix. A container s quality must also remain constant during a working cycle, for example, if the production is for 60 cups per working cycle WALL THICKNESS DISTRIBUTION Normally, the exact positions of the measuring points for measuring the wall thickness distribution are at the container walls, often at the angles. If necessitated by the geometry of the container, measurements are also taken at the each container s base Examples of Measuring Wall Thickness of Cups The exact positions of the measuring points ( x, y, z ) are often indicated by the customer (see Figure 24.1 ). The measuring points at the cup wall and at the angle are measured four times at the circumference of the cups each case with a 90 offset. The customer indicates the minimum wall thickness for the particular measuring points that must be maintained with a confidence level for all cups of one multicavity matrix. The measured values will have a certain tolerance range due to processing differences, and they will cluster around an average value. For example, if the required minimum thickness at the middle of the wall is 300 μ m, this means that when the results are statistically evaluated, the average values must be within the tolerance range 3 σ above 300 μm. In more simplified terms, the background is as follows: the products that the customer must fill into the cups may be sensitive to oxygen and water vapor. For this reason, films with so - called barrier layers are used for thermoforming. The
163 24.2 Top Load 153 Metering point 1 Metering point 2 Metering point 3 Figure 24.2 Metering points on thermoformed cut for microtome cut (EVOH- layer) multiple layer films then should have a barrier layer against oxygen and water vapor. For thermoforming from the flat basic film to the fabricated container the wall thickness of the finished container is inevitably smaller than the thickness of the basic film. The thickness reduction of the barrier layer is disproportionately greater than the reduction of the other film layers, particularly at the corners of the containers. If the barrier layer of the container shows areas that are too thin, the product s shelf life will be curtailed or the product will deteriorate. So verification of the container quality by means of the wall thickness measuring must be done with exact measurement of the individual layers including the barrier layer at critical areas of the container (e.g., at the corners). This is carried out with so - called microtome cuts (see Figures 24.2 to 24.5 ). If the quality of the cups does not meet the expectations of the customer, an optimization of the working process may need to be carried out. The attempt to compensate for poor wall thickness distribution just by increasing the thickness of the basic film is not the best solution. Nondestructive wall thickness measurements are carried out by means of a thickness measuring gauge. A magnetic - inductive measuring method is offered, for example, by Panametrics (called Magna Mike 800). First, the measuring points are marked on the cups by means of a template. A measuring ball with a defined diameter is then introduced into the interior of the cup; subsequently, a measuring sensor is applied to the defined measuring points from the outside. The measuring sensor draws the measuring ball to the defined point. The measuring values are recorded by a pedal-operated switch TOP LOAD The stability, that is, the solidity, of the thermoformed container is determined by a top load test. This test provides information regarding further treatment to improve
165 24.2 Top Load μm 5 μm 14 μm 244 μm EVOH, 5 mm Figure 24.5 Metering point 3 the load - bearing capacity of the cups. For example, this test helps determine the pressure of yogurt cups when stacked one above the other in several layers. The container stability is closely connected to the wall thickness distribution of the container. In each case both the required top load and the related wall thickness distribution must be optimized by an adequate choice of thermoforming films and an optimal setting of the thermoforming parameters. For the top load values the same principle applies as for the values of the wall thickness: the measured top load values must with a confidence interval level be higher than the demanded minimal top load values, namely the statistically determined range; the average value of bearing pressure from the measuring and standard deviation 3 σ must be higher than the required minimum value. Also, due to process - related reasons, the measured top load values will have a certain variation, that is, tolerance, comparable to the values of the wall thickness distribution. This is the case for the multitude of measurements both at a particular cavity and for the cavities of the whole matrix. Simplified, the top load measurement is conducted as follows: the empty containers are introduced into a suitable test equipment with the opening pointing downward. A plate that is coupled with a pressure cell moves down from above with a defined speed onto the containers, which are compressed. The force of the container is measured and recorded. As the container buckles for the first time, the bearing pressure measuring is finished. The top load then equals the maximum force value. The measuring principle is illustrated in Figure 24.6.
166 156 Chapter 24 Analysis of Thermoformed Products Movement of plate Pressure plate Specimen Base plate Figure 24.6 Principle of measuring the top load of a cup 24.3 VISUAL APPEARANCE For evaluation of the visual appearance of the formed container, the following points are of particular relevance: Is the definition of the form completely finished everywhere? Critical points are sharp edges or corners. Is the container s shape otherwise okay? Unintentional free shrinkage of the container volume can occur in containers made of polypropylene, which can happen when the cooling during the forming process was insufficient. Are there chill marks (visible as flowmarks, etc.) on the inside of the container? This can occur when a wrong plug - assist material has been chosen, namely when a wrong plug - assist geometry has been used. However, chill marks can also be caused by wrong temperatures used in the heating of the film. Chill marks can particularly be obvious in transparent containers WATER VAPOR PERMEABILITY Food is generally less sensitive to water vapor than to oxygen. For this reason the requirements concerning water vapor proof packaging extreme cases excluded are not so high for food with a moderate sensitivity and/or shorter storage time; packaging with only tightly folded closures can be used. Normally, water vapor permeability is specified as g 100 μm/m 2. DIN standardizes the conditions for measuring the permeability of water vapor through packaging material. In this connection 23 C, 85 0% r.h., and 38 C, 90 0% r.h. are preferred. A machine manufactured by the company Mocon (Elk River, Minnesota) can be used for measuring the water vapor permeability (PERMATRAN - W 3/31). This
167 24.7 Testing Device for the Practical Assessment of Thermoformability 157 machine uses a special infrared sensor to detect water vapor permeability of flat films and completely formed packages OXYGEN PERMEABILITY The gas permeability of films, namely oxygen permeability, is the most important kind of permeation. The gas permeability is measured according to DIN A measuring instrument OX - TRAN 2/20 produced by Mocon is an example of a device that can be used to measure oxygen permeability. With this device, flat films as well as formed packages can be tested. A special sensor is utilized for the test. The flat pre-cut film parts are clamped to a diffusion cell that is subsequently cleaned from residual oxygen traces by an oxygen - free carrier gas. The carrier gas is directed to the sensor until a stable zero value is reached. Then pure oxygen is passed to the outside of the diffusion cell. Any oxygen molecules that diffuse through the film to the inner chamber are transported to the sensor by the carrier gas TRANSPARENCY During transportation and distribution, food packages are often exposed to natural light. The danger of damage to food from light exposure has risen in recent years because often the wall thickness of semitransparent packages (e.g., plastic cups) is reduced for ecological reasons. A measure of the quantity of light that permeates packaging material is haze. For semitransparent packages a part of the light is remitted and another part is absorbed besides the portion of the light that goes through the material. The measured values are thus represented as: percentage of light transmission, subject to the thickness of the packaging material remission (reflection) UV-absorbing filter additives can be added to the packaging materials 24.7 TESTING DEVICE FOR THE PRACTICAL ASSESSMENT OF THERMOFORMABILITY * Until now problems connected to a description of the thermoformability of plastic films was complicated and depended on communication between manufacturers of packaging materials and manufacturers of machines and their fabricators. 2 * Under the aegis of Fraunhofer Anwendungszentrum f ür Verarbeitungsmaschinen und Verpackungstechnik AVV, Dresden. 2 Tilo Hanke and Ronald Claus, Fraunhofer Anwendungszentrum f ü r Verarbeitungsmaschinen und Verpackungstechnik AVV, Dresden, 2011.
168 158 Chapter 24 Analysis of Thermoformed Products Because of problems with the thermoformability of films from different manufacturers, fabricators initiated a search for a practical testing method that could assess the thermoformability of films. A study group of the Industrial Organisation for Food Technology and Packaging e. V. (IVLV) composed of film and machine manufacturers as well as the Fraunhofer AVV - Institute developed a method that tests specimens under defined conditions using a thermoform test rig. The wall thickness distribution, which is measured at exactly defined points in connection with selected parameters, serves as the standard measure for assessment of a film s suitability. The thermoform test rig facilitates the calibration of temperature (heating up to 160 C), forming pressure (up to 6 bar), and forming time (starting at 250 ms). Depending on the desired degree of deformation, it is also possible to vary the forming depth in the test specimen and thus determine the limits of deformation. During the pilot/preliminary study a cup form with an outside diameter of 100 mm was used to test geometry. The height of the cup varied between 50 and 80 mm. The bottom insert was designed in such a way that an offset with a width of 1 mm is created in the area of the rotundity of the cup. With help of this offset the molding of the film could be verified. By means of a slight draft angle of 5 easy demolding could be ensured. The final test form in the test rig of the Fraunhofer AVV had an outside diameter of 50 mm and a height of the cup that could be varied in steps of 5 mm (from 15 to 45 mm). The following advantages result for the user from the recognition of the processability of the film in connection with the forming parameters: Exact definition of the working range of the film. Possibility of assessment before the film is processed in the machine Setting of parameters in accord with functional area of the film. Due to this knowledge concerning the thermoformability of thermoplastics a better process stability could be attained. The quality of the manufactured products could be improved and down times could be minimized Against the background of the minimization of the effort in measurement, successful trials without a bottom insert were carried out in the context of process optimization. Here the attainable forming depth and the thereby obtained wall thickness in the center of the form are collected as characteristic values in connection with forming pressure and heating temperature. By this means deviant forming behavior of a film could be detected with little time and effort. Currently, the focus is on the further development of this method as well as the use of heating elements in order to heat the film specifically and irregularly. For this reason purpose - built, impulse - driven contact heating units with nine concentrically positioned heating circuits that are separately adjustable and controllable have been developed. With the help of these heating systems, a targeted heat input is successfully implemented and thus the forming behavior is influenced. The exact application of energy during the pre - heating of the film offers, among other things, the following advantages:
169 24.7 Testing Device for the Practical Assessment of Thermoformability 159 Simplifying the thermoforming process with regard to the renunciation of plug - assist units. Minimizing material usage through targeted heat input and the ensuing interaction of the wall thickness distribution. Reducing the energy input through impulse-driven contact heating systems.
170 Chapter 25 Analysis of Completely Formed, Filled, and Sealed Containers Written in cooperation with Manfred Reidast, Remshalden, Germany In Chapters 22 to 24 test methods were described concerning thermoforming film thickness measurements, shrinkage, gloss level, DSC, DMA, and some others. Analytical methods for completely formed containers have yet to be explained. This chapter details the most important analysis methods for completely formed, filled, and sealed containers. 1 This concerns mainly the determination of: Burst pressure and impermeability (which are closely connected) Opening force Methods for the examination of the overall quality of the finished and closed containers are discussed, particularly, the quality of the sealing, by which the lid film is applied to the filled containers. 1 Dr. Manfred Reichert, InnoNET - Partner in Cooperation with Innoform Coaching GbR, Hasbergen and Innoform GmbH Testservice, Oldenburg, Germany, Inno Letter Thermoformen, Analytik der Thermoformergebnisse, Volume 4, Innoform GmbH, Oldenburg, Innoform Coaching GbR, Hasbergen, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 160
171 25.1 Burst Pressure and Impermeability BURST PRESSURE AND IMPERMEABILITY Vacuum A vacuum chamber is used to determine the quality of the sealing of the lid film onto filled and closed cups or trays. Sealing quality mainly depends on: Sealing conditions (time, pressure, and temperature) Type and quality of the sealing medium of the lid film Type of the bottom film The vacuum chamber is usually filled with water, so that the containers are immersed in water. Slowly a vacuum is created in the chamber. The emerging pressure difference tasks the sealed seams, and potential leakages can be discovered as air bubbles leak out of the interior of the container into the surrounding water. The exact test conditions (vacuum settings, test duration) vary case by case, depending on what the user s demands are. The test time is approximately 15 to 20 seconds, and in extreme cases up to 1 minute. The vacuum created (pressure difference with respect to the normal pressure) oscillates between 200 and 800 mbar. A common example is the testing of the miniature cups that contain milk or cream to be added to coffee. A certain number of random samples of these cups are examined in a vacuum chamber filled with water (the exact number depends on the requirements of the user). As the vacuum is created in the vacuum chamber, major leaks can be detected through ascending air bubbles. However, it is not possible to determine the extent of a leak. The recognizable pore size for this test is approximately 15 μ m and larger. It is nevertheless possible to detect capillaries with lengths of more than 15 μ m (source: Innoform Company, Osnabr ü ck and Fraunhofer Institute AAV Dresden). Vacuum tests are helpful in the localizing defective sealing of film, and so are a pre - condition for troubleshooting and fault finding. These tests are widely used because they can be carried out relatively quickly and easily. An example of vacuum chamber equipment manufactured by a California company, Haug Quality Equipment, will be briefly described. Haug is one of the leading manufacturers of leakage detection systems for the food industry. The test equipment is an apparatus type Pack - Vac Leak Detector that functions according to the following procedure: Test of the packaging in a vacuum chamber filled with water Test time, up to 30 seconds per test specimen Test specimen observed to detect ascending air bubbles (evidence of leakage) and to a localize the leak In practice, there is often the conflicting issue of choosing between strength of the sealed seam (opening forces; see below) and impermeability. This is because, to be on the safe side, the packaging could be too tightly sealed and thus difficult to open.
172 162 Chapter 25 Analysis of Completely Formed, Filled, and Sealed Containers The opening force depends very much on the material combination of the sealing plastics (sealing lacquer or sealing layer of the lid film in relation to the sealing layer of the bottom film). Often, different material combinations must be examined in order to find the most suitable combination for each individual application. Therefore prior consultation with the film supplier (for lid and bottom film) as well as the thermoformer/user is part of the optimization process, and often solely project - related. The opening force also depends on the sealing profile (Figure 25.3, below). An optimal adjustment of tear - open strength and impermeability is thus necessary Air Pressure In an examination for burst pressure and impermeability, there is always the possibility of excess pressure exerted in the packs. It is possible to determine exactly the pressure when the sealed seam begins to yield and to evaluate if the packaging is not tight. That is done by sticking a needle into the pack. A septum seals the system while the test is conducted. Test equipment manufactured by Lippke, Neuwied, Germany the Package Test Systems Lippke 4000 and Lippke 4500 is designed for leakage and strength measurement on practically all types of flexible, semi - rigid, and rigid packages. 2 The Lippke 4000 and Lippke 4500 systems provide exact, definable, and reproducible test conditions. The Lippke 4000 is ideally suited for direct application on the production line because it is very robust and easy to operate. The computerized system Lippke 4500 provides extended analysis Field of Application This test device can be used for: Determination of optimal sealing parameters Packaging material clarification and sorting Quality control Validation of packaging machines Advantages High flow option for porous packaging testing (i.e., Tyvek ) Real hole size calculation with flow sensor Compliance with FDA regulation 21 CFR Part 11 Validation documentation for IQ/OQ 2 Package Test Systems Lippke 4000 and Lippke 4500,
173 25.1 Burst Pressure and Impermeability 163 Easy to integrate several interfaces are available (LAN, USB, and Bluetooth) Immediate availability of test results in the company network High data security because of central data processing System can be operated with barcode reader or touch screen Package testing and oxygen analysis in one system Multilingual user guidance Test Methods Seal Strength Test In this case a seal strength test is a burst test. It is conducted by increasing the internal pressure of a package at a given rate to the point where the seal bursts. The burst test is in compliance with ASTM F Leakage Testing For the leakage test, a pre - selected pressure is built up in the package and is then held at a constant rate for the required test time. The pressure loss after that time is an indication of package integrity and can be used to calculate the hole size. The pressure loss measurement and leakage testing are conducted according to ASTM F Creep Test In the creep test, a constant pressure is built up in the package. The time it takes for the seal to peel is an indication of the peelability (the creep test in compliance with ASTM F1140) Leak Size Determination In the leak size test, a preselected pressure is built up in the package and then is held at a constant level. The flow needed to keep the pressure constant is an indication of the leak size (based on the Hagen Poiseuille law) Oxygen Analysis Determination of Residual Oxygen in MAP Packaging For the acceptance test of a cheese packaging, a tolerance range of 250 to 500 mbar was defined for burst pressure. This package was thermoformed from an A - PET/PE film with a thickness of 450 μ m and ultrasonically sealed with a PA/PE lid film having a thickness of 100 μ m. At issue are both the strength of the sealed seam and the packaging s impermeability.
174 164 Chapter 25 Analysis of Completely Formed, Filled, and Sealed Containers Figure 25.1 Package filled with a rhodamine solution 25.2 RHODAMINE TEST The rhodamine test is another rapid test for the examination of the impermeability of sealed seams. The packaging to be examined is cut open at the bottom. The sealed seam to be tested is wetted with some milliliters of a solution consisting of 0.5% rhodamine (red powder) dissolved in propanol (see Figure 25.1 ); then the packaging is dried with warm air. Subsequent to its complete drying (approximately 2 to 9 hours), it can be verified if the red test liquid leaked at some point to the outside of the package. If the red rhodamine cannot be seen at the opposite side of the sealing, it may be supposed that the sealing is, in the context of the recognizable leakage size, tight. When the sealed seams are completely dry, they can be torn apart. 1 With this test it is possible to detect leaks (capillaries) measuring less than 15 μm. The rhodamine test can be used also to check if small contaminations were also unintentionally sealed with the product (in cheese, yogurt, herbs, etc.). If the packaging is transparent, the test liquid can be filled into the thermoformed package before it is sealed. The package is then placed in an upright position so that the sealing seam is wetted with the liquid. For aluminium multilayer films this test is carried out after cleaning and removal of the lacquer and aluminium GENERAL REMARK ON IMPERMEABILITY TESTS Many other impermeability tests exist. It is not possible to detail them all in this book. Only the most exemplary methods, and those most often used, have been
175 25.4 Opening Force 165 Figure 25.2 Device for measuring the opening force N N N S S Figure 25.3 Opening forces for different sealing geometries S mentioned. Services and seminars on the topic of impermeability tests are offered by some companies, for example, Innoform GmbH in Osnabr ück, Germany OPENING FORCE The opening force determines the force with which the lid film will be torn from the container. This measurement also depends on the measurement of burst pressure. In order to measure the opening force, the packaging is clamped into a tensile testing
176 166 Chapter 25 Analysis of Completely Formed, Filled, and Sealed Containers machine and locked into position by a clamping device in an angle of 45 (see Figure 25.2 ). The tear tab is located in the lower part of the lid. This tab is also connected with the load cell via a clamping device and a cord. The traverse of the testing machine moves with a defined speed downward and the packaging is slowly opened. Normally, the tear initiation force that is measured at the beginning is stronger than the subsequent tear propagation force. The geometry of the sealing profile has, of course, a decisive influence on the opening force, especially in the area of the tear tab. Figure 25.3 shows the opening forces for different sealing geometries. So far no standard has been developped for the examination of sealed seams of packaging.
177 Chapter 26 Automated Packaging Written in cooperation with Laura Gascho, Gerhard Schubert GmbH, Germany Many thermoform projects call for production rationalization, particularly packaging applications. Form, fill, and seal (FFS) machines have become established in the packaging sector and have gained a substantial share in the market. FFS machines are a very good basis for automated packaging. Over the years many advancements have been made to facilitate product flow and ensure a failure - free packaging process. For example, machine stops can be avoided by an automatic change of the film roll. With continuous product flow, all good products can be packaged and scrap is reduced to a minimum. Complete packaging lines are created using standard machine components; this presents enormous advantages for automated packaging. Such systems utilize robots for loading of thermoformed trays and for handling of packaging. Many packaging lines present the possibility of loading closed thermoform packaging directly into cartons or cases, and subsequently palletizing the cartons or cases. The machine suppliers also offer such additional functions as labeling and the tracing of products. Automated packaging lines must conform to demands for greater efficiency and higher flexibility. Small batch sizes that are produced to fulfill the demands of particular customers call for frequent format changes. Today s packaging lines must facilitate rapid format changes. A versatile use of the machine components is a pre - condition for the standardization of machine construction. Thus packaging lines could be used in the most diverse industrial sectors. The machine components are characterized not only by their versatility, but also by the possibility that, already in the planning phase, they can be placed within the line as needed. This means that in nearly every industrial sector, lines for different applications can be realized. Such systems, as are produced by Gerhard Schubert GmbH, Germany, do not only facilitate conventional form, fill, and seal/punching (FFS) processes; line configurations for forming, punching, and subsequent filling are also possible. This line may be necessary if the tray cannot or must not be closed, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 167
178 168 Chapter 26 Automated Packaging which is the case for vial packages, because the vials protrude over a tray. Another example is the production and filling of blisters that are closed by a backing card. As the dimensions of the blister are smaller than the dimensions of the backing card, the blister must be punched before closing CUTTING SUBSEQUENT TO FORMING Another alternative to connect the individual machine components is the use of the transmodule, which was developed by Gerhard Schubert GmbH. The transmodule is a robotic vehicle. With this device the connection of very long or already existing picker lines with a thermoform, ultrasonic sealing, and punching station is possible. In these lines the trays are not punched out of the film and separated subsequent to punching, but a special device facilitates the cross - cutting of the film and the formed matrices directly after the forming process. Or the cross - cutting can be effected after the forming of a certain number of matrices. These cavities are placed into the transmodule transport systems of the picker line and loaded by four - axis robots. The trays are sealed and punched in an ultrasonic sealing and punching device after having passed through the picker line CHARACTERISTICS OF THERMOFORMING PACKAGING LINES The packaging machine control offers the possibility of a graphic processing of the individual process steps. By means of a process analysis, the operating sequences in the forming station can be optimally adjusted to ensure constant production. Depending on the process sequence, one of the three possible production types is selected: Indexed Continuous Quasi-continuous The thermoforming machines of Gerhard Schubert GmbH can be operated with all three production types, which substantially increases the flexibility of the machines. As a rule, the more flexible the machine is, the more versatile is its use in different industrial sectors. The three ways to operate a production system (indexed, continuous, or quasi - continuous) are described below Indexed Production Indexed production is the production principle most frequently used. This means that a continuous process is created from a chain of single process steps. The com-
179 26.3 Characteristics of Packaging Machine Control 169 plete operating sequence is separated into many small individual operations that are carried out in individual workstations. The product is transported sequentially through the workstations. The production cycle is identical for all stations, so the material does not need to be buffered. A disadvantage of indexed production is that all production steps need to have the same duration so that all the steps are adapted to the speed of the workstation having the longest processing time Continuous Production Continuous production means that the material is continuously fed to the machine and the process steps are carried out accordingly. This type of production is characterized by a uniform feed of the material during processing. Typical continuous production processes are the following: Continuous extrusion processes for plastic tubes, films Manufacturing of paper Reel-fed printing The higher the continuity, the fewer abrupt, erratic changes are to be expected. Thus the process sequence is reliable and fail - safe. The advantage of the continuous process is that the material does not need to be constantly accelerated or decelerated. Due to the constant speeds and mass inertias, high uniformity and high quality production is generated Quasi-Continuous Production A Schubert thermoforming device can function either indexed, quasi - continuously, or continuously. Depending on the product, and above all on the requirements of the downstream equipment, it adapts to the process flow. Originally, the packaging machines of Gerhard Schubert GmbH ran continuously. This means that the infeed of packaging material, in our case the film web, always adapts to the working sequence of the four - axis robots, and varies between a speed of 0 and 100% CHARACTERISTICS OF PACKAGING MACHINE CONTROL If the continuous movement of the film web is not possible, the forming process can be carried out only when the machines are at a standstill. In contrast, in the thermoforming device of Schubert FFS, lines are mounted on a mobile carriage so that the film can be formed during the forward motion.
180 170 Chapter 26 Automated Packaging Indexed Production The time that a two - axis robot needs for its working cycle is significantly less than the processing time of the thermoforming device. Thus the manufacturing method of Schubert machines differs from the usual indexed production. It can be said that this more like a quasi - continuous process flow Continuous Production If two - axis robots are integrated into the downstream machines, the film web must be stopped, because the two - axis robot cannot be synchronized with the speed of the film web movement Quasi-Continuous Production Synchronization of the different processing systems is made possible by using the packaging machine control (VMS), which is an in - house development of Gerhard Schubert GmbH. The performance of different components can vary considerably so that synchronization problems may arise that lead to a reduction of the overall efficiency. So far the biggest top - loading machine (TLM) packaging line controlled by VMS that has been built is driven by over 200 servo motors. Because of the multitude of production programs that can be programmed using VMS, the modular assembly, and the high degree of automation, Schubert thermoforming machines are extremely flexible packaging machines. Nearly every conceivable combination of process steps can be realized. The basis for this is the operating sequence of the main functions, namely the thermoforming, punching, loading of the molded product, and its sealing. Different operating sequences are possible: FFS, FPF, and FCFS. These systems will be explained in detail in the following FORMING, FILLING, AND SEALING ( FFS) The most common line configuration is forming, filling, and sealing (FFS). Punching is effected at the same time as sealing, due to the use of ultrasonic technology. A distinction is drawn between picker lines, speed lines, and other systems with automatic product handling The Picker Line For a picker line the products run in counterflow direction to the film web containing the thermoformed trays. The film web and the product belt correlate in a quasi - continuous counterflow. Examples for this process sequence are the packaging lines for big dairy companies (Figure 26.1 ).
181 26.4 Forming, Filling, and Sealing (FFS) 171 Figure 26.1 Automatic cheese packaging in thermoformed cavities (Courtesy of Gerhard Schubert GmbH) Speed Lines Packaging lines are often used for the packaging of assortments. For these applications the products are fed to the packaging lines on several infeed belts that are placed perpendicular to the direction of the film flow. An example is the line for a pharmaceutical company: 1. Thermoforming station. Trays are formed (heating section with three heating plates) subsequent to automatic feeding of the film. 2. Loading area for product 1. Infeed of syringes and loading of the trays by F44 robots. 3. Loading area for product 2. Infeed of needles by an F4 robot. 4. Printer and fi lm infeed. Infeed of the lid film printed with the user s instruction. 5. Ultrasonic device. Trays are ultrasonically punched and sealed at the same time Lines with Automatic Handling Instead of using picker lines and speed lines, some products are packaged with lines having automatic handling. In this way toothbrushes, printer cartridges, other items are packaged on Schubert FFS lines. Example 1: Toothbrushes 1. Packaging line. Products are pre - grouped by F44 robots. 2. Thermoforming station. Subsequent to the automatic feeding of the film, trays are formed.
182 172 Chapter 26 Automated Packaging 3. Loading area. Pre - grouped products are placed into blisters. 4. Film infeed and ultrasonic device. Lid film is fed; trays are ultrasonically punched and sealed at the same time. Example 2: Printer Cartridges 1. Thermoforming station. Trays are formed subsequent to the automatic infeed of the film. 2. Loading area. Infeed of products and pucks. Every puck contains one product and six pucks create a formation (pre- grouping). 3. Film infeed. Infeed of the lid film for loaded trays. 4. Ultrasonic device. Trays are ultrasonically punched and sealed at the same time. Example 3: Forming, Filling, and Sealing of Blisters The TLM packaging line has two sections: (1) the thermoforming, filling, and closing section and (2) the final packaging section of the line. All sections are interlinked with a Manufacturing Execution System (MES) recently developed by Schubert. As it is normally the case with Schubert thermoforming lines, the film transport system is automatically loaded with thermoforming film by the double - reel stand. The film feed - in device supports automatic film roll changing. Once the film has been heated to the forming temperature in the heating section, the semifinished material is transported to the forming station. The forming station enables quick changing of the mold and its components. An A - PET/PE multilayer film with a thickness of 600 μ m is used for the blister production. The temperature of each single heating zone can be set individually, and thus optimally, to the film combination. Blisters are formed at the forming station. The forming vacuum, forming pressure, and plug assist can be adjusted to the requirements of the application. All movements are generated by servo motors. VMS process analysis provides excellent monitoring and optimization options here. F44 filling robots (four - axis robots) place the filled syringes in blisters formed in the film strip. The finger grip has been oriented horizontally beforehand. Another F44 station in the filling section uses its arms to insert the hollow needles and apply the patient labels. Once all the products have been inserted, the blisters are sealed with ultrasound and punched at the same time. The sealing film has been fed onto the blisters prior to this operation. The sealing film is comprised of several layers and is pre - printed on both sides. On the inside are usage instructions, and on the outside are attractive advertising decorations. The printing registration marks allow for the sealing film to be set precisely over the base cavities. The product data are applied to the surface of the sealing film using a thermal transfer printer. Just like the cartons, the sealing film has a velvety feel.
183 26.5 Forming, Punching, Filling, and Sealing (FPF) 173 Sealing and punching are carried out in less than 250 ms at the ultrasound sealing and punching station. The ultrasound is applied with a frequency of 20 khz during the brief sealing time, and heat is generated only in the joint surfaces and cutting line. This way the product and packaging are subjected to a minimal thermal load. Airtight sealing seams are created. An important requirement is that the package be simple and easy to open. The package can be opened easily, even by a user wearing examination gloves. The low punching forces created by the ultrasound enables low - wear punching, even of harder materials such as PET. The ultrasound - generating oscillating units are on the machine side and do not need to be changed. The sealing and punching station is equipped with a protective film transport device. The protective film enables the quick change of sealing and punching tools, and therefore the shortest possible size change times. The fully punched - out packages reach the product discharge belt thanks to an F2 removal robot (two - axis robot). At the discharge belt an image - processing system checks whether the package contents are all there, as well as their quality and the consistency of the product data. The data are entered in the batch log. Blisters determined to be good are transported to the final packaging section of the line for further processing. The carton blanks are erected in this section of the line. There may be different carton blanks, depending on the size. The erected carton blanks are filled with blisters. Once the informational brochures have been inserted, an F2 robot closes the boxes FORMING, PUNCHING, FILLING, AND SEALING ( FPF) Although FFS lines cover a wide range of packaging possibilities, this packaging principle can be unsuitable for certain applications. One such example is mentioned below. A pharmaceutical company has the task to package a product, where the packaging consists of a tray that is sealed with a carton backing card. As this backing card is bigger than the tray, simultaneous sealing and punching is not possible. For this reason the system of forming, punching, and subsequent filling (FPF) is used (see Figure 26.2 ). This means that the trays are punched subsequent to their forming process and only then filled. In this example the filled trays are sealed with the backing cards and then packaged in shipping cases. 1. Thermoforming station. Trays are formed subsequent to the automatic feeding of the film. 2. Punching station. The trays are punched using ultrasonic technology. 3. Transfer and fi lling section. A two - axis robot places the trays into the sealing anvils (in four lanes). The two - axis robot takes the products out of the accumulation chain and places them into the trays. Subsequently, the backing cards are placed onto the trays. 4. Sealing station. The trays are sealed ultrasonically with the backing cards.
184 174 Chapter 26 Automated Packaging Figure 26.2 Packaging line running forming, punching, filling, and sealing mode, with case packer and palletizer (Courtesy of Gerhard Schubert GmbH) Example 1: Vials In another example of the application of the FPF systems the size of the product is relevant. A manufacturer of pharmaceutical products requires placement of syringe vials into trays that are then loaded into a box. As the vials are higher than the tray, these trays must be punched before filling. In this case the film web must not be fed to the sealing station, and so a film shredder (for the processing of the punching scrap) and other peripheral devices can be placed between the second and third module. 1. Thermoforming station. Trays are formed subsequent to the automatic infeed of the film. 2. Punching station. Trays are punched ultrasonically. 3. Box erecting and loading station. The boxes are erected and loaded with the help of F2 robots. Example 2: Cardboard Blisters In the thermoforming line for the production of cardboard blisters, the operator has the option of choosing the size in which to package the products. The actual products are plastic vials filled with tablets. The vials waiting to be packaged are supplied by an upstream top - loading line. The thermoforming and punching modules are configured in such a way that the line runs in the following sequence: forming, punching, filling, and then sealing. Prior to this, the thermoforming film is unrolled from the reel stand and routed into the machine s chain conveyor system. The semifinished material is fed in using the automatic film draw-in. The film draw - in direction also enables automatic film reel changes. For this purpose the reel stand is equipped with two film reels. If one film reel is emptied during the process, film from the second reel is automatically fed in. It is then possible to replace the first reel while the film of the second reel is being thermoformed.
185 26.5 Forming, Punching, Filling, and Sealing (FPF) 175 Figure 26.3 Blister with undercut (Courtesy of Gerhard Schubert GmbH) The thermoforming unit heats the film to the forming temperature. All thermoformable packaging plastics can be processed. A - PET film is used for the application described here. So - called standing blisters require molds with an undercut. Parts formed with an undercut can be de - molded only with special mold technology (Figure 26.3 ). The integrated mechanisms for undercut forming do not impair a simple handling of the format change. As a result even complexly molded packaging parts can be produced with size flexibility. In the forming station, servo motors carry out the movements (Figure 26.4 ). This results in reproducible sequences that enable the production of uniform article qualities. The controller also enables a graphic processing of movements in the process analysis. Other parameters, such as forming pressure, vacuum, or process times, can also be graphically analyzed. As a result the process analysis helps to adjust the processes optimally in the forming station. Proven ultrasonic technology carries out the punching and sealing. However, punching and sealing are carried out separately in this application, since the outer dimensions of the sealing cardboard are larger than those of the molded plastic part. Like all Schubert TLM components in the packaging line, the thermoforming station and the sealing and punching station can be combined in accordance with the task.
186 176 Chapter 26 Automated Packaging Figure 26.4 Forming station (Courtesy of Gerhard Schubert GmbH) This means that the sequence in this line is not forming, filling, sealing, and punching (FFS), but forming, punching, filling, and sealing, instead. The punched blisters are then removed from the punching tool. As the film is subjected to oscillations of 20,000 Hz during the ultrasonic process, the plastic heats up where the tool makes contact. The heat resulting in the cutting line greatly reduces the punching forces and considerably minimizes wear. Only the cutting tool must be changed in order to switch to another format. The oscillating bodies that generate the ultrasound are integrated in the machine and need not be replaced. The punching station is equipped with a protective film transport device. This particular film prevents the need for size - dependent ultrasonic equipment and ensures rapid format changes. The blisters removed from the punching tool are placed in sealing anvils. These sealing anvils are located on the conveyor systems, similar to those in vacuum conveyor technology. The vials are placed inside and the sealing card is set on top of the blisters, which are located in the sealing anvils. Equipped in this way, the anvil moves into the sealing press where ultrasonic sealing is carried out. As the sealing process is carried out in a few hundred milliseconds, the oscillating bodies bundled in the sealing press can supply four anvil conveyor paths. This makes it possible to achieve high outputs with small, inexpensive ultrasonic units. Following the sealing process, the cardboard blisters are removed, grouped, packed in cardboard boxes, and palletized. Depending on the product and the packaging, it is possible to configure the Schubert machine components in different ways. Different formats can be run on the same Schubert packaging line. This means that different products, different packaging dimensions, and different packaging schemes can be produced on a single packaging line. To increase the packaging possibilities even more, the line configuration spectrum is augmented by the system of FCFS (forming, cross - cutting, filling, sealing/punching).
187 26.6 FORMING, CROSS -CUTTING, FILLING, SEALING/PUNCHING ( FCFS) 26.7 Conclusion 177 Under certain circumstances it may happen that a classic FFS application cannot be utilized, for example, if it is necessary to bridge a very long loading section with the film web. Subsequent to thermoforming, the film cools, and thus it shrinks, which entails the loss of the fitting accuracy of film web and sealing/punching tool. The so - called offset effect produces the same result. This effect is created by the totaling of tolerances that lead to an offset of the film web. To a certain degree these two effects can be compensated for by the VMS control of the Schubert packaging lines. However, the longer the distance between thermoforming device and sealing/punching station, the bigger is the offset. For a long loading section it is not possible to implement the classic FFS application. The FCFS system offers a solution to this problem. The trays/bowls/cups are formed as usual but are subsequently cross - cut. This means that the matrices (also called jumbo trays) are separated prior to their transport to the downstream workstation. A matrix comprises several cavities. The loading of these cavities can be carried out during the continuous movement of the transport device while forming is indexed. The advantage of such continuous processes is that the material is not perpetually accelerated or decelerated. At constant speeds and mass inertias, the production process stays highly uniform. The cross - cutting function of the Schubert line can also be used for existing packaging lines. If a thermoforming station is integrated into an existing picker line, the forming and cross - cutting (FC) stations would be located prior to the filling and sealing (FS) stations. Separation of the two operations offers the advantage that the jumbo trays can be buffered to counteract any production downtime. Example 1: Traysealer Application as a Variation of FCFS On the Schubert machine the trays are loaded with products, and subsequently these trays are sealed and punched. The tray matrices (jumbo trays) that are needed for this application are prefabricated. These tray matrices are separated in the magazine of the tray sealer prior to loading and simultaneous sealing and punching. The tray sealer line has three components: 1. Transfer device. The tray matrices are destacked. 2. Picker line. The tray matrices are loaded by F44 robots. 3. Ultrasonic device. The trays are sealed and punched using ultrasonic technology CONCLUSION A significant advantage of thermoforming packaging trays is the low - priced tooling in comparison with blow forming and injection molding processes. For small
188 178 Chapter 26 Automated Packaging batches, the reduced cost of tooling is particularly relevant. For the production of large quantities, the economic advantage results from savings of material, since with thermoforming it is possible to achieve the same form stability, even when the wall thickness is reduced. The Schubert thermoforming packaging lines provide a great deal of modular design freedom and also a high degree of automation; the VMS control significantly accounts for this.
189 Chapter 27 Production of Flowerpots Written in cooperation with Thomas Huber, Kiefel GmbH, Germany, Berry Smeulders, Bosch Sprang B.V., The Netherlands, and Noel J. Tessier, CMT Materials, Inc., USA Most people do not give a flowerpot made of plastic a second look (Figure 27.1 ). But if you look closer, you might guess the highly developed production process behind it. The flowerpot needs holes in the bottom. The edges need to show tag - slots. Flowerpots are produced in large quantities. Flowerpots made of plastic have significantly less mass than flowerpots made of clay. This is a considerable advantage in the transport chain and so justifies the application of huge and fast - running thermoform facilities. A good example is the flowerpot made of polypropylene. In most cases recycled material is used. During production (extrusion), the PP film is filled with a filler material; in this case it is chalk (whiting). While the whiting does influence the film s thermoforming behavior, the cost factor requires use of recycled material and filler. Flowerpot production can be used to demonstrate the superiority of thermoforming. Two - colored formed parts are produced. This requires using co - extrusion for the semifinished product. The extrusion process enables the production of film with two differently colored sides. That is why it is possible to have the outside of the flowerpot look like terracotta and the inside dyed black THE THERMOFORMING MACHINE An automated compressed - air system with tilting mold is used for the production of the flowerpots. This facility allows for changes of forming and punching tools so that the machine can produce different flowerpot types. Increased use of Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 179
190 180 Chapter 27 Production of Flowerpots Figure 27.1 Flowerpots Figure 27.2 Thermoforming machine Kiefel KTR6 polypropylene in the last 10 years as a material for products that can be thermoformed has inspired machine designers to expand their repertory and innovate more. The KTR6 speed machine with a floor hole punch KDS75/54 (Kiefel) for such an application is displayed in Figure This machine has a forming area of mm and offers a draw depth up to 190 mm. With this draw depth a film thickness of 1.8 mm is needed. Film made of polypropylene requires longer processing than films made of polystyrene due to the length of the ray heating system. And with that it is not enough just to extend the standard ray heating system; the PP film must be allowed the possibility of expansion before it is inserted to the chain rail film transport system. A further warm - up of the film within the ray heating system requires compensation of the film sagging with the chain rail film transport system. Therefore the transport profiles will be able to be spread and so avoid film sagging. The thermoforming station has its own film transport system with a servo drive. Before entering the forming station the film is taken off the transport system underneath the heating zone and put back into the film transport system of the forming
191 27.2 Heating System 181 station. The higher speed of the chain causes the film to spread lengthways, and with this an even film is created that is ready to be formed. The Kiefel KTR6 machine has a forming capacity of 45 drycycles/min. In the application, the forming mold Ø 108 mm and a deep drawing depth of 95 mm can yield 26 cycles/min. The forming mold Ø 165 mm and deep drawing depth of 190 mm yields 19 cycles/min. Constant quality of the formed parts is ensured by a plug assist with a servo drive. The pneumatically controlled plug assist delays for a short moment the downward run of the impact, just long enough for the air pressure to overcome the resistance toward the film. This leads to stretchmarks. Where stretchmarks occur, there is unevenness of wall thickness. To reach an acceptable reduction in film thickness, it is very important to avoid uneven wall thickness. The servo - driven plug assist offers substantial advantages. The sturdy forming station allows punching forces up to 600 kn. The servo - motor technology in combination with an intelligent control system offers substantial advantages. In the past such machines were controlled by cam plates. Contemporary machine actuators allow for timely overlapping process steps. Each function can be started ahead of the next function. This keeps the machine constantly up to speed. A central water supply prevents the buildup of condensation. A pump delivers 16 C and 18 C water to all peripheral points of the KTR6. This ensures that a maximal volume of water with laminar flow and an ideal temperature is distributed throughout the system HEATING SYSTEM For consistent molding results and qualitatively premium products, attention must be paid to the heater. As the term of the procedure thermoforming implies, the warm - up of the semi - finished products has great impact on the success of the application. At the beginning, the temperature needs to be spread homogeneously over a cross - section of the film. As the film of the reel is being handled, the warmth from the outer film needs to distribute to the inner film. When using an inline procedure, meaning with film extrusion into the thermoforming machine, the warmed - up film is brought to the film transport system of the thermoformer. In the core of the film a raised temperature dominates. The film of inline extrusion requires different regulation of the heating system than with film that is being used from reels. The inline extrusion technique is advantageous from the energy savings point of view. In addition, the logistics provide for potential time savings. However, the changeover times on inline facilities are unequally longer than for applications where film reels are used. The start - up of the line is much more time - intensive and requires an extensive manual effort periodically. The staff is nevertheless required to master the skills and knowledge needed to operate both processing procedures. In the application, the film is unwound from a reel and fed first into the integrated preheating station of the thermoforming machine. In this station the film is heated using convection heat and, in some instances, contact heat. It is possible to use separate preheating stations with the KVH from Kiefel GmbH. In this device,
192 182 Chapter 27 Production of Flowerpots which is called a heating cabinet, the film is led in a serpentine pattern over several rollers. The compact heating cabinet has only a small floor space requirement and can accommodate 23 meters of film. The recirculating air is controlled by an automated production and machine stop adjustment. The machine stop adjustment keeps the film from overheating. While the film is still in the preheating station and not yet in the film chain rail transport system, it is not fixed and therefore can expand in a cross direction. Consequently, an already pre - expanded film in cross - section will be inducted. For this reason the film chain rail transport system does not need to accomplish the complete stretching of the film with the spreading of the film chain rail transport system profiles. Certain variations in temperature produced during storage of the film reel can be balanced out. It is recommended to keep the film reels for at least 24 hours before use in an area close to the production site or at the same temperature as that of the production hall. Or constant temperatures should be maintained in the storage facility. Attention must be paid not only to different temperatures of the surroundings but also to the outer reel and its circumference, which can influence the temperature within the reel. Different outside temperatures can influence the process reliability of the facility per reel. As the reels take on different temperatures, the thermoforming process will be compromised even more. It could happen that the film, in short intervals, shows different temperatures. This can arise if the floor of the storage room is cold but solar irradiation has heated the upper part of the film reel. Such inhomogeneous conditions prevent the production of articles with consistently good quality. After leaving the preheating station, the film should be inducted into the film chain rail transport system at a surface temperature of 100 C. To effectively bring the PP film up to forming temperature, radiators are more suited than contact heating plates. In most cases ceramic radiators or quartz radiators will be used. The KTR6 - thermoforming machine is equipped with standard quartz radiators. As soon as the film is heated up over the radiators, precaution has to be taken. It is absolutely necessary that in the format of the forming area integer heating steps are conducted. This ensures uniform warming. If uneven warming occurs over the forming surface of the film, that will cause irregular quality of the formed parts within that batch. To reach uniform temperatures on and within the film, a heating system with differentiated controllable heat zones is necessary. The heat is divided into zones for the bottom and top areas. Both radiators are mounted to a sliding gantry. This rack allows the heaters to be exactly positioned in the area of the film that is warming while the production is going on and can be immediately withdrawn if there is a production stop. Application of heat during a stoppage could have disastrous effects. Long exposure of film to heat can thermically degrade the film or even ignite it and start a fire. For this reason, the heating drive is equipped with a forced movement, which ceases if a power outage occurs and ensures that the heat is off. Bottom and top heat areas have lengthwise and crosswise rows of radiators. These lengthwise and crosswise rows are set to different temperatures so that a certain heating profile over the width of the film is maintained. The outer longitudinal rows of heaters are set warmer than the longitudinal heaters in the middle of the film path. Due to the
193 27.3 The Forming Station 183 Figure 27.3 KTR6 tilting mold (Courtesy of Bosch Sprang B.V.) heat application, the film transport systems must be kept cool. The absorption of the heat through the film transport profiles, however, demands higher ray heating temperatures. Even the chilled thermoforming mold absorbs heat, and loss of heat needs to be compensated for with so - called cross - ray heating control THE FORMING STATION It is amazing how many technological advancements resulted from thermoforming flowerpots. The greater part of design and quality of the molded part is determined by the forming and punching tool and production speed (Figure 27.3 ). The mold production machines are located in air - conditioned rooms. These rooms have hardly any tolerance for temperature fluctuations and humidity. In 24 hours temperature can vary only 0.25 C and within 1 hour only 0.1 C. Such high precision is necessary because the cutting gaps of the forming and punching tool have a tolerance of only a few micrometers. A cutting gap greater than 10 μ m causes problems when punching warm PP film. Safe production is compromised when upper and lower molds have different temperatures, which can lead to dangerously large cutting gaps. When this happens, the machine will be shut down by a safety mechanism. The mold maker has now
194 184 Chapter 27 Production of Flowerpots the very complicated job of finding a compromise between good warmth conduction and abrasion resistance for the material of the die plate. It is just as complicated to cool the formed parts as it is to warm the film for thermoforming and reach the demolding temperature. For this it is essential to design cooling channels around every single cavity, which is a real challenge considering the little space that is available. All cavities need to have the same cooling conditions to achieve the same benefit for all formed parts. The weight of the molding and punching tools is a factor that the designer needs to take into account. Modern thermoform machines with a tilt mechanism allow over 35 cycles per minute. The big flowerpot machine weighs 1800 kg. Reduction of weight is a high priority, since the form and punching tool works in tilt mode at a high - speed work cycle. And great forces build up through acceleration and deceleration. The plug assist starts to move downward and to stretch the warm film when the forming and punching tool is closed. The speed, the design, and the plug - assist material are coordinated to ideally distribute the material for the walls of the part. Plug assists are used when H D where H = depth of draw D = diameter of the part H = 04. ( in some cases = 035. ), D (For parts with a small sidewall demolding angle, <10, and a small bottom-wall radius, < 6 mm, plug assists are put into use when the drawing ratio is 0.35 and smaller.) The plug assist has to provide very good isolation and to resist high temperatures. Also advantageous is a low specific weight to allow a fast process speed. Pressure resistance is essential. Since the plug assist is machined to receive its shape (milling, turning), the material it is made of needs to have a good mechanical workability. The plug assist should ensure evenly distributed wall thicknesses and must not leave marks or irregularities on the thermoformed article. Dimensional stability and high durability should likewise be attributes of the plug assist. Characteristics of the plug assist that influence wall thickness distribution are as follows: Shape and definition of the plug assist Movement of the plug assist Material of the plug assist Temperature of the plug assist The timing of the forming air in relation to the plug - assist movement
195 27.3 The Forming Station 185 Temperature of the semifinished product as it is being formed as well as temperatures of upper - and underside of the semifinished product Sum of the cross - section of ventilation holes to the displaced air volume while the part is formed Contact time of the plug assist with the film 1 The plug - assist material properties relevant to thermoforming are as follows: Ability to be shaped or machined Temperature resistance Abrasion resistance Thermal conductivity Thermal mass (specific heat) Thermal diffusivity Compression heat Surface roughness Coefficient of thermal expansion Abuse resistance Cost A Massachusetts company, CMT Materials, specializes in the production of plug materials. CMT offers a complete line of plug materials for all kinds of uses. Hytac-B1X 2 Hytac - B1X (CMT) is the first plug - assist material to combine the toughness of an engineering thermoplastic with low thermal conductivity of a syntactic foam. Plug assists made from Hytac - B1X will resist the chips and dings associated with production abuse while reducing mark - off and sticking of difficult to process polymers. Hytac - B1X maintains the high thermal stability required to process thermoformed polymers in use today. In addition Hytac - B1X eliminates the machining difficulties of conventional syntactic foams. This material does not produce dust during machining and finishing of plugs. High toughness and durability. With high toughness, machine downtime due to damaged plugs is reduced. Lower downtime decreases costs. Superb machinability. No dust collection equipment or respirators are required due to the large, nonabrasive chips. Plugs can be machined more than three times faster than syntactic foams due to easy chip formation. 1 Thomas J. Murray, Noel J. Tessier, Bernhard Hegemann, Thomas Gallagher, Ted Gabor, and Tim Roberts, Presentation, Investigation of Plug Assist Material Properties Relative to the Thermoforming Process, CMT Material-Brochure, 2010.
196 186 Chapter 27 Production of Flowerpots Excellent temperature resistance. Hytac - B1X is specially formulated for service up 180 C with minimum loss in mechanical properties. Almost all polymers can be replaced by Hytac - B1X. It is less suitable for polyethylene and multilayer film with polyethylene. Hytac-B Sometimes finer plug - assist details are required that are not obtainable or maintainable with syntactic foam plugs. For these high detail applications, where high toughness and easy machinability are required, a special formulated blend of engineering polymer has been developed. Material removal from the blind side of the plug will result in thermal conductivity and overall heat absorption, which approximate syntactic foam s excellent properties. High toughness and durability. With high toughness, machine downtime due to damaged plugs is reduced. Lower downtime decreases costs. Superb machinability. No dust collection equipment or respirators are required for the large, nonabrasive chips. Plugs can be machined over three times faster than syntactic foam due to the easy chip formation. Excellent temperature resistance. Hytac - B is especially intended for service up to 180 C with minimum loss in mechanical properties. Hytac - B can only be used for polystyrene and polyvinyl chloride; it is less suited for other synthetic material. Hytac-FLX Hytac - FLX is one of the latest developments in high - performance syntactic materials. This thermoset copolymer syntactic is unique in combining the toughness and flexibility of a thermoplastic material with thermal stability of a thermoset. Like other syntactic materials, FLX has a low thermal conductivity and specific heat needed by thermoformers, yielding better material distribution and clarity, reduced mark - off, lower start - up and cycle times, and lower plug operating temperatures. It also offers the added machining benefit of little or no dust and minimal wear on tools. This tough syntactic can even be easily polished to a smooth surface for a desired part finish. FLX may be used in plug applications especially suited to areas requiring high durability. As compared to standard thermoset epoxy syntactic, FLX has been designed with 1.5 times the flex strength and more than five times the toughness. Most important, with more than four times the elongation to break, FLX will withstand the most rigorous plug environments without the brittle failure often encountered in epoxy syntactic. The advantages of the FLX material are: Good dimensional stability Excellent toughness and durability
197 27.3 The Forming Station 187 Superb machinability Temperature resistance Low thermal conductivity Hytac-WF Hytac - WF is an epoxy syntactic plug - assist material that was designed to reduce problems associated with conventional epoxy syntactic. Hytac - WF will result in improved clarity for A - PET and other clear polymers. It will reduce sticking of difficult to process polymers such as PE - HD and C - PET. Low thermal conductivity and specifi c heat. The syntactic foam structure of Hytac - WF maintains the low thermal conductivity desired in a plug - assist material. High strength and stiffness. Hytac-WF contains a high-strength glass sphere providing nearly three times the strength and twice the stiffness of standard epoxy syntactic foams. Dimensionally stable. The low coefficient of thermal expansion means that the plug maintains its shape over a wide temperature range. Smooth surface. The glass sphere used in Hytac - WF has a diameter more than 50% smaller than those found in conventional syntactic materials. This translates to a smoother surface. Excellent temperature resistance. Hytac - WF is specially formulated with an epoxy resin that maintains a high modulus at elevated temperatures. Light weight. This increases the life of capital equipment due to the reduced wear and tear on moving parts. Easily machined. Hytac - WF can be easily machined to any size or shape using conventional equipment. Hytac-WFT Hytac - WFT is a material combining the unique technologies found in high - strength Hytac - WF and the smooth surfaced Teflon containing Hytac - WT. The result is a syntactic plug - assist material with a smooth hard surface able to resist temperatures up to 219 C. The intended uses of Hytac - WFT are for the most difficult film sticking problems or in situations where an extremely smooth surface is critical for the quality of the part. The material has also found applications in areas where excessive buildup of residue on the plug from the film is a problem. It is thought that the low heat transfer properties of the syntactic plug help reduce residue buildup to the lower plug temperature. A Teflon - enhanced surface makes removal of impurities easy.
198 188 Chapter 27 Production of Flowerpots As with other syntactic materials, Hytac - WFT offers the following advantages: Low thermal conductivity and specific heat Dimensional stability Excellent temperature resistance Light weight Variety of shapes and sizes Improved toughness Plug Materials Polyoxymethylene ( POM) (e.g., Delrin [DuPont], Ultraform [ BASF]) Low-priced plug material Problem-free workablility Excellent material for transparent parts Unsuitable for PVC Low permanent temperature, max. 110 C to 120 C Surface becomes smoother, forms cracks, and turns brownish In most cases the plug needs roughening up only after 30 to 100 work hours, except for polished plugs for transparent parts Start-up problem when processing PS film, a determent due to a cold plug assist. Hardened Felt No start-up problems with PS or PVC films Not qualified for transparent parts due to severe marks on the part Not qualified for PP due to adherence to film Easy connection with the plug-rod possible Relatively expensive material Impurities on the formed part due to felt fibers Syntactic Foam (e.g., Syntac 350 [Cumming, USA], Hytac W [ CMT]) Universal in use with little limitations Machining creates dust Permanent use resistance of 180 C
199 27.3 The Forming Station 189 Definition of Syntactic Foam The name of syntactic foam is derived from the Greek word syntax, meaning allocation. In this case it refers to the compounding of epoxy resin with microscopic hollow glass beads. The foam - like material is cured and becomes pressure resistant. Syntactic Thermoplastic, Hytac-B1X Universal use, even for transparent parts No dust while machining Extremely break-proof Good cohesiveness Definition of Syntactic Thermoplastic As with syntactic foam, microscopic small hollow glass beads are mixed with a thermoplastic material (matrix) in a defined composition. Polysulfone ( PSU) Polyamide 6 molded with glass beads, PA 6 G Less dense than POM Less thermal conductivity Specific Values of Plug Materials For the properties of plug - assist materials and decision matrices, including choice of plug - assist material (independent of material price), see Table The U.S. Company CMT specializes in the production of materials for plugs. Since different synthetic materials have different processing properties, it is necessary to choose a plug assist depending on the particular properties of the film. At the moment there is no material that can be used for all purposes and that simultaneously gives the best formed - part quality. Tables 27.1 and 27.2 show the properties of plug materials and their suitability for the corresponding synthetic material. Table 27.1 Decision Matrix: Choice of Plug - Assist Material (Independent of Price) Plug-Assist Material Semi-Finished Product Material Syntactic Thermoplast (Hytac B1X) Syntactic Foam (Duromer, e.g., Syntac 350) POM PA6 GGK Felt PS-HI x x? x PP x x x (x) A - PET x x PVC x x x PE - HD?
200 Table 27.2 Hytac-Materials Product Color Service Temperature ( C) Thermal Conductivity (W/m K) Density (kg/m3 ) Compressive Strength (MPa) Coefficient of Thermal Expansion 10 6 (m/m/ C) Hytac-W White Hytac-B1X Light blue Hytac-WF White Hytac-WFT Green Hytac - FLX Almond Hytac-B Blue Hytac-C White Hytac-LP Almond
201 27.4 Forming Air 191 Machine valve Tool valves per row Tool valves per row Figure 27.4 Air-Save-System (Courtesy of Bosch Sprang B.V.) 27.4 FORMING AIR The supply of forming air is important for cycle time and the production run. There are systems of forming - air supply that attempt to establish the forming air expressly within the period of forming. The Air - Save - System from Bosch Sprang B.V. is able to fill an entire forming mold in seconds with a 6 - bar forming pressure (Figure 27.4 ). Such filling speeds are dedicated mostly to air bag systems produced by the automotive industry. The set - up times and costs can be lowered when forming inserts, ejector bases, and plugs are changed with a quick - change system. This enables the production of several different articles with one base tool block. These articles can vary in volume, draft angle, and depth of draw. The punching diameter stays the same. One of the newest developments of Bosch Sprang B.V. is called Tag-Slots. To label the flowerpots filled with soil and seed, a method was established that sticks a small label in a slot located in the U - shaped rim of the flowerpot. The slots are made during the process of thermoforming. Special punching tools secure the wasteless cut in the rim of the pot. After the forming, punching of the pot, and simultaneous punching of the tag - slots are done, the tool tilts over and delivers, with the ejector bottom, the pots to a robot unit that transfers the whole array to the punching unit for punching the holes in the bottom of the pots. These holes in the bottom are necessary for irrigation and
202 192 Chapter 27 Production of Flowerpots ventilation. The number and size depends on the type of the plant, and this was researched in academic studies. In some nurseries the water level of a tide is simulated to yield the best growth for the plants. Of course, the size of the hole plays a big part in this. When the location, number, and size of holes are ascertained, the punching can tool be designed. Up to 500 holes per punching cycle can be produced, and in this application, at 26 cycles per minute. Another step in the thermoforming process is the stacking of the formed parts. The stacking height is determined by how many flowerpots can be stacked together. This is influenced by the shipping boxes or carrier pallet, so stacking height is a cost factor. The wall thickness distribution is a big factor for stacking height. Therefore it is important to observe the plug design and plug speed. The stacking of the flowerpots and punching of the bottom holes is fully automated. Stacking takes place after the demolding of the punched pots from the mold with the use of a 75/54 Stacker from Kiefel GmbH. Stacking is accomplished with all parts taken from the forming tool with the help of a robot. The robot puts the flowerpots on a stacking carrier that is accompanied by three additional carriers on a rotary carousel. The carousel rotates the flowerpots to the punching station for bottom holes and, after this, to the position where the formed parts are pushed into the stacking cage. From there they move to the final stage of packaging. Many flowerpots have printed designs on them. With modern printing machines, which can print up to six colors on the pot, it is possible to bring photo - realistic pictures to the pots. It is possible to have the print in line with the tag - slots CHALK AS A FILLER Chalk is calcium carbonate (CaCO 3 ). In different forms calcium carbonate can be found as marble or limestone. The chalk in plastics technologies, and especially in semifinished products, is a popular filler for thermoforming Calcium Carbonate in Thermoforming Applications Calcium carbonate serves as a functional additive in thermoforming. One of its major applications is for manufacturing polypropylene trays, which are widely used in the packaging of food and disposable items. Other applications include plant - propagation trays, automotive parts, construction material, household items, and plant pots, which are described above. Many advantages can be obtained by using calcium carbonate in thermoforming applications. 3 Calcium Carbonate in Thermoforming Applications, Omya Applied Technology Services, Segment Plastic, Review, Technical Information Plastics R4-05, Omya International AG, Oftringen, Switzerland, 2009.
203 27.5 Chalk as a Filler Natural Calcium Carbonate Mineral additives open up a variety of opportunities for polyolefin processors to improve their products in a cost - effective way. Natural ground calcium carbonate, both coated and uncoated, is the most important mineral in the plastics industry. There are many reasons to use it in polyolefins: High chemical purity Nontoxic, with excellent sensory properties and meeting food safety criteria Particle size distribution that allows a surface coating to be tailored to a particular application Excellent dispersibility, capable of being readily processed with reliable mechanical properties Cost-efficient Finely ground calcium carbonate is usually incorporated into the polymer as a ready - to - use compound or masterbatch. The calcium carbonate is then processed as a granular molding compound. For mass - production applications, inline compounding or direct extrusion is a possible alternative. In this case the mineral is added directly as a powder without first being compounded. In order to put the properties of polypropylene (PP) and calcium carbonate modified PP into context with the properties of polystyrene (HIPS, high impact polystyrene), HIPS is presently a widely used material for thermoforming but is being progressively replaced by polypropylene Advantages of Calcium Carbonate Higher thermal diffusity and improved mechanical properties are the most important advantages of calcium carbonate in thermoforming applications. Higher thermal conductivity results in higher output. Since the end product has better mechanical properties, it can be manufactured with lower wall thickness, which allows raw material costs to be reduced. Sheet Extrusion Calcium carbonate modifies the properties of polymer melts. The rate of all heating and cooling processes is determined by the material s thermal diffusivity. Calcium carbonate has a thermal diffusivity that is many times greater than that of most polymers. It is therefore an effective additive for increasing the thermal conductivity of polypropylene. This results in faster melting in the extruder, faster cooling on the cooling roll, and a more homogeneous melt temperature. The faster cooling permits faster machine speeds as calcium carbonate reduces cooling capacity. Another benefit of
204 194 Chapter 27 Production of Flowerpots calcium carbonate is the low coefficient of thermal expansion, which remains constant over a wide temperature range. In contrast to semicrystalline polymers, such as PP, thermal expansion is greater at the melting point. Calcium carbonate modified polymers therefore have a lower melt volume than the virgin polymers. This fact, together with decreased adhesion to barrel wall, has found to reduce torque and pressure during extrusion. Overall, modification of thermoplastics with calcium carbonate offers the opportunity to significantly increase output to an extent depending on machine equipment and processing conditions. The introduction of calcium carbonate into the polymer matrix reduces the amount of viscoelastic material in the formulation. Thus it reduces typical viscoelastic phenomena, such as die swell, neck - in, and shark skin. The mineral particles increase the internal shear forces, and therefore the melt viscosity. This improves the dispersion and distribution of other additives. Thermoforming The extruded sheets can be thermoformed from the roll, either directly or after storage. In the latter case, semicrystalline polymers, such as PP, are often heated in two stages, first preheated in circulating air oven and then by a main heater. In general, only a thin surface layer is heated directly. The heat is transported by thermal conduction into the core of the film. The higher thermal diffusivity of calcium carbonate therefore improves the heating process. On roll - fed machines equipped with film preheating, the cycle time is determined by the cooling time. The higher the cooling rate, as made possible by calcium carbonate, the more significantly the output is increased. Productivity can be increased by 12%, in some cases even by 35% or higher. Semicrystalline polymers such as PP have a very narrow processing window, which is the result of the sharp transition from a rubbery elastic solid to a relatively low viscosity melt. The addition of calcium carbonate modifies the melt rheology, imparting a pronounced pseudoplastic behavior. That means that the melt has a high viscosity at low shear rates. Consequently, there is a broader temperature range in which the material can be successfully shaped. Moreover, the pseudoplasticity, together with the lower thermal expansion, reduces the sagging of the film. Stretching during film transportation, which is necessary for most semicrystalline plastics, can be reduced accordingly. The deformation behavior of the molten polymer changes from viscoelastic to plastic. Correspondingly, the definition (shaping fidelity) of the parts is visibly improved. This leads to more clearly pronounced surface details and sharper edges. The lower thermal expansion, together with the lack of volume expansion at the melting point, reduces the processing shrinkage of the formulation. Correspondingly, the mold can be designed with less allowance for shrinkage. The calcium carbonate particles embedded in the plastic surface reduce the forces of adhesion between the material and the mold, which facilitates demolding. Punching out is also made easier in many cases.
205 Property Improvements 27.5 Chalk as a Filler 195 In thermoforming applications, between 10% and 40% calcium carbonate is added. The mineral additive increases the stiffness of polymers. While the yield stress of identical parts is reduced, the cross - machine direction of breaking elongation is significantly increased, resulting in more durable final products. The improved impact strength and reduced directional dependency of the breaking stress are principally the result of the increased isotropy of the material. The aspect ratio of calcium carbonate, defined as the ratio of particle length of thickness, is approximately 1:1. That makes it impossible for the particles to align themselves in a preferred direction. In addition the better homogenization by minerals reduces the molecular orientation of the polymer. This effect can be demonstrated by infrared studies. A further advantage of the lower orientation, synonymous with less frozen tension, is significant reduction of the warpage of the thermoformed parts. In many cases the maximum load (top load) that the thermoformed parts can withstand is increased, especially in applications with a low forming ratio. The plant pot has a high deep draw ratio and requires certain precautions in processing, especially because of the greater amount of calcium carbonate in the polymer matrix (more than the described 35%). The improvement of mechanical properties often allows the film thickness to be reduced while maintaining stability requirements. Film containing calcium carbonate is gauged down in thickness to the extent that the thermoformed parts are just as heavy as the virgin PP regardless of the higher density of the calcium carbonate in the film. The results show that the top load of the thickness - reduced film with 20% calcium carbonate is even higher than that of the virgin PP. Molecular orientation and crystallinity have an influence on all mechanical properties. Both parameters are affected by the processing conditions and the thermoformed part s design. The heating and cooling conditions, in particular, as well as machine speeds during extrusion and thermoforming, offer the possibility of optimizing the mechanical properties. In Europe, if a film must be in direct contact with acidic foods (ph < 4.5), use of multilayer films is recommended with calcium carbonate in the core layer to meet EU limits of migration. The more that the polymer is replaced with the calcium carbonate, the more tortuous the diffusion path becomes, but the barrier properties of the parts produced are better. The polymer is more permeable than calcium carbonate (impermeable). Permeability to water vapor and oxygen fall with increasing calcium carbonate content. In the absence of pigments, calcium carbonate produces an opaque white color in transparent plastics. Black, dark - colored, cream, or white pigmented formulations do not require an additional color to the masterbatch. If fluorescent colors are required, especially when pigment systems with relatively low opacity such as red and blue are used, it may be advisable to use multilayer sheets. Polyolefins have very low surface energy. Anchorage of printing inks is therefore restricted. The addition of calcium carbonate improves printability, since it has
206 196 Chapter 27 Production of Flowerpots a high surface energy and a certain micro roughness. A matting effect may occur if very high amounts are added. Cost Reduction While polymer prices have risen greatly in recent years, the price of calcium carbonate has stayed relatively stable. This opens up the possibility for significant cost savings, besides the improvement in mechanical properties that often results and the reduction of film thickness. The increased stiffness achieved with calcium carbonate has interested many researchers. For a case study, the Young s modulus for carbonate - reinforced PP film was measured. The data were used to determine the film thickness at which the desired stiffness could be achieved. It was found that the film with 30% calcium carbonate can be reduced in thickness by 13%. Based on April 2006 prices, that represents a 14% reduction of material costs; without reduction of film thickness, the cost saving would be 2%. Also, the production costs are reduced by the increased output as a result of higher thermal diffusivity. To estimate the overall costs, a batch size of 10 million cups was chosen as an example. The calculation started with μm-thick PP film produced offline. The film with calcium carbonate was reduced in thickness to obtain the same stiffness. The time was determined on an Illig RDM 75 k automatic roll - fed machine with infrared heating and preheating of the PP reels. The cups were pressure formed with an 18 - up aluminium mold. The manufacturing costs were reduced by 12% with 30% calcium carbonate Summary The use of calcium carbonate provides several advantages in thermoforming applications. The improved thermal efficiency throughout the entire processing chain pays off in higher output. The improved mechanical properties result in reduced wall thicknesses. Overall, the introduction of calcium carbonate is a very economically attractive solution for film manufacturers and thermoformers.
207 Chapter 28 Steel Rule Die Punching Written in cooperation with Dieter Kamml, Kiefel GmbH, Freilassing, Germany 28.1 BASICS The purpose of punching is to separate the formed parts from the film web. In conventional thermoforming with roll - fed machines, there is a distinction between matched metal punching and steel rule die punching. Lately, ultrasonic systems are also being used for punching out thermoformed parts. In this chapter we focus on steel rule die punching. Band steel, milled, or forged cutting lines are used for steel rule die punching. 1 Band steel cutting lines can be purchased in trimmed, sharpened, and polished versions. Trimmed band steel has many applications. Sharpened band steel can be ground and used to cut hard and coated materials. Polished band steel cutting lines tend to have very smooth surfaces on the cutting edges, and provide very good punching and bending behavior. The low friction of the smooth surfaces at the cutting edges enable the punching to be precise SHAPES OF CUTTING EDGES Steel rule die knifes can be supplied in a variety of cutting edge shapes. They can be worked one - sided, double - sided, with one - sided or double - side facet. For special applications there are cutting edges that are offset or centered with different cutting angles. There are even linear and concave cutting edges. Steel rule dies are subject to wear. The width of a new knife is about mm. Higher punching pressure is needed and bad cutting occurs in some applications 1 Presentation, Know How Verpackung, Kiefel GmbH, Freilassing, Germany, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 197
208 198 Chapter 28 Steel Rule Die Punching Figure 28.1 Wear of cutting edge of steel rule die (Courtesy of Kiefel GmbH) when the cutting edge width reaches 0.2 mm (see Figure 28.1 ). For successful punching, the punching counterplate has great influence. The punching counterplate can be made from aluminum, steel, or stainless steel. Punching tools are part of the format set installed in the punching presses of the thermoforming machine. They are described by the punching force - deflection graph. This is determined using four load cells. Each film material has its own characteristic diagram CREATION OF ANGEL HAIR DURING STEEL RULE DIE CUTTING Thermoformed parts have to be separated from the film web during forming or after they are formed. After separation the film web is called a skeleton. Separation of formed parts from the film web in roll - fed machines is mainly done by punching. Different punching methods are available for this purpose. One version uses the steel rule die system. This process is important in the packaging industry. Another method of punching utilizes a matched metal die. This section of the chapter focuses on the phenomenon of angel hair being created while using a steel rule die. This punching method mainly creates angel hair when grades of polystyrene, its blends, and also ABS are being processed. In some rare instances angel hair can be created while processing filled PP or C - PET. Angel hairs are polymer fibers that appear during the punching process. These fibers have thicknesses of 0.01 to 0.1 mm and are usually several centimeters long. Angel hair is not only an optical defect; it can contaminate the packaging, the product, and the machine.
209 28.3 Creation of Angel Hair during Steel Rule Die Cutting Development of Angel Hair Angel hair may occur as different mechanical properties are incorporated in the material (e.g., hard and elastic portions). In addition, plastics with a soft layer of lacquer might be subject to the creation of angel hair. The development of angel hair can be counteracted by taking certain measures. The so - called melting cut lowers the probability of angel hair being created. In addition, the shape of the steel rule die may affect the creation of angel hair Influence of Steel Rule Temperature on the Creation of Angel Hair The temperature of the steel rule die has a large influence on the creation of angel hair. Tests as well as practical experience show that heated steel rule dies significantly decrease the creation of angel hair. Some machines and applications enable the heating of the steel rule die up to 120 C. At these temperatures, punching forces and wear of the steel rule die decrease considerably. Problems arise, however, if the machine, forming mold, or application does not permit the above - mentioned temperatures, such as when punching occurs directly in the forming station. In this case the heating of the steel rule die would be counterproductive to the cooling of the mold. The cutting edge compresses the polymer (e.g., PS - HI) under the steel rule die. The two phases in the polymer cause cracks to develop under the steel rule die. The material is not punched out 100%; some parts remain underneath the steel rule die. This and the small specific force account for the longer service life when PS is punched Influence of Film Material on Creation of Angel Hair Film material also can cause angel hair to be created. The punching behavior of the various polymers differs significantly. But also within a certain type of polymer the choice of grade and recipe can increase or decrease the creation of angel hair. The sharpening and geometry of the steel rule die are important factors. Ground steel rule dies are in most cases better than trimmed ones at reducing angel hair.
210 Chapter 29 Production of Meat Trays Written in cooperation with Uwe Heer, Kiefel GmbH, Freilassing, Germany A trend of the last 10 years that has not only given the material and machine developers new challenges but also created a new market is that of the PP meat tray (Figure 29.1 ). This article was created to meet the packaging requirements for fresh meats marketed by supermarkets and discounters. The PP tray is only part of the packaging system. Basically, the packaging procedure calls for modified atmosphere to be used and so is referred to as modified atmosphere packaging (MAP). MAP is really subsidiary to protective atmosphere packaging. If you look closely, you will find the protective atmosphere packaging subdivided by method of manufacture: Vacuum packaging Active packaging MAP packaging, which is two types, equilibrium modified atmosphere packaging (EMAP) and controlled atmosphere packaging (CAP) 29.1 VACUUM PACKAGING During vacuum packaging, air is removed from the package to create a vacuum inside the package. For many decades this procedure was used to pack perishable foods such as meat, cheese, and coffee ACTIVE PACKAGING Active packaging is still at the early stages of development. Attention is mostly directed toward oxygen scavengers. The wrapping film is so equipped that the film absorbs the oxygen from inside the package. This ought to extend the shelf life. Over Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 200
211 29.3 MAP 201 Figure 29.1 Thermoformed meat trays (Courtesy of Kiefel GmbH) the next years only a few packagers are planning to implement this technology. Some countries have legal concerns regarding the application of this procedure MAP MAP was developed toward the end of the 1920s to pack meats, and recently MAP has also been used for cooled convenience food, crackers, and coffee. The advantage is that fragile foods are less exposed to mechanical strain with MAP than with vacuum packaging. When using MAP, the air is replaced with a gas mixture that consists, depending on the application, of carbon dioxide, nitrogen, and/or oxygen (Table 29.1 ). The gas atmosphere controls chemical, enzymatic, and microbiological activities. The shelf life can be greatly extended (Table 29.2 ). MAP technology is also called gas flushing. The advantages of MAP are many: Shape and consistency of the product are unaltered. Vitamins, taste, and fat content are preserved. The natural color of the product does not change. The use of preservatives can be reduced and even eliminated. The shelf life can be maximized by 50% to 400%. The longer shelf life of products brings advantages concerning their storage and distribution. Commercial loss is reduced. The product can be attractively presented in closed cases in retail markets. Easier separation for sliced products.
212 202 Chapter 29 Production of Meat Trays Table 29.1 Gas Mixtures for Food Products Mixture of Gas (%) Product CO 2 N 2 O 2 Cheese Unsliced cheese Sliced cheese Dried cheese (e.g., Parmesan) Raw meat 30 (25) 0 (5) 70 Poultry Processed meat and sausage Bakery products Prebaked products Pieces of cake Convenience food Ready to eat dishes Deli dishes (e.g., salads) Fresh pasta Table 29.2 Shelf-life Extent with MAP Days Product Exposed to Air MAP Beef 4 12 Pork 4 9 Poultry 6 18 Prepared foods 7 28 Fish * 2 10 Bread 7 21 Fresh pasta dishes 2 50 (60) Coffee (18 months) *For packaging fish, MAP applications should be done only with the utmost caution! In contrast, the disadvantages of MAP are few: Production cost is higher (machine, semifinished products, gas, etc.). Differential combinations of gas may be necessary. Special machines and training of the workforce is necessary. Each package has a higher volume.
213 29.4 Production Process for the PP Tray 203 The entire MAP package consists of the PP tray, the fleece in the tray, the sealing film, and, of course, the fresh meat. The advertised expiration date is also part of the package and is valid only once the package is opened, and storage accordingly is away from light in a dry and cool environment. The recommended storage temperature is +2 C and +4 C. The sealing film is considerably thinner than that of the tray film, and it is almost always a multilayer film. The sealing film is often equipped with special qualities, for example, antifogging. The thermoforming film for the tray is made of PP homopolymer (see Chapter 36 ). In most instances a nucleated type of film is used, mixed with small amounts of random copolymers. When there is a special demand, for example, a very long shelf life ( > 6 days), multilayer films are used instead of the usual mono films. The multilayer structures are made of PP adhesive EVOH adhesive PP. The EVOH acts as the oxygen barrier. To produce a structure made of PP and EVOH (ethylene vinyl alcohol), and in order to receive connection between the layers, a primer (adhesive) is used. But because of the high cost of EVOH, in the multilayer structure it is used in less than 10 μ m. EVOH is hygroscopic and is protected from humidity by the PP layers on the outside of the structure. Ultrasonic bonding or a hot - melt glue is used to fix the absorbable fleece either inline or offline (in a downstream process) in the tray. Requirements for MAP packaging are extension of shelf life for microbially vulnerable foods, restriction of the growth of microorganisms, extension of deadlines for distributive trades, retail markets, and private homes, economization of delivery, avoidance and reduction of return shipments, cover protection for packaged goods, as well closed cases to protect the goods in retail markets PRODUCTION PROCESS FOR THE PP TRAY For the production of meat trays made of polypropylene, automated forming utilities with steel rule die technology are used. These machines provide a combination of forming and punching at the forming station. A KMD 85 BFS thermoforming machine from Kiefel GmbH, Germany, is the type used for this example. Another option is to produce PP trays not in combination, but with forming and punching separate. But this would mean an additional station. Then there is the question of precision. With combined forming and punching the outline is less consequential because the shrinkage of the formed trays and free shrinkage of thermoforming film pertaining to accuracy of fit is less relevant. The film reel station feeds the thermoforming machine with film. Alternatively, the thermoforming machine may be directly connected to an extruder. For the processing of PP, a precise heating system with adequate heat is essential. Ideally, the heating system should be equipped with the option of a single heating element setting. For precise temperature steps based on an indexing length, a cooled cover plate is necessary. To keep the heating temperature for the film as precise as possible, the use of infrared pyrometers is recommended. The goal is to homogeneously heat up the film. Over the entire forming area a constant and evenly distributed temperature is important to keep the conditions within the utility (shot) the same.
214 204 Chapter 29 Production of Meat Trays If the meat tray is produced with inline extrusion, the temperature conditions across the film cross section are different from those without. The film is directly guided from the extruder to the thermoform facility so that the core of the film stays relatively hot. The outer layers of the film cool down on their way from the extruder to the thermoform machine. So, before the thermoforming process can take place, the heating system of the thermoforming machine has to bring the temperature of the film back up to the processing temperature. For this, only relatively little heating is necessary, which is a certain economic advantage. Another temperature change occurs across the cross - section of film thickness when the film is coming off the reel, without inline extrusion. That brings the heater of the thermoforming machine to heat from the outside to the inside. These varying temperature conditions can lead to varying flow conditions of the thermoforming film. The flow behavior has a direct influence on the wall thickness distribution of the molded components. Temperature tuning needs to be considered when introducing new thermoforming molds. It is important to watch for the so - called film sagging effect and to counteract that as the polypropylene film is being heated in the thermoforming machines. For processing PP film it is essential to use a thermoforming machine with a spreading film transport system. Better results can be obtained when there is an additional spreading implemented before the heated film is guided through the forming station. To maintain product quality, it is advantageous for the thermoformed parts to have all relevant movements powered by a servo motor. The same applies to the plug - assist drive. A servo - motor - driven plug assist prevents stretchmark damage to the formed parts. It works with positioning accuracy and can be operated with acceleration and speed profiles. For a faster and reproducible thermoforming production, the forming pressure must be applied in the mold quickly and also released again quickly from the forming mold. A good practice is to monitor the pressure in the mold with a sensor. In addition, special valves are available on the market that apply and release the air pressure within tenths of a second. In the case of the meat tray, the formed parts are punched with a steel rule die tool in the forming station (see Figure 29.2 ). It is also possible in this procedure to have forming and punching separate (see Figure 29.3 ). But it is advantageous to do the punching in the forming station, since that eliminates the risk of a forming and punching offset on the formed parts. The fleece for absorbing the meat juice can be applied in the next station, right after the forming station NEW DEVELOPMENTS The field of pressure - forming machines is experiencing a trend toward more economically efficient mass production. 1 Machines are under development that can reduce the production costs of the forming parts. One such development is the Kiefel 1 Pressure forming machine Speedformer KMD 80, Brochure, Fa. Kiefel, Freilassing, 2010.
215 29.5 New Developments 205 Figure 29.2 Forming and punching station (Courtesy of Kiefel GmbH) Speedformer KMD 80, which, thanks to issues of energy recovery, has demonstrated low energy consumption, an operating speed of up to 65 cycles per minute, and reduced material consumption through an optimum utilization of the forming area and an innovative film-conveying system. The system uses a forming area measuring mm. The innovative drive provides high clamping forces combined with highest precision. An innovative chain guide system keeps the feed rate exactly constant. The thermoforming offers exceptional smoothness at high operating speeds in all the movement sequences Symmetric Drives New, reinforced symmetric drives for the forming and cutting station with four columns, four cams, and two servo motors provide the best performance, thanks to reduced vibration. Other features are an extended service life, due to larger
216 206 Chapter 29 Production of Meat Trays Figure 29.3 Thermoforming machine Kiefel KMD 85 B (Courtesy of Kiefel GmbH) reinforced drives, and optimized positioning of the plate - guide lubrication points, which reduces the risk of the film material becoming soiled or contaminated Reduced Energy Consumption New design developments place even greater emphasis on reduced energy consumption. The KMD 80 system provides reduced production costs, thanks to the use of more - efficient heating elements. It enables energy recovery via servo motors. During the braking phase, the motors function as generators to feed energy back into the system. In addition, there is reduced compressed - air consumption, due to the servo - motor - actuated clamping - frame mechanism. The servo motor is more cost - efficient than a pneumatic drive system. The machine has a new way to cool the film temperature measurement device without blown air, and this reduces air consumption Yoke Adjustment for the Lower Drive The motorized adjustment of the lower and upper yoke allows adaptation to the required position. Simpler tools of different heights can be used. There is no need for shims or readjustment due to machine wear of tool components Computer-Aided Teaching The identification and optimization of adjustment parameters (times, movements, stroke - length, heater settings, etc.) are carried out automatically by the system
217 29.5 New Developments 207 software (e.g., Kiefel CAT system). The operator only needs to enter the main tool and film material data into the control system, which does everything else independently. The use of computer - aided teaching systems yields cost reductions because of the shorter tooling times. Reduced staff costs, due to the elimination of the need for specialist personnel, is another benefit. The machine s simple operation makes it easy to use. An optimized program for maximum output and best - possible product quality can also be applied using the computer - aided teaching systems Film Chain Transport System Horizontally, the aligned chain for the index drive system has a greatly reduced chain profile. The essential savings of material is due to an optimized combination of a new clamping - frame/chain profile. The system permits the use of simpler tools, as the profile requires less space. Ideal film temperatures remain even at the edges, due to optimized profile geometry. The horizontally aligned chain enables a longer service life. The pull on the film material is taken up by the chain rollers, which greatly reduces wear due to friction Index Direction: Left to Right or Right to Left The direction of the machine can be specified in the planning phase according to the production process and the conditions in the production plant. The benefits are as follows: Reduced floor space back - to - back: clearance between two mirrored machines can be reduced drastically. Reduced staff costs: a single operator can operate two machines simultaneously from the same workstation.
218 Chapter 30 Multilayer Films for Thermoforming Applications Multilayer films are applied when, for example, there is demand for improved product protection, extension of the shelf life of a packaged product, and scarce material usage. For these reasons multilayer films for thermoforming applications must possess the following capabilities: High oxygen, gas, water vapor, and aroma barrier High product neutrality Light protection and UV barrier Excellent thermoformability and sealability Good mechanic characteristics Good printability Peelability Another characteristic concerning applications for convenience food should be temperature resistance. The above - described requirements are fulfilled through the use of different polymer materials. In order to reduce costs for certain applications, multilayer films can be used but with each layer consisting of the same type of plastic. For the inner layer of the film, recycled material is often used. So - called double films are used when large film thicknesses or an even distribution of the mechanical characteristics are desired. Double films are assembled from the same basic raw material. Another application area for the use of multilayer film results when it is necessary to sterilize the packaging material, as is the case in many applications. With form, fill, and seal machines, mainly three sterilization methods are used: treatment with hydrogen peroxide (H 2 O 2 ), container sterilization with heat, and the neutral aseptic system (NAS, a system patented by the company Erca Formseal). In NAS Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 208
219 Chapter 30 Multilayer Films for Thermoforming Applications 209 another polypropylene layer is applied to a multilayer film. This PP layer is taken off within the FFS line, and thus a sterile surface is laid open. This means that the PP layer is sacrificed and is not a component of the finished pack. The advantage of the NAS method is the fact that no chemically active ingredient is necessary for the disinfection of the packaging material. Multilayer films can be produced by the following methods: lamination, coextrusion, and lacquer coating, or by a combination of these methods. There is a difference between similar and dissimilar films. For dissimilar films an adhesive layer is necessary for the realization of good composite characteristics of the individual polymer layers (e.g., PP AL EVOH AL PP). Today, chloric plastics, for example, PVC and PVDC, are no longer accepted by retailers and consumers. Their excellent barrier characteristics have had to be replaced by a combination of other plastics. The barrier effect against water vapor, oxygen, and flavoring substances is important for all food packaging. The retention of nitrogen in modified atmosphere packs (MAP) is increasingly significant. The thickness of multilayer films ranges from 20 μ m to 1.5 mm, whereas the barrier layer accounts for at most 3% to 10% of the complete thickness of the film structure. Therefore, due to their thickness range, multilayer films are used for flexible packaging as well as for rigid packaging. The quality of a thermoformed part depends not only on even material distribution but also on the minimum thickness of the barrier layer. In other words, for the thermoformed part, the complete thickness of the film as well as the thickness of the barrier layer are important. Multilayer films for FFS applications mostly consist of carrier layers, barrier layers, heat sealing layers, and adhesive layers. Carrier layers. Polyethylene terephthalate (PET), polypropylene (PP), polyvinyl chloride (PVC), polyamide 6 (PA), polyethylene (PE- HD), polystyrene (PS), ionomer, and transparent (cellulose) film. Barrier layers. Polyvinylidene chloride (PVDC), ethylene vinyl alcohol (EVOH), polyvinyl alcohol (PVOH), polyacrylonitrile (PAN), aluminizing or SiO x -vaporization, and aluminium foil. Hot sealing layers. Polyethylene (PE-LD, PE-MD, PE-HD, PE-LLD), ethylene vinyl acetate copolymer (EVA), ionomer, MSA - grafted polyolefins, and polypropylene (PP). Adhesive layers. Glue (glue lamination), primer (extrusion coating), ionomers, EVA, EAA, and ozone (coextrusion). A common multilayer film with high barrier characteristics against oxygen is PP EVOH PP, consisting of polypropylene outer layers, two adhesive layers, and the EVOH barrier layer. But, instead of using compact layers, it is also possible to include foam layers in a film. Packages made of foam films are lighter and provide insulation advantages. Concerning barrier films there is a difference between heightened and high barrier characteristics. PS/PET-G and PET-G/PS/PET-G feature heightened barrier characteristics. These structures are used for aliphatic products such as margarine,
220 210 Chapter 30 Multilayer Films for Thermoforming Applications butter, and cheese. If a water vapor barrier for aliphatic products such as cheese, margarine, butter, honey, marmalade, cosmetics, and pharmaceutical products is necessary, then PS/PE/PS or PS/PE is used. Because high barrier characteristics are required against oxygen, water vapor, gas, or aromas for the packaging of pharmaceutical products and moisture - sensitive products such as soft cheese, fruit drinks, milk, and desserts, and because pasta, meat, salad, marinated fish, or sauces must be packaged under modified atmosphere, it is necessary to use the high - barrier plastics PVDC or EVOH for the manufacturing of the film. The gas barrier characteristics of EVOH are influenced by moisture; this means that the barrier characteristic worsens beginning with a relative air moisture of 80%. The barrier characteristics of PVDC are not influenced by moisture. Typical composite films are PS EVOH PS, PS PVDC PS, PS EVOH PE, and PS PVDC PE. The composite PP EVOH PP is used if the packages must also be suitable for pasteurization and sterilization or for heating in microwave ovens. If the customer wants to reseal the package, then the film must possess a reseal layer. Modern packaging for convenience foods guarantees a longer shelf life of the food. The reseal layers are adapted to the respective application. For example, the number of times that the lid film of a pack of sliced cheese with a peel layer is resealable must be equivalent to the number of cheese slices in the pack. As is evident, many packaging applications can be realized with thermoformable multilayer films, and the packages are indeed high-tech products.
221 Chapter 31 PET in Thermoforming Applications Over the past two decades PET (polyethylene terephthalte) gained rank among the top five of thermoplastic resins. 1 In film and sheet selection, a variety of different material types are available: A-PET PET-G Multilayer film GAG (PET G/A PET/PET G) C - PET In case of A - PET, crystallization is minimized to allow for easier thermoforming and improved clarity. In case of crystallized PET or C - PET, crystallization is enhanced for high temperature end use. The overwhelming majority of PET volume ( > 90%) is used for bottles and containers. Packaging and film application volumes include most of the applications where PET has been substituted for polystyrene volume in recent years. A-PET resins and final articles have variety of desirable properties. A - PET has very low haze levels (0.5%), which makes it desirable for any packaging application where the display or presentation of the packaged article in its container is required. In addition, A - PET is a tough material, as is shown by its high tensile elongation at break and high tensile modulus. The only two limitations to the use of A - PET resins are the low Vicat heat distortion and high specific gravity. The low heat distortion eliminates its applications in some food service applications such as hot soup. The high specific gravity increases its cost per unit volume compared with polymers with lower specific gravities such as polystyrene and polypropylene. 1 Rudi Salmang, Interview, PET in Thermoforming, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 211
222 212 Chapter 31 PET in Thermoforming Applications 31.1 EXTRUSION AND THERMOFORMING OF A-PET RESINS PET has several properties that together with its lower cost have turned into the most attractive material in the packaging industry, despite its high specific gravity. Many of the difficulties associated with its processing (drying, low melt strength, and trimming) have been overcome in part by the machine manufacturers. In order to understand the characteristics of PET processing compared, for example, with polystyrene, it is essential to review the basic differences in terms of the polymers Crystallization and PET Properties PET is a crystallizable polymer. Hence its crystallization rate needs to be controlled in order to achieve the desired properties (described later). Crystallization can be inhibited by rapid cooling of the film/sheet and can be promoted by nucleation and slow cooling. As discussed in the next section, crystallization is a critical variable for the ancillary equipment design. Also, due to its crystallizable nature, streamlined design is to be followed to avoid dead spots Drying to Inhibit Degradation PET is a condensation polymer, and therefore any residual water will cause its hydrolytic degradation. The loss of molecular weight results in a decay of its physical properties (instrinsic viscosity breakdown). Drying PET to an acceptable level (< 30 ppm) requires high temperatures ( 180 C) in order to encompass the drying residence time with the extrusion output rates without the need of exaggerated large holding silos. At this temperature and with dehumidified air, crystallized PET (C - PET) needs approximately four hours in the dryer to become processable. However, amorphous PET (A - PET) will soften and stick to itself at around 120 C to 125 C. Therefore A - PET should be crystallized before initiating its drying cycle. This is an important step for recycling the thermoforming skeleton web. Usually a predryer or re-crystallization silo is installed upstream of the high temperature dryer to initiate the crystallization (130 C). One other strategy is to blend the A - PET regrind with C - PET (virgin PET is supplied in crystalline state) and to place the blend directly in the high - temperature dryer. High - efficiency vented screws have been designed to handle such blends as well Extrusion Extruders need to be capable of very good heating and cooling control because of the required high processing temperatures and sharp cooling profiles (290 C reversed profile down to 240 C). The water - cooled extruder has almost become the norm, and the venting system is essential for continuously efficient operation. The screws for PET have evolved into a barrier - type design (30 L/D) to keep the molten low - viscosity polymer being metered forward as fast as possible and to
223 31.1 Extrusion and Thermoforming of A-PET Resins 213 recover viscosity at the minimum possible melt temperature. The melt gear pump has become the standard for the PET extrusion lines to stabilize the flow and to reduce the pressure sensitivity in the screw. The die design is a critical factor to be considered from the width requirements for two main reasons: No deckles should be used to adjust the width (avoiding stagnation sites for crystallization), and hence the edge trim may become of considerable undesirable proportions. Deckles also increase the unsupported film/sheet distance between the die and the roll gap. The low melt strength calls for the narrowest possible die to increase the line speed, thus minimizing sheet sagging. This implies, of course, designing for very high line speeds, but it also reduces costs from the roll stack width. The calender or roll stack needs very accurate temperature control to ensure the proper cooling rate so as to avoid any undesirable crystallization. Since the strategy is to quench the film/sheet as soon as possible, an extra hardened surface of the rolls is desirable to reduce indentation of the chrome coating due to eventually overcooled spots on the film. The calendering force is relatively low compared with the usual level needed for high quality in other polymers. Machine manufacturers still debate whether horizontal or vertical disposition of the rolls for PET film/sheet is preferable. The horizontal type seems to ease the handling of the film sagging better but brings with it the inconvenience of having to move the calender quickly away from the die. Roll stack systems have been introduced to the market that offer high versatility in allowing any disposition between vertical and horizontal by a quick satellite adjustment of the rolls to overcome these problems Thermoformed Packaging Applications Thermoforming of A - PET is quite similar to that of PS - HI and PVC in terms of equipment characteristics. However, as in extrusion, a few differences from its crystallizable nature and moisture sensitivity are to be observed: Drying. One critical point perceived today in A - PET thermoforming is the moisture - based loss of properties that is not as evident as in the case of moisture - related defects in other polymers. The film/sheet stock has to be kept dry, and depending on the logistics and operations design, pre - drying of the roll stock (1 2 hours at 65 C) may be required. Heating forming. Overheating must be avoided, as it will cause undesirable crystallization, film excess sagging, and haze, accompanied by loss of toughness. The thicker the film, the more difficult is the thermoforming of A - PET film in terms of haze and crystallinity. The typical forming temperature is close to 125 C, which is to be achieved in the shortest possible heating cycle to avoid undesirable crystallization. Two examples of industrially optimized applications illustrate the differences in forming characteristics:
224 214 Chapter 31 PET in Thermoforming Applications For FFS thermoforming, contact heating (PTFE- coated pads) is largely done for energy effectiveness (e.g., water packaging, blister packaging). Preformed cups (450 ml) are thermoformed at 40 cycles/minute (PS) and 35 cycles/minute (PP) in cut - in - place machines. Cutting trimming. Cutting and trimming are perhaps the most frustrating difficulties of A - PET compared with PS and PVC. The main reason is the need to cut through the whole thickness in the case of A - PET film in order to separate the parts from the skeleton web, while in the case of PS the cutting is initiated ( 2/3 thickness) after which a fracture propagation takes place. A - PET requires very sharp and hardened tooling, and small clearances. Two main types of trimming are used with a few modifications in the case of A-PET: Steel rule die and forged die ( kiss-cut system) for small and medium volumes are used in the trim press as well as in the cut - in - place machines, and are driven through the film against a stainless steel backing plate. Usually, hot cutting is performed in these systems to reduce cutting forces and hence extend tooling life. Matched die or punch and die is the preferred system for large volumes, as otherwise the result is too expensive for the hardness and precision required (55 Rockwell C, 2 μ m radial clearance). This system is used in both cut - in - place and trim press stations. To reduce the cutting force and hence extend the tool life in either case, coining is done on the rim area down to two - thirds of the thickness. The maximum trim length is defined by the shear cutting forces capabilities (cut- in - place) of the thermoforming machine. Two additional differences should be noted: A - PET exhibits the best or longest living hinge characteristics for clamshell or lidded containers. The draft angle in PET cups has to be a little larger (6.5 versus 4.5 for PS), or a higher denesting shoulder must be used. This is due to the very high optical properties of its surface, and, as in OPS, usually a slip and/or anti - static bath is applied to the film Processing and End -Use Differences between PS and A-PET In Table 31.1, processing and end-use differences between PS and A-PET are shown PET FOR ELECTRONIC PACKAGING As the electronics industry continues its trend toward miniaturization and improved performance, the resultant increased sensitivity makes the need for ultraclean
225 31.2 PET for Electronic Packaging 215 Table 31.1 Comparison of PS and A-PET Process PS A-PET Drying None Requires pre-drying to avoid hydrolytic degradation Regrind requires crystallization prior to pre - drying Extrusion process Calendering characteristics Typical specific output Thermoforming process Typical output Trimming/ cutting process Amorphous processing (170 C 240 C) Defects can be detected during extrusion No practical limitation in sheet width or line speed Higher calendering force required 5.5 kg/kwh No pre-drying required PS is considered the reference for ease of thermoforming and nonspecial requirements PS in FFS is still the reference for ease of thermoforming and for unitizing/snappability Thermoforming output 40 cycles/minute for a ml cup (cut- in - place mold) Fracture propagation mechanism after 2/3 of sheet thickness is sheared Normal backing plate for steel rule die cutting PS taken as the reference for tooling life Crystalline melting point >240 C Processing (290 C 240 C) Properties lost due to the degradation are not easily detectable during extrusion Melt is very pressure sensitive; gear pump is essential. Very low viscosity, barrier screw required. Width flexibility limitations due to low melt strength and crystallization potential Extra hardened roll surface desired to avoid damage from uncontrolled cooling 4.7 kg/kwh Pre-drying is essential Nondetectable loss of properties due to moisture Undesired crystallization potential Thermoforming difficulties increase with sheet thickness FFS water packaging introduced by shearing through the packages; no unitizing/snapping concept pursued Thermoforming output 31 cycles/ minute for a 450-mL cup (cut-in-place mold) Needs to be sheared through 100% of sheet thickness Hot cutting preferred (for steel rule die) to reduce force requirements and to extend tooling life Matched die cutting requires extremely low clearances and tooling life may be only 1/6 before re -sharpening (Continued)
226 216 Chapter 31 PET in Thermoforming Applications Table 31.1 (Continued) Process PS A-PET End-use performance Taste and odor Optics Toughness Stiffness Lasting hinge <300 ppm requirements and still limited in some applications OPS is the only alternative that matches PET performance. BDS blend performs 2nd best Highest performing commodity resin No long-lasting hinge Superior performance, reference in the market Superior performance, haze <1% Best long-lasting hinge packaging even more critical. 2 The inherent cleanliness and balance of properties of PET copolyester such as Eastar from Eastman make it the perfect material to meet this need. When the packaging requires protection against electrostatic discharge (ESD), the properties of Eastar copolyester make it the ideal foundation for most ESD control technologies. Major ESD control technologies (e.g., nonpermanent topical coatings and compounding internal systems) can be successfully integrated with copolyester to impart conductive or static dissipative properties to the film. These films are fabricated into trays or clamshells to satisfy the packaging needs of the electronics industry, from hard disk drives to semiconductors to passive devices and components PET-G (GLYCOL -MODIFIED POLYETHYLENE TEREPHTHALATE) Glycol-modified polyethylene terephthalate (PET - G) is a clear amorphous polymer. 3 The modification is made by adding a second glycol, cyclohexanedimethanol (CHDM), during the polymerization stages. The second glycol is added in proper proportion to produce an amorphous polymer. In this chapter data of the material Eastar copolyester 6763 is used but it does not apply to all generic PET - G products. Eastar copolyester 6763 does not crystallize and thus offers wider processing latitude than conventional crystallizable polyesters; plasticizers or stabilizers are not required. This polymer offers an excellent combination of clarity, toughness, and melt strength that makes it useful for a variety of processing techniques and end - use 2 Eastar Copolyester for Electronics Packaging, Publication MBS B, Eastman Chemical Company, Eastar Copolyester 6763, Thermoforming, Publication TRS - 65 M, Eastman Chemical Company, 2002.
227 31.3 PET-G (Glycol-Modified Polyethylene Terephthalate) 217 applications. Processing methods include extrusion and thermoforming of film and sheet Film Extrusion Processes Film produced from Eastar copolyester 6763 has excellent optical properties and can be thermoformed readily with wide processing latitude. Most of the film manufactured commercially is produced on a three - roll stack that permits nip polishing. This improves the appearance of the film. In some cases a two - roll S wrap (cast film) process is used. Film produced by this technology can be formed successfully, but it may sag more during thermoforming. Also, since only one side (the bottom) is polished, die lines may be apparent. Therefore nip - polished film is usually preferred Benefits of Glycol -Modified Polyethylene Terephthalate Eastar Copolyester Using film made from Eastar copolyester 6763 for thermoforming offers the benefits listed below: Can be used in contact with food. Has sparkling clarity. Is tough, even at temperatures as low as 29 C. Has yield 4% greater than PVC. Offers scrap reuse up to 30% or 40%. May be successfully sterilized with ethylene oxide, gamma radiation, and electron beam. Offers fast forming cycles can be formed at faster cycles than materials such as PVC when heater capacity is a limiting factor. Does not stress-whiten. Adapts to conventional forming and sealing equipment. Heat - seals to most standard multipurpose coated blister board that is used for PVC and cellulosic films. Is noncorrosive. Does not generate noxious fumes. Typical thermoformed packaging applications for Eastar copolyester 6763 film include the following: Candy Cosmetics Hardware items
228 218 Chapter 31 PET in Thermoforming Applications Toys Medical devices Electronic parts Foods When using Eastar copolyester 6763 for medical and pharmaceutical packaging, the material: Is tough and durable, with high clarity and gloss. Generates a minimal amount of particulate matter when cut. Does not stress-whiten when flexed. Can be heat-sealed to coated Tyvek lid stock from DuPont. Can be successfully sterilized with ethylene oxide, gamma radiation, and electron beam Sterilization Distortion can be minimized by reducing cycle time, temperature, and humidity and/ or increasing film thickness. The temperature should not exceed 54 C; relative humidity should not exceed 50%. The glass transition temperature or softening temperature of Eastar copolyester 6763 (80 C) will vary depending on the temperature and humidity. Prolonged exposure at EtO sterilization conditions increases the probability of stress relaxation; therefore it is important that the following variables are controlled: Cycle time Temperature Relative humidity Film thickness Eastar copolyester 6763 can be sterilized by gamma radiation methods up to 5.0 megarads with no noticeable loss in properties Thermoforming Heating A uniform temperature across the film must be maintained in the forming operation; therefore, air currents near the thermoforming machine must be minimized. Contact heating (direct conduction) is used in form, fill, and seal lines; however, Teflon - coated aluminium plates are required because Eastar copolyester 6763 tends to adhere to hot metal. Convection heating, which is about half as efficient as contact heating, is generally used only in roll - fed thermoforming systems.
229 31.3 PET-G (Glycol-Modified Polyethylene Terephthalate) 219 (For continuous roll - fed systems, combinations of radiant and convection heating are used as Eastar copolyester 6763 is being thermoformed. Radiant heaters that use ceramic or quartz lamps generate infrared energy that heats the center of the film more efficiently.) When heating a continuous film, it is often possible to utilize only the last two indexes before the mold. To prevent excessive sag of the film, the heating cycle should be as short as possible, provided that the proper film temperature is reached. To prevent cold - forming, it is essential that a temperature - sensing device be used to monitor the sheet temperature as it enters the mold. Optical pyrometers are excellent for this use. PET-G film extruded from Eastar copolyester 6763 can be thermoformed on fast cycle using conventional forming equipment. Tests in Eastman s laborartory indicate that the surface temperature of the film prior to forming will range from 140 C to 150 C Mold Design for Thermoforming PET-G Aluminium, or aluminium oxide powder, is the material of choice for the construction of molds, although other materials such as wood and epoxy can also be used. Aluminium provides good heat transfer and is cost - effective because of its good machinability and wear properties. For the production of quality parts at minimum cycles, molds should be cored for temperature control and, when appropriate, cooling channels added. Anodized hard coats can be applied to the mold surface to extend service life. Sometimes when thermoforming large, flat surfaces, the plastic sheet/film does not come in contact with the mold because of air entrapment. When there are problems with air entrapment, more vacuum holes should be added to the surface of the mold. Sandblasting or vapor - honing the mold can help with air entrapment. However, sandblasting and vapor - honing will change the thermoformed part s surface from shiny/glossy to matt and the amount of matt will change as the mold wears. Vacuum holes should be drilled through the mold surface with a mm drill. Each hole should be back - drilled oversize to within 1.6 mm of the surface to permit rapid evacuation. The holes should be located in an inside radius. Vacuum slots should be no wider than 50 to 70 μm. Individual cavities are usually spaced two or more flange widths apart. Female molds with a generous draft angle provide better flanges and easier removal with fewer problems from bridging; however, thin bottoms can be a problem. Severe undercuts must be avoided, and radii should be as generous as possible. Pressure boxes have two advantages. They improve cycles and provide better definition and uniformity. In addition, they can provide a coining action that will greatly simplify the cutting operation. A plug assist is suggested for parts with deep draws. Plug dimensions, depths, and clearances commonly used in thermoforming industry can be used to ensure rapid mold confirmation and uniform wall thickness. A plug assist is helpful if the
230 220 Chapter 31 PET in Thermoforming Applications Figure 31.1 Polarized light objective is to get orientation in the part. There are many types of material available for construction of plug assists Forming Many options exist for the forming action. For example, male or female molds can be used; plug assists can be used for female cavities; cutting can be in place, at the next index, or in an extra step; and a pressure box can be incorporated to provide pressure for forming as well as coining to aid the cutting. If the sheet/film temperature right before forming is too low, there will be internal stresses in the thermoformed part. Polarized lenses or a polarized light box (Figure 31.1 ) should be used during the initial setup procedures to help define the operating conditions that will produce quality parts. Polarized lenses and polarized light box are available from Strainoptic Technologies (North Wales, PA, USA) Sealing Radio Frequency Sealing The variables in the radio frequency (RF) sealing process are described below: Heated tool Sealing pressure (air pressure) Preheat time Sealing time
231 Cooling time Power setting Buffer or insulation 31.3 PET-G (Glycol-Modified Polyethylene Terephthalate) 221 Heated Tool The tool needs to be heated to reduce heat loss and raise the temperature of Eastar copolyester 6763 to increase molecular activity. The temperature of the heated platen is typically set at 120 C. Sealing Pressure Sufficient force must be applied to provide the cutting action on tear-seal or seal-and-cut operations. Preheat Time A time of 0.75 to 1.0 seconds is generally used. This is the time needed to push the tool into direct contact with the upper film before the RF power is applied. Sealing Time The time during which the RF energy is applied softens Eastar copolyester The clamping pressure then forces the tool into the copolyester, sealing and, if desired, cutting through the copolyester. A typical sealing time for a 10 - kw machine is 1.0 to 1.5 seconds. Cooling Time The time typically required is 0.5 seconds. This is the time that is used to hold the seal in place until the bond solidifies. Power Setting The power setting depends on the machine and power available. A 10 - kw machine would typically be run at 75% power to seal and cut mm films in 1.0 to 1.5 seconds. Typical plate current and grid meter readings are 0.5 amps, and 0.4 amps, respectively. Buffer or Insulation The suggested materials include biaxially oriented PET and phenolic impregnated cloth. Heated Bar Sealing The variables in the heated bar sealing process are as follows: Sealing temperature Sealing pressure (air pressure) Dwell or seal time Sealing Temperature Typically, only the top bar is heated; however, in some cases, both bars or sealing surfaces are heated. Sealing Pressure Air pressure is applied to cylinders attached to the jaws. Dwell or Sealing Time This is the time during which heat is applied.
232 222 Chapter 31 PET in Thermoforming Applications Impulse Sealing Variables in the impulse sealing process are as follows: Power setting Sealing pressure (air pressure) Dwell or seal time Cooling time Power Setting Power is applied to a resistance metal band, giving instant heat in the upper and/or lower jaw. This band can be of various widths, depending on the bond desired. The power level is adjustable. Sealing Pressure Air pressure is applied to cylinders attached to the jaws. Dwell or Seal Time This is the time during which heat is applied. Cooling Time This is the time the seal is held in place for the bond to solidify Cutting Materials such as PVC or PS - HI fracture after being cut only approximately 75% through the thickness, but an Eastar copolyester film can be cut completely through so as to cleanly separate the parts. Although there are many ways to cut thermoformed film, this chapter only covers steel rule and matched metal dies Cutting with a Steel Rule The steel rule dies offer a very cost - effective option for small - volume cutting. These dies are usually mounted in a 15 - to 20 - mm thick wood chase by the die maker. Although it is best to accurately measure shrinkage from an actual cavity, mm per mm is a good rule of thumb to use with Eastar copolyester For cutting simple shapes, use a long center bevel or a double bevel die shape with hardness of Rockwell C, especially if the film is thicker than 0.25 mm. The die should be thick enough to prevent flexing. Although harder dies wear better, softer dies of Rockwell C may have to be used to prevent breakage during fabrication when complex shapes and sharp bends are used. Dies must be installed in a press that can close smoothly as the cut progresses and that is capable of consistently bringing the die through the Eastar copolyester 6763, the same line on the backing plate. The clamp requirement can be estimated from the total steel rule length, the film thickness, and the nominal cutting force for Eastar copolyester The preferred material for the backing plate is either milled or stainless steel with a hardness less than that of the die; this way the backing plate will suffer the wear and dulling of the die will be avoided. Aluminium is not recommended for the
233 31.3 PET-G (Glycol-Modified Polyethylene Terephthalate) 223 backing plate because it has a short life and tends to splinter, which will contaminate the parts. Heating the steel rule knife and/or the backing plate to 50 C to 70 C may improve the cutting of Eastar copolyester 6763 and reduce blade wear. Higher temperatures may cause the plastic to rejoin or stick to the blade. Since the dies must have contact with the backing plate in order to get completely cut through, great care must be taken during make - ready or commissioning to ensure that the dies are not damaged. Use the following make - ready procedure: 1. Locate the position of the cutting die in the press by taping a make - ready sheet of to mm kraft wrapping paper to the cutting surface of the backing plate. 2. Place carbon paper face - down on the kraft paper and carefully bring the die down against the paper so that the location of the die is marked. 3. Mark the location of the paper on the cutting plate so that it can be placed under the plate in the same location as it was on top. 4. Place the make - ready paper under the plate and a film of Eastar copolyester 6763 in position to be cut. Be sure the press is backed off so as not to cut too deeply on the first hit. 5. Repeatedly and with careful adjustments, bring the press down until 75% to 80% of the film is cut through. 6. Remove the make-ready paper and place 0.8- to 0.15-mm make-ready tape on areas that are not cutting. Do not overlap the tape. 7. Place the make - ready paper under the cutting plate again and carefully take another hit. 8. Repeat this buildup procedure until the entire die is fully cutting. Die life can be extended if bearers are placed outside the sheet area to provide a positive stop for platens. They are particularly recommended on punch presses and two - post presses to ensure that the platens are always in the same relative position when fully closed. They also help prevent die damage during make - ready cutting (commissioning) Matched Metal Dies A matched metal die, also referred to as a punch and die, is recommended for high - volume applications. It is mounted in a separate cutting press through which the continuously formed film passes. It is designed so that the parts nest as they are punched through the die. There are also systems on the market where forming and punching take place in the same station. In matched dies, a hardened punch is used with a softer die. The typical hardness is 43 Rockwell C for the die and 55 for the punch. It is essential that a zero clearance be maintained. As wear progresses, the die be peened to recover a zero clearance.
234 224 Chapter 31 PET in Thermoforming Applications An alternative to using a soft die and peening is a hard punch and die, both at 62 Rockwell C. Zero clearance is maintained by resurfacing the punch and die, which involves removing the tool from the press. If only one set of tooling is available, downtime is increased. It cannot be emphasized too strongly that zero clearance must be maintained to ensure clean cutting of sheet made of Eastar copolyester Matched dies can be designed so that all cutting edges are parallel and all cutting begins at the same instant. A useful option to extend die life is to use shear point cutting, wherein the die is crowned by slightly raising the center line of the die. This permits the punch to contact the higher center line first. As the punch moves into the die, it does so with a shearing action as the cutting progresses to the die edges. If provision can be made during thermoforming, coining should also be used; this reduction in thickness will substantially increase die life. Part shrinkage must be considered to properly match the location the location of coining to the cutting die Denesting Thermoformed Parts Eastar copolyester 6763 has a high gloss and will often block, making it difficult to denest the formed parts. In this event an denesting concentrate or antiblocking agent can be added during film/sheet extrusion. An alternative is to run the extruded film through a bath of the antiblocking agent (silicone coating). Silicone coatings can be used as a denesting aid when applied either to the thermoformed parts or to one side of the film during the extrusion process. Coating both sides of the film is generally unnecessary because the silicone will transfer to the uncoated side after winding. Silicone coatings should always be applied in the least amount and lowest concentration practical. Crazing or stress cracking caused by silicone emulsion can be minimized by uniformly applying a well - mixed emulsion at the lowest practical level. Never heat the silicone solution. Use moderately heated air ( <50 C) to dry and remove carrier solvent (usually water) prior to winding. Silicone coatings provide better clarity than an internal denest concentrate and also provide a degree of slip during forming that can improve material distribution. A silicone coating cannot be used in some applications because it may affect certain secondary operations such as printing and sealing. There are many suppliers for denesting concentrates in the market such as Eastman and Sukano SLIP AND ANTIBLOCK MASTERBATCHES Slip and antiblock masterbatches from suppliers like Sukano Products Ltd., Switzerland, reduce the coefficient of friction (COF) of films, heavy gauge sheets, and molded parts made from PET, PET - G, PC, PP, PS, or PLA. 4 Thus thermoforming applications demold and denest much easier; films have much less tendency to stick 4 Sukano Product Portfolio, Slip/Antiblock Masterbatches, Sukano Products LTD., 2009.
235 31.4 Slip and Antiblock Masterbatches 225 Figure 31.2 Function of slip effect (Courtesy of Sukano Products Ltd.) Figure 31.3 Function of antiblock effect during winding and unwinding; and thermoforming parts are destacked without surface abrasion. (See Figures 31.2 and 31.3.) Applications for Slip and Antiblock Masterbatches Food and medical packaging Cups, boxes, and trays Biodegradable packaging Oriented films Shrink films Properties Excellent slip with less adhesion Efficient demolding Low coefficient of friction Low haze and good transparency Food packaging compliance available Combinable with color masterbatches Dosage To achieve optimum performance, follow the dosage recommendations in the technical data sheets.
236 226 Chapter 31 PET in Thermoforming Applications Secondary Operations Thermoforming Ultrasonic and laser welding, heat sealing Offset printing, gravure printing, and embossing Finishing operations Metalizing Processing Temperature Temperature is set in accordance with the raw material supplier s processing conditions Drying Amorphous PET and PET - G masterbatches should be dried at a temperature no higher than 60 C for at least 4 hours, and PC 120 C for at least 3 hours. PLA masterbatches should be dried no higher than 50 C for at least 4 hours. For PP and PS, no drying is required. Use a dehumidifying air dryer with a dew point lower than 40 C. It is recommended that dry air be used in the conveying system. Storage/Supply Form Store in a dry area and at room temperature; reseal opened bags. Sukano PET masterbatches are available in crystallized from. Standard pellet length is 3.2 mm (small pellets of 1.6 mm or long pellets of 4.8 mm are available on request). Packaging Standard packaging is 25 kg PE bags on 1000 kg single-trip pallets. Big-Bags or Octabins are available in different sizes upon request. This procedure combined with denest lugs should provide satisfactory part separation. Some concentrates will, however, produce a slight haze in the film and the formed part RECLAIMING SCRAP Blister - forming operations will often generate large amounts of trim scrap. 5 PET-G materials such as Eastar copolyester 6763 can be reground, blended with virgin pellets, and reprocessed. The actual percentage of regrind may depend on processing parameters such as extruder L/D and screw design, melt temperature, residence time, and use of gear pump. However, levels of scrap reuse up to 30% or 40% are not unusual as long as the regrind is kept clean, dry, and free of contamination. 5 Eastar Copolyester 6763, Thermoforming, Publication TRS - 65 M, Eastman Chemical Company, 2002.
237 Chapter 32 Thermoformed Packaging Made of PLA Polylactides (PLA) represent a relatively new group of thermoplastics for packaging applications obtained from renewable resources. In extensive tests the functional and thermoforming properties of PLA are compared with those of other polymers. 1 PLA s properties make it suitable for various thermoforming applications, particularly cups for cold bevarages and trays for fruit and vegetables. To produce high - molecular PLA, a process is used that is sustainable, solvent - free, and environmentally friendly. PLA is obtained entirely from maize. PLA can equally be produced from other renewable resources, such as wheat, sugar beet, or agricultural by - products containing natural plant sugars. First, dextrose is fermented to form lactic acid, which is subsequently converted into cylic dimers (lactides) by condensation and esterification. The dimers are converted to polylactide by catalytic ring - opening polymerization. Lactic acic occurs in two isomeric forms: L - lactic acid and D - lactic acid. The ratio of the isomer units in the polymer chain can be varied during the polymerization process PHYSICAL PROPERTIES At room temperature, PLA is a crystal - clear polymer with glass transition temperature between 55 C and 65 C. The physical properties of PLA are improved by orientation of the material, for example, biaxially oriented sheets. PLA with a D - lactic acid content of less than 8% can be semicrystalline if it has been nucleated, annealed, or stretched in an orientation process. The increases in crystallinity results in improved stiffness and heat resistance. The melting point of PLA is increased 1 Luc Bosiers and Sven Engelmann, Thermoformed Packaging Made of PLA, Kunststoffe Plast Europe, pages 21 23, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 227
238 228 Chapter 32 Thermoformed Packaging Made of PLA with decreasing content of D - isomer; it is between 130 C and 175 C. PLA has a critical surface tension of 38 mn/m (dynes). The result of this is that corona treatment has a lasting effect. PLA is therefore easy to print and metallize COMPOSTABILITY The fact that PLA is compostable can reduce the vendor s waste disposal costs. This is the case wherever waste is separated before collection. PLA biodegrades by hydrolysis and scission of the ester groups in the molecular chain. The molecular weight is reduced until the lactic acid and oligomers with low molecular weight have been metabolized naturally by microorganisms with the generation of carbon dioxide and water. In environments with high atmospheric humidity and high temperatures (55 70 C), such as are found in active composting systems, PLA degrades rapidly. The low temperature and low air humidity found in storage rooms and under service conditions do not pose a problem. At 60 C and relative air humidity of 80% PLA will degrade completely after 60 days PROCESSING OF PLA FILM Three packaging technologies used for processing PLA were considered in detail: high - quality films and blow - molded and thermoformed food containers. The service characteristics include high stiffness, high gloss and transparency, foldability, and twist wrap. Like other polyesters, PLA s physical properties are affected by hydrolysis. PLA must therefore be protected against air humidity and dried to less than 200 ppm residual moisture content before extrusion. PLA is advantageously extruded slightly below the melt temperature recommended for PE. These data were determined on a conventional coextrusion line for PE. Extensive tests were carried out to determine the thermoforming behavior of PLA with other polymers, such as polystyrene (PS), polypropylene (PP), and amorphous polyethylene terephthalate (A - PET). The points considered were the material properties, thermoformability, transportability of the film, punching behavior, winding of the skeleton stackability, de - stackability of the finished articles, and the behavior of PLA in the mill. To determine these, numerous experiments were carried out on various thermoforming lines. The sheet is processed as roll stock on all production lines used. The films were produced using Nature Works PLA pellet stock 2002D from Cargill Dow with small amounts of blue masterbatch and antiblocking agent. An extruder with a two - stage multipurpose PS/PET screw with a diameter of 90 mm was used. The film widths were between 500 and 735 mm; the film thicknesses were 0.5 to 1.2 mm.
239 Transparency and Density 32.3 Processing of PLA Sheet Film 229 For drinking cups or for packaging foods such as salad or vegetables, high transparency is often required. In these thermoforming applications, materials such as A - PET, biaxially oriented polystyrene (OPS), or styrene butadiene styrene (SBS) is used. PLA is only slightly less transparent than A - PET but more transparent than PP, SBS, or even OPS. The density of PLA, at 1.25 g/cm 3, is less than that of A - PET(1.34 g/cm 3 ). However, the densities of PS (1.05 g/cm 3 ) and PP (0.91 g/cm 3 ) are well below that of PLA. Transport of raw material, the semifinished product, and the finished article can have an influence on which plastic to use Mechanical Properties The stiffness of a thermoformed article is of immense importance for the stability. Different plastics are often compared by way of modulus of elasticity. A high modulus of elasticity results in high stiffness of the thermoformed article. This allows reductions in wall thicknesses and, as a consequence, weight and cost savings. In the comparison of the modulus of elasticity of different packaging materials PS - GP (general purpose polystyrene) has the highest modulus of elasticity of the styrene materials. However, because of its high brittleness, it is usually only thermoformed by the inline process, with the extruder connected directly to the thermoformer. At 3500 MPa, PLA has the highest modulus of elasticity of all the polymers compared. The high stiffness of PLA permits automatic stacking of containers. However, to allow de - stacking, it is necessary to add an antiblocking agent during the production of PLA film Thermal Behavior and Shrinkage An important characteristic for the thermoformer is the softening point. The PP grades used in packaging have softening points of about 150 C, followed by A-PET at 86 C. The softening point of PS is 80 C. In the case of PLA, a Vicat softening point of 58 C was determined. Polypropylene block copolymer has a very large service temperature range. Application temperatures from 30 C to 100 C are possible. The continuous service temperatures of polystyrenes and A - PET can satisfy a large number of applications. For PLA, the maximum continuous service temperature is approximately 45 C. PLA is therefore not suitable for hotfilling. However, PLA can be used down to 20 C. Because of the continuous service temperature range, PLA is suitable for applications ranging from cups for soft drinks, trays for fruit and vegetables, and packaging for refrigeration and deep freezing. Semicrystalline plastics generally show greater shrinkage than amorphous plastics. PP also has the greatest shrinkage in this comparison (1.5 to 1.8%). The shrinkage of amorphous materials, such as PS, A - PET, and also PLA, is about 0.5%. In
240 230 Chapter 32 Thermoformed Packaging Made of PLA this chapter, A - PET and PLA are considered as amorphous plastics, since they undergo negligibly small crystallization under typical extrusion and thermoforming conditions. That means that in some circumstances PLA applications can also be implemented on existing PS or A-PET tools THERMOFORMING OF PLA PLA film can be thermoformed with vacuum, compressed air/vacuum, or only compressed air assistance. The radiant heater of the thermoforming line for PLA must be adjusted to very low temperatures. While preheating is not absolutely necessary, it has the general advantage that the film is homogeneously heated. Unlike PP, PLA does not undergo significant film sagging during heating in the thermoforming process. The low processing temperature must be noted. Thermoformed articles produced from PLA film can have outstanding forming definition. PLA requires a relatively long cooling phase in the mold. Rim rolling of thermoformed drinking cups is possible. The thermoforming temperature is measured at the film surface. Compared with other plastics, the forming temperature of PLA is very low. PLA has a wide forming temperature range ( C). The maximum temperature range of A - PET is between 100 C and approximately 120 C. PS - HI has the widest forming temperature range ( C). The maximum forming temperature range of PP during thermoforming on roll - fed machines is slightly below the crystallite melting range of 150 C to 165 C. During the start - up of PLA production, it is advisable to approach the processing temperature window with the radiator set at a low temperature. Tests were carried out on machines that form separately and punch with steel rule dies, as well as on machines that form and punch in a single operation (drop punch). Both punching processes are suitable for processing PLA film. The appropriate tests were carried out on various machines (RDM, RV, RD, and RDK series from Illig). In the case of controlled - temperature steel rule dies, the die temperature was 120 C FILM TRANSPORT In a roll - fed thermoforming machine, the material is fed by two parallel motorized spike chains. The spikes of these transport chains pierce the edges of the film and convey it through the thermoforming line. Since the PLA film is very brittle, the spikes punch out small particles of the film as they convey it. These material particles may disrupt production. In offline processing, the use of edge - strip heating is recommended. Heating of the film edges makes it so flexible that no material particles are punched out. The film is heated by means of an edge strip heater, either by contact or radiant heating. The machine must not stop longer than the solidification time of the cooling film. Otherwise, the solidified material could jam at small deflection radii of the
241 32.5 Film Transport 231 machine when the machine is restarted. This was only rarely observed during the series of tests. The PLA skeleton is so brittle that it can break during winding. If the skeleton is not shredded subsequent to processing, a special skeleton winder is recommended. This winder operates at two different speeds. Immediately after an operating cycle, the material must be rapidly transported. Shortly before the skeleton end position of the respective cycle is reached, the winding reel switches to a lower speed to minimize the tensile stresses. Breaking of the skeleton can also be prevented by increasing the deflection radius. If PLA is processed with correct processing temperatures, it can be reliably reground. PLA regrind can be returned to the process. It is possible to feed the skeleton in a linear direction or offset by 90 to the grinding mill. Here too the take - off rate of the shredding mill must be adjusted to take account of the high brittleness of the cooled film. PLA has excellent service and processing properties, and it is therefore comparable with traditional thermoplastics, and even superior in certain cases. This product family represents a genuine breakthrough for packaging materials derived from renewable resources.
242 Chapter 33 Peel and Reseal Different thermoform applications require a multitude of semifinished products. In the good old times many convenience goods were sold without packaging because suitable packaging materials simply were not available. Besides sacks, baskets, and leather tubes, bulky clay containers partly closed by resin - impregnated textiles and wooden barrels were for centuries the only transport containers that were used, not only for oil and wine but also for grain, sugar, and salt. 1 The clay containers were bulky, heavy, and easily breakable. At that time the packaging offered mostly inadequate protection against deterioration and loss through humidity and against exposure to all kinds of vermin, making the flour sifter an important piece of kitchen equipment until the mid - twentieth century. Food hygiene was subject to many hazards. As transport and storage containers were heavy and expensive, this resulted in a standard offer of foodstuffs that cannot in the least be compared to today s diversity of goods. Fresh fruit and vegetables could be sold only in the respective seasons. Today approximately 90% of all foodstuffs are bought in the supermarket. The reasons are obvious: approximately 50 years of fast means of transport, refrigeration, suitable packaging materials, and in particular plastic packaging materials have revolutionized the way in which we transport, buy, and sell goods. More and more families are living in cities, and families are getting smaller. The number of dual - income families is growing as fast as the number of single households, and populations are aging. Smaller households need smaller food portions, so small packages are becoming increasingly important. People who have little time for shopping and cooking are asking for ready - to - serve and portioned meals that are suitable for storage, so that it is not necessary to go shopping every day. Modern packaging is an indispensable component for maintaining the quality of life. Polymer films are widely used in the packaging technology, and they have widespread applications. Usually, these films have a thickness of only some 1 Jürgen Jentschke, Alexander Rösler, and Julian Matzik, Studienarbeit: Untersuchungen der Verschweissbarkeit und Resealf ä higkeit von wiederverschliessbaren Folien, HTW Aalen, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 232
243 33.1 Film Materials 233 hundredths or thousandths of a millimeter. However, films can have extraordinary properties. Often, a certain demand cannot be fulfilled by using only one type of material. Then the films are tailored by creating a cleverly devised multilayer structure. There are, for example, integrated gas barriers that prevent the penetration of gas and vapors as well as the release of aromas so that the taste and the aromas of the food are conserved over a long period of time FILM MATERIALS There are many ways to package and store products using plastic packaging materials, but there also are many demands concerning these plastics. Depending on what is to be stored, where the storage takes place, and how the packaging should be carried out, there are specific requirements concerning the materials. If, for example, food is to be packaged, then it is self - evident that contact with the plastic will be harmless and that the packaging will serve as a barrier that keeps noxious gases or environmental matter away from the food. For convenience food, the packaging must additionally be suitable for microwave ovens. Today, easily perishable foods are already packaged with an acceptable mono - layer (not multilayer) barrier film such as PA, PVC, and A - PET. If the barrier properties of these film types are not sufficient, it is possible to improve the barrier effect by introducing EVOH (which makes the packaging gas - tight) or even aluminium (which provides an absolutely impenetrable gas barrier). Packaging is divided into two categories: flexible packs and rigid packs. Flexible packs are used for fresh food such as for cheese, sausages, and meat. For flexible packages PA/PE combinations with a thickness of 200 to 250 μ m are used. Sharp - edged products, such as cheese blocks and smoked meat, and foodstuffs undergoing special modes of export shipment may require thicker packaging material and, accordingly, a composite packaging material. If the content needs to have a long shelf life or needs to meet certain quality requirements that call for more barrier protection, PA/PE combinations with an EVOH layer as a gas barrier can be used. For some cheeses, in contrast, it is necessary to use a material combination with high CO 2 permeability due to the ripening process in the packaging so that the gas originated by the ripening can escape. Representative materials that fulfill these requirements are OPP/PE combinations and so are often used for lidding and multilayer films. Rigid packs, on the other hand, have a more stable structure. Rigid packs are therefore especially suited for the packaging of sliced foods such as cheese and sausages, which are sold by standard weight in supermarkets. The usual materials are OPA/PE peel combinations for lid films, and A - PET, that is, APET/PE combinations, for bottom films. Under normal circumstances it is possible to dispense with the A-PET/PE bottom film because an A - PET bottom film already possesses a sufficient gas and water vapor barrier for most applications. In cases where oversized rigid packs need to be manufactured, as for the wholesale trade, then mostly PS/ EVOH/PE bottom films in combination with OPA/PE lid films are used. Then again,
244 234 Chapter 33 Peel and Reseal for the packaging of fresh meat a lid film is used that is equipped with a so - called antifog mixture in order to prevent any condensation that would obstruct the food s visibility. Food that is to be pasteurized in the packaging requires materials that withstand high temperatures. Suitable materials for the bottom parts are PP/EVOH/ PP combinations. A PA/PE combination with an additional PP sealing layer can be used as the material for the lids PE Films Polyethylene (PE) is among the most important thermoplastics for the production of films. Because of the multitude of production possibilities, PE products can differ greatly from each other. On the one hand, polyethylene is converted to monofilms; on the other hand, it is also used for the production of multilayer films and multilayer materials. PE films are mostly produced by the blow extrusion film method, and its mechanic material characteristics can be adjusted by a combination of different polyethylenes. The primary quality of PE is its slight water vapor permeability and additionally its gas and aroma permeability. It is also desensitized to water, acids, alkalis, and all current chemical dissolvents. Toxicologically, PE is harmless, which is why it has high suitability for food packaging. However, it is necessary to keep in mind that some of the additives can be toxicologically harmful, so they should not be used in contact with food. Another important characteristic of this material is that it is ductile and its elastic structure has a cold resistance of 50 C. The maximum temperatures for the use of PE are 70 C to 80 C for PE-LD and over 100 C for PE - HD. For the heat - sealing of the films, temperatures of 120 C to 140 C are necessary. PE-LD PE-LD is low-density polyethylene ( g/cm 3 ). Very high pressure and very high temperatures are necessary for the production of PE - LD, with the processing done in so - called tube reactors or autoclaves. The material characteristics of PE - LD are determined by the strong branching of its polymer chain. The low crystallinity of this structure entails a low melting temperature and only a slight stability. PE - LD films have a waxen texture. The application range of PE - LD, however, is very diversified. For example, the material can be converted to sacks and agricultural films with a thickness of 150 to 250 μ m. It can also be used for the manufacturing of carrier bags with film thicknesses of between 30 and 65 μ m or for the manufacturing of pouches for self - service shops with film thicknesses of 10 μ m or less. PE-LLD PE-LLD is linear low density polyethylene ( g/cm 3 ). It is produced in solutions or gaseous phases. PE - LLD is similar to PE - HD due to the linear branching of its polymer chain. It combines the softness and the ductility of PE - LD as well as
245 33.1 Film Materials 235 the high mechanical stability of PE - HD. Its permeability for water vapor and oxygen is similar to that of PE - LD and PE - HD. With these characteristics it is possible to produce PE - LLD films that are thinner than PE - LD films. Film thicknesses of up to 5 μ m can be attained. PE - LLD currently can replace PE - LD in composite films because it makes the production of ever thinner films possible. PE-HD PE - HD is mechanically the most robust PE - film; the abbreviation HD stands for high density. Similar to PE - LLD, PE - HD has a linear chain structure, but its specific density ( g/cm 3 ) is considerably higher compared with PE - LLD. The production process of PE - HD is similar to the production process of PE - LLD. However, PE - HD is not often used for the production of films. Its main application is the processing of hollow pieces that are manufactured using the blow molding process. The manufacture of injection molding parts with PE - HD also is not a problem PET Films Polyethylene terephthalate (PET) is normally known as polyester and often mentioned in connection with the term PET bottle. In the early 1960s the production of the so - called polyester films began. As raw materials for PET the petrochemicals P - dimethylbenzene and ethylene are used. From this terephthalic acid dimethylester and ethylene glycol are made. There are two different ways to produce PET. In the course of polycondensation, PET is obtained from terephthalic acid and diethylene glycol by splitting off the water. The second and more commonly used process is the transesterification of terephthalic acid dimethylester with ethylene glycol by splitting off the methanol. The reaction occurs through heat at temperatures between 260 C and 270 C. After several hours of heating the remaining water is reduced to values of under 0.01%. On the one hand, the hydrolytic decomposition of the final products is thus prevented; on the other hand, the mechanical characteristics are significantly improved. PET is very often chemically modified in order to influence the crystallization and in this connection raise the melting point. There are mainly three groups of PET (see Chapter 31 ). The group designated as amorphous PET (A - PET) has a lower crystallinity and also a lower meting point. Amorphous PET can be processed using a wide range of temperatures without the danger of a melt fracture, that is, its tearing during deformation by heat. A - PET is mainly used for the production of transparent thermoformed cups, containers, and bottles used to package food, cosmetics, and chemical - technical products, such as toothbrushes and printer cartridges. The group designated as crystalline PET (C - PET) is, in contrast to A - PET, highly crystalline, and it has a high melting point of more than 280 C. A special quality of C - PET products is their dual ovenability, meaning that they are
246 236 Chapter 33 Peel and Reseal heat - proof when used in convection or microwave ovens. So C - PET packaging is perfectly suited for so - called convenience food (ready - made meals, etc.). Finally, there is PET - G, which is described in detail in Chapter 31. Polyester films are generally created by flat film extrusion. After the extrusion process, the films are quickly cooled to obtain a very fine crystalline state of the polymer. Subsequently, these films are often further processed to obtain oriented polyester films. The consequence is a considerable increase in the crystallinity. Through prolonged heating it is possible to obtain further crystallization, and especially to fix the film structure, which together leads to excellent mechanical characteristics. For this reason polyester films have an especially good tensile strength, shock resistance, and abrasion resistance as well as an excellent ductility. The thermal characteristics are also outstanding. PET is cold resistant up to temperatures of approximately 70 C, and the upper limit of the temperature is approximately 150 C, even for prolonged use. Polyester films are increasingly used as packaging material for food destined for heating in microwave ovens. Furthermore, PET films have a very low permeability regarding water vapor, oxygen, and aromatic substances. They contain no plastizers and are therefore physiologically unobjectionable. The films are odorless, tasteless, and resistant against most organic chemicals, dissolvers, greases, and oils. In regard to the packaging technology, PET films are often used in combination with PE. It is possible to include additional barrier layers into this composite material consisting of, for example, EVOH. Important areas of application are use as boil - in - bag packages and meal trays with dual ovenability, baking films in conventional kitchen ovens, and films for sterile medical packaging. Moreover, PET can easily be metallized and printed PA Films Polyamides have a high number of molecular building blocks composed of very different chemical structures. The main characteristic of these building blocks is that they are linked together by peptides, in particular, amide bonds. Natural polyamides are peptides and proteins that can be found in nature, for example, hair, wool, silk, and egg white. Synthetic polyamides were launched in the United States in 1939 with the brand name Nylon, which has predominantly a thermoplastic, partially crystalline structure. The composition of synthetic polyamides is similar to natural proteins such as silk, but with excellent stability and a very good temperature resistance. For this reason PA is suitable for injection molding and extrusion and is used for many applications in the automobile industry, electrical engineering, electronic engineering, mechanical engineering, precision engineering, and packaging technology. Polyamide films can be produced by either the flat film extrusion method or the blow film extrusion method. The film thickness normally ranges from 20 to 50 μm. The films have good mechanical properties as well as show good resistance against chemicals. Although their permeability regarding gases and aromatic substances is
247 33.2 Production of Films for Packaging 237 low, it has to be kept in mind that their permeability depends very much on humidity. This is due to the fact that polyamide absorbs water because of its hygroscopic structure. The permeability of PA films regarding water vapor is accordingly high. Nevertheless, the thermoformability for packaging applications is good, and therefore its suitability for sealing or welding is also good. Polyamides temperature resistance against low temperatures (of up to 40 C) is particularly outstanding. Polyamides can be used in multilayered films, since, especially as PA/PE films, they possess, in combination with polyethylene, characteristics that are very suitable for the packaging of food. However, the use of PA monofilms is relatively rare due to the hygroscopic structure of PA. Some polyamide films undergo additional stretching to improve their mechanical properties. It is also possible to produce biaxial stretched PA films through the application of the relatively new simultaneous stretching method EVOH Ethylene vinyl alcohol (EVOH) films are mainly manufactured using the co - extrusion process in combination with other polymers. As EVOH possesses an excellent barrier effect against gases, the importance of this polymer for the packaging of food is ever more increasing. Good material properties also contribute significantly to EVOH s increased use. For example, EVOH has a very high tear propagation resistance and a good ductility in humid conditions as well as a high resistance against organic chemicals. Therefore, EVOH can also serve as a barrier to grease and aromatic substances, and it has very good resistance to light and aging. The disadvantage of EVOH is its water solubility. However, as EVOH is mainly used as a composite layer between other types of film, this does not present a problem, at least not for packaging technology PRODUCTION OF FILMS FOR PACKAGING Films are produced by application of the blow film extrusion method, the flat film extrusion method, or the casting of solutions. The characteristics of blow film and flat film manufacturing are described in this section Blow Film Production The extrusion of blow films is important for the production of films. This method offers economic efficiency as well as other advantages, for example, variability regarding the width and the thickness of the film as well as balanced mechanical properties due to the biaxial orientation of the solidifying melt after the die. Generally, the blowing of films is a continual forming process for the production of flexible film tubes. The blow films are produced with the help of tubular dies; the circumference of the tube can be up to 16 m and the thickness varies between 10 to
248 238 Chapter 33 Peel and Reseal 300 μ m. If a mandrel tool is used, then the melt yields a pin that is clamped in housing with the infeed channel designed to attain constant flow in the axial direction. The joint line at the back of the pin, which cannot be avoided, is apparent in the extruded material. To a smaller extent this is also the case when spider - type die tooling is used. Marks from the spider - type die tooling can be avoided when using a breaker plate and a spiral melt distributor. As the melt is exiting the die, the film is blown up with supportive air pressure to the desired tube diameter. After being cooled, the film is flattened and wound up Flat Film Production Flat film extrusion is a procedure where the melt formed in the slot die is absorbed by a cooling roll where it is cooled and then rolled up according to an effective width. For flat film extrusion the molten film is discharged downward at an angle and then put tangentially on a cooling roll. In this connection the film can be stretched to a thickness of 8 to 15 μ m in the extrusion direction. When special stretchers are used, cold or warm stretching, uniaxial or biaxial, with extremely high degrees of stretching power, is possible. For the double - stage procedure the film is, first of all, stretched in longitudinal direction between two rolls that have different rotational speeds. Thereafter the diagonal stretching is effected by gripping the lateral edges of the film with grippers; subsequently, during the transport of the film, these lateral edges are led outward in a longitudinal direction. For the simultaneous biaxial stretching, the grippers are led outward with increasing speed in the direction of travel. This happens at the same time. By stretching and a thermic finishing treatment (thermofixing), the stability, the transparency, the barrier property, the cold resistance, and the electrical behavior are improved Multilayer Film Production/Coextrusion Today there is a growing trend toward high - quality films, along with a trend toward increasing output. This can be deduced from the fact that investments in monofilm lines are rare; nevertheless, investments in lines for coextruded films, in particular, multilayer films, are ever increasing. The use of multilayer films facilitates the creation of tailored film products for all sectors, for example, films for carrier - bags and for food packaging. Not only are various barrier properties thus created but also costs are reduced significantly by utilizing recycled materials. Coextruded films, in particular, multilayer films, can be produced using the blow film or flat film extrusion method. There are three different methods for the manufacture of coextruded flat films: the adapter method, the multichannel die method, or a combination of both. For the flat film coextrusion method, the melt is put onto a cooling roll through a die gap. The velocity of the cooling roll determines the flow rate and the final thickness of
249 33.2 Production of Films for Packaging 239 the structure. An additional factor for the determination of the final thickness of the overall structure is the distance between the rollers of the cooling roll. For the blow film method, it is not unusual to combine up to nine layers; usually a spiral - mandrel distributor is used for this purpose. Different polymers coming from several extruders are joined together via a blow head Lamination Technically, lamination signifies the joining of several layers consisting of the same or of different materials. For adhesive lamination, the adhesive is applied to the supporting film, dried in the drying tunnel, and brought to room temperature by a cooling roll. Subsequently, the two films are joined together in the laminating machine under exactly the same tensile strength (due to the curl). Semicomposites, for example, PET/aluminium, can be produced on such a machine as well. In the next production step they can be converted to a three - layer PET/aluminium/PE composite on the same machine. This composite film is characterized by an exact, curl - free flatness. For extruder lamination, the advantage is the use of PE from the melt as means of lamination. When required, the side to be laminated is primered (using an adhesion promoter) Coextrusion Films or Lamination A comparison between lamination film and coextrusion film is shown in Table Adhesives Thermoplastic adhesives are usually used for flat - bed laminating machines because they are environmentally friendly, easy to handle, and obtainable for nearly every application. Recyclability or requirements regarding monomaterial, fogging, ecological harmlessness, and health friendliness can easily be achieved with thermoplastic adhesives. Depending on the task and requirement, other adhesives, such as reactive adhesives, can be combined with laminating machines. Adhesive Systems Generally, there are different kinds of adhesives for the creation of multilayer structures: Thermoplastics Reactive adhesives Solvent adhesives Depending on the application, these adhesives are needed in different consistencies:
250 240 Chapter 33 Peel and Reseal Table 33.1 Comparison between Lamination Film and Coextrusion Film Property/Feature Lamination Film Coextrusion Film Remark Options for combination X Multilayer films with oriented and metalized films With coex-films not possible Thermoplastic adhesive Sandwich print/ X reverse print Soft, elastic, X thermoformability, shrinkage Counteraction with X Migration of monomers filled product Surface phenomena X Anti-sealing effects due to migration of adhesive Planarity, machineability X X Critical for symmetrical structures when using different polymers in coex - process Production costs, effort X Several production steps, curing times Recycling X Depending on material structure Thickness of layers X Number of production steps X X = advantageous. Powdery Area-measured material (webs, nets, and films) Thermo-liquefied granulates or dispersed, pasty, or dissolved block forms 33.3 PRODUCTION OF RESEALABLE FOOD PACKAGING Resealable polymer films present a big gain for the packaging of food. Some years ago food packages offered protection for easily perishable food only until the polymer film was opened for the first time. Once opened, cooling was the only way to protect the food against quick deterioration. Packaging then served at the best means for storage. If the food were to be kept edible for a longer time, it was necessary to put it into reclosable containers. By means of the resealable characteristic, even standard packaging today presents the possibility of storing food in a protected
251 33.3 Production of Resealable Food Packaging 241 container. If one buys a pack of sliced cheese, then it is possible to take out one slice and then reseal the pack. Complicated and time - consuming repacking in other containers is no longer necessary The Film Partners Much needs to be considered regarding the creation of packaging with a sealing layer. It is not sufficient to heat - seal two simple (mono) films in order to create such packaging. The standard packages consist of a bottom and an upper film. The upper film normally is a flexible, thin film that can be easily peeled off the thicker and more rigid bottom film. The Top Film (Lid Film) Top films must fulfill certain requirements. For the packaging of food they must have a food - safe barrier effect; they must be printable for advertisement and identification purposes; they must be resealable; and, of course, they must be compatible with the bottom films. By compatibility, that means a film with PE as the sealing layer cannot be heat - sealed with a bottom film whose sealing layer consists of another polymer material. This would inevitably lead to an imperfect connection of the two films because of the different melting temperatures. To be compatible, the top film must consist of a multilayer film that is mostly coextruded, and comprised of seven or more layers. A typical film used for lidding packages consists of PET, EVOH, and PE with a thickness of 80 μm. Essentially, the multilayer top film is as follows: Layer 1: PET Layer 2: PSA (layer of contact adhesive) Layer 3: PE Layer 4: EVOH Layer 5: PE Layer 1 A - PET has very good tensile strength, shock, and abrasion resistance as well as very good ductility, so the PET film essentially serves to protect the packaging. Furthermore, PET is thermally resistant. However, besides protection, the storage life of the foodstuff to be packaged is important, and PET also possesses a good barrier effect against water vapor. Then again, besides serving as protection for the packaging, this layer also should be pleasing to the eye, as it is the outer layer seen by the consumer. PET films have good brilliance and high transparency, and they are very suitable for printing. Layer 2 For the reseal mechanism the second layer is the most important. PSA (pressure - sensitive adhesive) is a long - lasting contact adhesive that facilitates the
252 242 Chapter 33 Peel and Reseal resealing of the upper film with the bottom film as often as necessary once the packaging is opened. Layer 3 This PE layer mainly serves as composite partner between the PSA adhesive and the next EVOH layer. Layer 4 For the protection of food against deterioration, this layer is the most important. EVOH s extreme barrier effect against gases makes it nearly irreplaceable. Today, nearly all types of cheeses and sausages are packaged in a protective atmosphere, which means that it is an inert atmosphere. To conserve this atmosphere, it is necessary to have a layer that prevents the permeation of deleterious gases (e.g., oxygen) into the package or, in case of a protective atmosphere, that impedes the diffusion of the gases out of the packaging. An EVOH layer fulfills both requirements. Layer 5 The fifth layer is also designated as a sealing layer. Essentially, the function of this layer is to ensure the sealability of the upper film with the bottom film. If the sealing layer of the upper film consists of a material different from the sealing layer of the bottom film, then closure by adhesive force is not easily realizable. Recently, film suppliers have overcome these problems with new developments. The Bottom Film The bottom film similar to the upper film must have a great many characteristics that conform to the purpose of food - safe packaging. Besides having the nearly obligatory barrier effect, this film must be suitable for resealing. A sealing layer consisting of the same material as used for the sealing layer of the upper film is therefore essential. However, in contrast to the upper film, printability is of subordinate importance, as the bottom film normally is only labeled. Its thermoformability is more important. For this reason bottom films are nearly always much thicker than upper films. Like the top film the bottom film is produced by the coextrusion method. To obtain the bowl shape that is important for packaging food, the film is thermoformed. Despite the thermoforming process by which a film consisting of one layer would be easier to handle, the bottom film usually consists of several layers in order to fulfill all the requirements mentioned above. A typical bottom film with a barrier would be made out of A - PET, EVOH, and PE layers with a total thickness of 350 μm. The structure of the multilayer bottom film is as follows: Layer 1 This layer is seen by the consumers because it is on the outside of the packaging. As already mentioned for the upper film, this layer also needs to fulfill certain usual criteria. Beside these criteria, the properties of PET as were already mentioned for the upper film should have a positive impact on the multilayer film.
253 33.4 Peel and Reseal 243 Layer 2 A top film equipped with an EVOH barrier would be ineffective unless the bottom film is equipped with a respective barrier layer. So the EVOH layer also serves as complete protection against deterioration of the packaged food. Layer 3 The third layer is the sealing layer, and it corresponds to the fifth layer of the upper film. This layer must exactly fit the sealing layer of the upper film so that a substance - to - substance bond is created during the sealing process. The sealing of the two films occurs because both films (bottom and upper film) have a PE sealing layer Sealing of the Film Partners Sealing of film partners can be done in different ways. The most common is heat sealing. This is relatively cost - effective, and also rapid, and thus economical. The quality of the seal generated depends on whether the sealing parameters for the sealing device were chosen correctly and are adequate for the combined films. The composite created should have sealing that is liquid - tight. The function of the reseal mechanism of the film also depends on a set of appropriate parameters. The sealing process of film partners is explained in the following paragraphs. Step 1 The film combination is placed on the sealing plate. It is important that the films are exactly aligned and flat on top of each other. Inexact positioning inevitably leads to bad sealing. Step 2 The sealing process is triggered. The films are pressed together with a defined amount of pressure. The parameters sealing time, temperature, and pressure all control the sealing process. Step 3 After the sealing the firmly connected films are taken out of the sealing device. Both film partners should be so firmly linked at the corresponding sealing layers that they can be separated from each other only by tearing PEEL AND RESEAL 1 Subsequent to the purchase of packaged food is storage and consumption. The pack is taken out of the refrigerator, opened, the contents are consumed. In the case of a resealable pack, the pack is closed before it is put back into the refrigerator. However, most users are not aware of the hidden processes involved in the simple opening
254 244 Chapter 33 Peel and Reseal and reclosing of the pack. The first opening so-called peeling depends on whether the film of the pack can be separated partially by tearing when peeled. If the pack cannot be opened properly, the film will not reseal The Peeling Process Each company that produces packaging films and also peelable films has its own definition and conception of the term to peel. According to the definition of this book, to peel describes the process of removal of a sealing layer from the contact adhesive layer of an sealed package. When the packaging is opened for the first time, the peeling process activates the functional layer integrated into the film that is responsible for reclosure of the packaging. In most cases this is a PSA contact adhesive. Ideally, the film structure should tear exactly at the spot where the transition of the PSA layer to the next film layer is located, due to the different surface adhesions of the film partners (bottom film and top film). The contact adhesive should be laid open in order to reclose the now destroyed composite layer if a reclosure of the packaging is desired. In reality this decisive step for the resealing of a packaging depends on many factors. Below is an overview and a description of these factors The Peeling Process in Detail Peeling Force and Peeling Angle The peeling force designates the strength that is needed to open a film composite (Figure 33.1 ). The sealing layer polymers and the parameter adjustments used for the sealing process are decisive for the peeling force. Figure 33.1 Peeling force/angle
255 33.4 Peel and Reseal 245 Figure 33.2 Left: interlaminar crack; right: translaminar crack The peeling angle describes the angle that is created between the two film partners as the packaging is opened. Scientific tests normally presuppose a peeling angle of 90 or 180. However, by taking measurements, it can be discovered that the peeling angle depends on the consumer s touch and is really between 100 and 150. Interlaminar and Translaminar Tear Characteristics Interlaminar means that the created tension does not act within a layer but between the layers (film partners) at the boundary surface. Translaminar means that the created tension leads to a tear that reaches the surface and does not allow neat peeling (Figure 33.2 ) Different Kinds of Peeling Boundary Surface Peel (Adhesion Peel) The boundary surface peel (Figure 33.3 ) is the ideal type of peel. One talks about boundary surface peel when the two film partners can be separated from each other in a specific manner. This means that there are no material remainders on the separation plane (see Figure 33.3 ). The Tear Peel In a tear peel the separation of the two film partners takes place at the interface of the two materials as the packaging is pulled open (Figure 33.4 ). However, the separation does not work for the whole joining area, and the result is that the peeling force creates a fissure between the sealing surfaces. Film separation also depends on the parameters used for the welding of the two films. The Cohesive Peel In a cohesive peel the separation of the two film partners is different. Basically, the cohesive peel involves a combination of boundary surface peel and tear peel. The film composite of PE and PB (polybutylene) illustrated in Figure 33.5 is based on the principle of boundary surface failure. The minor amount of PB in the PE matrix
257 33.4 Peel and Reseal 247 Portion of mass Peel action Boundary layer PE/PB-1 Peel off PE Sealing PB-1 A Peel force < B Greater shear in margin area is the cause for smaller PB-1 sections on the outside Figure 33.5 Cohesive peel results in only a small contact surface in the PE layer. The more PB is present in the PE layer, the smaller is the contact surface in the PE layer, and thus the peeling strength. Beside the usual sealing parameters, the cohesive peel presents the possibility of controlling peeling strength. However, that sealing strength is reduced by the presence of PB in PE because only PE can be welded with PE (refer to the sealing layer) and PE cannot be welded with PB. The Reseal Process Resealing is the opposite of peeling, and means the reclosure of the package. Similar to the peel process, there are many decisive factors for the reseal process. However, the reseal process depends not only on the sealing parameters but also on the peeling process. If the peeling process does not work satisfactorily, it is practically impossible for the reseal to be executed. Another critical factor for a correct reseal is the contact adhesive layer that is integrated into one of the two film partners and that connects the two film partners during the reseal process. The protection of the packaged food is once again guaranteed when the packaging is resealed. No reseal process would be possible without the layer of contact adhesive because, by peeling, the sealing layer of both films is laid bare and the packaging cannot be closed again unless the contact adhesive works. Function of the Reseal Mechanism The layer of contact adhesive consists of PSA integrated into the packaging, called the functional layer. The thickness of such a layer is usually between 30 and 50 μm, but significantly thinner layers of up to 2 μ m are also possible. The schema in Figure
258 248 Chapter 33 Peel and Reseal Polymer 2 Laminating adhesive (reverse printing) Polymer 1 Contact adhesive (Hotmelt) Sealable and peelable layer Sealing layer Polymer 3 Top film (Lid film) Sealing and peeling layer created by the welding of the peeling layers of the top and bottom film Bottom film (Tray) Figure 33.6 Sealed film composite 33.6 shows this process with a top film as the lid film and bottom film as the tray of the food package. Step 1 In the first step for the creation of a reseal, the two sealing layers of the individual films (e.g., a PE top film and a PE bottom film) are fused to a single layer. This integrally joined composite can be disintegrated only by the destruction of the created layer. This is exactly what happens during opening of a nonresealable package the peeling layer is destroyed. With a resealable package the peeling layer remains intact as the packaging is opened for the first time. Instead of the peeling layer, the contact adhesive layer is torn apart. The top and bottom film retain a layer of contact adhesive that can be pressed together to reseal the package. Together, the adhesion power of the two sealing layers as they are brought together is what reseals the package (Figure 33.7 ). Step 2 In the second step, the condition after the first opening of the packaging, the layer of contact adhesive, as mentioned in step 1, is separated in the middle by the peeling strength created during the first opening (shown in Figure 33.8 ). The seal and peelable layer of the top film that sticks to the contact adhesive layer is noticeable. Prior to step 1 the bowl form of the bottom film does not have a suitable sealing partner in the bottom film during the sealing. This layer simply was not sealed. The contact adhesive layer was not torn apart at this point, as the necessary peeling strength, which is transmitted through the welded sealing layer at the sides of the packaging, had not yet taken effect. Step 3 In this step the actual reseal takes place (Figure 33.8 ). The contact adhesive layer that was separated by the peeling process is brought together by compression of the two film partners. The packaging is compressed at the edges exactly where the now separated contact adhesive layers are brought together and preferably the whole seam surface touches the contact adhesive layer so it is completely closed and the best possible resealing is achieved.
259 33.4 Peel and Reseal 249 Peel force F Polymer 2 Laminating adhesive (reverse printing) Polymer 1 Contact adhesive (Hotmelt) Sealable and peelable layer Remaining sealing layer (complete, not damaged) that sticks to the PSA contact adhesive due to the missing adhesion regarding the sealing layer of the bottom film Separated contact adhesive layer created by the first opening of the packaging Sealing layer Polymer 3 Peel force F Figure 33.7 Package after first opening Polymer 2 Laminating adhesive (reverse printing) Polymer 1 Contact adhesive (Hotmelt) Sealable and peelable layer Reseal force F Polymer 2 Laminating adhesive (reverse printing) Polymer 1 Sealable and peelable layer Sealing layer Polymer 3 Figure 33.8 The reseal procedure Sealing layer Polymer 3 Rebonded contact adhesive layer created by the reseal process
260 Chapter 34 Foam Packaging with PP and PS 34.1 POLYPROPYLENE 1 Polymeric foams consume around 3.5 million tons of plastics materials annually and account for about 10% of all polymer usage in Europe. Foamed polymers are used in a wide number of application areas, which range from construction, automotive, and household products to food and protective packaging. Among the many benefits of foamed materials are their good mechanical rigidity at low specific gravity, thermal and acoustic insulation, cushioning against mechanical shock, and a significant contribution to source reduction in raw material usage. The foam market is dominated by the amorphous polymers (PS, PU, PVC, etc.), which have been industrially foamed for more than 50 years. Polypropylene (PP) foams are a relative latecomer to this market. The reasons for this lie in the molecular structure: standard polypropylene grades are semicrystalline materials with a linear molecular structure. They lack the required extensional rheological properties in the melt phase for the production of extruded low - density foams with a fine and controlled cell structure. This limitation is resolved by high melt strength polypropylene (HMS - PP) such as the Borealis Daploy. These are long - chain branched materials that combine both high melt strength and extensibility in the melt phase. They open up the possibility of bringing the many well - known property benefits of PP into the world of low - density polymeric foams. These benefits include a wide mechanical property range, high heat stability, good chemical resistance, and no monomer issues. PP also brings its good environmental credentials to this market. From a fairly recent and small beginning, the global PP foam market is growing rapidly ( > 20% per year). Current PP foam applications include automotive, insulation, and food and protective packaging. In Europe, the dominant PP foam applications are in the food packaging and automotive areas (Figure 34.1 and Table 34.1 ). 1 Borealis brochure, Daploy HMS Polypropylene for Foam Extrusion, page 02, Borealis AG, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 250
261 34.1 Polypropylene 251 Market size (kt/yr) Figure 34.1 Global market growth (Courtesy of Borealis AG) Table 34.1 Current Applications for Extruded PP Foams (Courtesy of Borealis AG) Automotive Food Packaging Insulation Protective Packaging Volume (kg/m 3 ) Examples Door liners Engine shields Roof/trunk liners Impact protection Food trays Fruit trays Tableware In the case of food packaging, PP offers a lightweight packaging solution with excellent grease/fat resistance (no stress cracking) and with no issues surrounding its monomer. Its high heat stability means products are microwaveable, with good thermal insulation, providing a cool touch during removal. In automotive applications, lightweight foam solutions have helped improve vehicle performance and fuel efficiency. With increasing pressure for end - of - life vehicle recycling, mono - material solutions are being sought and, with PP becoming a preferred polymer, recyclable foamed PP solutions are a logical next step. PP foams have an excellent moisture barrier and chemical resistance that is important for durability and functionality in the presence of hot oil, grease, or fuel. Its high heat stability opens up the possibility for under - the - hood applications. PP foams also have very good cushioning properties, thereby contributing to improved driver and passenger safety. Leading polypropylene suppliers such as Borealis are committed to supporting the development of the extruded PP foam market through grades such as Daploy HMS PP products and by offering PP foam solutions High Melt Strength Polypropylene The basic extensional rheological properties of the long - branched HMS - PP products such as Daploy are different in comparison to those of standard linear polypropylene grades. The high melt strength and extensibility defines the requirements for a
262 252 Chapter 34 Foam Packaging with PP and PS high - performance foaming grade. With such long - chain branched polymers, it is possible to produce very long density (20 50 kg/m 3 ) extruded PP foams that have a fine and controlled closed cell structure. This is not possible with standard linear polypropylene grades or modified materials that fall outside the critical high - performance foaming window. High melt strength products can be blended with the full range of standard PP extrusion grades and other polyolefinic products. This offers the opportunity to tailor the foam properties to meet the particular demands of the end - use application. Furthermore, HMS products are specifically designed to be suitable for processing on most types of existing industrial foaming equipment. HMS products and their blends are not crosslinked. This means that extruded PP foams produced from them are fully recyclable, an increasingly important demand within the polymer industry Foam Extrusion Process The first steps in the foaming process (polymer feeding and melting) are common to all extrusion processes. However, three later stages are specific and critical to the process, as illustrated in Figure These three specific steps in the foam extrusion process consist of the following: 1. Dissolving of a blow agent gas in the polymer melt 2. Cell nucleation 3. Cell growth and stabilization In order to perform these additional steps, foaming extruders are longer than standard types, typically with overall L/D ratio > 40, in either a single or tandem extruder configuration. Figure 34.2 Processing steps in foam extrusion (Courtesy of Borealis AG)
263 34.1 Polypropylene 253 Polymer Gas Solution A blowing agent is introduced into the polymer melt either by direct gas injection (physical foaming) or by decomposition of an added chemical blowing agent (chemical foaming). For both methods, a key requirement is a uniform and controlled cell structure that is a homogeneous polymer gas solution. This is controlled by two factors: the solubility of the blowing agent gas in the polymer and the sorption kinetics. The solubility itself is not a limiting factor for foaming when using the more common industrial foaming agents, butane and carbon dioxide. With the gas concentrations typically used in foam extrusion, these can be quantitatively dissolved with standard extrusion pressures up to 10 MPa (100 bar). The achievement of equilibrium solubility is determined by the sorption kinetics, and this is therefore a time - dependent process. This process can be accelerated by raising the melt temperature and using screw designs that promote good mixing of the polymer melt and injected gas. Cell Nucleation Control of cell nucleation is crucial to obtaining the desired fine and uniform cell structure of the final foam. It is a complex area with several, often interrelated, factors playing a role. The three main factors that influence the cell nucleation are the pressure drop in the die, the concentration of the blowing agent, and the concentration of the external cell nucleating agent. The rate of the pressure drop at the die is determined by the die geometry. Higher rates of pressure drop at the die significantly increase the cell density, regardless of the concentration of blowing agent gas or external nucleator. Higher shear rates are also believed to play a role in promoting cell nucleation. It has also been established that higher concentrations of blowing agent gas lead to increased cell density. The addition of external nucleating agents is the most commonly used method of controlling cell nucleation in the foaming process. These are basically finely divided and dispersed solid particles (e.g., talc) that provide sites for cell nucleation. Cell Growth and Stabilization Melt temperature is one of the most important process parameters in foam extrusion. In the case of PP foam, depending on the type and concentration of the foaming agent used, the optimum in melt temperature may vary from approximately 130 C to 180 C. When the melt temperature is too low, foaming is limited because the material solidifies before the cells have the possibility to expand fully. When the temperature is too high, the foam first expands, then collapses due to the lack of stabilization of the structure. There is an optimum melt temperature window for foaming in which lowest densities are achieved; this temperature is lower than standard PP melt temperatures ( C). The latter part of the foam extruder is dedicated to the melt cooling and mixing of the polymer gas system.
264 254 Chapter 34 Foam Packaging with PP and PS It is during this part of the process that the high melt strength polypropylene (Daploy) plays its crucial role. It high melt strength and extensibility help to control cell growth. By a strain hardening mechanism, it prevents rupture of the cell walls and coalescence, which would otherwise lead to a polymer containing a few rather large holes far from the desired fine and closed cell structure. The foam is finally stabilized by a cooling stage before winding. This is either by means of a calibrating mandrel in the case of an annular die or by a conventional roll stack when a flat die is used High Melt Strength Polypropylenes and Foamability In order to modify the final foam properties, HMS - PP grades such as Daploy can be blended with standard extrusion - grade PP types. An important consideration, however, is the foamability of such blends. When a long - chain branched PP is mixed with a standard PP, it is evident that this will have a diluting effect on the melt strength and extensibility of the blend compared with that of pure HMS - PP. Quite high levels (approx. 60%) of blend partner can be added before the extensional rheological properties of the blend begin to fall outside the critical high - performance foaming window. It is verified that the minimum achievable foam density is a function of the HMS - PP content in the blend. A wide range of blend compositions where it is possible to produce low - density ( <100 kg/m3 ) PP foams exist. Modification of foam properties is a crucial requirement in order to be able to produce polypropylene foams with properties that meet the technical performance demands of particular end - use applications. The homopolymer - based HMS - PP grades can be used pure or blended with standard homopolymers, providing foams with high stiffness and heat stability. Enhancements in impact strength and toughness of the foam can be achieved by using random or heterophasic (block) copolymers as blend partners. In the case of random copolymers, impact performance is improved at temperatures above approximately 0 C. If good impact performance is required at low temperatures ( < 0 C), then heterophasic copolymers should be used. Further interesting property modifications can be made available by using random heterophasic copolymers as blend partners, such as Borealis Borsoft. These are soft PP grades (tensile modulus 400 MPa). The blend with these products provides the opportunity to produce soft PP foams with good impact strength and toughness at low temperatures. Even softer foams can be obtained by blending HMS - PP with various polymeric materials such as metallocene LLD - PE, TPO, and EVA. The industry has recently developed random copolymer - based HMS - PP. Blends with this product family will result in even softer foam and enable their use in a wide range of existing and newly developed applications (Table 34.2 ). The proceeding general description of HMS blends can be further refined to provide more quantitative predictions of PP foam properties. This makes use
265 34.2 Polystyrene 255 Table 34.2 Blend Partner Types and Their Influence on Foam Properties (Courtesy of Borealis AG) * Blend Partner Foam Property Modification Recommended Borealis Grades Homopolymers High stiffness Poor impact Block copolymers Low temperatures Reduced stiffness Improved toughness Random copolymers Softer foams Improved toughness Borsoft PPs Soft foams Low temperature impact m-pes, TPOs, EVAs Very soft foams Low temperature impact HC600TF, HC205TF BC250MO, BC240TF, BC245MO RB501BF, RA130E, RB206MO Borsoft SA233CF *For more information and technical data sheets, see of various theoretical models for describing foam properties. One of the more important foam properties is the tensile modulus, which is determined by three basic parameters: Tensile modulus of the compact material Foam density Foam structure The tensile modulus of the starting (compact) material is determined by the chosen blend partner and the composition typically, this modulus will be in the range of 750 to 2000 MPa. The tensile modulus of the foamed material will decrease as the density decreases. The third parameter is foam structure, and this relates to factors such as the relative proportions of open and closed cells and cell size. There are experimental data available for tensile modulus as a function of foam density for different blend partners. The agreement with the theoretical predictions is good, and this provides confidence in the ability to use this as a quantitative tool POLYSTYRENE 2 In this section a new foam technology for polystyrene is described. The demands of cost competiveness and raw material weight reduction put constant pressure on the packaging industry. Significant density reduction helps reduce costs and weight. A rather new foaming technology for polystyrene uses a physical blowing agent. The so-called CO 2 RE Foaming Technology from Styron applies liquid CO 2 to the extruding process. Liquid CO 2 is injected directly into the polymer stream during 2 Styron, Fast Facts, brochure on CO2 RE Foaming Technology, Styron LLC, 2010.
266 256 Chapter 34 Foam Packaging with PP and PS extrusion, where it dissolves into the material. As soon as the polymer exits the die, the CO 2 expands, resulting in significant density reductions. This technology allows the polystyrene sheet to be fabricated with a foamed core layer. Foamed materials produced with CO 2 RE Foaming Technology provide significant density reductions of 13% to 20%. In reducing polystyrene packaging density, the outcome of CO 2 RE Foaming Technology is light weight, resulting in benefits across the value chain: Converters use less raw material and energy to produce the packaging Brand owners benefit from lower packaging waste disposable tax. The lower the density, the higher is the value extracted using foam. Foamed sheets satisfy the growing demand from customers and legislators for less packaging. As a direct result of raw material and energy savings, the carbon footprint of rigid polystyrene packaging applications will improve significantly, with potential reductions of between 10% and 20%.
267 Chapter 35 Blister Packaging of Syringes For the packaging of pharmaceutical applications, hygiene is of utmost importance. Thus the control of the packaging process is critical. In this chapter an application for the fully automatic packaging of ready - filled syringes is detailed. For this application a multilayer film consisting of A - PET/PE is used. The sealing film is made of PA/PE. The loaded and closed blister tray is loaded into a carton box in an end - of - line packaging machine. From a downstream equipment the filled syringe, two cannulas, and an instruction label are fed to the thermoforming/cartoning machine. Easy opening of the packaging, namely peeling of the sealing film, as well as completeness of the packaging contents are essential criteria. For the pharmaceutical sector product tracing must be possible. For this reason the production line must be validated and have the possibility to create batch protocols. For applications that fulfill these demands, the packaging machines of, for example, Schubert GmbH could be utilized. Standard components are used that are assembled based on the conception of the line. These machines function according to the top - loading principle (TLM). From a standard range of components, two - axis, three - axis, or four - axis robots can be chosen. The TLM packaging line consists of two main parts: a thermoforming, loading, and closing machine and a downstream end - of - the - line packaging machine. The scope of supply also comprises a manufacturing execution system (MES). It is usual in the Schubert thermoforming lines for the film to be fed automatically to the film transport system via a double roller block. The film feeding device facilitates automatic film reel change. Once the film has been heated to the forming temperature in the heating section, the semifinished material is transported to the forming station. The thermoforming tool in the forming station can be rapidly exchanged. An A-PET/PE multilayer film with a thickness of 600 μ m is used for blister production. Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 257
268 258 Chapter 35 Blister Packaging of Syringes 35.1 A -PET/PE 1 The European consumers negative attitude toward PVC has surely influenced the market for multilayer films in general, and especially for PET/PE composites, but in a positive way. However, while the sale of PVC is decreasing, the sale of PET/ PE laminates has increased in Germany from 29.1 thousand tons in 2002 to 29.5 thousand tons in The multilayer films that contain, for example, EVOH, are not included in these numbers. No current survey shows a decrease of the sales of PET/PE. There is neither a demographic trend toward bigger households nor a reduction of hygiene directives for the food trade. In addition, the customer demands concerning the quality of the packaged products will not decrease in the foreseeable future. For example, the increasingly tough competition in the food trade has made it more and more difficult to find fresh food in the supermarkets due to high labor costs. In almost the same manner, a reduction in material costs for pharmaceutical packaging can be observed in the meantime MATERIAL DESCRIPTION A typical packaging of PET/PE consists of a rigid bottom film and a flexible lid film. Normally, film composites that have a thickness between 30 and 100 μ m are used as lid films. Some examples are OPP/PE laminates, PA/PE composites, PET/PE composites, and, of course, coextruded blow films. In order to implement an absolutely tight gas barrier, a composite with an aluminium layer is used. The bottom film of rigid packages with barrier layers is composed of the PET carrier layers, the functional layers (e.g., EVOH, adhesive layer), and the PE sealing and peel layers. The PE carrier layer is produced on a calender line; it mainly consists of two layers, whereby the outer layer is equipped with antiblock additives in order to guarantee a good formability for further treatment. The thickness of commercially available PET/PE thermoforming films is between 250 and 600 μ m, whereas the percentage of PET and PET - antiblock layers is up to 70% to 80% of the whole composite. Depending on the production process, the other layers make up for the remaining 20% to 30% of the thickness. However, film manufacturers are also able to produce thicker films. Thus sometimes films with a thickness of 800 μ m are processed THE MANUFACTURING PROCESS A significant aspect of the extrusion of PET is the degradation of the material through fusion, which is measured as the diminution of the IV value (IV stands for intrinsic 1 Andreas Blin, Machines for the Production of Thermoforming Films Consisting of PET Respectively PET/PE Composites, pages , Extrusion and Thermoforming of Packaging Films, VDI Verlag GmbH Düsseldorf, 2004.
269 35.3 The Manufacturing Process 259 viscosity ). Not all the different possible processes (predrying of the raw material, degassing of the melt in the single - or double - screw extruder) will be described in this chapter, although they have a substantial influence on the characteristics of the final product. Rather, the different possibilities for the manufacturing process of PET/EVOH/PE film will be reviewed. The factor common to all these processes is the necessity to create a sufficient adhesion between PET and PE, in order to prevent delamination of the film during the thermoforming or opening of the package Coextrusion The direct way to create a PET/EVOH/PE thermoforming film is by coextrusion. In the coextrusion methods, adhesive layers are used to bind PET, EVOH, and PET together. Because of these requirements a composite consisting of six layers is necessary: PET antiblock (10%) PET (60%) Adhesive layer (5%) EVOH (5%) Adhesive layer (5%) PE, peel (15%) Such films are manufactured by means of a feedblock coextrusion. The advantages of the process are the comparatively low investment costs and the low labor requirements. The individual layers can be optimized to the material costs. The fundamental disadvantage of every kind of barrier composite is the fact that the edge trimming cannot be recycled into the extrusion. When 50 mm per side are cut from a film with a width of 1400 mm, this amounts to a material loss of 7%. If the production process is optimized, this value can be reduced to 5%; however, even this percentage represents an important cost factor. Consider that, on average, the costs for the raw material account for 80% of the direct production costs of every extruded product. For coextruded films the lamination mainly depends on the quantity of the adhesive in the adhesive layer. Therefore, manufacturers of PET/PE composites that are produced by coextrusion are able to adapt the properties of the product to the customer requirements Thermolamination If thermoforming composites are created using the thermolamination process, the problem of the recycling of the edge trims does not exist. PET films with the configuration PET - antiblock/pet are manufactured on a calendar and exactly cut according to the width of the barrier film that is fed to the machine. The monomaterial edge trim can be ground and recycled into the extrusion process.
270 260 Chapter 35 Blister Packaging of Syringes Coextrusion blow films with the EVOH and PE peel layers are produced offline and fed to the process via a continuous moving unwind. The product is created by means of heating and impacting of the two films in a roller clearance. Here the adhesion is mainly determined by the outer layer of the blow film, and compared with other processes, the adhesion is limited. However, it is possible to influence the main characteristics of the composite by optimizing the blow film. The significant advantage of this system is that, contrary to glue lamination, neither solvents nor water, which must be disposed of, are needed. This fact and the reusability of the edge trim make it the most environment - friendly way of producing the bottom film for FFS machines Glue Lamination Companies producing PET/PE composites via glue lamination do not depend on adhesion, which is created via thermal or mechanic energy contrary to the thermolamination process. They instead use a method wherein the PET base is glued to the coextruded blow film. There are different production methods where solvents may be used or not. However, methods for which the utilization of solvents is necessary are in decline, due to the expenses related to the disposal or recycling of these materials. For multilayer adhesion, glue lamination is the best possible production method. Glue lamination is also very flexible, and it is not necessary to incorporate a special layer into the blow film (as with thermolamination). Therefore, this method is especially suitable for companies that produce blow film or that want to buy this kind of film from different subsuppliers. For glue lamination a homogeneous cut of the film edges is also possible, so that not much waste is created Extrusion Coating Extrusion coating finds a place in between coextrusion and thermo/glue lamination. In extrusion coating, a PET film consisting of two layers is coated inline with a coextrusion configuration AL/PE. Additionally, blow film can be fed to the coating roller device, which is used for the application of a barrier or sealing layers. Apart from high investment costs, extrustion coating combines all the advantages of the above - mentioned other production methods: the first edge trimming can be recycled, the composite adhesion is very good, and by utilizing different films and combinations, the final product can have the required characteristics SUMMARY OF THE PRODUCTION METHODS FOR A -PET/PE FILMS The last few years in this industrial sector have shown that, contrary to expectations, no production method has become widely accepted. This is mainly because the pre -
271 35.5 Production of Blisters in the Packaging Line 261 conditions of the companies that work or commence working in this sector are very different. Technically, the above - mentioned production methods do not differ significantly from each other and in all cases adhesion as well as transparency are sufficient for industrial applications. Furthermore, all films can be processed on thermoforming machines. However, with the increasing number of vendors of these films, pricing pressure has increased. The manufacturers including the thermoforming machine manufacturers are constrained to find alternatives within the production processes in order to reduce costs. This mainly concerns different extrusion systems that do not necessitate the pre - drying of the raw material. In this connection some degassing methods are already being implemented. The use of recycled material can also help lower costs. Yet legislators in many countries prohibit the re -use of postconsumer recycled material for food packaging (not even in the intermediate layers of coextruded films). The cost-effectiveness of PET/EVOH/PE films depends to a surprisingly high extent on the recyclability of the edge trim. As already said, the edge trim accounts for approximately 7% of the material consumption, and this is a significant cost factor. More attention must be paid to the winding technology of the above - described machines, but this is a topic that exceeds the scope of this book. For each new project, machine constructors must find a solution to the problem of using either inline technology (i.e., roll cutting on a winder) or offline technology (i.e., roll cutting on a slitter - rewinder). As indicated by the large quantity of FFS machines that are built and delivered each year, the growth in the sales of thermoforming films and lid films will continue to increase. In this connection it must be mentioned that the PET/EVOH/PE composite is only one of several possible composites that can be used for this application. It is no longer possible to imagine our daily life without composite films, because to a certain extent they make our lifestyle possible in the first place. As has already happened, other basic materials for packaging, and especially for food packaging, will increasingly be used PRODUCTION OF BLISTERS IN THE PACKAGING LINE For this application a fully automated thermoforming and packaging line from Schubert is used. The temperature of each single heating section can be set individually and thus optimally according to the film combination. The blisters are formed in the forming station. The use of forming vacuum, forming pressure, and plug assist can be adapted to the requirements of each application. All movements are servo motor - driven. The process analysis provides excellent possibilities for the control and optimization of the working process. The ready-filled syringes are picked up with F44 robots, oriented horizontally, and precisely placed into the blisters that were formed in the film strip. The cannulas
272 262 Chapter 35 Blister Packaging of Syringes Figure 35.1 Picking and placing of syringes into thermoformed blisters (Courtesy of Gerhard Schubert GmbH) are also placed into these blisters, and the instruction label is applied by a group of F44 robots in the loading section (see Figure 35.1 ). Subsequent to the placement of all product components into the blisters, the blisters are sealed with ultrasound and punched at the same. Prior to this, the sealing film is fed to the machine and placed onto the blisters. The sealing film consists of several layers and is printed on both sides. The usage instructions are printed on the inner side; the outside is printed with attractive advertising. The print mark controls the positions of the sealing film exactly above the base cavities. A thermal transfer printer prints the product data onto the surface of the sealing film. Just as the carton, the sealing film has a velvety haptic texture. Sealing and punching is carried out in the ultrasonic sealing and punching station within 250 ms. In applying ultrasound with a frequency of 20 khz during such a short time period, the sealing heat is generated only at the joining area and the cutting line. So product and packaging are subjected to only a minimal thermal load and tightly sealed seams are created. An important criterion is the simple and easy opening of the packaging, even by a user wearing rubber gloves. Low - wear punching, even for rigid materials such as PET, is possible thanks to the low punching pressure created by ultrasound (Figure 35.2 ). The oscillating units that create the ultrasound are integrated into the machine and do not have to be exchanged. The sealing and punching station is equipped with a transport device for the protective film. The protective film facilitates the quick exchange of the sealing and punching tools so that the changeover times for a format change are minimal. The completely punched - out packages are placed on the product discharge belt by an F2 robot. An image processing system checks the completeness of the contents, the quality, and the consistency of the product data. These data are entered into the batch protocol.
273 35.5 Production of Blisters in the Packaging Line 263 Figure 35.2 Ultrasonic sealing and punching station (Courtesy of Gerhard Schubert GmbH) Blisters that are determined to be good are transported to the end of line packaging for further processing. In this section of the line the carton blanks are erected. Depending on the format, carton blanks with different sizes can be processed. The blisters are loaded into the erected cartons. Subsequent to the placement of instruction leaflets, the cartons are closed by an F2 robot.
274 Chapter 36 The Production of Drinking Cups Written in cooperation with Paul de Mink, Borealis AG, Austria, and Norbert Hufnagl, Kiefel GmbH, Germany Drinking cups made from plastic are used all over the world. The reasons for their use are quite different. Organizers of big events appreciate the safety aspect of plastic cups compared with glass containers to avoid the possibility of breakage. Plastic cups thus prevent accidents. Their one - time usage also eliminates cleaning of cups. Some regions of the world do not have decent working water pipelines. This makes the supply of water a hygienic problem. The solution could be water in thermoformed and sealed containers. These containers could be packaged in transport trays and delivered directly to the consumer. Plastic containers are being used for millions of items. The item described in this chapter is the drinking cup made of polypropylene (Figure 36.1 ). There has been great innovation in the manufacture of polypropylene in the recent years. 1 Because of the recycling trend promoted by an environmentally conscious public, and also economic factors, the use of PP has greatly increased. In particular, extruded PP applications mostly in the packaging industry are the motivation for continual development of the entire group of this material. The extensive research that is being done has brought much variability to the characteristics and properties of PP (better catalytic converters, better polymerization technology, compounding, etc.). It is now possible to expand into areas of applications where before the standard PP could not be used. Thanks to the willingness of the engineering industry (extrusion, thermoforming, etc.) to innovate and develop polypropylene, PP is in a position to take a dominant position in the packaging industry. 1 Paul de Mink, PP in der Thermoformung, pages 31 36, Extrudieren und Thermoformen von Verpackungsfolien, VDI Verlag GmbH Düsseldorf, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 264
275 36.1 From Monomer to Polymer 265 Figure 36.1 Drinking cups (Courtesy of Kiefel GmbH) In this chapter the example of the drinking cup is used to show the basics of PP, its modifications and developments. Additionally, the discussion will extend to all major influences on PP film s characteristics and the ability to thermoform it due to the different processing conditions in the production of PP film. With an average growth of 6% to 7% per year, the worldwide demand for PP is for more than 30 million tons. Western Europe, North America, and Asia handle 70% of this demand. The major areas of applications are found in the food industry, consumer items, and the automotive industry. The most important customers in western Europe are Germany, Italy, the United Kingdom, and France. The factors responsible for the relatively high growth rate of polypropylen are, next to its broad variety of use, its economic and environmental advantages. These attractive characteristics of polypropylene are quite numerous: Economical material (monomer costs) Low density (0.9 g/cm3 ) High durability temperature Good chemical resistance Good processing and recycling performance Modifiable in a wide range Ecological benefits 36.1 FROM MONOMER TO POLYMER The first time polypropylene was polymerized and used in a technical way was at Montecatini, Italy, in the 1950s. With the rapid development of catalysts it
276 H H H 266 Chapter 36 The Production of Drinking Cups Polymerization Polypropylene (PP) Monomer Polymerization Polymer H H H H H H H C C C C C C C H H C H Mitsui Slurry Himont Spheripol,... Borealis Borstar H H C H H H C H H Propylene C 3 Polypropylene Figure 36.2 Polymerization (Courtesy of Borealis AG) was possible to increase the PP turnover enormously per catalyst unit. Polyolefins such as polypropylene and polyethylene are produced through polymerization (Figure 36.2 ). Polymerization is the connection between a single molecule (monomer) to a bigger molecule (macromolecule) with the employment of the correspondent catalyst system. The size of the macromolecule is determined and stated by its molecular weight or the degree of polymerization. The degree of polymerization is the number of smaller molecules (monomers) combined to form one macromolecule. The weight of the molecules is defined by the combined weight of atoms that are contained in one molecule. The weight of the macromolecules is calculated by mulitiplication of molecular weight of the monomers with the degree of polymerization. The CH 3 groups can be placed in different orders in space. This has an influence on crystallinity. There are isotactic, syntactic, and atactic orders MECHANICAL AND THERMAL BEHAVIOR OF PP Areas of processing and application (temperatures of usage) of PP are mainly determined by the thermal mobility of the macromolecules. The characteristical conditions and transitional areas are simplified in Figure The glasscondition of thermoplastics is based on a strong cohesive strength due to the low temperatures. Because of the high minor valence forces between the macromolecules, only mobility between the hydrogen atoms is possible (vibration, oscillation, and rotation). With a corresponding raising of the temperature, the glass transitional temperature (ceding to a brittle - glassy thermoelastical condition) reached. This is the point where minor valences, which lie in disarray between the chains of molecules, are overcome and become movable against each other. There will be oscillations of
277 36.2 Mechanical and Thermal Behavior of PP 267 atomic mobility: vibration rotation micro-brownian molecular movement micro-brownian molecular movement degradation of the molecules vibration of chain segments glide off of molecular chains chain fission T g T m glass transition temp. melting temp. decomposition temp. Figure 36.3 Thermal mobility of macromolecules (Courtesy of Borealis AG) T z T s T g T g T m G G d G d 0 T 0 T amorphous thermoplasics working temperature below T g partially crystalline thermoplastics working temperature between T g and T m T s...secondary transition temperature T g...glass transition temperature T m...crystallite melting range G...elastic component of shear modulus d...loss factor Figure 36.4 States and working ranges (Courtesy of Borealis AG) chain segments (micro - Brownian molecule movements). In practice, it is at this point that the polypropylene has reached the usage temperature. At the usage temperature, all adhesive points between the macromolecules dissolve, and slip - off occurs in the molecular chains (melting range). This is the area where the micro - Brownian molecular movement transitions to the macro - Brownian molecular movement (melting condition). As the temperature decline is reached, there occurs a decline of molecules due to the high thermal strain. This transitional behavior is described by the torsion pendulum test. The successive curves of the mechanical - thermal behavior of amorphous, semicrystalline thermoplastic are shown in Figure 36.4 and illustrate
278 268 Chapter 36 The Production of Drinking Cups 10000,00 T g 1000,00 PP Strength 100,00 10,00 1,00 PS 0,10 Temperature ( C) 0, T g T m Pressure (6 bar) Too Soft (No Melt Strength) PS - Amorphous Polymer: Gradual Softening above T g PP - Crystalline Polymer: Rapid Loss of Strength around T m PP has Narrow Thermoforming Temperature Range PP: C PS: C Figure 36.5 Strength/temperature (Courtesy of Borealis AG) the fact that PP (partially crystalline) thermoforming is, in comparision to, for example, polystyrene (which is amorphous), a little more critically structured. The ideal state during thermoforming of thermoplastics is when the substance is in the transitional stage between thermoelastic and thermoplastic. The glass - transitional temperature of amorphous thermoplastics is higher than the usage temperature. The mechanical ease factor d (damping) reaches its maximum in this stage. There will be then a relatively broad thermoforming range due to a gradual softening. Unlike the semicrystalline thermoplastics that have their glass - transitional point below the usage temperature, the maximum of mechanical alleviating factor (maximum mobility of the molecular chain) is reached just before the crystalline melting point. A more or less abrupt changeover from thermoelastic to thermoplastic condition occurs in the tide processing window when working with the thermoforming of polypropylene. The diagram in Figure 36.5 shows that fact very clearly. 2 While with raising temperature the PS curve shows great length in the working range (pressure 6 bar and too soft, no melt strength), the curve of PP drops nearly through this area. For PP processing more temperature control is necessary in the thermoform machine. To keep the film from sagging, the machine needs to supply longer heating length of the heating system and a spreading film transport system, which will be described next. The relative heat absorption, that is, the specific heat conductivity, of polypropylene differs greatly compared with amorphous thermoplastics. That is 2 Paul de Mink, PP in der Thermoformung, pages 37ff., Extrudieren und Thermoformen von Verpackungsfolien, VDI Verlag GmbH D üsseldorf, 2004.
279 36.3 Difference between Mold Shrinkage and Free Shrinkage 269 Heat Content PP PS Temperature ( C) More heat needed to raise temperature of PP than PS 2.3 times more heat needed to reach forming/extrusion temperatures Additional heat must be removed after processing Figure 36.6 States of heating/cooling (Courtesy of Borealis AG) why more energy is needed to heat up or cool down PP compared with PS (Figure 36.6 ). The torsion pendulum test can be used to describe the mechanical - thermal behavior of thermoforming films. Besides the material - specific characteristics, this shows the influence of the film s production history (influence of PP film production on crystallinity and morphology) based on corresponding differences in the curve s progression. From the shape of the curve, conclusions can be drawn about the thermoforming behavior of the PP film. One more considerable difference between amorphous and semicrystalline materials during processing (extrusion and thermoforming) is the shrinkage of these materials. Allowance must be made in the mold design to compensate for shrinkage. Shrinkage guideline values for different thermoplastics as used to calculate thermoforming molds and tools are shown in Table DIFFERENCE BETWEEN MOLD SHRINKAGE AND FREE SHRINKAGE It is important for the processor of plastics and consequently for the thermoformer to understand the difference between mold shrinkage and free shrinkage Mold Shrinkage Thermoplastics are subject to a volume contraction during freezing in a cavity. This causes the dimensions of the formed parts to be smaller than the respective tool dimensions by a certain shrinkage value.
280 270 Chapter 36 The Production of Drinking Cups Table 36.1 Shrinkage Data (Courtesy of Borealis AG) Material Shrinkage (%) ABS SAN MIPS PS LDPE HDPE PP RPVC FPVC PC PMMA Free Shrinkage If thermoplastics are heated beyond the glass - transition temperature, there is shrinkage due to an orientation relaxation of the molecules. The extent of shrinkage depends on the degree of orientation forced on the thermoplastic during processing. A number of factors can contribute to shrinkage: Shape of formed part Evenness of wall thickness of formed part Tool temperature Deep drawing ratio Forming temperature Filling material in the plastic The total shrinkage follows from the processing shrinkage and the post - shrinkage. Most shrinkage occurs shortly after processing. However, to measure the total shrinkage, it is necessary to also take the post - shrinkage into consideration. This is why the measuring of a particular part for shrinkage should take place after 24 hours POLYPROPYLENE MODIFICATIONS Basically, there are three types of PP modifications (Figure 36.7 ) 3 : Homopolymer. Polymerization from pure propylene. Random copolymer. Polymerization from propylene with ethylene as comonomer, which is statistically distributed in the chain. 3 Paul de Mink, PP in der Thermoformung, pages 38ff., Extrudieren und Thermoformen von Verpackungsfolien, VDI Verlag GmbH D üsseldorf, 2004.
281 36.4 Polypropylene Modifications 271 Figure 36.7 Basic polymer diagram (Courtesy of Borealis AG) E-modulus tenacity haze gloss TF-temp. range block copolymer random copolymer homopolymer Figure 36.8 Mechanical and optical properties (Courtesy of Borealis AG) Block copolymer. Heterophasic system, with one homopolymer as a continuous phase in which the EPR as a second component is polymerized. The choice of PP modifications appropriate for a certain application is always based on the requirement profile of the finished part. Figure 36.8 compares the different PP modifcations and shows the mechanical and optical attributes of the thermoforming films. The greatest stiffness with relatively low toughness is reached with the PP homopolymers. PP block copolymers are used when toughness is needed, even at low temperatures. Block copolymers are, based on their rather poor optical attributes, not adequate for transparent applications. Random copolymers display good optical attributes. Random copolymers are rarely used for thermoforming because of their insufficient stiffness and weak thermal resistance. Random copolymers are used for certain applications when a gloss - and - sealable coating is needed, or for a blending component to enhance optical and toughness factors and processibility in transparent applications. With regard to thermal moldability, copolymers as compared with PP homopolymers are characterized by a broader temperature - remoldability range.
282 272 Chapter 36 The Production of Drinking Cups total working capacity (J/mm) block copolymer random copolymer homopolymer +23 C +4 C 0 C 10 C 20 C 30 C Figure 36.9 Toughness on TF films (Courtesy of Borealis AG) Another important criterion when choosing a corresponding PP material is the application temperature range of the finished part (Figure 36.9 ). Based on the predetermined glass - transitional temperature range of the single PP modification, use of the PP homopolymer is possible only above 0 C. The thermoformed packaging of, for example, yogurt, which is stored without a mechanical enchroachment on cooled shelfs at + 7 C, is a standard application for PP homopolymers. PP random copolymers show, depending on their C 2 concentration, greater toughness at lower temperatures. However, the temperature - durability upward is reduced. The PP modification with the most diverse temperature - application range is the PP block copolymer. Because of their excellent toughness in the lower temperature ranges, combined with the corresponding temperature durability upward (similar to PP homopolymer), PP block copolymers are suitable for frozen food packaging applications (e.g., convenience food). These can be microwaved as needed. The market demands even more property improvements, 4 and the end of property improvements has not yet been reached. Research aiming to create a material with the following properties is continuing at companies such as Borealis AG: Stiffness like PP homopolymers Toughness like PP heterophasic copolymer (even at low temperatures) Transparency like PP random copolymers Processability like PS While it still is not possible to quite meet all these properties in a single PP type, the profile of the present heterophasic PP type has been enlarged to include stiffness like PP homopolymers, toughness like the standard PP heterophasic copolymers, and transparency like the PP homopolymers. 4 Paul de Mink, PP in der Thermoformung, page 41, Extrudieren und Thermoformen von Verpackungsfolien, VDI Verlag GmbH D üsseldorf, 2004.
283 36.5 Thermoforming Conditions and Finished Part Attributes THERMOFORMING CONDITIONS AND FINISHED PART ATTRIBUTES 5 Figure shows the basic visual differences achieved with PP modification. In addition there is, with rising thermoforming temperature, the issue of greater haze. As is implied, PP random copolymer types have the widest and homopolymers the narrowest forming temperature ranges. The dependencies of mechanical characteristics are shown in Figure With diminishing thermoforming temperatures, a definite increase in E-modulus is evident based on the according higher degree of stretching (orientation). Not shown, however, and worth mentioning is that with declining forming temperature, shrinkage will also rise. haze random copolymer homopolymer block copolymer thermoforming temperature Figure Transparency versus TF temperature (Courtesy of Borealis AG) E-modulus random copolymer block copolymer homopolymer 0 thermoforming temperature [ C] Figure E-modulus versus TF temperature (Courtesy of Borealis AG) 5 Paul de Mink, PP in der Thermoformung, pages 42ff., Extrudieren und Thermoformen von Verpackungsfolien, VDI Verlag GmbH D üsseldorf, 2004.
284 274 Chapter 36 The Production of Drinking Cups Figure Molecular weight distribution (Courtesy of Borealis AG) 36.6 DISTRIBUTION OF MOLECULAR WEIGHT Besides the basic (general) differences in characteristics of different PP modifications, the mechanics, optics, and thermoforming behavior will be influenced by the distribution of molecular weight of the particular polypropylene. 6 Basically, a distinction is drawn between the standard PP (ST - PP, with broad molecular weight distribution) and CR - PP (controlled rheology PP, with narrow molecular weight distribution); see Figure In simple terms, the molecular weight distribution is the ratio of the medium molecular mass (depending on the length of the macromolecules) to the number of molecule chains. In the production of CR - PP, standardization of the existing macromolecular chain length is reached through chemical degradation with peroxide. This modification causes a change in the flow characteristics (viscosity) and morphology, on the one hand, and in the mechanics and optics of the thermoforming film, on the other hand. In addition, the forming temperature range will be influenced (Figure ). The biggest advantage of CR - PP while thermoforming is the relatively low mold shrinkage. This is associated with a narrower forming temperature range INFLUENCE OF NUCLEATION OF PP ON PROCESSING AND CHARACTERISTICS OF THE FINISHED PART The thermoformabilty and, accordingly, the properties of a finished part depend primarily on the morphological structure of the film. These properties are altered by chilling or by the addition of germs (nucleation). After the extruder a chill roll or calendar stack, as a chilling unit, will follow, depending on the thickness of the film. 6 Paul de Mink, PP in der Thermoformung, pages 44ff., Extrudieren und Thermoformen von Verpackungsfolien, VDI Verlag GmbH D üsseldorf, 2004.
285 36.7 Influence of Nucleation of PP on Processing and Characteristics 275 broad MWD narrow MWD yield stress elongation E-modulus transparency shrinkage thermoforming range Figure Molecular weight distribution, mechanical, optical, and processing properties (Courtesy of Borealis AG) Figure Nucleating effect, morphological structure (Courtesy of Borealis AG) Next is the high chilling effort for non - nucleated PP, to reach a fine-grained structural composition over the cross - section of the film, which for nucleated types has no relevance. That means that unlike the unfavorable influence of increasing chilling temperatures on the crystalline structure of standard PP, the brittleness and optics will be less affected with the nucleated film (Figure ). As a result a higher speed of production (less time at the calendar stack) is possible Types of Nucleation Basically, there are two types of heterogenic nucleating agents: Inorganic nucleating agents (e.g., talcum, mica, kaolin) Organic nucleating agents (e.g., benzoate, sorbitol)
286 276 Chapter 36 The Production of Drinking Cups heat of reaction (J/g) Tk a Tk b cooling a: non-nucleated b: nucleated heating Ts temperature Figure Nucleating effect (Courtesy of Borealis AG) film thickness, 300 μm yield stress elongation E-modulus transparency gloss Figure Nucleation impact on mechanical and optical properties (Courtesy of Borealis AG) Mode of action of nucleation: Changed crystalline behavior (Figure ) Higher crystallization due to the higher crystalline temperature Fine spherulite structural conditions (improved optical properties) Improved thermoform film properties (mechanical properties such as E - modulus and yield stress, and optical properties such as transparency and gloss; Figure ) 36.8 High Crystalline/High Stiffness Polypropylene In comparison to standard PP, the high stiffness PP has a higher isotactical index (> 98%) and higher stereoregularity (even order of CH 3 side groups). 7 Crystallization 7 Paul de Mink, PP in der Thermoformung, pages 47ff., Extrudieren und Thermoformen von Verpackungsfolien, VDI Verlag GmbH D üsseldorf, 2004.
287 36.9 Influence of Film Production Technology 277 Figure High-crystalline and high-stiffness PP (Courtesy of Borealis AG) of the produced film will be higher with this combination, and also, from the special nucleating agent, a fine spherolitic structural condition will be achieved. The advantages of such modifications are excellent thermoformability (high output, faster forming cycles, easily stacked finished parts), high stiffness, good toughness, and also high temperature durability. In addition, the finished parts have a better water vapor barrier (Figure ). The advantages for the thermoformer are, on the one hand, a higher productivity (faster cycles) and, on the other hand, the possibility of a thickness reduction and accordingly a weight reduction, to save material and costs INFLUENCE OF FILM PRODUCTION TECHNOLOGY The choice of technology for the production of thermoforming film has a major influence on the mechanical, thermal, and optical properties and also on the subsequent processing. 8 Borealis AG has reviewed these properties with regard to blister applications on forming, filling, and sealing machines. A major feature of the Borealis study was the substitution of PVC for blister wrapping in the packaging of medications and luxury foods with polypropylene. Using the FSS lines of packaging machine producers, packaging and pharmaceutical companies were asked to approve films that were produced by water bath technology, and also films that were produced with conventional technology. 8 Paul de Mink, PP in der Thermoformung, pages 51ff., Extrudieren und Thermoformen von Verpackungsfolien, VDI Verlag GmbH D üsseldorf, 2004.
288 278 Chapter 36 The Production of Drinking Cups Next to the choice of material, the technology used has a major influence on the behavior of the subsequent processing of the produced film. More precisely, in this study the previous history of μ m blister film was at issue. The production technologies that were tested were as follows: Chill roll technology (Figure ) Calender stack technology (Figure ) Water bath technology (Figure ) Steel belt technology (Figure ) The material used was Bormed DM55pharm (PP homopolymer; MFR 2.8 g/10 min). Blister films with a thickness of 300 μ m were produced. Different technologies and a particular product were used as a base to collect data on specific influences. The analysis and results were discussed and carried out within this group of technologies. This way a direct comparison of the technologies could be made. Pulling Test/Tensile Test As was expected, the single technologies, based on their different cooling conditions, turned out to have a large influence on crystalline behavior and, accordingly, the stiffness of the produced film (Figure ). Due to the shock of evenly cooling the film by water bath technology, there was a relatively small E - modulus with almost identical results in the longitudinal and cross directions. Films that were produced by steel belt technology had also, due to Figure Chill roll technology (Courtesy of Borealis AG)
289 36.9 Influence of Film Production Technology 279 Figure Calender stack technology (Courtesy of Borealis AG) Figure Water bath technology (Courtesy of Borealis AG)
290 280 Chapter 36 The Production of Drinking Cups Figure Steel belt technology (Courtesy of Borealis AG) Material: Bormed TM DM55pharm Film thickness: 300 μm E-modulus (MPa) chill roll roll stack water bath steel belt Figure Stiffness (Courtesy of Borealis AG) MD TD even cooling of the inside and outside, a small difference in the longitudinal and cross directions. The higher E-modulus ( 200 μ m) of steel belt films compared with water bath films is connected to the lesser cooling capacity (in this case a belt temperature of approximately 50 C). The E - modulus data of calendar stack films are comparable to the data of steel belt films. However, there is a certain anisotropism of the longitudinal and cross directions. This is caused by the orientation in combination with the necessary rolling bank and the corresponding temperatures of the polishing rolls. The highest E - modulus was measured on the chill roll film with the lowest cooling capacity. This phenomenon is explained by the fact that the use of chill roll technology for the production of μ m thick PP film under different cooling conditions of inside (air knife) and outside (chill roll) is critical. For film production the high chill roll temperatues ( > 80 C) were adjusted to obtain adequate film surface and flatness. The data in the longitudinal and cross directions were fairly consistent, but the high amount of crystallization led to a high E-modulus.
291 36.10 Optical Properties 281 Toughness The study of toughness showed clearly that water bath technology, due to its very homogeneous and intensive cooling period, prevents the crystallization from becoming too dense and so reaches a higher toughness compared with other production technologies. The energy puncturing the water bath film was about 700% higher than that for the steel belt film OPTICAL PROPERTIES Surface Gloss 9 Among other things, surface quality is based on the optical characteristic of the film. This means that with better transparency comes better surface gloss. If the four researched cooling technologies are compared for surface gloss, it becomes clear that the technologies where the cooling period of the melt is done by bilateral contact cooling on polished steel surfaces have the advantage. Even contact cooling between the chilling roll and the cooled steel belt can achieve high surface gloss on both sides. A relatively high gloss on the inside of the film (contact with chill roll 1) can be obtained with the calendar stack technology. There will be a low gloss on the film outside due to the line - shaped contact (outside) of the polishing stack and the deferred timing when the film meets the second chill roll and through that the consequent advanced crystallization. A second polishing stack between chill roll 1 and chill roll 2 would help even out the gloss (Figure ). However, this is possible only when the cooling temperature is relatively high and a single chill roll drive is available (to prevent wrinkling due to shrinkage). An even gloss on both sides can be achieved when using the water bath technology (homogeneous cooling). With this procedure there is no polishing stack Material: Bormed TM DM55pharm Film thickness: 300 μm gloss (%) outside inside chill roll roll stack water bath steel belt Figure Optical properties: gloss (Courtesy of Borealis AG) 9 Paul de Mink, PP in der Thermoformung, pages 57ff., Extrudieren und Thermoformen von Verpackungsfolien, VDI Verlag GmbH D üsseldorf, 2004.
292 282 Chapter 36 The Production of Drinking Cups Material: Bormed TM DM55pharm Film thickness: 300 μm HAZE (%) chill roll roll stack water bath steel belt Figure Haze (Courtesy of Borealis AG) to raise the surface gloss and that is why the gloss data are lower compared with steel belt film. The least favorable way to attain good optical properties of the film in this thickness range (300 μ m) appears to be chill roll technology. There will be no particular gloss on both sides of the film because of the air knife used and the subsequent low surface pressure on the chill roll. Haze The measured data on haze resulting from the different technologies used to produce the films suggest the following. The highest haze data, and therefore least transparency, are found in films produced with chill roll technology. On the one hand, this is due to the low surface gloss and, on the other hand, to the formation of a coarse spheroidal structure from the high cooling temperatures used to produce the film. The best transparency (least haze) was obtained using the water bath technology. The main reason for this is the even, bilateral chilling of the film, which shocks and inhibits the formation of spherulites, so the amorphous character of the smelter more or less remains. The somewhat higher haze data measured with steel belt film is followed by the calendar stack films (Figure ). Compared with the water bath film there is higher crystallization, and the good transparency has a positive effect on the surface gloss FILM MORPHOLOGY Microscopic Examination 10 Based on a structural cross - sectional analysis of all films (water bath, steel belt, and calendar stack) there are definite differences in the morphology, and these dif- 10 Paul de Mink, PP in der Thermoformung, pages 59ff., Extrudieren und Thermoformen von Verpackungsfolien, VDI Verlag GmbH D üsseldorf, 2004.
293 36.11 Film Morphology 283 water bath steel belt roll stack Figure Morphological structure (Courtesy of Borealis AG) ferences are supported and explained by the results of previous research (Figure ). Clearly, the best and finest structural condition is reached by water bath technology (Figure ). It is noticeable that the outer layers have a certain starting crystallization that is a result of belated temperature activity. It turns out therefore that water bath films have, in the mid - cross - section, a finer structure than in the outer layers. Compared with other technologies this is unique, and the homogeneous temperature over the cross - section is an enormous advantage for thermoforming. In comparison, the structure of the steel belt film reveals fine-grained edges that grow toward the middle of the film. The high temperature cannot be reduced fast enough during the cooling down of the film. As a result, the crystallization in the middle of the film s cross - section is higher. This effect is rather disadvantageous for the subsequent thermoforming. To reach a certain molecule chain movement at the center of the film while it is being heated, enough energy must be supplied (PP has a low thermal conductivity). Compared with water bath film, there are slightly less beneficial conditions for processing on FFS lines. The morphology of the polished films is where the differences are extreme. As with the steel belt technology, the growth of crystallization toward the middle of the film can be observed. The growth correlates with the film thickness, and there is a certain formation of layer structures. In the production of polished films it may be that a good thickness distribution and a high surface gloss is reached between the calendar stack and the first chill roll worked with a rolling bank. The thinner the chosen thickness of the film, the higher must be the line pressures between the calendar stack and the chill roll. In addition, the mass of the rolling bank correlates with the film thickness. This means that the distance of the rolling bank to the appointed polishing gap is about 400 μ m and the deformation mechanism causes differing moving speeds of the circulating melt in the rolling bank. At the center of the rolling bank the moving speed is next to zero. The material layers located next to the roll surface come close to their speed, based on their adhesion to the cylinder
294 284 Chapter 36 The Production of Drinking Cups 10 4 shear modulus roll stack steel belt water bath chill roll Temp. ( C) Figure Mechanical-thermal behavior (Courtesy of Borealis AG) wall. This is why there are formations of different layer structures in the cross - section when the film is cooled down. Mechanical-Thermal Behavior 11 Recall that the thermoforming of PP takes place in the transitional state from thermoelastic to thermoplastic, which is when maximum movability of the molecules occurs. It is possible, with the help of a modulus of shear/temperature diagram (torision pendulum test), to draw conclusions as to the behavior and subsequent processing of the thermoforming film (Figure ). In the figure the values for the shear modulus in the temperature range between 100 C and 150 C are compared for the water bath film, steel belt film, and chill roll film. Considerably higher modulus of shear data is attained in polished film with the rollstack method. This means that the movability of macromolecules in the polished film is within this temperature range, compared with films that are produced with different technologies. This suggests that an application of higher energy is needed to reach acceptable thermoforming. From these results films that are produced with the water bath technology seem to be most advantageous for subsequent processing with FSS equipment. The low crystallization of the produced film is due to a low deformation temperature, which leads to a relatively low E - modulus but with high damping (optimal movability of the molecules) THE THERMOFORMING MACHINE For the production of drinking cups made of polypropylene an automatic thermoforming machine of the KTR series manufactured by the company Kiefel was used. 11 Paul de Mink, PP in der Thermoformung, pages 61ff., Extrudieren und Thermoformen von Verpackungsfolien, VDI Verlag GmbH D üsseldorf, 2004.
295 36.14 Stacking 285 These KTR thermoforming machines are detailed in Chapter 27, Production of Flower Pots. If only a few format changes are required, then the connection of an extrusion line to the thermoforming machine is advisable. For the processing of PP the heating section in the thermoforming machine must be extended, unlike the processing of other kinds of plastics. This is achieved by a preheating station or by an integrated preheating in the thermoforming machine. Such an integrated preheating has upper and lower heating devices the same as the main heating. It is important for this application that the thermoforming machine be equipped with a spreadable film transport system in order to compensate for the extreme sagging of the heated polypropylene film. One option is to integrate a film transport system with longitudinal expansion. The transport system should nevertheless be expanded to prevent the sagging of the heated film so that a flat and tightened film is fed to the thermoforming station. In this way the same conditions can be ensured anywhere in the multi - cavity tooling. This is an essential pre - condition in order to achieve reproducibility of quality within the array of the mold surface. To increase the cycle speed, the use of servo drives in the forming station is also necessary for this application; the plug assist is also driven by a servo motor. For the manufacturing of thermoformed parts for example, drinking cups made of PP homogeneous heating of the film is indispensable. The processing temperature must be kept constant and uniformly distributed over the mold surface. Prestretching of the film is absolutely necessary and achieved by quick and precise servo drives. A precise definition of the formed parts can be achieved if the individual cavities of the mold are filled with forming air very quickly. It is difficult to heat the polypropylene film, and it is also difficult to draw the heat from the formed part consisting of polypropylene. Therefore the use of an efficient cooling system is necessary THE MOLD For some applications it may happen that the forming tool consists of 50 cavities, whereas the respective drinking cup has a punching diameter of 70.3 mm. From a film that has an original thickness of approximately 1 mm, cups with a weight of 2.3 g are thermoformed. The output is 40 cycles/minute. For such speeds the use of directly cooled tools is necessary STACKING The stacking of 50 formed parts for a cycle speed of 40 products per minute makes the use of high - performance stacking devices necessary, such as the stacking devices of the KIST type manufactured by Kiefel or pickup stacker devices. The unloading of the formed parts from the tools is done with an unloading mandrel. Subsequently, a predefined number of cups is stacked to form a pile.
296 286 Chapter 36 The Production of Drinking Cups DOWNSTREAM DEVICES Many drinking cups are produced with a so - called U - rim in the forming tool. Drinking cups with the U - rim are beaded by a rim rolling device. The rim rolling device curls the U - rim, and thus a round lip at the rim of the cup is created. Normally, a rim rolling device consists of three heated screws with axes of symmetry that are parallel to each other. In order to transport the cups through the machine in the center of the rim rolling device, the screws are placed in a similar way as in a planetary drive. The screws have tapered threads; thus the U - rims of the cups are deformed as the cups are moved through the device. Some cups are printed. Subsequently, the cups arrive at the flow wrapper where stacks of cups are packaged. In the next step the cup stacks are packed into boxes, upright or lying flat, and then palletized.
297 Chapter 37 Ultrasonic Sealing and Cutting in Thermoforming In common thermoforming, filling, and sealing applications the processes of sealing and cutting are performed in two separate steps. 1 In order to combine sealing and cutting in one station a new device has been developed employing ultrasonic technology so that both functions can be executed simultaneously. The ultrasonic sealing and cutting station reduces sealing times, cutting forces, wear and tear, as well as floor space, facilitating fast format changes. Contaminated rims can be sealed without compromising the sealing integrity and thus preventing any exposure to the atmosphere, so that neither are food items permitted to spoil nor medical items to lose their sterility. This device provides data for logged sealing quality and is linked with the control system of the entire packaging line BACKGROUND When in the past Schubert robotic picker lines were connected inline with thermoform lines and sealing stations, the four - axis robots (F44) could not attain their full efficiency. The intermittent mode of operation of the thermoform module and the sealing station impeded the continuous run of the packaging film and the trays molded therein. A newly developed thermoforming machine system works with moving and repeating forming and sealing/cutting modules. The reciprocating modules facilitate a continuous running of the packaging film and thus the efficiency of the picker line increases. The principal forming, filling, and sealing operations are as follows: Unrolling of the film Heating of the film 1 Sven Engelmann, Ultrasonic Sealing and Cutting in Thermoforming, ANTEC, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 287
298 288 Chapter 37 Ultrasonic Sealing and Cutting in Thermoforming Forming of the film to create form parts Filling Sealing Cutting Removal of the pack A Schubert toploading forming filling and sealing machine (TLM- FFS) therefore consists of a forming station, a picker line, and an ultrasonic sealing and cutting station. The continuous motion of the film is not the only characteristic of the TLM - FFS worth mentioning. The line also facilitates an automatic change of the film reel, meaning that if the film of a reel is exhausted during operation, the film of a second roll is fed automatically to the line. While the film of the second reel is being thermoformed, the first film reel can be replaced. In the forming station the thermoform process can be effected by using compressed air and/or a vacuum. All thermoformable packaging plastics can be processed. The application spectrum comprises soft packs as well as hard packs. Sealing is done with the ultrasonic method. This entails the slightest thermal exposure, which results in minimal sealing times. Furthermore, even unclean sealing surfaces can be tightly closed. The sealing station also serves as a cutting station. The plastic pack is separated from the film by an ultrasonic - sealing/cutting tool. Cutting by ultrasound requires less punching force than conventional cutting, which therefore requires less elaborate punching presses. The result is less wear for tooling and machine modules DEVELOPMENT OF ULTRASONIC SEALING AND CUTTING TECHNOLOGY It is necessary that the working stations move at the same speed as the packaging film, in a synchronized movement, until the working cycle is completed in order to facilitate the continuous running of the film. Then the station moves contrary to the direction of travel of the film back to its point of origin and thereafter a new cycle starts. This requires the use of lightweight units in order to make fast movements possible. For conventional thermoforming high cutting pressure needs to be applied, and this required solid punch presses. If sealing is done as a first step, then the pack that has to be sealed must be put under pressure and exposed to heat in a press. So the task was the development of a lightweight unit that is able to punch the usual cutting line lengths with slight cutting pressure. Cutting and sealing of the packs should be done simultaneously in the projected station, allowing the development of space - saving machines. A quick exchange of the sealing/cutting tools was another objective. For conventional thermoforming the cutting pressure can be lessened to a certain extent, for example, by warming the steel rule die of the cutting edge or by warming the thermoform film. The result was the procedure of warming the plastic
299 37.2 Development of Ultrasonic Sealing and Cutting Technology 289 material during the sealing and cutting process only at the points where heat is absolutely necessary. This heat is generated only for the time of the sealing and cutting by applying the principle of ultrasound The Principle of Ultrasound Sound waves above the limit of audibility are called ultrasound. A generator converts the main voltage (50 Hz) in high - frequency AC current (20,000 or 35,000 Hz). This AC current is conducted to the converter by a shielded high - frequency cable. Using the piezo - ceramic effect the converter transforms electrical oscillation into mechanical oscillation. Ceramic disks are loaded with high - frequency current. Depending on the frequency, the alternating current generates a continuously alternating change of length the amplitude. To transform the oscillation to the sonotrode (horn), a so - called booster is used. The booster also acts as a transmitter. Certain transmission ratios are responsible to increase or decrease the amplitude. Maximum amplitudes are around 30 μ m. Converter, booster, and sonotrode form an oscillation unit (Figure 37.1 ). A certain number of oscillation units together form a flat surface under which almost any geometry can be sealed and cut. This enables format flexibility. The anvil is the countersupport of the sonotrode. It is shaped to focus the energy in the cutting as well as in the sealing area. The energy focus is achieved via energy directors. Due to the energy directors underneath and the oscillating sonotrodes above, lid and bottom films generate heat as the ultrasound is applied. The heat is only created where it is necessary and only for a short time Results and Discussion Combining all oscillation units requires some measurements to obtain an even and flat surface of mm with which almost any sealing and cutting geometry can be achieved. For instance, the device needs to guarantee that the amplitude Generator HF cable Converter Booster Sonotrode Oscillation: 32 μm Figure 37.1 Generator and oscillation unit
300 290 Chapter 37 Ultrasonic Sealing and Cutting in Thermoforming Figure 37.2 Amplitude distribution of sonotrode (Courtesy of Sonotronic Nagel GmbH. Karlsbad, Germany) Sealing times Time Heat sealing Ultrasonic sealing Sealing method Figure 37.3 Sealing times distribution is the same across the entire surface (Figure 37.2 ), especially when applying press pressure. After the sealing and cutting, the station has to divide itself to release sealed and cut packages. This enables the unloading robot to pick up the packages and send them on their way to the final packaging station. Concerning sealing and cutting time, the system provides fast cycle times. All applications achieved so far required sealing and cutting times in the range of 200 to 500 ms (Figure 37.3 ). Common forming, filling, and sealing applications require sealing times between 1 and 1.5 seconds.
301 37.3 Conclusions 291 Cutting force (t), A-PET, thickness: 450 μm, cutting length: 1810 mm Cutting force (t) Steel rule die (cold) Ultrasonic device Cutting procedure Figure 37.4 Cutting forces Most important is the decrease of cutting force in comparison with steel rule die. For example, a cutting line length of 1810 mm for A - PET film (thickness: 450 μ m) requires using the steel rule die process (cold) with a cutting force of 20.7 tons. Cutting the same length with the ultrasonic cutting station requires 1.2 tons, which is times less force (Figure 37.4 ). The cutting edge and sealing area of the anvil need to be adjusted to the thicknesses of the bottom and lid films. Fast format changeovers are possible with this system. Since the ultrasonic equipment belongs to the machine (generators and oscillation units), only the anvil has to be changed. In comparison with other ultrasonic systems, the ultrasonic equipment does not have to be changed when switching to another format. When applying ultrasound so that the tool cuts through the film, contact between anvil and sonotrode has to be avoided, and this makes the use of a protection film necessary. Depending on the application, this protective film can be made of paper, paper/polymer laminate, or polymer. When dealing with oscillation and amplitudes in the range of a few micrometers the press has to be exactly parallel to the plane. Tolerance in other directions can be high, which makes the operation easy in rough circumstances CONCLUSIONS The development of ultrasonic systems has resulted in the creation of a new sealing and cutting device for thermoforming machines. This ultrasonic device can be used for forming and cutting applications as well as for forming, filling, and sealing/ cutting processes. The ultrasonic station enables fast format changeover. Low press pressure is required, and therefore the presses can be built in smaller dimensions. Less wear and tear occurs because the material heats up only in the area
302 292 Chapter 37 Ultrasonic Sealing and Cutting in Thermoforming Figure 37.5 Ultrasonic sealing and cutting station, and automatic unloading of punched trays (Courtesy of Gerhard Schubert GmbH) where the ultrasound energy is directed. The equipment is designed to allow automatic unloading of packages and trays (Figure 37.5 ). Energy input during sealing can be controlled. The machine control system will reject packages that were not sealed with energy within a preset operation window. With a protection film, a complicated sonotrode system can be avoided, enabling the same sonotrodes to be used for all formats. This development has helped make automated packaging lines more efficient.
303 Chapter 38 Understanding the Brittle Behavior of Polystyrene Cups Written in cooperation with Rudi Salmang, Terneuzen, The Netherlands A dairy packaging producer reported a brittleness in ml cups under fast squeezing rates, with either supplier A or supplier B polystyrene materials. PS - HI (A) from supplier A was approved and implemented for the production of the cups for a period of 3 months. During the first 3 weeks of use of PS - HI (A), good cups were produced; thereafter the cups produced were brittle. However, the same lots of PS - HI (A) at other producers were not brittle. The polystyrene cups were made from extruded films and thermoformed offline. The extrusion process consisted of the continuous melting, mixing, and pressing of plastic pellets into a homogeneous film of the desired thickness. Thermoforming consisted of heating the extruded film until it was stretched into a cavity by means of a plug. Then the hot film was forced against the mold s wall by use of a vacuum or air pressure. After cooling, the film retained the mold s shape and detail. Determining an optimum processing window in thermoforming is critical to achieving high - quality cups, while inconsistent thermoforming usually gives extremely unbalanced orientation and, hence, defective cups. Orientation is defined as a time - dependant recoverable elastic deformation, and it is the result of stress buildup and stress relaxation. The orientation can be affected by material properties as well as the processing conditions, and this is measured by the heat shrinkage test. The measure of orientation in the wall of the cup gives a good indication of its mechanical performance. To understand the unusual brittle behavior of the ml cups described above, and to show the importance of orientation and proper thermoforming settings, the raw materials were analyzed, and measurements of the orientation in the wall of the cups were performed. Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 293
304 294 Chapter 38 Understanding the Brittle Behavior of Polystyrene Cups Table 38.1 Analytical Methods Used in This Study * Property Method Units Remarks Izod impact ASTM D256-93A J/m Injection molded bars Tensile yield ASTM D638M-93 MPa Injection molded bars (5 mm/min) Elongation ASTM D638M-93 % Injection molded bars (5 mm/min) MFR ASTM D g/10 min Vicat ASTM D C Injection molded bars Mw DOWM g/mol Rubber particle size (RPS) ML-AM μm Coulter counter 50 μm tubes Rubber content Infrared spectroscopy % Mineral oil content Gravimetric % * The injection molded plaques were made with an injection molding machine EXPERIMENTAL METHODS Analysis Performed on the Raw Materials Samples of PS - HI (A) used by the customer were taken and analyzed by the methods noted in Table Measurement of the Film s Orientation The orientation of the film was measured at the customer s plant by cutting cm sheets and placing them in an oven at 130 C for 1 hour. The shrinkage level was then measured for each disk in the draw and hoop directions Analysis Carried Out on the Cups FT-IR Spectroscopy Analysis FT - IR analysis was carried out to obtain information about the composition of the material. The samples were prepared by slicing a cross - section along the cup wall. FT - IR spectra were obtained using a IR spectrometer operating in transmission mode. TEM Micrographs of the Different Cups TEM micrograph pictures were taken to obtain data about the morphology of the rubber. Samples were mounted in a sample holder and cross - sectioned with a ultra-
305 38.1 Experimental Methods Machine direction Figure 38.1 Position of the cavity in the thermoforming mold Table 38.2 Cups Tested for the Orientation Test Cup Number Products Cavity 1 PS-HI (A)/PS-GP (A) 5 2 PS-HI (A)/PS-GP (A) 7 3 PS-HI (A)/PS-GP (A) 5 4 PS-HI (A)/PS-GP (A) 7 5 PS-HI (A)/PS-GP (B) 5 6 PS-HI (A)/PS-GP (B) 7 7 PS-HI (B)/PS-GP (B) 5 8 PS-HI (B)/PS-GP (B) 7 microtome using a glass knife. Then they were stained with OsO 4 vapor. The sections were studied with a light microscope operating with transmitted light and differential interference contrast. A digital camera was used to make the digital images of the samples Determination of Orientation in the Cups Eight ml cups with identical geometry (average cup weight g) were chosen for the orientation measurements. They were thermoformed at the producer, where the brittleness problem occurred, on a thermoforming machine equipped with a 10 - cavity tilting mold to produce the cups (Figure 38.1 ). All cups were produced under the same processing parameters. The cups analyzed were formed in two different cavities (cavity 5 and 7) to capture different positions of the cavities in the mold, cavity 5 being on the edge and cavity 7 close to the center of the mold (Figure 38.1 ). The raw material for these cups was polystyrene either from supplier A or from supplier B. In Table 38.2 a list of the cups analyzed is shown Sample Preparation The orientation in the walls of the cups was measured according to the procedure explained in the Appendix of this chapter.
306 296 Chapter 38 Understanding the Brittle Behavior of Polystyrene Cups Rim hoop Middle hoop Draw axis Bottom hoop Figure 38.2 Left: view of a cup; right: cup wall laid flat The bottom of each cup was removed to ease the cutting. Three vertical axes at approximately 120 apart (0, 120, 240, randomly assigned) and three horizontal ones (rim, middle, and bottom hoop) were marked on the cup walls (Figure 38.2, left and right). The axes were selected to differentiate at least two different locations regardless of the position of the cup in the mold with respect to the extrusion direction. The draw axis is the axis parallel to the plug travel direction, while the hoop is normal to this axis. Disks were selected to restrain shrinkage at the corners. All disks were labeled and subjected to the shrinkage test. The disks were placed between two metal plates previously sprayed with a slip agent. The test conditions were as follows: Diameter of the disk: d = mm Oven temperature: 150 C Time in the oven: 15 min Calculation of Disk Shrinkage Because the volume of the disks remained constant, the shrinkage could be calculated as a function of the dimensional change after the shrinkage test. The shrinkage was calculated from the following expression (Figure 38.3 ) Hoop shrinkage (%): SH = (( d H) / d) 100 Draw shrinkage (%): SD = (( d D) / d) 100 The basis weight ( D bw ) in g/m 2 (defined as the weight per unit area) of each disk was calculated as follows: D bw = m A
307 38.2 Results and Discussion 297 Figure 38.3 Shape orientation behavior after the shrinkage test Table 38.3 Physical Properties of the PS-HI (A ) Units Film Cups #1 4 Film Cups #5 6 Specification for PS-HI (A) Lot number 1 2 Izod impact J/m (101 min) Tensile yield MPa (16 min) Elongation % min MFR g/10 min (4 6) Vicat C (98.5 min) Mw g/mol aim RPS μ m Mineral oil % ( ) Rubber % ( ) where A = area of each disk = π (d /2)2 = π ( /2) 2 = m 2 and m = weight of each disk (g) RESULTS AND DISCUSSION Cups made from different materials, at different dates, and from different cavities were analyzed Results of the Raw Materials Analyses Table 38.3 gives the results of analytical tests that compared the properties of materials to the specifications defined for PS - HI (A). These analyses show that all properties are within the specifications.
308 298 Chapter 38 Understanding the Brittle Behavior of Polystyrene Cups Table 38.4 Film Orientation Measured at the Manufacturer Cups Materials Machine Direction (%) Cross Direction (%) 1, 2 PS-HI (A)/PS-GP (A) 3 1 3, 4 PS-HI (A)/PS-GP (A) 3 0 5, 6 PS-HI (A)/PS-GP (B) NA NA 7, 8 PS-HI (B)/PS-GP (B) Orientation of the Films The thickness of the films extruded was 1.75 mm. The extrusion parameters were not available. The orientation data are shown in Table The values obtained are within typical ranges and considered low orientation values TEM and FT-IR Analysis The FT - IR analysis shows the expected spectra for HI - PS and GP - PS. Hence the rubber morphology of the HI - PS depicted on the TEM analysis does not exhibit any features to explain the brittleness of the cups CUP ORIENTATION RESULTS During the shrinkage test, the two axes as identified in Figure 38.3 D for the draw direction and H for the hoop direction were altered as a result of the molecular stress relaxation. The shrinkage was higher in the direction where the strain during the thermoforming was higher (i.e., the draw axis); therefore the disks ended up in the shape of ellipses (Figure 38.3 ). The percentage of shrinkage of each disk was calculated for the hoop and the draw direction of each cup. From these data, graphs of the orientation of the hoop and draw directions versus the basis weight were plotted for each cup. For the hoop and draw directions, the graphs were plotted for the three vertical axes of each cup (0, 120, 240 ). To facilitate the understanding of these data, lines connecting the different data points (from bottom to rim) for the three different axis were drawn (Figures ) Definition of the Perfect Cup The minimum requirement for a good cup is that it exhibit the same orientation (shrinkage) values along a given hoop level, though the values may differ from one hoop level to another depending on the draw. However, a high monoaxial orientation in the draw direction will lead to the typical brittleness in the cups.
309 38.3 Cup Orientation Results 299 (a) Hoop orientation for a theoretical and good practical cup Orientation hoop direction (%) 35 Theoretical Theoretical cup - Axis 0 30 Bottom Theoretical cup - Axis Middle 10 Theoretical cup - Axis 240 Good practical cup - Axis 0 Good practical cup - Axis Good practical cup - Axis 240 Rim Basis weight (g/m 2 ) (b) Draw orientation for a theoretical and good practical cup Orientation draw direction (%) 90 Theoretical Theoretical cup - Axis Bottom Theoretical cup - Axis 120 Theoretical cup - Axis 240 Good practical cup - Axis 0 75 Middle Rim Good practical cup - Axis 120 Good practical cup - Axis Basis weight (g/m 2 ) Figure 38.4 Hoop and draw orientation for a theoretical and good practical cup A good cup should show a concentrated distribution (close clusters) of data points for each hoop, indicating a homogeneous deformation of material along the periphery (no basis weight or orientation variation) and ideally along the draw axis as well (Figure 38.4, theoretical curve). However, this is very difficult to achieve due to the geometry and requirement of the cups. The hoop deformation at the rim is very small, since the film starts to be deformed when it is already very close to the mold walls. On the other end, the bottom section has to be stretched from the tip of the plug (the smallest diameter of all) to the walls of the cavity at the bottom. Depending on the processing conditions (temperature, speed profile, and timing of the forming air), the draw deformation changes from the start to the end of the cycle. At the beginning of the cycle, friction forces between the film and plugs
310 (a) Cup 1 Hoop orientation (b) Cup 1 Draw orientation PS-HI (A)/PS-GP (A) Cavity 5 PS-HI (A)/PS-GP (A) Cavity 5 Figure 38.5 Hoop and draw orientation for cups 1 and 2 Orientation hoop direction (%) Orientation draw direction (%) Middle Bottom Rim Axis 0 Axis 120 Axis Middle Bottom Rim Axis 0 Axis 120 Axis 240 Basis weight (g/m 2 ) Basis weight (g/m 2 ) (c) Cup 2 Hoop orientation PS-HI (A)/PS-GP (A) Cavity 7 Axis 0 Axis 120 Axis 240 (d) Cup 2 Draw orientation PS-HI (A)/PS-GP (A) Cavity 7 Axis 0 Axis 120 Axis 240 Orientation hoop direction (%) Orientation draw direction (%) Bottom 60 Middle 55 Bottom Rim Middle Rim Basis weight (g/m 2 ) Basis weight (g/m 2 ) 300
311 (a) Cup 3 Hoop orientation (b) PS-HI (A)/PS-GP (A) Cavity 5 Cup 3 Draw orientation PS-HI (A)/PS-GP (A) Cavity Bottom Middle Rim Orientation hoop direction (%) Basis weight (g/m 2 ) Axis 0 Axis 120 Axis Middle Bottom Rim (c) Cup 4 Hoop orientation PS-HI (A)/PS-GP (A) Cavity Bottom Middle Rim Axis 0 Axis 120 Figure 38.6 Hoop and draw orientation for cups 3 and 4 Axis 0 Axis 120 Orientation hoop Direction (%) Orientation draw direction (%) Basis weight (g/m 2 ) Axis 0 Axis 120 Axis 240 (d) Cup 4 Draw orientation PS-HI (A)/PS-GP (A) Cavity 5 Orientation draw direction (%) Basis weight (g/m 2 ) Middle Bottom Rim Basis weight (g/m 2 ) 301
312 (a) Cup 5 Hoop orientation PS-HI (A)/PS-GP (B) Cavity Bottom Middle (b) Cup 5 Draw orientation PS-HI (A)/PS-GP (B) Cavity 5 Orientation hoop direction (%) Basis weight (g/m 2 ) Axis 0 Axis 120 Axis 240 Rim Bottom Middle Axis 0 Axis 120 Axis 240 Rim (c) Cup 6 Hoop orientation PS-HI (A)/PS-GP (B) Cavity 7 (d) Cup 6 Draw orientation PS-HI (A)/PS-GP (B) Cavity Middle Bottom Rim Bottom Figure 38.7 Hoop and draw orientation for cups 5 and 6 Middle Rim Orientation hoop direction (%) Orientation draw direction (%) Basis weight (g/m 2 ) Basis weight (g/m 2 ) Axis 0 Axis 120 Axis Axis 0 Axis 120 Axis 240 Orientation draw direction (%) Basis weight (g/m 2 ) 302
313 (a) Cup 7 Hoop orientation (b) Cup 7 Draw orientation PS-HI (B)/PS-GP (B) Cavity 5 PS-HI (B)/PS-GP (B) Cavity Bottom Middle Rim Orientation hoop direction (%) Basis weight (g/m 2 ) Axis 0 Axis 120 Axis Middle Bottom Rim (c) Cup 8 Hoop orientation PS-HI (B)/PS-GP (B) Cavity Bottom Middle 5 Rim Orientation hoop direction (%) Orientation draw direction (%) Basis weight (g/m 2 ) Axis 0 Axis 120 Axis 240 Basis weight (g/m 2 ) Axis 0 Axis 120 Axis 240 Figure 38.8 Hoop and draw orientation for cups 7 and (d) Cup 8 Draw orientation PS-HI (B)/PS-GP (B) Cavity 7 Middle Rim Bottom Orientation draw direction (%) Basis weight (g/m 2 ) Axis 0 Axis 120 Axis
314 304 Chapter 38 Understanding the Brittle Behavior of Polystyrene Cups override the melt strength of the film, and hence the free area of film (not attached to the plug) will stretch. At a certain moment, a transition of this latter mechanism will occur, and the melt strength will increase as a result of the former stretching and cooling until it overrides the friction forces. This transition will ultimately affect the balance between hoop and draw ratios. In addition, a negative hoop orientation value shows that no shrinkage occurred in the hoop direction, but an expansion of the disk occurred instead, due to faulty thermoforming conditions. Moreover, a high value of the draw orientation in the rim or middle area of the cup shows that there was not enough bi - axial deformation to cause a brittle cup Experimental Cups from the Plant The orientation of cups 1 to 4 made with PS - HI (A)/PS - GP (A) can be seen in Figures 38.5 and These cups were produced with the same lot of PS - HI (A) (Table 38.3 ) but on different days. For these two different types of cups, cavities 5 and 7 exhibit the same faulty behavior. The orientation of cups 5 and 6 made with PS - HI (A)/PS - GP (B) can be seen in Figures 38.7a d. Note the poor distribution of the material along the cup, with a lower basis weight at the bottom than at the rim. The cup coming from cavity 5 exhibits even more differences in the basis weight from the rim to the bottom than the one coming from cavity 7. Moreover, in Figure 38.7 b, the draw orientation at the middle is higher than at the rim. The orientation of cups 7 and 8 made with PS - HI (B)/PS - GP (B) can be seen in Figures 38.8a d. Both cups also exhibit faulty behavior. Figure 38.8 a and b shows inconsistent data, not a concentrated distribution, as well as a very low orientation in the hoop direction. Figure 38.8 c and d, however, shows more consistent data, but the hoop orientation at the rim remains very low, as does the basis weight, compared with the basis weight at the middle of the cup. The results from the PS - HI (A) analysis, TEM and FT - IR analysis, and the orientation of the films showed the expected values. However, the results obtained from the shrinkage test revealed some inconsistencies. Nevertheless, these inconsistencies do not seem to be related to the raw materials, since the cups were made with either supplier A or supplier B materials. The inconsistencies are probably due to faulty processing conditions. Thus faulty thermoforming conditions can explain the observed phenomenon. During thermoforming, the film is subjected to different stretch ratios depending on the temperature, plug travel speed, and timing of the forming air. An incorrect setting regarding the following thermoforming parameters could be the cause of the problem: 1. Temperature differences across the film will generate a differential melt strength along the hoop during the drawing, resulting in different orientation or basis weight.
315 38.5 Appendix: Orientation in Vending Cups 305 This phenomenon is depicted in the Figures 38.5 a and 38.8 a. In these two figures, with cups formed in cavity 5, the basis weight for one of the axes is too low compared with that of the two other cups. From the position of cavity 5 in the mold, it can be surmised that the axis shift was caused by colder film along the edges. A cup thermoformed at the same time (Figure 38.5 c, formed in cavity 7) does not show this defect. However, for this cup, another defect explains the brittleness of the cups (see point 2). 2. Premature contact of the film with the mold. The negative values at the height of the rim shoulder area indicate poor stretching (Figures 38.5 c and 38.7 c). Premature contact with the mold can cause low melt strength as when forming air comes into contact with the plug prematurely. However, for the other cups, the hoop values at the rim are positive but still too low. 3. Wrong indexing (non-100% synchronization) of the film for a multi - row mold. This will exhibit the same symptom as the first characteristic (temperature differences across the sheet), giving brittleness to the cup. 4. Plug dragging an uneven amount of material. An uneven distribution of material is shown in the Figure 38.5 b (bottom value). At a similar draw orientation a huge difference in basis weight is observed. An example of a good plug dragging amount is seen in Figures 38.7 a and b. 5. Poor draw profile, shown by thin bottom. Figure 38.5 a and b exhibits this problem, where very low values for the basis weight are found. However, consistent values of hoop orientation (a little spread out) are observed CONCLUSION The analyses proved that the brittleness of the cups was not due to a poor stock of raw material, as similar faulty cups were obtained with polystyrene from both suppliers A and B. Hence the brittle aspect of the cups was probably from faulty processing conditions, in particular, the thermoforming conditions APPENDIX: ORIENTATION IN VENDING CUPS This chapter describes a method for determining dimensional change in the draw and hoop (peripheral) directions on a thermoformed disposable or dairy container. For more information, the reader should consult ISO Plastics: Film and Sheeting Determination of Dimensional Change on Heating.
316 306 Chapter 38 Understanding the Brittle Behavior of Polystyrene Cups Apparatus Gloves for handling hot parts. Circulated-air oven with thermostatically controlled temperature. The accuracy must be within ±2 C of the specified temperature. Set of brass backup plates and aluminum foil, which can be placed in the circulated air oven. Slip agent (mixture of 20 wt% talc and 80 wt% heat stabilized silicone oil with a viscosity of 200 Mpa. Calibrated gauge calipers and scale (accuracy 0.00). Circular punching knife with an exact known diameter (i.e., 20 mm) Test Specimens Mark a reference position (0 ) on the cup wall (i.e., at the cavity or part number). Also mark the angles 120 and 240. The use of different color markers is recommended. Cut off the top plate and rim from the container. Cut and unfold the cup wall. From each position, punch three disks from the rim, middle, and top (MD). Always use the same reference positions for comparing materials and cavity numbers. Identify each disk with angle, MD, and CD position. Measure the thickness of each disk Procedure Measure and record the weight of each disk. Put the disks on the brass backup plate with aluminum foil and the slip agent. Coat the disks with the agent completely. Coat the aluminum top foil with the agent too and put the other backup plate on top. Place and heat the plates in a preheated oven for 15 minutes. Take the hot plates out (use gloves), and let the plates cool to room temperature. Measure the plates thickness, DD, and HD dimensions. Calculate shrinkage and weight per disk area (basis weight) Calculation Shrinkage (%) = T1 100, T where ØT 1 = diameter after disk shrinkage (mm), ØT 0 = diameter of original disk (mm). 0
317 38.5 Appendix: Orientation in Vending Cups 307 Weight Disk area where weight = disk weight (g). 2 = basis weight ( g/cm ), Report Disk area = r 2 2 cm 100 ( ). Note the test and sample number/cavity. Add the average and standard deviation for shrinkage (%) and basis weight (g/cm 2 ), and also note any visible defects.
318 Chapter 39 Preprinted Film for Lid Thermoforming For thermoforming of preprinted film, some knowledge about thermoforming methods is required of all parties involved in the process. The printing demands of manufacturers as well as customers are ever - increasing. Today an offset of print is no longer acceptable on the thermoformed part. So the thermoforming machine technology has had to become more and more precise. As is true for other kinds of thermoforming applications, it is necessary to take the whole production process into consideration in order to successfully produce thermoformed parts. It is clearly imperative that all participating parties work very closely together, that is, the extruder, printer, and thermoformer. Often it is better that extrusion and thermoforming be carried out in the same company, because then it is possible to immediately address the requirements of extrusion based on knowledge gained during the thermoforming. Even better, the film could also be printed at the same company. However, all three processes are only rarely carried out in the same company. The film has to have a distortion print on it in order to show the correct image after thermoforming. The film index is controlled by print mark registration and a print mark sensor. A good technique is to integrate the print mark sensor in the thermoforming station, between the forming tool and the transport profile of the film transport. Unfortunately, it is then necessary to extrude the material a little wider. It is generally recommended for the production of preprinted lids that the material be extruded wider because then the influence of the transport system s temperature is minimized. With the positioning of the print mark sensor in the area of the forming tool, the start - up waste can be reduced to 20 cycles. In the past, start - up times of 15 to 20 minutes could be observed for similar machine applications where the print mark sensor was located in the area of the film infeed. The adjustment of the printed impression for such machines is laborious and time - consuming and must be repeated after every reel change! Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 308
319 Chapter 39 Preprinted Film for Lid Thermoforming 309 Figure 39.1 Preprinted film for a lid showing millimeter grid lines Naturally, the extrusion has a significant influence on the thermoforming of film. The heat control of the thermoform machine must also be exact. It is necessary to set the heating of the machine in such a way that a parallel alignment of the grid lines relative to the lid rim is facilitated (Figure 39.1 ). Before the sensor is adjusted for a special application, it must be verified that the color contrasts are sufficient. This is important as in praxis widely differing color mixtures do occur. The film transport system must be capable of rapid speed and have a creep speed modus for its feed motion (film step). Here a certain feed stroke of the index can be moved in rapid speed. Shortly before the print mark is reached, the creep speed is switched on. For the detection of the print mark by the print mark sensor, it is helpful if a correction value is entered into the control system. This correction value permits an exact positioning of the print in the mold. In this way, excessive advancement of the print can be avoided. The print mark sensor must be protected by a film strip - off device. Otherwise, during start - up of the machine the sensor could be damaged. If the material is not threaded carefully, it could bend over and be transported with a bow wave ahead.
320 310 Chapter 39 Preprinted Film for Lid Thermoforming Thermoformed lids must have an exact wall thickness distribution. The lids are shaped in such a way that they snap over the rim of the cup during closing. It is important to maintain the free shrinkage of the film and the mold shrinkage of the forming part, so that the snap - fit works. Naturally, the above - mentioned measures also apply to the production of the cup. It is advantageous that the suppliers of lid and cup be in close contact with each other if these are not produced within the same company. Repeatability is significantly enhanced by all these precautions. Repeatability can be determined by measuring the manufactured formed parts, with the exact positions of the printing on the part used as a reference. However, only parts that are formed in the same cavity can be measured and compared with each other.
321 Chapter 40 Flexible Films Written in cooperation with Claudia Müller and Peter Brass, S ü dpack Verpackungen GmbH & Co. KG, Ochsenhausen, Germany 40.1 FLEXIBLE PACKAGING MATERIAL Flexible films are often multilayer films of polyamide/polyethylene, and they are chiefly used for thermoforming purposes. These films are processed on forming, filling, and closing machines to create vacuum packs. As described earlier in the book, multilayer films are composite films that combine the properties of their respective film layers: Polyamide High barrier against oxygen and aromatic chemicals High thermal resistance High mechanical properties Good thermoformability Polyethylene High water vapor barrier Sealability Multilayer films consisting of polyamide/polyethylene can be produced as flat films by coextrusion, extrusion coating, or lamination, or as blow film by coextrusion. As a rule, the thicker the polyamide layer, the deeper the film can be formed. Unlike rigid parts, parts made from flexible films are not dimensionally stable (Table 40.1 ). Subsequent to the forming procedure, the film is subject to a certain resilience, which is also referred to as immediate shrinkage. The free shrinkage and mold Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 311
322 Table 40.1 Flexible Films Economic Efficiency Process Range of Thickness (in μm) Large Batches and Standards Small Batches and Specialties Thermoformability Skin Packaging Lid Film and Pouch Remarks Coextrusion cast film Extrusion coating Good Poor Very good Some Some Thermoforming behavior very good. Very good for large batches 10 metric tons or standards Very good Very poor Good No Yes Strong competitive pressure advantages for pouch production Lamination Very poor Good Good No Yes Ideal for special Coextrusion blow film applications for batches less than 10 metric tons! Acceptable Acceptable Moderate No Yes Lid film on pouch applications Source : Courtesy of Südpack Verpackungen GmbH & Co. KG. 312
323 40.2 Main Flexible Film Types 313 shrinkage phenomena intermingle, with free shrinkage playing a more important role in the dimensional changes during the processing of flexible films. The term mold shrinkage applies only when one talks about rigid parts. When flexible film is processed, several kinds of shrinkage may occur: Immediate shrinkage. Resilience of the film directly after the forming process. This measurement is taken immediately after thermoforming. Time shrinkage. Postcrystallization and retardation lead to a further shrinkage of the forming part. This measurement is taken after 7 days. Pasteurization shrinkage. The film orientations caused by the thermoforming process are dissolved through heat impact. The measurement is taken after cooking (30 minutes at 95 C). For applications using flexible films it is very difficult to carry out comparative measurements of mold shrinkage and free shrinkage. The determined values depend on the machine used as well as the forming conditions. For this reason a comparison of films is possible only when the same thermoforming machine is used for the tests and the same forming conditions apply. The free shrinkage behavior of flexible films is influenced by a number of factors: Temperature Heating and forming times Overall film thickness Thickness of the polyamide layer Sealing layer Cooling conditions for polyamide 40.2 MAIN FLEXIBLE FILM TYPES Flexible films used for thermoforming purposes generally consist of several layers, in which polyamide and polyethylene are most commonly used. Depending on the product demand, mainly films with medium or high barrier films are utilized for thermoforming, and the application area ranges from the food sector to the nonfood sector. Cheese, meat, and sausages are products that are packaged in thermoformed flexible films. However, there are also numerous applications for the packaging of medicinal and technical articles in flexible films. Depending on the application, conventional flexible films used for thermoforming can consist of five or seven layers. For some special purposes, the films consist of even more layers. Films that are sterilized or pasteurized generally possess a polypropylene layer. EVOH is used as oxygen barrier. The layer thicknesses vary between 6 μm for an overall film thickness of 90 μm, and 16 μ m for an overall film thickness of 290 μm.
324 314 Chapter 40 Flexible Films Humidity has an influence on the oxygen barrier. If the humidity increases, the oxygen barrier is reduced. Humidity can also compromise the thermoforming behaviour of PA/PE composites; therefore PA/PE film reels should always be completely wrapped in a PE film. If PA/PE film reels are inappropriately packed, the outer windings of the film may absorb humidity. When the beginning of such a reel is thermoformed, the resulting products are of poor quality. Only after some meters of this film, that is, some windings, are thermoformed, good quality products are again produced (i.e., after the first layers of the PA/PE film containing too much humidity are used up and a film with a correct humidity content is processed) SEALING LAYERS 1 Material: EVA Description Ethylene vinyl acetate = polyethylene with maximum 5% VA co-monomer Low sealing start Good Sealing of contaminated seams Good Stability of sealed seams Average Pasteurization up to 85 C Yes Cooking up to 100 C No Semi-sterilization up to 110 C No Sterilization up to 121 C No Material: PE-LD Description Low-density polyethylene broad distribution of molecular weight with good processability characteristics Low sealing start Average Sealing of contaminated seams Average Stability of sealed seams Average Pasteurization up to 85 C Yes Cooking up to 100 C Yes Semi-sterilization up to 110 C No Sterilization up to 121 C No 1 Dr. Claudia Mü ller, Peter Brass, Firma S üdpack, Präsentation Weichfolie, 2010.
325 40.3 Sealing Layers 315 Material: PE-LLD Description Linear low-density polyethylene, polyethylene with alpha olefin co - monomer C4, C6, C8 manufacture mainly blended with PE/LD, with higher temperature resistance and solidity Low sealing start Poor Sealing of contaminated seams Good Stability of sealed seams Very good Pasteurization up to 85 C Yes Cooking up to 100 C Yes Semi-sterilization up to 110 C Yes Sterilization up to 121 C No Material: PE-VLD Description Very low density PE-LLD with a higher co-monomer percentage with dropped density g/cm3, mostly produced with single - site (metallocene) catalyzers. These products have outstanding ductility and a low sealing temperature. Low sealing start Very good Sealing of contaminated seams Very good Stability of sealed seams Average Pasteurization up to 85 C Yes Cooking up to 100 C No Semi-sterilization up to 110 C No Sterilization up to 121 C No Material: PB-1 Description Polybutylene as mixing partner for peel mixtures for sealing against PE and itself. The polybutylene is mixed with 12% to 20% added amounts of polyethylene as a dry - blend and forms an inhomogeneous component in the polyethylene matrix. Low sealing start Depends on the mixing partner PE Sealing of contaminated seams Depends on the mixing partner PE Stability of sealed seams Peel Pasteurization up to 85 C Possible, depending on the set peel force Cooking up to 100 C Possible, depending on the set peel force Semi-sterilization up to 110 C No Sterilization up to 121 C No
326 Chapter 41 Simulation Written in cooperation with Karel Kouba, Accuform, Zlin, Czech Repubic, Rupert Gschwendtner, and Hans Lochner, Kiefel GmbH, Freilassing, Germany Unlike in other fields of polymer processing, such as injection molding, use of computer simulation is rather new and less developed in thermoforming. The thermoformers that use simulation in most cases work with T - SIM software from the Accuform company in Zlin, Czech Republic T-SIM COMPUTER SIMULATION OF THERMOFORMING 1 T - SIM is a software package that predicts the final wall thickness distribution based on the specified processing parameters: the pressure level, the speed of tools, the film/sheet temperature distribution, and so on. The simulation can also predict image distortion and pre-distortion. Why simulate a thermoforming process? To reduce the design time for your products. No need to perform expensive trial-and-error procedures. To select an optimum design from many possible alternatives. To get optimum thickness distribution on final product via a temperature setup on the film/sheet. To design pre-distorted images for an in-mold decoration. 1 Dr. Karel Kuoba, T - SIM website, Accuform, Zlin, Czech Republic, Advanced Thermoforming: Methods, Machines and Materials, Applications and Automation, First Edition. Sven Engelmann John Wiley & Sons, Inc. Published 2012 by John Wiley & Sons, Inc. 316
327 41.2 Features of Simulation Software Such as T-SIM FEATURES OF SIMULATION SOFTWARE SUCH AS T-SIM WLF temperature dependence Simulates positive/negative forming with/without plug assistance Time-dependent deformation is described by viscoelastic K-BKZ model Three different damping functions for a better material data fit (strain hardening) Material database containing, for example, PE, PP, PET, PC, and PMMA Imports general 3D molds from IGES, VDA - FS via stereolithographic STL file, DXF, or Patran Neutral file All molds movable (up to ten tools can be used in one simulation project) Time-dependent film/sheet sagging included Friction between stretched plastic material and tools Heat transfer between material/tools and material/air User-friendly setup of technological parameters with graphic Windows context sensitive help, tutorials, and hands-on examples OpenGL included, allowing dynamic image rotation, zooming, and panning, enabling fast shading or wire frames and visualization of contact options Easy, completely editable setup of T - SIM project, with a tight connection between initial project and result files Many typical thermoforming problems solved and distributed on an installation CD Material T-SIM uses time-dependent viscoelastic K-BKZ model Data of frequently used polymers are available in the T - SIM material database Any material can be tested (in cooperation with IKP Stuttgart, Germany, or DatapointLabs, USA) and its data imported into T-SIM Solver Very fast iterative multithreaded solver makes use of parallel processing on PC with more than one processor Upper limit of sheet elements or mold elements is limited only by the PC memory available Fast contact analysis Solving a set of thermoforming problems in a batch mode, enabling automatic case study solution
328 318 Chapter 41 Simulation Results 3D cuts 3D color maps of thickness, temperature, stress, extension Investigate contact between plastic material and molds Easy refinement of the grid in 3D areas of interest from the postprocessing window Export results for structural analysis to Ansys, IGES, DXF, Cosmos/M, or Patran files Output to Patran format enables structural analysis and calculation of cooling Interactive thickness/temperature/position information with a simple mouse click Export animation file to Microsoft Video Player format Cooling calculation 41.3 PRE-DISTORTION OF IMAGES Many thermoformed products are preprinted and require a pre - distorted print of images, for instance, lids for tubs in margarine packaging or globes where two separately formed hemispheres are put together. Thermoforming software such as T - SIM assists in the prediction of printed image deformation. T-SIM is able to pre-distort images for printing on the flat sheet, so that once thermoformed, the images appear true Image projection manager enables projection of multiple images using various projection methods (planar, cylindrical, and spherical projection) IGES polylines can be projected, distorted/pre - distorted, and exported back to IGES 3D VRML models can be also used for image pre-distortion T-SIM Example 1 This example shows simulation used as an optimization tool for tuning the processing conditions. The part a transportation tray is produced using plug - assisted thermoforming. Tray Process Optimization The transportation tray is made of PET with an initial film thickness of 0.8 mm. The task was to achieve an optimum thickness profile that would result in the acceptable mechanical properties. The optimization
329 41.3 Pre-Distortion of Images 319 procedure focused on the final plug depth, namely because the only modified parameter in this optimization was the final plug position. Final Plug Position Influence Simulation AnalysisFour final plug positions were used for simulation in order to ascertain the influence of the final plug position on the final thickness profile: Bottom Plug stops 1 mm from the mold bottom +1 cm Plug stops 11 mm from the mold bottom +2 cm Plug stops 21 mm from the mold bottom +3 cm Plug stops 31 mm from the mold bottom The four plug positions were calculated and postprocessed in order to get thickness values for proper analysis along the following cut. The simulated thickness profiles were compared, as shown in Figures 41.1 and From the comparison it was deduced that the optimal final plug position should be about 11 mm above the mold bottom. Final plug position influence was subjected to an experimental analysis. To test the agreement between simulation and experimental results, four samples produced with four different final plug positions (identical to those used in simulation) were measured, and the measured thickness values were compared with the simulations. Thickness (mm) Bottom +1 cm +2 cm +3 cm Point # Figure 41.1 Comparison of thickness profiles for different plug positions (Courtesy of Accuform, Zlin, Czech Republic)
Endex International Innovation for the Future Endex Foam Extrusion General Information Guide Section 01 - Foam Extrusion Foam extrusion, in simple terms, consists of mixing a chemical foaming agent with
GETTING STARTED IN PERSONAL AND EXECUTIVE COACHING How to Create a Thriving Coaching Practice Stephen G. Fairley Chris E. Stout John Wiley & Sons, Inc. GETTING STARTED IN PERSONAL AND EXECUTIVE COACHING
KEY COM PONENTS FOR PLASTICS PROCESSING MIXING. FOAMING. COOLING. MIXING NOZZLES AND STATIC MIXERS FOR INJECTION MOLDING MIXING NOZZLES AND STATIC MIXERS FOR INJECTION MOLDING HOW YOU BENEFIT TWICE WITH
D-LFT PROCESS: IN-LINE COMPOUNDING & COMPRESSION MOLDING OF LONG-GLASS-FIBER REINFORCED POLYMERS Daniel Schwendemann and Gerald Münz Coperion Werner & Pfleiderer GmbH & Co. KG Abstract Long fiber-reinforced
Co-Rotating Twin-Screw Extruder Herausgegeben von Klemens Kohlgrüber ISBN-10: 3-446-41372-3 ISBN-13: 978-3-446-41372-6 Leseprobe Weitere Informationen oder Bestellungen unter http://www.hanser.de/978-3-446-41372-6
ATYPICAL TWIN SCREW EXTRUSION COMPOUNDING SYSTEMS FOR POLYOLEFINS Charlie Martin, Leistritz Extrusion, 175 Meister Avenue, Somerville, New Jersey 08876, U.S.A. Abstract Plastics is a major worldwide industry
mixing nozzles Cost savings and quality improvements in plastics processing melt Blenders Foam extrusion systems melt Coolers trust the leader Mixing nozzles and static Mixers for injection Molding Mixing
Bridge Design and Evaluation Bridge Design and Evaluation LRFD and LRFR Gongkang Fu John Wiley & Sons, Inc. Cover Design: Michael Rutkowski Cover Photograph: Courtesy of Alamy Creativity/Alamy This book
Troubleshooting the Sequencing Batch Reactor Illustrations by Brittany Lytle A John Wiley & Sons, Inc., Publication Troubleshooting the Sequencing Batch Reactor WASTEWATER MICROBIOLOGY SERIES Editor Nitrification
The Concept The continuous compounding of polymers, technical ceramics and foodstuffs whilst miing in various additives at specific points along the etruder barrel is an established technique used in the
BEST PRACTICES IN PLANNING AND PERFORMANCE MANAGEMENT RADICALLY RETHINKING MANAGEMENT FOR A VOLATILE WORLD Third Edition David A. J. Axson Best Practices in Planning and Performance Management Best Practices
FLEXPACKCON SPE Flexible Packaging Division Strategies to Avoid Interfacial Instability in Multilayer Films October 31, 2018 Phoenix, Arizona Presented by: Paul Waller Plastics Touchpoint Group, Inc. Optical
An Introduction to Single Screw Extrusion Sponsored by Dynisco Feb 14 2017 Table of Contents Single Screw Extrusion Extrusion and Thermoplastics Extruder Classification Machine Construction Post Extrusion
Credit Risk Scorecards Developing and Implementing Intelligent Credit Scoring Naeem Siddiqi John Wiley & Sons, Inc. Additional praise for Credit Risk Scorecards... An essential book for anyone interested
Extruding Plastics Extruding Plastics A practical processing handbook D. V. Rosato Plastics Institute of America Rhode Island School of Design Chatham, MA, 02633 USA ^^ SPR1NGER-SCIENCE+BUSINESS MEDIA,
Injection Molding Guide for KEPITAL R&D Center 1. Safety recommendations (1) Safety precautions during processing In processing KEPITAL, an extraction hood should be equipped over the barrel unit and measures
SCREW DESIGN BASICS The Processor Point Of View Andrew W. Christie Optex Process Solutions, LLC www.optexprocesssolutions.com Outline Define the goal Review basic extruder components Discuss process elements
DESIGN OF WATER SUPPLY PIPE NETWORKS DESIGN OF WATER SUPPLY PIPE NETWORKS Prabhata K. Swamee Ashok K. Sharma Copyright # 2008 by John Wiley & Sons, Inc. All rights reserved Published by John Wiley & Sons,
JUST ADD LIQUID Quick guide to ColorMatrix liquid color for plastics and silicones THE RIGHT COLORANT FOR YOU Understanding which colorant technology best suits your particular product application will
Extrusion Technology Twin Screw Extrusion Systems to Process PLA More Efficiently Innovation Takes Root 2012 Charlie Martin/Leistritz Ph: 908/685-2333, E-mail: firstname.lastname@example.org February 22, 2012 Twin
IN-line thermoforming system INTEC 500/700/900/1000/1100 serie Complete IN-LINE plants for cups, plates and yogurt pots INTEC: High EFFICIENCY - High quality More than just fast: Reliable the IN-line process
Accounts Payable Best Practices Mary S. Schaeffer Executive Editor IOMA s Report on Managing Accounts Payable Co-creator The Accounts Payable Certification Programs John Wiley & Sons, Inc. Accounts Payable
LCM CC & TCC A member of the Possehl Group LCM LONG CONTINUOUS MIXERS These continuous mixers compete with the quality level of products obtained by discontinuous internal mixers. They overcome both processing
Technical Information High Performance Materials Processing Durethan by extrusion blow molding 1 Preparation of the material, drying... 1 2 Surface quality... 2 3 The plasticizing unit... 3 4 Barrel temperatures...
Processing of non-dried PET-Bottle-Scrap using Co-rotating Twin Screw Extruders Sabine Schönfeld, Sr. Process Engineer: Coperion Werner & Pfleiderer, Germany Paul Andersen, Director, Process Technology:
STRUCTURAL STABILITY OF STEEL: CONCEPTS AND APPLICATIONS FOR STRUCTURAL ENGINEERS Structural Stability of Steel: Concepts and Applications for Structural Engineers Theodore V. Galambos Andrea E. Surovek
IN-LINE THERMOFORMING MACHINES Complete turn key IN-LINE installations from material handling through to boxing units of finished products More than just fast: Reliable the IN LINE process IN LINE technology
IN-LINE THERMOFORMING MACHINES Complete turn key IN-LINE installations from material handling through to boxing units of finished products More than just fast: Reliable the IN LINE process IN LINE technology
MANAGEMENT OF TECHNOLOGY MANAGEMENT OF TECHNOLOGY Managing Effectively in Technology-Intensive Organizations Hans J. Thamhain This book is printed on acid-free paper. Copyright 2005 by John Wiley & Sons,
Simultaneox Simultaneous orientation for barrier film Presented by Giovanni Stocchetti GAP Driving element Reduce packaging weight up to 4 times Saving packaging cost up to 4 times Increase barrier and
Unit 156: Polymer Manufacturing Processes Unit code J/615/3315 Unit level 4 Credit value 15 Aim This unit is designed to develop students knowledge and understanding of the main manufacturing processes
Underwater pelletizing systems. www.bkg.de Page 1 Content The complete perspective. The detail in focus. About Nordson BKG................. 3 Excellence is our standard. Optimized down to the last detail.
FEED ENHANCEMENT TECHNOLOGY FOR LOW BULK DENSITY MATERIAL INTO CO-ROTATING TWIN-SCREW COMPOUNDING EXTRUDERS Paul G. Andersen, Coperion Corporation, Ramsey, NJ Maria Hoelzel and Thorsten Stirner, Coperion
Colour and Additive Preparations for Extruded Polyolefin Foams COLOUR AND ADDITIVE PREPARATION FOR EXTRUDED POLYOLEFIN FOAMS ADDITIVES for POLYOLEFIN FOAM HP 73940 FR Flame retardant masterbatch for LDPE-films,
Sarbanes-Oxley Internal Controls Effective Auditing with AS5, CobiT, and ITIL ROBERT R. MOELLER John Wiley & Sons, Inc. Sarbanes-Oxley Internal Controls Sarbanes-Oxley Internal Controls Effective Auditing
Plastic Forming Processes Plastic Forming Processes Maurice Reyne First published in France in 2006 by Hermes Science/Lavoisier entitled: Transformations, assemblages et traitements des plastiques First
In-House Coloring of Terluran Standard (World Grades) In-House Coloring of Terluran Standard (World Grades) Introduction Choosing the coloring solution that is right for your business is critical to success
Chemical Foaming Alternatives to Azodicarbonamide 2 Foaming Agents What are they and how do you use them? CFA Endothermic & Exothermic Challenges - Regulatory and Technical Case Study: PP Foam Cellular
Developments in Small Scale Twin Screw Extruders for Color Development Charlie Martin, Leistritz Extruson Abstract Plastics is a major worldwide industry that plays a role in all facets of modern life,
James L. Throne Understanding Thermoforming ISBN-10: 3-446-40796-0 ISBN-13: 978-3-446-40796-1 Table of Contents For further information and order see http://www.hanser.de/978-3-446-40796-1 or contact your
Gear Pumps Kreyenborg Gear Pumps - An Addition to our Range The best guarantee for continuous and economic machine performance is a closed loop system with well-matched units. The Kreyenborg system, right
MANUFACTURING TECHNOLOGY UNIT II Hot & Cold Working Forging & Rolling Mechanical Working of Metals In this method no machining process is carried out, but it is used to achieve optimum mechanical properties
Calcium Carbonate in Blown HDPE Film New Developments to Increase Productivity and Profitability by Gil Morieras - Marketing Manager Polyolefines (Omya) and Dr. Gerard Schaeffer (GS Technology) Many interesting
PROCESSING MICA BASED PIGMENT MASTERBATCH Robert Roden, STEER Engineering Prakash Hadimani, STEER Engineering Dr Pradeep Bakshi, STEER Engineering Abstract Many effect pigments used in thermoplastics such
Additive and Colour Preparations for Extruded Polystyrene Foams Additive and Colour Preparations ADDITIVE AND COLOUR PREPARATION FOR EXTRUDED POLYSTYRENE FOAMS ADDITIVES for EXTRUDED POLYSTYRENE FOAM (XPS)
Bin Level Indication Applications in the Plastic Processing Industries Introduction What is Plastic Processing? Simply, it is the processing or converting of raw plastic material into a finished or work-in-process
GRADE CODING Stanyl ForTii TM glass fiber reinforced and halogen-free flame retardant injection molding grades. MATERIAL HANDLING Storage In order to prevent moisture pick up and contamination, supplied
A UL Thermoplastics Testing Center White Paper COMPETITIVE ADVANTAGES & COST SAVINGS BY CONDUCTING A MORE THOROUGH ANALYSIS OF DEMOLDING PROPERTIES Measuring Friction Coefficient versus Sleeve Mold Release
Advances in Twin Screw Compounding Technology Extrusion technology from micro to production scale Ing. Manfred Dobersberger 19.08.2011 Labor- and Pilotanlagen für die Kunststoffverarbeitung, Dr. Collin
EXTRUSION LINES FOR MEDICAL APPLICATIONS Laboratory machines for the processing of polymers Blown Film Lines with water cooling The new and reliable system for the production of sterile multi-layer-tubes
Page 1 of 5 Date previous version 21 Apr 2016 PROCESSING GUIDE INJECTION MOLDING OF STANDARD AND HIGH HEAT PLA COMPOUNDS Interested in solutions for bioplastics? Please contact us at 2 www.total-corbion.com
Sarbanes-Oxley and the New Internal Auditing Rules ROBERT R. MOELLER John Wiley & Sons, Inc. Sarbanes-Oxley and the New Internal Auditing Rules Sarbanes-Oxley and the New Internal Auditing Rules ROBERT
Fundamental Approach to Screw Design By Jeffrey A. Myers, President of Barr Inc. Introduction The single stage extruder screw remains as the most widely used piece of equipment in the processing industry
Optimizing Extruder Controls, Part Two Lesson 6 I. The Compression Zone A. Most of the melting of raw material from solid plastic particles to molten plastic melt occurs in the compression zone. B. Goals
T H E PROFESSIONAL SERVICES FIRM BIBLE JOHN BASCHAB JON PIOT John Wiley & Sons, Inc. T H E PROFESSIONAL SERVICES FIRM BIBLE T H E PROFESSIONAL SERVICES FIRM BIBLE JOHN BASCHAB JON PIOT John Wiley & Sons,
Chapter 19 Forming and Shaping Plastics and Composite Materials Characteristics of Forming and Shaping Processes for Plastics and Composite Materials Forming and Shaping Processes for Plastics, Elastomers,
Chapter 19 Forming and Shaping Plastics and Composite Materials Characteristics of Forming and Shaping Processes for Plastics and Composite Materials 1 Forming and Shaping Processes for Plastics, Elastomers,
Plastic Behavior In The Compounding Twin Screw Extruder Lesson 4 I. Screw Terminology Screw Terminology A. Length to Diameter Ratio (L/D ratio) 1. The L/D ratio is the length of the flighted portion of
About This Book Why is this topic important? Trainers sometimes fail to ask enough questions or the right question prior to designing, redesigning, or presenting a training program as the solution to a
STEER BEST PRACTISES CONTROLLING SHEAR TO PRODUCE BRILLIANT EFFECT PIGMENT MASTERBATCHES WITHOUT DAMAGE TO THE MICA PLATELET STRUCTURE Mica - An integral part of most effect pigments Mica is a delicate,
COMPLYING WITH SARBANES- OXLEY SECTION 404 A Guide for Small Publicly Held Companies LYNFORD GRAHAM Complying with Sarbanes-Oxley Section 404 Complying with Sarbanes-Oxley Section 404 A Guide for Small
Technical Information Joncryl Technical Information Joncryl TI / EV/BX 001 e March 2014 TI / EV/BX 001 e March 2014 Page 1 of 6 Page 1 of 6 Functional Additives Functional Additives Joncryl is a registered
This technical paper was written and developed in November, 2000 when the author(s) was an employee of Dyneon LLC. Dyneon LLC was formerly a wholly-owned subsidiary of 3M Company and was fully integrated
Full-range supplier for refrigerated display cases Buergofol sees benefits in the use of recycled PET Text: Karin Regel, editor K-PROFI "Transparent PET packaging has been a popular discussion topic with
A Guide to Creating a Successful Algorithmic Trading Strategy The Wiley Trading series features books by traders who have survived the market s ever changing temperament and have prospered some by reinventing
Zenith Pumps PEP-II Series Gear Pumps Precise, Pulseless, Repeatable Performance In Polymer Applications. Zenith Pumps In 1926, Zenith Pumps developed the first precision metering gear pump for the extrusion
Solidification Process(2) - Polymer Processing (Chapter 8, 12) Seok-min Kim email@example.com Plastic Products Plastics can be shaped into a wide variety of products: Molded parts Extruded sections Films
Chapter 15-2: Processing of Polymers ISSUES TO ADDRESS... Other issues in polymers What are the primary polymer processing methods? Chapter 15-1 Polymer Synthesis Reactions There are two types of polymerization
INTRODUCTION Low-density polyethylene is produced through the polymerization of ethylene by a high-pressure process. Ateva EVA copolymers are produced but copolymerizing ethylene (E) with vinyl acetate
Biofuels Production Scrivener Publishing 100 Cummings Center, Suite 541J Beverly, MA 01915-6106 Publishers at Scrivener Martin Scrivener (firstname.lastname@example.org) Phillip Carmical (email@example.com)